364 35 51MB
English Pages [667] Year 2019
Table of contents :
Contents
List of Figures
List of Tables
Preface
Acknowledgments
1 From Atoms to Solids
1.1 Electronic Structure of Atoms
1.2 Forming Bonds Between Atoms
1.2.1 The Essence of Metallic Bonding: The FreeElectron Model
1.2.2 The Essence of Covalent Bonding
1.2.3 Other Types of Bonding in Solids
1.3 The Architecture of Crystals
1.3.1 Atoms with No Valence Electrons
1.3.2 Atoms with s Valence Electrons
1.3.3 Atoms with s and p Valence Electrons
1.3.4 Atoms with s and d Valence Electrons
1.3.5 Atoms with s, d, and f Valence Electrons
1.3.6 Solids with Two Types of Atoms
1.3.7 Hydrogen: A Special OnesValenceElectron Atom
1.3.8 Solids with More Than Two Types of Atoms
1.4 Bonding in Solids
Further Reading
Problems
2 Electrons in Crystals: Translational Periodicity
2.1 Translational Periodicity: Bloch States
2.2 Reciprocal Space: Brillouin Zones
2.2.1 Nature of WaveVector k
2.2.2 Brillouin Zones and Bragg Planes
2.2.3 Periodicity in Reciprocal Space
2.2.4 Symmetries Beyond Translational Periodicity
2.3 The FreeElectron and Nearly FreeElectron Models
2.4 Effective Mass, “k· p” Perturbation Theory
2.5 The TightBinding Approximation
2.5.1 Generalizations of the TBA
2.6 General BandStructure Methods
2.6.1 Crystal Pseudopotentials
2.7 Localized Wannier Functions
2.8 Density of States
2.8.1 FreeElectron Density of States
2.8.2 Local Density of States
2.8.3 Crystal DOS: Van Hove Singularities
Further Reading
Problems
3 Symmetries Beyond Translational Periodicity
3.1 TimeReversal Symmetry for Spinless Fermions
3.2 Crystal Groups: Definitions
3.3 Symmetries of 3D Crystals
3.4 Symmetries of the Band Structure
3.5 Application: Special kPoints
3.6 Group Representations
3.7 Application: The NVCenter in Diamond
Further Reading
Problems
4 From Many Particles to the SingleParticle Picture
4.1 The Hamiltonian of the Solid
4.1.1 Born–Oppenheimer Approximation
4.2 The Hydrogen Molecule
4.3 The Hartree and Hartree–Fock Approximations
4.3.1 The Hartree Approximation
4.3.2 The Hartree–Fock Approximation
4.4 Hartree–Fock Theory of Free Electrons
4.5 Density Functional Theory
4.5.1 Thomas–Fermi–Dirac Theory
4.5.2 General Formulation of DFT
4.5.3 SingleParticle Equations in DFT
4.5.4 The Exchange–Correlation Term in DFT
4.5.5 TimeDependent DFT
4.6 Quasiparticles and Collective Excitations
4.7 Screening: The Thomas–Fermi Model
4.8 Quasiparticle Energies: GW Approximation
4.9 The Pseudopotential
4.10 Energetics and Ion Dynamics
4.10.1 The Total Energy
4.10.2 Forces and Ion Dynamics
Further Reading
Problems
5 Electronic Properties of Crystals
5.1 Band Structure of Idealized 1D Solids
5.1.1 A Finite “1D Solid”: Benzene
5.1.2 An Infinite “1D Solid”: Polyacetylene
5.2 2D Solids: Graphene and Beyond
5.2.1 Carbon Nanotubes
5.3 3D Metallic Solids
5.4 3D Ionic and Covalent Solids
5.5 Doping of Ideal Crystals
5.5.1 Envelope Function Approximation
5.5.2 Effect of Doping in Semiconductors
5.5.3 The p–n Junction
5.5.4 Metal–Semiconductor Junction
Further Reading
Problems
6 Electronic Excitations
6.1 Optical Excitations
6.2 Conductivity and Dielectric Function
6.2.1 General Formulation
6.2.2 Drude and Lorentz Models
6.2.3 Connection to Microscopic Features
6.2.4 Implications for Crystals
6.2.5 Application: Optical Properties of Metals and Semiconductors
6.3 Excitons
6.3.1 General Considerations
6.3.2 Strongly Bound (Frenkel) Excitons
6.3.3 Weakly Bound (Wannier) Excitons
Further Reading
Problems
7 Lattice Vibrations and Deformations
7.1 Lattice Vibrations: Phonon Modes
7.2 The Born ForceConstant Model
7.3 Applications of the ForceConstant Model
7.4 Phonons as Harmonic Oscillators
7.5 Application: Specific Heat of Crystals
7.5.1 The Classical Picture
7.5.2 The QuantumMechanical Picture
7.5.3 The Debye Model
7.5.4 Thermal Expansion Coefficient
7.6 Application: Mo¨ssbauer Effect
7.7 Elastic Deformations of Solids
7.7.1 Phenomenological Models of Solid Deformation
7.7.2 Elasticity Theory: The Strain and Stress Tensors
7.7.3 Strain Energy Density
7.7.4 Isotropic Solid
7.7.5 Solid with Cubic Symmetry
7.7.6 Thin Plate Equilibrium
7.8 Application: Phonons of Graphene
Further Reading
Problems
8 Phonon Interactions
8.1 Phonon Scattering Processes
8.1.1 Scattering Formalism
8.2 Application: The Debye–Waller Factor
8.3 Phonon–Photon Interactions
8.3.1 Infrared Absorption
8.3.2 Raman Scattering
8.4 Phonon–Electron Interactions: Superconductivity
8.4.1 BCS Theory of Superconductivity
8.4.2 The McMillan Formula for Tc
8.4.3 HighTemperature Superconductors
Further Reading
Problems
9 Dynamics and Topological Constraints
9.1 Electrons in External Electromagnetic Fields
9.1.1 Classical Hall Effect
9.1.2 Landau Levels
9.1.3 Quantum Hall Effect
9.1.4 de Haas–van Alphen Effect
9.2 Dynamics of Crystal Electrons: SingleBand Picture
9.3 TimeReversal Invariance
9.3.1 Kramers Degeneracy
9.4 Berry’s Phase
9.4.1 General Formulation
9.4.2 Berry’s Phase for Electrons in Crystals
9.5 Applications of Berry’s Phase
9.5.1 Aharonov–Bohm Effect
9.5.2 Polarization of Crystals
9.5.3 Crystal Electrons in Uniform Electric Field
9.6 Chern Numbers
9.7 Broken Symmetry and Edge States
9.7.1 Broken Symmetry in Honeycomb Lattice
9.7.2 Edge States of Honeycomb Lattice
9.8 Topological Constraints
Further Reading
Problems
10 Magnetic Behavior of Solids
10.1 Overview of Magnetic Behavior of Insulators
10.2 Overview of Magnetic Behavior of Metals
10.2.1 Free Fermions in Magnetic Field: Pauli Paramagnetism
10.2.2 Magnetization in Hartree–Fock FreeElectron Model
10.2.3 Magnetization of Band Electrons
10.3 Classical Spins: Simple Models on a Lattice
10.3.1 Noninteracting Spins on a Lattice: Negative Temperature
10.3.2 Interacting Spins on a Lattice: Ising Model
10.4 Quantum Spins: Heisenberg Model
10.4.1 Motivation of the Heisenberg Model
10.4.2 Ground State of Heisenberg Ferromagnet
10.4.3 Spin Waves in Heisenberg Ferromagnet
10.4.4 Heisenberg Antiferromagnetic Spin Model
10.5 Magnetic Domains
Further Reading
Problems
Appendices
Appendix A Mathematical Tools
Appendix B Classical Electrodynamics
Appendix C Quantum Mechanics
Appendix D Thermodynamics and Statistical Mechanics
Index
Quantum Theory of Materials
This accessible new text introduces the theoretical concepts and tools essential for graduatelevel courses on the physics of materials in condensed matter physics, physical chemistry, materials science and engineering, and chemical engineering. Topics covered range from fundamentals such as crystal periodicity and symmetry, and derivation of singleparticle equations, to modern additions including graphene, twodimensional solids, carbon nanotubes, topological states, and Hall physics. Advanced topics such as phonon interactions with phonons, photons, and electrons, and magnetism, are presented in an accessible way, and a set of appendices reviewing crucial fundamental physics and mathematical tools makes this text suitable for students from a range of backgrounds. Students will beneﬁt from the emphasis on translating theory into practice, with worked examples explaining experimental observations, applications illustrating how theoretical concepts can be applied to real research problems, and 242 informative fullcolor illustrations. Endofchapter problems are included for homework and selfstudy, with solutions and lecture slides for instructors available online. is the John Hasbrouck Van Vleck Professor of Pure and Applied Physics at Harvard University. He holds joint appointments in the Department of Physics and the School of Engineering and Applied Sciences, and is an afﬁliate of the Department of Chemistry and Chemical Biology. He is the Founding Director of the Institute for Applied Computational Science, a Fellow of the American Physical Society, and a Chartered Physicist and Fellow of the Institute of Physics, London.
Efthimios Kaxiras
is the Francis Wright Davis Professor of Physics at MIT, where he is Director of the Institute for Soldier Nanotechnologies. He is a member of the National Academy of Sciences and American Academy of Arts and Sciences, a Fellow of the American Association for the Advancement of Science, a Fellow of the American Physical Society, and a Fellow of the World Technology Network. His awards include the MIT School of Science Graduate Teaching Award (1991), the William Buechner Teaching Prize of the MIT Department of Physics (1996), the David Adler Award (1997) and Aneesur Rahman Prize (2015) of the American Physical Society, and the Max Born Award of the Optical Society of America.
John D. Joannopoulos
Quantum Theory of Materials
EFTHIMIOS K AXIR AS H a r va rd U n i ve r s i t y
J O H N D. J OA N N O P O U LO S M a s s a c h u s e t t s I n s t i t u te o f Te c h n o l o g y
University Printing House, Cambridge CB2 8BS, United Kingdom One Liberty Plaza, 20th Floor, New York, NY 10006, USA 477 Williamstown Road, Port Melbourne, VIC 3207, Australia 314–321, 3rd Floor, Plot 3, Splendor Forum, Jasola District Centre, New Delhi – 110025, India 79 Anson Road, #0604/06, Singapore 079906 Cambridge University Press is part of the University of Cambridge. It furthers the University’s mission by disseminating knowledge in the pursuit of education, learning, and research at the highest international levels of excellence. www.cambridge.org Information on this title: www.cambridge.org/9780521117111 DOI: 10.1017/9781139030809 © Efthimios Kaxiras and John D. Joannopoulos 2019 This publication is in copyright. Subject to statutory exception and to the provisions of relevant collective licensing agreements, no reproduction of any part may take place without the written permission of Cambridge University Press. First published 2019 Printed in Singapore by Markono Print Media Pte Ltd A catalogue record for this publication is available from the British Library
.
ISBN 9780521117111 Hardback Additional resources for this publication at www.cambridge.org/9780521117111 Cambridge University Press has no responsibility for the persistence or accuracy of URLs for external or thirdparty internet websites referred to in this publication and does not guarantee that any content on such websites is, or will remain, accurate or appropriate.
Contents
List of Figures List of Tables Preface Acknowledgments 1
From Atoms to Solids
1.1 Electronic Structure of Atoms 1.2 Forming Bonds Between Atoms 1.2.1 The Essence of Metallic Bonding: The FreeElectron Model 1.2.2 The Essence of Covalent Bonding 1.2.3 Other Types of Bonding in Solids 1.3 The Architecture of Crystals 1.3.1 Atoms with No Valence Electrons 1.3.2 Atoms with s Valence Electrons 1.3.3 Atoms with s and p Valence Electrons 1.3.4 Atoms with s and d Valence Electrons 1.3.5 Atoms with s , d , and f Valence Electrons 1.3.6 Solids with Two Types of Atoms 1.3.7 Hydrogen: A Special Ones ValenceElectron Atom 1.3.8 Solids with More Than Two Types of Atoms 1.4 Bonding in Solids Further Reading Problems 2
Electrons in Crystals: Translational Periodicity
2.1 Translational Periodicity: Bloch States 2.2 Reciprocal Space: Brillouin Zones 2.2.1 Nature of WaveVector k 2.2.2 Brillouin Zones and Bragg Planes 2.2.3 Periodicity in Reciprocal Space 2.2.4 Symmetries Beyond Translational Periodicity 2.3 The FreeElectron and Nearly FreeElectron Models 2.4 Effective Mass, “ k · p” Perturbation Theory 2.5 The TightBinding Approximation 2.5.1 Generalizations of the TBA 2.6 General BandStructure Methods v
page x
xviii xxi xxiii 1 2 5 6 10 14 15 16 21 23 32 33 33 37 39 41 45 46 52 52 59 59 60 65 66 69 75 76 96 99
vi
Contents
2.6.1 Crystal Pseudopotentials 2.7 Localized Wannier Functions 2.8 Density of States 2.8.1 FreeElectron Density of States 2.8.2 Local Density of States 2.8.3 Crystal DOS: Van Hove Singularities Further Reading Problems 3
Symmetries Beyond Translational Periodicity
3.1 TimeReversal Symmetry for Spinless Fermions 3.2 Crystal Groups: Deﬁnitions 3.3 Symmetries of 3D Crystals 3.4 Symmetries of the Band Structure 3.5 Application: Special kPoints 3.6 Group Representations 3.7 Application: The N V Center in Diamond Further Reading Problems 4
From Many Particles to the SingleParticle Picture
4.1 The Hamiltonian of the Solid 4.1.1 Born–Oppenheimer Approximation 4.2 The Hydrogen Molecule 4.3 The Hartree and Hartree–Fock Approximations 4.3.1 The Hartree Approximation 4.3.2 The Hartree–Fock Approximation 4.4 Hartree–Fock Theory of Free Electrons 4.5 Density Functional Theory 4.5.1 Thomas–Fermi–Dirac Theory 4.5.2 General Formulation of DFT 4.5.3 SingleParticle Equations in DFT 4.5.4 The Exchange–Correlation Term in DFT 4.5.5 TimeDependent DFT 4.6 Quasiparticles and Collective Excitations 4.7 Screening: The Thomas–Fermi Model 4.8 Quasiparticle Energies: GW Approximation 4.9 The Pseudopotential 4.10 Energetics and Ion Dynamics 4.10.1 The Total Energy 4.10.2 Forces and Ion Dynamics Further Reading Problems
103 105 107 110 111 112 115 116 119 119 121 124 129 135 137 155 159 159 161 162 163 166 173 173 176 178 182 182 183 186 189 193 195 197 199 202 208 208 218 221 222
vii
Contents
5
Electronic Properties of Crystals
5.1 Band Structure of Idealized 1D Solids 5.1.1 A Finite “1D Solid”: Benzene 5.1.2 An Inﬁnite “1D Solid”: Polyacetylene 5.2 2D Solids: Graphene and Beyond 5.2.1 Carbon Nanotubes 5.3 3D Metallic Solids 5.4 3D Ionic and Covalent Solids 5.5 Doping of Ideal Crystals 5.5.1 Envelope Function Approximation 5.5.2 Effect of Doping in Semiconductors 5.5.3 The p–n Junction 5.5.4 Metal–Semiconductor Junction Further Reading Problems 6
Electronic Excitations
6.1 Optical Excitations 6.2 Conductivity and Dielectric Function 6.2.1 General Formulation 6.2.2 Drude and Lorentz Models 6.2.3 Connection to Microscopic Features 6.2.4 Implications for Crystals 6.2.5 Application: Optical Properties of Metals and Semiconductors 6.3 Excitons 6.3.1 General Considerations 6.3.2 Strongly Bound (Frenkel) Excitons 6.3.3 Weakly Bound (Wannier) Excitons Further Reading Problems 7
Lattice Vibrations and Deformations
7.1 7.2 7.3 7.4 7.5
Lattice Vibrations: Phonon Modes The Born ForceConstant Model Applications of the ForceConstant Model Phonons as Harmonic Oscillators Application: Speciﬁc Heat of Crystals 7.5.1 The Classical Picture 7.5.2 The QuantumMechanical Picture 7.5.3 The Debye Model 7.5.4 Thermal Expansion Coefﬁcient 7.6 Application: M¨ossbauer Effect 7.7 Elastic Deformations of Solids
227 227 227 231 235 239 244 248 256 256 261 265 273 276 276 280 280 284 285 286 291 293 299 302 303 308 311 316 317 319 319 324 328 340 343 343 344 346 349 350 353
viii
Contents
7.7.1 Phenomenological Models of Solid Deformation 7.7.2 Elasticity Theory: The Strain and Stress Tensors 7.7.3 Strain Energy Density 7.7.4 Isotropic Solid 7.7.5 Solid with Cubic Symmetry 7.7.6 Thin Plate Equilibrium 7.8 Application: Phonons of Graphene Further Reading Problems 8
Phonon Interactions
8.1 Phonon Scattering Processes 8.1.1 Scattering Formalism 8.2 Application: The Debye–Waller Factor 8.3 Phonon–Photon Interactions 8.3.1 Infrared Absorption 8.3.2 Raman Scattering 8.4 Phonon–Electron Interactions: Superconductivity 8.4.1 BCS Theory of Superconductivity 8.4.2 The McMillan Formula for T c 8.4.3 HighTemperature Superconductors Further Reading Problems 9
Dynamics and Topological Constraints
9.1 Electrons in External Electromagnetic Fields 9.1.1 Classical Hall Effect 9.1.2 Landau Levels 9.1.3 Quantum Hall Effect 9.1.4 de Haas–van Alphen Effect 9.2 Dynamics of Crystal Electrons: SingleBand Picture 9.3 TimeReversal Invariance 9.3.1 Kramers Degeneracy 9.4 Berry’s Phase 9.4.1 General Formulation 9.4.2 Berry’s Phase for Electrons in Crystals 9.5 Applications of Berry’s Phase 9.5.1 Aharonov–Bohm Effect 9.5.2 Polarization of Crystals 9.5.3 Crystal Electrons in Uniform Electric Field 9.6 Chern Numbers 9.7 Broken Symmetry and Edge States 9.7.1 Broken Symmetry in Honeycomb Lattice 9.7.2 Edge States of Honeycomb Lattice 9.8 Topological Constraints
354 356 361 363 368 369 371 375 375 379 379 381 385 387 389 390 392 394 411 412 415 415 417 417 419 421 424 431 434 438 440 440 441 446 454 454 456 458 459 463 463 465 469
ix
Contents
Further Reading Problems 10
Magnetic Behavior of Solids
10.1 Overview of Magnetic Behavior of Insulators 10.2 Overview of Magnetic Behavior of Metals 10.2.1 Free Fermions in Magnetic Field: Pauli Paramagnetism 10.2.2 Magnetization in Hartree–Fock FreeElectron Model 10.2.3 Magnetization of Band Electrons 10.3 Classical Spins: Simple Models on a Lattice 10.3.1 Noninteracting Spins on a Lattice: Negative Temperature 10.3.2 Interacting Spins on a Lattice: Ising Model 10.4 Quantum Spins: Heisenberg Model 10.4.1 Motivation of the Heisenberg Model 10.4.2 Ground State of Heisenberg Ferromagnet 10.4.3 Spin Waves in Heisenberg Ferromagnet 10.4.4 Heisenberg Antiferromagnetic Spin Model 10.5 Magnetic Domains Further Reading Problems
Appendices
Appendix Appendix Appendix Appendix Index
A Mathematical Tools B Classical Electrodynamics C Quantum Mechanics D Thermodynamics and Statistical Mechanics
476 476 480 481 486 487 490 493 497 497 502 509 510 514 516 520 522 525 525 529 531 549 565 610 646
List of Figures
1.1 1.2 1.3 1.4 1.5 1.6 1.7 1.8 1.9 1.10 1.11 1.12 1.13 1.14 1.15 1.16 1.17 1.18 1.19 1.20 1.21 1.22 1.23 1.24 1.25 1.26
x
Different forms of carbonbased solids page 2 Filling of electronic shells for the elements in the Periodic Table with atomic numbers Z = 1–18 3 Filling of electronic shells for elements with atomic numbers Z = 19–36 4 Periodic behavior of the properties of the elements 4 Schematic representation of the core and valence electrons in an atom 5 Illustration of metallic bonding between many atoms 6 A simple 1D model of the energy levels associated with the freeelectron model for a system of six “atoms” 9 Schematic representation of the formation of a bond between two atoms with one valence electron each 10 Symmetric (+), left panel, and antisymmetric (−), right panel, linear combinations of singleparticle orbitals 12 Illustration of covalent bonding between many atoms 14 Shapes of the unit cells in some lattices that appear in the Periodic Table 16 Illustration of the face centered cubic (FCC) crystal structure 17 Illustration of the hexagonal close packed (HCP) crystal structure 20 Illustration of two interpenetrating FCC or HCP lattices 20 Three different views of the regular icosahedron 21 Illustration of the body centered cubic (BCC) crystal structure 22 Representation of the character of s , p, d atomic orbitals 23 Illustration of covalent bonding in a single plane of graphite, called “graphene” 25 Illustration of atomic arrangement in graphite in a top view (left) and a perspective view (right) 27 The structure of the C 60 molecule or “buckyball” (left) and of carbon nanotubes (right) 27 Illustration of covalent bonding in the diamond lattice 29 The diamond crystal 30 The structure of the diamond lattice as revealed by the transmission electron microscope 30 Typical layer structures that groupV elements form 31 Illustration of cubic crystals formed by ionic solids 34 The zincblende lattice in which every atom is surrounded by four neighbors of the opposite type 34
xi
List of Figures
1.27 Example of an ioniccovalent amorphous structure, the silicondioxide glass 1.28 Illustration of the atomic and electronic structure of a layered transitionmetal dichalcogenide crystal, molybdenum disulﬁde 1.29 Illustration of hydrogen bonding between water molecules in ice 1.30 Illustration of the structure and bonding in perovskite crystals 1.31 The three effective potentials discussed in the text, Lennard–Jones, Morse, and harmonic oscillator 2.1 The 2D crystals deﬁned in Table 2.1 2.2 The 3D crystals deﬁned in Table 2.1 2.3 Energy bands in crystals 2.4 Illustration of boundaries in reciprocal space that bisect the reciprocal lattice vectors ±b 1, ±b 2, ±b3 for a cubic lattice 2.5 Schematic representation of Bragg scattering from atoms on successive atomic planes 2.6 Illustration of the construction of Brillouin zones in a 2D crystal 2.7 The ﬁrst six Brillouin zones of the 2D square lattice 2.8 The shape of occupied portions of the various Brillouin zones for the 2D square lattice with Z = 4 electrons per unit cell 2.9 Symmetries of the 2D square in reciprocal space 2.10 Symmetries of the 2D hexagon in reciprocal space 2.11 Energy bands of the freeelectron and nearly freeelectron models in one dimension 2.12 Free electron bands in the 3D FCC lattice and comparison to the bands of the aluminum crystal 2.13 The band structure for the 2D freeelectron model along the highsymmetry lines in the IBZ 2.14 Bloch states in the tightbinding approximation for a 1D model (p ) 2.15 Singleparticle energy eigenvalues ±k(s) and ±k in the ﬁrst BZ for the 1D inﬁnite chain model, with one atom per unit cell and one orbital per atom in the TBA with nearestneighbor interactions (+) (−) 2.16 Singleparticle energy eigenvalues ±k and ±k in the ﬁrst BZ for the 1D inﬁnite chain model, with one atom per unit cell that has one s orbital and one p orbital, in the TBA with nearestneighbor interactions 2.17 (Left) The 2D square lattice with atoms that possess s orbitals and p orbitals. (Right) The corresponding BZ with the irreducible part shaded 2.18 The TBA band structure of the 2D square lattice with parameters from Table 2.3 2.19 (Left) The square lattice with a twoatom basis. (Right) The corresponding ﬁrst BZ with the irreducible part shaded 2.20 Bands of the twoatom unit cell with p x , p y orbitals in one of the atoms and a dx2 −y2 orbital in the other atom, in the 2D square lattice 2.21 The landscape of the bands in the 2D square lattice with a twoatom basis which have a d orbital on one site and p x , p y orbitals on the other
35 36 38 40 44 54 54 59 61 62 64 64 65 68 69 70 72 74 80
82
83 85 87 91 93 94
xii
List of Figures
2.22 The graphene lattice and π bands 2.23 The landscape of the π bands in the 2D honeycomb lattice with a twoatom basis and a p z like orbital at each site 2.24 (Left) Two p orbitals at arbitrary directions θ1, θ2 relative to the line that joins their centers. (Right) An s orbital and a p orbital at an angle θ relative to the line that joins their centers 2.25 (Left) Illustration of the Wigner–Seitz cell for a 2D hexagonal lattice. (Right) Illustration of the mufﬁntin potential 2.26 Illustration of the calculation of the density of states 2.27 Illustration of the simple model for tunneling between a metal (left side) and a semiconductor (right side) 2.28 Illustration of the behavior of the density of states as a function of the energy ± , in the freeelectron model in three, two, and one dimensions 2.29 The behavior of DOS, g (± ), near critical points of different type in three dimensions 3.1 (Left) The symmetry operations of the 2D honeycomb lattice with a basis of two different atoms. (Right) The irreducible Brillouin zone for the 2D honeycomb lattice with C 3v symmetry 3.2 The conventional unit cells of the 14 Bravais lattices in the six systems in three dimensions 3.3 Illustration of symmetry axes of the tetrahedron and the octahedron 3.4 Stereograms for 30 point groups in three dimensions 3.5 Symmetry operations of the cube 3.6 (Left) The symmetry operations of the 2D square lattice. (Right) The irreducible Brillouin zone for the 2D square lattice with C 4v symmetry 3.7 (Left) The Brillouin zone and its irreducible part of the 2D square lattice. (Right) The energy bands of the square lattice with s , p x , p y orbitals on each site 3.8 Structure and symmetries of the N V center in diamond 3.9 Illustration of the occupation of states in the NV − center 4.1 Schematic representation of the hydrogen wavefunctions for isolated atoms and the linear combinations that preserve the inversion symmetry with respect to the center of the molecule 4.2 Energy ±k of singleparticle states as a function of momentum k / kF for two different values of r s = 1, 2 4.3 (Left) The charge density of valence electrons in the silicon crystal within the conventional cubic cell. (Right) A conventional ballandstick representation of the diamond structure of bulk Si 4.4 The original Coulomb potential and the total (screened) potential 4.5 Schematic illustration of typical calculated energy eigenvalues for ﬁctitious particles in the DFT/LDA approach and in the GW approach 4.6 Electron density as a function of radial distance from the nucleus, for four elements: C, Si, Ge, and Pb
95 96
97 101 108 109 111 115
123 125 126 127 129 134
153 156 158
168 180
193 200 202 203
xiii
List of Figures
4.7 4.8 5.1
5.2 5.3 5.4
5.5
5.6 5.7 5.8 5.9 5.10 5.11
5.12
5.13
5.14 5.15 5.16 5.17
Schematic representation of the construction of the atomic
pseudowavefunction φ˜ (r ) and the atomic pseudopotential V˜ (r ) Total energy as a function of volume for various crystal phases of silicon (Top row): The structure of benzene, C 6 H6. (Bottom row) The electronic density on a plane through the C and H atoms (left), and on a plane situated ˚ above the atoms (right) 0.5 A Interpretation of orbitals in benzene, C6 H6, as “Bloch” states Energy levels of benzene represented as a band structure (Top row) Illustration of the structure of transpolyacetylene, [ −C2 H2−]n . (Bottom row) The total charge density obtained from DFT calculations for the two models (Left) Energy bands of polyacetylene, [−C2 H2−]n , and density of states (far left). (Right) Wavefunctions of polyacetylene shown as linear combinations of p z orbitals Band structure of symmetric (left) and asymmetric (right) models of polyacetylene, obtained from DFT calculations Schematic illustration of the soliton motion in polyacetylene Band structure of graphene, as obtained from DFT calculations Valence electron charge density plots for graphene, on the plane of the atoms (left) and on a plane perpendicular to it Density of states of representative 2D crystals: graphene (top), a semimetal and BN (bottom), an insulator Density of states of representative 2D crystals: silicene (top), a structure similar to graphene but consisting of Si atoms, a semimetal and MoS2 (bottom), a semiconductor, representative of the metaldichalcogenide family of layered solids (Top) A graphene sheet with the ideal lattice vectors denoted as a1, a2 . (Bottom) Perspective views of the (7, 7) armchair tube, the (8, 4) chiral tube, and the (7, 0) zigzag tube, along their axes (a) The graphene Brillouin zone, with reciprocal lattice vectors b 1, b2 and tuberelated vectors b3 , b4 . (b) The folding of the full zone into the reduced zone, determined by the vectors ±b 3, ±b 4. (c) The Brillouin zone for (n, 0) tubes, and the example of the (6, 0) tube. (d) The Brillouin zone for (n , n ) tubes, and the example of the (4, 4) tube Examples of CNT band structures obtained with the tightbinding approximation Band structure of four metals, Al, Cu, Ag, Au, all in the FCC structure, along highsymmetry directions of the BZ shown in Fig. 2.12 Band structure of three metals, V, Cr, Fe, all in the BCC structure, along highsymmetry directions in the BZ Valence electron charge density plots on the (100) plane of the bulk (FCC) crystal structure for two metallic solids: Al (left) and Ag (right) ion
206 217
228 229 230
232
232 234 235 236 237 238
239
240
242 243 245 246 246
xiv
List of Figures
5.18 Density of states of representative 3D metallic crystals: a simple, freeelectron metal, Al (top) and a noble, d electron metal, Au (bottom) 5.19 Band structure of two ionic insulators, LiF and NaCl (both in rocksalt structure), a partially ionic/partially covalent insulator, BN (zincblende structure), and a covalently bonded insulator, C (diamond structure) 5.20 Band structure of representative semiconductors: Si and Ge in the diamond structure; AlP, GaAs, SiC, and ZnS, all in the zincblende structure 5.21 Valence electron charge density plots on the (110) plane of the bulk diamond or zincblende crystal structure for representative solids 5.22 Density of states of representative 3D semiconducting crystals 5.23 (Left) Schematic illustration of light and heavy electron and hole states. (Right) Schematic illustration of shallow donor and acceptor impurity states in a semiconductor with direct gap 5.24 Phosphorus dopant state in bulk silicon 5.25 Schematic representation of p–n junction elements 5.26 Band bending associated with a p–n junction 5.27 Origin of the intrinsic potential in the p–n junction 5.28 Schematic representation of the operation of a photovoltaic device (PVD) (left panel), a lightemitting diode (LED) (middle panel), and the effect of forward and reverse bias (middle and right panels, respectively), based on the p–n junction 5.29 Illustration of band bending in p–n junctions 5.30 The basic features of a MOSFET 5.31 Band alignment in metal–semiconductor junction 5.32 Band alignment in metal–oxide–semiconductor junction 5.33 Illustration of the structure of cispolyacetylene, [−C4 H4−]n , in the two possible arrangements of the singe/double bond sequence along nearestneighbor C atoms 6.1 The absorption spectrum of benzene, C6 H6 , as a function of the excitation energy, obtained using TDDFT 6.2 Illustration of the general behavior of the real and imaginary parts of the dielectric function 6.3 Example of the behavior of the real and imaginary parts of the dielectric function for Al, a representative freeelectronlike solid 6.4 Examples of the behavior of the real part of the dielectric function for Cu (top) and Ag (bottom) 6.5 Representative examples of the interband contributions to the dielectric function (real and imaginary parts, respectively) for semiconductors (Si, Ge, AlP, GaAs) and insulators (C, SiC), obtained from the band structures calculated by DFT methods 6.6 Examples of the behavior of the real and imaginary parts of the dielectric function for Cu (top) and Ag (bottom) 6.7 The dielectric function of Si (top) and Ge (bottom), real and imaginary parts
247
249 251 252 254
257 263 266 267 267
268 269 272 274 276
277 283 288 289 290
297 300 302
xv
List of Figures
6.8
6.9
6.10 7.1 7.2 7.3 7.4 7.5 7.6
7.7 7.8
7.9
7.10 7.11 7.12 7.13 7.14 7.15 8.1 8.2 8.3 8.4 8.5 8.6
(Left) Modiﬁcation of the absorption spectrum in the presence of excitons relative to the spectrum in the absence of excitons. (Right) Schematic representation of the conduction and valence bands and the energy levels in the gap corresponding to electron–hole bound states Comparison of Coulomb interaction contributions for excitonic states with the particle and hole situated in the same unit cell (left panel) and in different unit cells a distance R apart (right panel) (Left) Excitons in Cu2 O. (Right) Schematic illustration of the wavefunction of an s state of the exciton The origin of the bondbending term in the forceconstant model Bond stretching and bond bending in the forceconstant model Illustration of the 1D chain with lattice constant a and one atom of mass M per unit cell The atomic displacements corresponding to phonon modes in the 1D chain with one atom per unit cell Illustration of the 1D chain with lattice constant a and two atoms per unit cell (Top) Deﬁnition of the model of the periodic chain in 2D, with lattice constant a1 and two atoms per unit cell. (Bottom) The atomic displacements of the phonon modes for the periodic chain with lattice constant a1 and two atoms per unit cell The 2D square lattice with lattice constants a1, a2 , with one atom per unit cell (Top) The frequencies of the phonon modes of the 2D square lattice along different highsymmetry directions of the BZ. (Bottom) Atomic displacements of the phonon modes with frequencies marked as (a), (b), (c) and (d) (Top) The phonon spectrum of Si along highsymmetry directions, calculated within the forceconstant model. (Bottom) Atomic displacements associated with the phonon modes in Si at the ² and X points in the BZ (Left) Behavior of the speciﬁc heat c as a function of temperature T in the Debye model. (Right) Comparison of the density of states in the Debye model Fit of calculated total energies of various elemental solids to the universal binding energy relation Deﬁnition of the strain tensor for the cartesian coordinate system Deﬁnition of the stress tensor for the cartesian coordinate system The Born forceconstant model for graphene The phonon spectrum of the honeycomb lattice (graphene) in 3D space Diagrams for the one and twophonon scattering processes Illustration of excitations involved in Rayleigh, Stokes and antiStokes scattering, and infrared absorption Illustration of excitations involved in Raman scattering processes Illustration of attractive effective interaction between two electrons mediated by phonons Scattering between electrons of initial and ﬁnal wavevectors through the exchange of a phonon Features of the BCS model
304
311 316 326 326 330 331 332
334 336
337
339 347 356 357 359 372 374 384 388 391 395 405 408
xvi
List of Figures
8.7 9.1 9.2 9.3 9.4 9.5
9.6 9.7 9.8 9.9 9.10 9.11
9.12
9.13 9.14 9.15 9.16 9.17 9.18 9.19 9.20
9.21 9.22 9.23
Examples of the structure of high T c compounds The conﬁning potential, energies, and wavefunctions of the two lowest states at an insulator–semiconductor junction Geometry of the 2D electrons in the Hall effect Schematic representation of experimental measurements in the Hall effect Loop geometry for establishing the quantum Hall effect (Left) The energy levels of states in the ribbon as a function of the position of their centers. (Right) The density of states for the states that include edge effects and the ideal harmonic oscillator levels Schematic representation of classical orbits of charged particles, in the bulk and at the edges of a ribbon on the x , y plane Density of states and ﬁlling of Landau levels, including the effects of disorder, at different values of the magnetic ﬁeld B Illustration of the de Haas–van Alphen effect in a 2D electron gas The Fermi surface of Au Singleparticle energy eigenvalues for the simple example that illustrates the motion of electrons and holes in a oneband, 1D crystal The position vector r appearing in the ﬁeld of the Dirac monopole M situated at the origin, to illustrate the calculation of Berry’s phase in a system with two independent variables, the polar angle ϑ and the azimuthal angle ϕ (Left) The honeycomb lattice with the primitive lattice vectors a1, a2 and the primitive unit cell. (Right) The corresponding band structure, in solid lines, along the highsymmetry directions of the BZ Brillouin zone of the 2D honeycomb lattice, with the highsymmetry points identiﬁed Illustration of Aharonov–Bohm effect description in terms of Berry’s phase Illustration of the ambiguity in determining the dipole moment p in the unit cell of a 1D crystal with period a (Left) The band structure of a single layer of MoS2. (Right) The calculated Berry curvature for the highest valence band The ﬁrst Brillouin zone of the 2D square lattice Honeycomb lattice with broken timereversal symmetry The structure of ribbons with armchair (left panel) and zigzag (right panel) edges (a) The BZ of the original honeycomb lattice. (b) How sections are displaced by the reciprocal lattice vectors to be mapped into a new ﬁrst BZ (c) The armchairedged ribbon BZ. (d) The zigzagedged ribbon BZ Energy bands of ribbons cut from the 2D honeycomb lattice with armchair (left) or zigzag (right) edges Energy bands for zigzagedged ribbons of the honeycomb lattice, with broken symmetry Illustration of the analogy between the genus g of a surface and the topological or Chern invariant N for a band structure
414 418 419 422 424
428 429 430 433 433 437
445
449 451 455 457 460 462 464 466
467 467 468 470
xvii
List of Figures
9.24 Illustration of the behavior of edge states in the case of different values of the topological invariant 9.25 (Left) A 2D model square lattice with two atoms per unit cell. (Right) The corresponding energy bands 9.26 The four energy bands of the 3D cubic lattice model with two atoms per unit cell having an s like (even parity) and a p like (odd parity) orbital 10.1 The total energy multiplied by a factor of 10 and the magnetization m of the polarized electron gas, as functions of r s 10.2 Illustration of the occupation of spinup electron states and spindown electron states, with corresponding Fermi levels 10.3 The entropy per dipole and inverse temperature for the model of dipoles in an external magnetic ﬁeld 10.4 The average magnetization M as a function of temperature for the Ising model 10.5 Graphical solution of Eq. (10.33) 10.6 The free energy per particle as a function of the average magnetization per particle, for various values of T /T c 10.7 The three terms in the effective secondorder hamiltonian obtained from the Hubbard model in the limit U ² t 10.8 Illustration of a spin wave in the 2D square lattice with k = ( 61 , 61 ) πa , where a is the lattice constant 10.9 Illustration of the N´eel state on a 2D square lattice 10.10 Illustration of magnetic domains in a ferromagnet 10.11 Hysteresis curve of the magnetization M in a ferromagnet upon application of an external ﬁeld H A.1 (Left) The δ function as represented by a normalized gaussian, Eq. (A.55). (Right) The ϑ function as represented by Eq. (A.60) C.1 Illustration of the oscillatory and decaying exponential nature of the wavefunction in regions where the potential energy is lower than or higher than the total energy C.2 The transmission coefﬁcient of a square barrier for an incident quantum mechanical particle C.3 The lowest six eigenfunctions of the 1D harmonic oscillator potential C.4 Contours of constant value for representative p , d , and f orbitals C.5 The lowest six radial eigenfunctions of the Coulomb potential for the hydrogen atom D.1 The Maxwell construction D.2 Isotherms on the P –V plane (left plot) and phase boundaries between the solid, liquid, and gas phases on the P –T plane (right plot) D.3 Average occupation numbers in the Maxwell–Boltzmann, Fermi–Dirac, and Bose–Einstein distributions D.4 Effective interaction potential for a pair of bosons or fermions
471 472 474 493 494 500 504 507 508 513 519 521 524 525 540
568 569 580 583 584 619 621 627 641
List of Tables
1.1 1.2 1.3 1.4 2.1 2.2 2.3
2.4 3.1 3.2 3.3 3.4 3.5 3.6 3.7 3.8 4.1 5.1 5.2 5.3
xviii
The linear combinations of s and p atomic orbitals that form the sp 2 hybrids for the two atoms per unit cell in the graphite structure page 26 The linear combinations of s and p atomic orbitals that form the sp 3 hybrids for the two atoms per unit cell in the diamond structure 28 Parameters for the Lennard–Jones potential for noble gases 42 Comparison of the three effective potentials, Lennard–Jones VLJ (r ), Morse V M (r ), and harmonic oscillator VHO (r ) 42 Examples of 2D and 3D crystals 53 Matrix elements for the 2D square lattice with s , p x , p y , p z orbitals at highsymmetry points 88 Values of the onsite and hopping matrix elements for the band structure of the 2D square lattice with an orthogonal s and p basis and nearestneighbor interactions 89 Symbols, multiplicity, type, and characteristic behavior of the coefﬁcients α i , i = 1, 2, 3 along the principal axes for critical points in d = 3 dimensions 113 Symmetry operations and group multiplication table for symmetries of the C 3v group 123 The seven crystal systems and the associated 32 point groups for crystals in three dimensions 124 The 24 symmetry operations of the cube that involve rotations by π , π/3, π/2, and 2 π 128 Group multiplication table for symmetries of the 2D square lattice 134 Class multiplication table for the C 3v group 145 Character table for the irreducible representations of the C 3v group 146 Character table for the irreducible representations of the C 4v group 150 Character tables for the irreducible representations corresponding to the X and ± highsymmetry points of the 2D square lattice 153 Correlation energy functionals and exchange–correlation potentials in various models 191 Structural and electronic properties of common metals, grouped according to crystal structure and the type of valence electrons 248 Structural and electronic properties of common semiconductors, grouped according to the type of elements that form the crystal 255 Effective masses at the CBM and VBM of representative elemental (Si and Ge) and compound semiconductors (GaAs) 262
xix
List of Tables
6.1 6.2
Plasma frequencies for various metal and semiconductor crystals Examples of Frenkel excitons in ionic solids and Mott–Wannier excitons in semiconductors 6.3 Spin conﬁgurations for a particle–particle pair and a particle–hole pair for spin1/2 particles 7.1 Frequencies of four highsymmetry phonon modes in Si, at the center (² ) and the boundary (X) of the Brillouin zone, obtained by theoretical calculations and experimental measurements 7.2 Debye temperatures and frequencies for several elemental solids 7.3 Values of the shear modulus, Lam´e’s constant, and Poisson’s ratio for representative covalent and ionic solids (left column) and metals (right column) 7.4 Bulk moduli and elastic constants for representative cubic crystals at room temperature 7.5 Dynamical matrix for graphene in the Born forceconstant model, including contributions from ﬁrst nearest neighbors only 8.1 Critical temperature, critical ﬁeld, and Debye frequency of elemental conventional superconductors 8.2 Critical temperature of representative hightemperature superconductors 10.1 Total spin S, orbital angular momentum L , and total angular momentum J numbers for the l = 2 (d shell) and l = 3 (f shell) as they are being ﬁlled by n electrons 10.2 Examples of elemental and compound ferromagnets and antiferromagnets C.1 The lowest six eigenfunctions of the 1D harmonic oscillator potential C.2 The spherical harmonics Y lm (θ , φ ) for l = 0, 1, 2, 3 along with the x , y , z representation of the linear combinations for given l and  m  and the identiﬁcation of those representations as s , p, d , f orbitals C.3 The radial wavefunctions for n = 1, 2, 3 and the associated Laguerre polynomials used in their deﬁnition
301 304 306
340 348
365 370 373 393 413
483 523 579
582 585
Preface
Why do various materials behave the way they do? For instance, what makes a material behave like a good insulator, instead of being a good conductor or a semiconductor? What determines the strength of a material? How can we account for the color of different solids? Questions like these have attracted curious minds for centuries. Materials, after all, are of central importance to humanity: they deﬁne the stage of civilization, as in “Stone Age,” “Bronze Age,” “Iron Age,” and the current “Silicon Age.” The scientiﬁc study of the properties of materials in the last two centuries has produced a body of knowledge referred to as the “physics of materials” that goes a long way toward explaining and even predicting their properties from ﬁrstprinciples theoretical concepts. Our book aims to present these concepts in a concise and accessible manner. The book emerged as the result of many years of teaching this subject at Harvard and MIT. The intended audience is graduate or advanced undergraduate students in physics, applied physics, materials science, chemistry, and related engineering and applied science ﬁelds. There are classic textbooks on the subject, the venerable work by N. W. Ashcroft and N. D. Mermin, Solid State Physics , being a standard example; there are also numerous more recent works, for instance Fundamentals of Condensed Matter Physics by M. L. Cohen and S. G. Louie, a work of great depth and clarity, and the delightfully intuitive Physics of Solids by E. N. Economou. We mention most of these books as suggestions for further reading at the end of each chapter, as appropriate. Taken together, these sources quite nicely cover all important aspects of the subject. The present work aims to ﬁll a gap in the literature, by providing a single book that covers all the essential topics, including recent advances, at a level that can be accessible to a wider audience than the typical graduate student in condensed matter physics. This is what prompted us to use the word “materials” (rather than “solids” or “condensed matter”) in the title of the book. Consistent with this aim, we have included topics beyond the standard fare, like elasticity theory and group theory, that hopefully cover the needs, and address the interests, of this wider community of readers. To facilitate accessibility, we have intentionally kept the mathematical formalism at the simplest possible level, for example, avoiding second quantization notation except when it proved absolutely necessary (the discussion of the BCS model for superconductivity, Chapter 8). Instead, we tried to emphasize physical concepts and supply all the information needed to motivate how they translate into speciﬁc expressions that relate physical quantities to experimental measurements. The book concentrates on theoretical concepts and tools, developed during the last few decades to understand the properties of materials. As such, we did not undertake an xxi
xxii
Preface
extensive survey of experimental data. Rather, we compare the results of the theoretical models to key experimental ﬁndings throughout the book. We also give examples of how the theory can be applied to explain what experiment observes, as well as several compilations of experimental data to capture the range of behavior encountered in various types of materials. The book can be used to teach a onesemester graduatelevel course (approximately 40 hours of lecture time) on the physics of materials. For an audience with strong physics and math background and some previous exposure to solidstate physics, this can be accomplished by devoting an introductory lecture to Chapter 1, and covering the contents of Chapters 2–7 thoroughly. Topics from Chapters 8, 9, and 10 can then be covered as time permits and the instructor’s interest dictates. An alternative approach, emphasizing more the applications of the theory and aimed at an audience with no prior exposure to solidstate physics, is to cover thoroughly Chapters 1 and 2, skip Chapter 3, cover Sections 4.1– 4.7, Chapters 5 and 6, Sections 7.1–7.5, Sections 8.3 and 8.4, and selected topics from Chapters 9 and 10 as time permits. Many examples and applications are carefully worked out in the text, illustrating how the theoretical concepts and tools can be applied to simple and more sophisticated models. Not all of these need to be presented in lectures; in fact, the reason for giving their detailed solutions was to make it possible for the student to follow them on their own, reserving lecture time for discussions of key ideas and derivations. We have also included several problems at the end of each chapter and we strongly encourage the interested student to work through them in detail, as this is the only meaningful way of mastering the subject. Finally, we have included an extensive set of appendices, covering basic mathematical tools and elements from classical electrodynamics, quantum mechanics, and thermodynamics and statistical mechanics. The purpose of these appendices is to serve as a reference for material that students may have seen in a different context or at a different level, so that they can easily refresh their memory of it, or become familiar with the level required for understanding the discussion in the main text, without having to search a different source.
Acknowledgments
When trying to explain something, it is often difﬁcult to keep track of how your own understanding of the ideas was formed. Acknowledging all the sources of inspiration and insight can therefore be an impossible task, but some of these sources deﬁnitely stand out. We wish to thank our teacher and mentor Marvin Cohen as an especially important inﬂuence on our thinking and understanding of physics. EK wishes to express a deep debt of gratitude to his teachers at various stages of his career, John Joannopoulos, Kosal Pandey, and Lefteris Economou, all of whom served as role models and shaped his thinking. Many colleagues have played an equally important role, including Bert Halperin, David Nelson, Nihat Berker, and Stratos Manousakis. The students who patiently followed several iterations of the manuscript, helping to improve it in ways big and small, are the ultimate reason for putting a vast collection of handwritten notes into a coherent text – we thank them sincerely, and hope they beneﬁtted from the experience. Some of them put an extraordinary amount of energy and care into writing solutions to the problems at the end of the chapters, for which we are thankful. The most recent and careful compilation was made by Cedric Flamant, who also corrected some problem statements and several inaccuracies in the text – he deserves special thanks. Daniel Larson read Chapter 9 very carefully, and provided much useful feedback and suggestions for improving the presentation. We also thank Eugene Mele for many useful comments on the physics of topological states. Last but not least, we wish to acknowledge the essential, or more appropriately, existential role that our partners Eleni and Kyriaki played in this endeavor; they have put up with innumerable hours of distraction while we were working out some idea to include in the book. Without their support and patience, the book would simply not exist; we gratefully dedicate it to them.
xxiii
1
From Atoms to Solids
Materials exhibit an extremely wide range of properties, which is what makes them so useful and indispensable to humankind. The extremely wide range of the properties of materials is surprising, because most of them are made up from a relatively small subset of the elements in the Periodic Table: about 20 or 30 elements, out of more than 100 total, are encountered in most common materials. Moreover, most materials contain only very few of these elements, from one to half a dozen or so. Despite this relative simplicity in composition, materials exhibit a huge variety of properties over ranges that differ by many orders of magnitude. It is quite extraordinary that even among materials composed of single elements, physical properties can differ by many orders of magnitude. One example is the ability of materials to conduct electricity. What is actually measured in experiments is the resistivity, that is, the difﬁculty with which electrical current passes through a material. Some typical singleelement metallic solids (like Ag, Cu, Al) have roomtemperature resistivities of 1–5 µ±·cm, while some metallic alloys (like nichrome) have resistivities of 102 µ±·cm. All these materials are considered good conductors of electrical current. Certain singleelement solids (like Si and Ge) have roomtemperature resistivities much higher than good conductors, for instance, 2.3 × 1011 µ±·cm for Si, and they are considered semiconductors. Finally, certain common materials like wood (with a rather complex structure and chemical composition) or quartz (with a rather simple structure and composed of two elements, Si and O) have roomtemperature resistivities of 1016 –1019 µ±·cm (for wood) to 1025 µ ±·cm (for quartz). These solids are considered insulators. The range of electrical resistivities covers an impressive 25 orders of magnitude. Even for two materials that are composed of the same element, carbon, their resistivity can differ by many orders of magnitude: graphitic carbon has resistivity 3.5 × 103 µ ±· cm and is considered a semimetal, while in the diamond form, carbon has a much higher resistivity of ∼ 1022 µ±·cm, the difference being entirely due to the different crystal structure of the two forms, as shown in Fig. 1.1. Another example has to do with the mechanical properties of materials. Solids are classiﬁed as ductile when they yield plastically when stressed, or brittle when they do not yield easily, but instead break when stressed. A useful measure of this behavior is the yield stress σY , which is the stress up to which the solid behaves as a linear elastic medium when stressed, that is, it returns to its original state when the external stress is removed. Yield stresses in materials, measured in units of MPa, range from 40 in Al, a rather soft and ductile metal, to 5 × 104 in diamond, the hardest material, a brittle insulator. The yield stresses of common steels range from 200 to 2000 MPa. Again we see an impressive range of more than three orders of magnitude in how a material responds to an external agent, in this case a mechanical stress. 1
2
Fig. 1.1
1
From Atoms to Solids
Different forms of carbonbased solids. Left: A diamond in raw form, in the shape of an ideal octahedron. The structure of the diamond crystal offers many equivalent planes along which it can be cleaved, exposing a shape of very high symmetry in polished (“cut”) form. Right: Graphite [source: Rob Lavinsky, iRocks.com CCBYSA3.0, via Wikimedia Commons].
Naively, one might expect that the origin of these widely different properties is related to great differences in the concentration of atoms, and correspondingly that of electrons. This is far from the truth. Concentrations of atoms in a solid range from 1022 cm−3 in Cs, a representative alkali metal, to 17 × 1022 cm−3 in C, a representative covalently bonded solid. Anywhere from one to a dozen electrons per atom participate actively in determining the properties of solids. These considerations give a range of atomic concentrations of roughly 20, and of available electron concentrations1 of roughly 100. These ranges are nowhere close to the ranges of yield stresses and electrical resistivities mentioned above. Rather, the variation of the properties of solids has to do with the speciﬁc ways in which the available electrons of the constituent atoms interact when these atoms are brought together at dis˚ = 10 −10 m = 10−1 nm). Typical distances between nearesttances of a few angstroms (1 A ˚ The way in which the available electrons neighbor atoms in solids range from 1.5 to 3 A. interact determines the atomic structure, and this in turn determines all the other properties of the solid, including mechanical, electrical, optical, thermal, and magnetic properties.
1.1
Electronic Structure of Atoms
We invoked above, on several occasions, the term “available electrons” for speciﬁc types of atoms. This is not a very precise term, but was intended to convey the message that not all of the electrons of an atom are necessarily involved in determining the properties of a solid in which this atom exists. Some electrons eagerly participate in the formation of the solid, by being shared among several atoms and thus serving as the “glue” that holds those atoms together, while other electrons are very tightly bound to the nuclei of the constituent 1 The highest concentration of atoms does not correspond to the highest number of available electrons per atom.
3
Fig. 1.2
1.1
Z
n
l
m
H
1
1
0
0
He
2
1
0
0
Li
3
2
0
0
Be
4
2
0
0
B
5
2
1
+1
C
6
2
1
0
N
7
2
1
1
O
8
2
1
+1
F
9
2
1
0
Ne
10
2
1
1
Na
11
3
0
0
Mg 12
3
0
0
Al
13
3
1
+1
Si
14
3
1
0
P
15
3
1
1
S
16
3
1
+1
Cl
17
3
1
0
Ar
18
3
1
1
Electronic Structure of Atoms
1s
2s
2p
3s
3p
3d
Filling of electronic shells for the elements in the Periodic Table with atomic numbers Z = 1–18: s shells (l = 0, m = 0) are represented by one red box, p shells ( l = 1, m = 0, ±1) by three blue boxes, and d shells (l = 2, m = 0, ±1, ±2) by ﬁve green boxes. Each box can contain up to two electrons of opposite spin (up and down arrows). For each element, we show the values of the principal (n) and angular momentum (l) quantum numbers, as well as the value of the magnetic ( m) quantum number of the last electron.
atoms, almost in exactly the same way as if the atoms were in complete isolation from each other; the latter electrons play essentially no role in determining the properties of the solid. This is an important distinction, which deserves further discussion. The solution of the Schr¨odinger equation for the isolated atom produces a number of states in which electrons can exist. The total number of electrons in the neutral atom, equal to the total number of protons in its nucleus, called the atomic number Z , determines how many of the allowed states are occupied. The occupation of the allowed states leads to a certain number of shells being completely full (the ones with the lowest energy and wavefunctions that are closest to the nucleus), while some shells can be partially ﬁlled (the ones with higher energy and wavefunctions that extend farther from the nucleus).2 A schematic representation of the ﬁlling of electronic shells for atoms with Z = 1–36 is given in Figs 1.2 and 1.3, where it becomes obvious which shells are completely ﬁlled and which are partially ﬁlled by electrons for each element. A continuation of this sequence of ﬁlling of electronic shells leads to the Periodic Table, presented in the next section. The periodic ﬁlling of the electronic shells is actually quite evident in some basic properties of atoms, like their physical size or their tendency to attract electrons, referred 2 A more detailed discussion is given in Appendix C.
4
Fig. 1.3
1
Z
n
l
m
K
19
4
0
0
Ca
20
4
0
0
Sc
21
3
2
+2
Ti
22
3
2
+1
V
23
3
2
0
Cr * 24
3
2
1
Mn 25
3
2
2
Fe
26
3
2
+2
Co
27
3
2
+1
Ni
28
3
2
0
Cu* 29
3
2
1
Zn
30
3
2
2
Ga
31
4
1
+1
Ge
32
4
1
0
As
33
4
1
1
Se
34
4
1
+1
Br
35
4
1
0
Kr
36
4
1
1
1s
2s
From Atoms to Solids
2p
3s
3p
4s
3d
4p
Filling of electronic shells for elements with atomic numbers Z = 19–36. The notation is the same as in Fig. 1.2. Elements marked by an asterisk have electronic levels ﬁlled out of the regular order: for example, Cu has a 3d10 4s 1 shell rather than a 3d94s2 shell. A
ENS
2.5
4.0
2.0 3.0
1.5
2.0
1.0
1.0
0.5
0.0 2 Fig. 1.4
10
18
36
54 Z
0.0
2
10
18
36
54 Z
˚ and electronegativity scale Periodic behavior of the properties of the elements: atomic radii (A) (ENS), for elements with atomic numbers Z from 1 to 54. The values corresponding to closed electronic shells, Z = 2, 10, 18, 36, 54, that is, the elements He, Ne, Ar, Kr, Xe, are indicated. The color coding corresponds to the different types of electronic shells that are being gradually ﬁlled: red for the s shells, blue for the p shells, and green for the d shells.
5
1.2
Forming Bonds Between Atoms
to as the “electronegativity scale” (ENS), as shown in Fig. 1.4. Interestingly, as the number of protons in the nucleus increases (Z increases), the electron wavefunctions become more compact and the atom shrinks in size, while the levels for a particular ( n, l) set are being gradually ﬁlled by electrons. After a shell is full, as is the case for the elements He (Z = 2), Ne (Z = 10), Ar (Z = 18), and Kr (Z = 36), the socalled noble gases, the size is a local minimum; there is an abrupt increase in size for the elements with one more proton, when the next electronic shell starts being ﬁlled. Similarly, the ENS exhibits a regular pattern, that is, with steadily increasing values within each partially ﬁlled shell and the highest value corresponding to those elements that are just one electron short of having a completely ﬁlled electronic shell, like F (Z = 9), Cl (Z = 17), Br (Z = 35).
1.2
Forming Bonds Between Atoms
The electrons in the outermost, partially ﬁlled shells of the isolated atom are the ones that interact strongly with similar electrons in neighboring atoms in the solid; these are called valence electrons, while the remaining electrons in the completely ﬁlled shells of the atom are called core electrons. This is shown schematically in Fig. 1.5. Core electrons are essentially unaffected when the atom is surrounded by its neighbors in the solid. For most practical purposes it is quite reasonable to neglect the presence of the core electrons as far as the solid is concerned, and consider how the valence electrons behave. The core electrons and the nucleus form the ion, which has a positive net charge equal in magnitude to the number of valence electrons. The description of the solid can then be based on the behavior of ions and the accompanying valence electrons. The classiﬁcation of electrons in the atom into core and valence is very useful when we address the issue of how atoms come together to form a solid. This is illustrated next in two representative and very broad cases. The ﬁrst concerns the type of bonding found in metallic solids, the second the type of bonding common in insulating or semiconducting materials, called covalent bonding.
Fig. 1.5
Schematic representation of the core and valence electrons in an atom, shown as the red and blue clouds, respectively.
6
1
1.2.1
From Atoms to Solids
The Essence of Metallic Bonding: The FreeElectron Model
The simplest possible arrangement of the valence electrons is to have them stripped apart from the ions and distributed uniformly through the solid. This is illustrated in Fig. 1.6. The bonding comes from the fact that the electrons are now shared by all the ions and act as a glue between them. The total energy E tot of the system is then lower than the energy of isolated, neutral ions. The difference is deﬁned as the “binding energy,” E b , of the solid. This quantity is characteristic of the stability of the solid. To make it a number independent of the size of the solid, we deﬁne it as the energy per atom gained by putting all the atoms together so they can share their valence electrons. For a system composed of N atoms, each with energy E 0 when isolated from all the others, we have: Eb
= N1 (E tot − NE 0 )
(1.1)
The general behavior of the binding energy is shown in Fig. 1.6: when the atoms are far apart, the binding energy is zero. The valence electrons are bound to the ions, occupying states with energy lower than zero; in the simple example shown in Fig. 1.6, this energy is labeled ²0 for the case of the isolated atoms. When the atoms are brought together, the attractive potential due to the presence of many ions leads to lower values for the energy of the bound valence electrons (blue line). However, there is also a Coulomb repulsion E c between the positive ions (green line). The competition between the two terms leads to a binding energy per atom E b that is negative, that is, overall the system gains energy by having all the electrons shared among all the ions. When the distance between the E
0
Eb
d
ygrenE
Ec
0
0
Distance
Fig. 1.6
Illustration of metallic bonding between many atoms. Left : The binding energy E b of the solid as a function of the distance between the ions; E c is the Coulomb repulsion between the ions and ²0 is the energy of the valence electrons in the isolated neutral atom. The insets indicate schematically the charge distribution, with red circles representing the ions and blue clouds representing the valence electrons which end up being uniformly distributed between the ions in the solid. Right: The corresponding energylevel diagram. The original N degenerate levels of the isolated individual atoms (at large distances) form a distribution of states in the solid that span a wide energy range, as the distance between atoms decreases.
7
1.2
Forming Bonds Between Atoms
ions becomes too small, the Coulomb repulsion between ions becomes too strong and the binding energy rises and eventually becomes positive, at which point the solid is not stable any longer. There is an optimal distance between the ions at which the binding energy attains its lowest value, which corresponds to the optimal structure of the solid. An interesting issue is the behavior of the electron energy levels as the distance between the ions decreases. As shown in the right panel of Fig. 1.6, these energy levels are degenerate in the case of isolated atoms. Because electrons are fermions, they cannot all reside on the same energy level when the atoms are very close to each other. As a result, when the atoms get closer together the electron energy levels break the degeneracy and form a distribution over a range of values. The closer the distance between ions, the wider this energy range is, as the distance between ions approaches that of interatomic distances in the solid. In the limit of a very large number of atoms (as is the case for typical solids), the difference between consecutive energy values becomes inﬁnitesimally small and the electron energy levels form a continuum distribution. To put these notions on a more quantitative basis, we will use a very simple model in which the ionic potential is a uniformly distributed positive background. This frees us from needing to consider the detailed behavior of the ions. Moreover, we will neglect any kind of interaction between the electrons (coming from their Coulomb repulsion or from exchange and correlation effects). This is referred to as the “freeelectron” or “jellium” model. Although evidently oversimpliﬁed, this model is quite useful in describing many of the properties of metallic solids, at least in a qualitative way. In this model, the electronic states must also reﬂect this symmetry of the potential which is uniform, so they must be plane waves: ψi (r)
= √1
V
eiki ·r
(1.2)
where V is the volume of the solid and k i the wavevector which characterizes state ψi . Since the wavevectors sufﬁce to characterize the singleparticle states, we will use those as the only index, that is, ψi → ψk . Plane waves are actually a very convenient and useful basis for expressing various physical quantities. In particular, they allow the use of Fourier transform techniques, which simplify the calculations. In the following we will be using relations implied by the Fourier transform method, which are discussed in Appendix A. We identify the state of such an electron by its wavevector k , which takes values from 0 up to a maximum magnitude k F , called the “Fermi momentum.” In threedimensional (3D) cartesian coordinates the wavevector is written as k = k xxˆ + k y yˆ + k z zˆ and the energy of the state with wavevector k is:
= h¯2mk
2 2
²k
e
(1.3)
We consider that the solid is a rectangular object with sides L x , L y , L z , with V = L x L y L z its total volume. For a typical solid, the values of L x , L y , L z are very large on the scale of
8
1
From Atoms to Solids
˚ with atomic units, of order 108 –109 a 0, where a 0 is the Bohr radius (a0 = 0.529177 A, − 10 ˚ = 10 1A m). From Fourier analysis, we can take dkx , dk y , dk z to be given by: dk xdk y dk z
(2π )3
dk (2π )3
= L L L ²⇒ x y z
1
= V ²⇒ L ,L lim ,L →∞ x
y
±
z
k
=V
²
dk (2π )3
(1.4)
as discussed in Appendix A, Eq. (A.46). For each freeelectron state characterized by k there is a multiplicity factor of 2 coming from the spin, which allows each electron to exist in two possible states, spin up or down, for a given value of its energy. Therefore, the total number of states available to the system is: 2
±
k ≤kF
= 2V
²
kF
0
dk (2π )3
k3
= 3πF2 V = N
(1.5)
which we have set equal to the total number of electrons N in the solid. This leads to the following relation between the density n = N /V and the Fermi momentum k F : 3
n
= 3kπF2
(1.6)
which in turn gives for the energy of the highest occupied state energy”:
= h2¯ mk F = h¯ 2 2
²F
e
2
(3π 2 n)2/ 3 2m e
²F ,
called the “Fermi (1.7)
These results help us make some sense of the spectrum of energy levels in the solid: the energy of electronic states is now given by Eq. (1.3), which is a continuous set of values, from 0 up to ²F . This is to be compared to the set of N individual atomic levels, when the atoms are isolated, as illustrated in Fig. 1.6. Moreover, if we assume that each atom has one valence electron in the atomic state, we will need only N /2 freeelectron states to accommodate all these electrons in the solid due to spin degeneracy, as worked out above, in Eq. (1.5). The binding or cohesive energy in this case comes from the much more delocalized nature of the states in the solid as compared to those in individual isolated atoms.
Example 1.1 1D model of atoms in a box To illustrate these ideas, we consider a simple example of six “atoms” in one dimension, each represented by a box of size a, as shown in Fig. 1.7. Consistent with the freeelectron model, we will take the electron in such an atom to have a sinusoidal wavefunction ψ0 (x) and energy ²0 given by: ψ0 (x )
=
³
2 a
sin
´πxµ a
,
²0
2 2 = 2h¯mπa 2
e
corresponding to the largest possible wavelength of λ0 = 2a within the box of the isolated atom. If we condense these six atoms into a onedimensional (1D) “solid” of size L = 6a , the lowest energy level in the solid will have energy ²1 = ²0 /36 = 0.028² 0 . Assuming that each atom has one valence electron, all the electrons in this 1D solid can be accommodated by the three lowest states with
9
1.2
Forming Bonds Between Atoms
"solid"
isolated "atoms"
0
1.0 0.75
0.50
0.25
0.0 Fig. 1.7
A simple 1D model of the energy levels associated with the freeelectron model for a system of six “atoms.” The red sinusoidal curves represent the singleparticle wavefunctions. In each atom, contained in a small box of size a, the lowest freeelectron state within the box has wavelength λ = 2a and energy ²0 = h¯ 2π 2/ 2me a2 . For six atoms forming a “solid” of size L = 6a, the six lowestenergy states and their corresponding energies in units of ²0 are shown on the vertical axis.
energies ²1 , ²2 = 0.111 ²0 , ²3 = 0.25²0, giving a much lower total energy for the condensed system of E tot = 0.778²0 compared to the six isolated atoms, and a binding energy per atom of E b = − 0.870²0. This component, namely the electronic kinetic energy contribution to the total energy, is the dominant component within our simple model. The actual total energy of the solid must include also the Coulomb repulsion of the electrons, as well as the electron–ion attraction, but these terms cancel each other for uniform and equal densities of the two oppositely charged sets of particles. Generalizing this simple model, and considering only the kinetic energy of the electrons in the freeelectron model, including a factor of 2 for the spin degeneracy, we ﬁnd that the total energy of this system is given by: E
kin
=2
±
 k≤kF
²k
= 2V
² 0
kF
dk h¯ 2k 2 (2π )3 2m e
h¯ 2 k 5F = πV2 10 = 53 N ²F m e
(1.8)
This quantity is evidently positive and only depends on the density of electrons in the solid, n . The attraction of electrons to the positive charge of the ions provides the bonding for the atoms in the solid, but we have eliminated these terms from the freeelectron model. In thinking about the properties of metallic solids, it is often useful to express equations in terms of another quantity, called r s , which is deﬁned as the radius of the sphere whose volume corresponds to the average volume per electron in the solid: 4π 3 r 3 s
= VN = n −1 = 3π3
2
kF
(1.9)
10
1
From Atoms to Solids
and r s is typically measured in atomic units. This gives the following expression for k F : 1/3
1/ 3
kF
4) = (9π/r 4) ²⇒ kF a0 = (9(π/ r /a ) s
s
0
(1.10)
where the last expression contains the dimensionless combinations of variables k F a 0 and r s /a 0. In actual metals (r s /a 0 ) varies between 2 and 6. It is helpful to introduce here the units of energy that are typically involved in the formation of bonds in solids. The rydberg (Ry) is the natural unit for energies in atoms:
¯
h2
2m e a20
2
= 2ea = 1 Ry
(1.11)
0
Another useful unit is the electronvolt (eV), the potential energy gained by an electron when it moves across a voltage difference of 1 V. The rydberg and the electronvolt are related by: 1 Ry
= 13.6058 eV
(1.12)
Typical binding energies per atom, for metallic solids, are in the range of a few electronvolts. 1.2.2
The Essence of Covalent Bonding
We consider next what can happen when two atoms of the same type come together to form a diatomic molecule. For simplicity, we will assume that each atom has only one valence electron outside its core, in a state with energy ²1 , as indicated in Fig. 1.8; this corresponds, E
Ec 0
Eb
d
1
a 1
1
b
b Fig. 1.8
Schematic representation of the formation of a bond between two atoms with one valence electron each. Left: When separated, the atoms each have a valence state of energy ²1 with one electron in it; when they are brought together, new states are formed, the bonding state with energy ²b < ²1 and the antibonding state with energy ²a > ²1; the two available valence electrons occupy the lowerenergy bonding state. Right: The binding energy E b per atom (black line) of a diatomic molecule as a function of the distance d between the ions composing it. The energy of the bonding state ²b is shown as a red line; for large distances it approaches the value ²1 of the electron state in the isolated atom. The Coulomb repulsion between the two cores (Ec ) is shown as a green line.
11
1.2
Forming Bonds Between Atoms
for example, to an element like Li (Z = 3).3 When two such atoms come closer together, the presence of the two ions in close proximity creates new levels for the valence electrons, labeled ²b (for bonding, the lowerenergy state) and ²a (for antibonding, the higherenergy state). The core electrons are unaffected, but the valence electrons can take advantage of the new states, by occupying the lowerenergy one which can accommodate both of them. The wavefunction of the new state with lower energy is different from the wavefunction of the valence state in the isolated atom, and has more weight between the two ions. This creates a bond between the two ions, which share both of the valence electrons. The net result is a very stable unit consisting of two ions and the two shared valence electrons, that is, a diatomic molecule. The stability is the result of the lower energy of the entire system, compared to the energy of two isolated atoms, because each of the valence electrons now occupies a lowerenergy state, ²a < ²1. As a result of the rearrangement of the charge, there is a strong electrostatic attraction between the two shared valence electrons lying near the center of the molecule and the two positively charged ions. The higherenergy state is called an antibonding state because its wavefunction has different character: it has a node in the region between the two ions and more weight in the regions away from the molecule center. If this state were to be occupied by electrons, it would lead to a weakening of the bond, because of the unfavorable distribution of electrons relative to the positions of the ions (this is the reason it is called an antibonding state). As in the case of the metallic solid, there is an optimal distance between the two atoms, which corresponds to maximum bonding by sharing of the valence electrons. At distances larger than this optimal distance, the bond is weaker because there is not enough concentration of electrons between the two ions. At distances shorter than the optimal one, there is not enough space between the ions to accommodate the valence electrons (which also feel a mutually repulsive force), and the valence electrons are displaced from the interionic region, which also weakens the bond. When the two ions come very close together the net interaction is quite repulsive, because the valence electrons are not able to shield the two ionic cores. The binding energy E b has a minimum at the optimal distance between the two atoms in the diatomic molecule (N = 2); it approaches 0 for very large distances and it starts rising from the minimum for distances smaller than the optimal distance and eventually becomes positive, which corresponds to a net repulsion between the ions, as illustrated in Fig. 1.8.
Example 1.2 1D model of covalent bond in a twoatom molecule We wish to demonstrate in a simple 1D example that symmetric and antisymmetric combinations of singleparticle orbitals give rise to bonding and antibonding states. Though evidently oversimpliﬁed, this example is relevant to the hydrogen molecule which is discussed at length in Chapter 4. We begin with an atom consisting of an ion of charge +e and a single valence electron: the electron–ion interaction potential is V (x ) = − e 2/ x , arising from the ion which is situated at 3 The case of the H atom and the H molecule is also covered by this discussion, the only difference being that 2
H lacks a core, since it only has one electron and its core is the bare proton.
12
1
x
From Atoms to Solids
= 0; we will take the normalized wavefunction for the ground state of the electron
to be:
φ(x )
= √1a e−x a /
(1.13)
where a is a constant. We next consider two such atoms, the ﬁrst ion at x = − b/2 and the second at x = + b /2, with b the distance between them (also referred to as the “bond length”). From the two wavefunctions associated with the electrons in each originally isolated atom: φ1(x )
= √1a e−x−b 2 a, /
φ2 (x )
/
= √1a e−x+b 2 a /
(1.14)
/
we construct the symmetric (+) and antisymmetric (−) combinations: ψ
(±)
(x ) =
√
1
± [φ1 (x ) ± φ2 (x)] ,
N
N( )
(±)
¶
·
= 2 1 ± e−b/a 1 + b
¸¹ (1.15)
a
where N (±) are the normalization factors. The difference between the probability of the electron being in the symmetric or the antisymmetric state rather than in the average of the states φ1(x ) and φ2 (x), is given by: 1
¶
·
¸´
µ¹
b δn (x ) = ± (±) 2φ1( x)φ2 (x ) − e−b/a 1 + φ1 (x )2 + φ 2(x )2 (1.16) N a A plot of the probabilities ψ (±) (x )2 and the differences δ n (±) (x ) is given in Fig. 1.9 (±)
for the choice b = 2.5a . Using this plot, we can justify the bonding character of state ψ (+)(x ) and the antibonding character of state ψ (−)(x ), taking into account the enhanced Coulomb attraction between the electron and the two ions in the region 0.6
0.6
0.3
0.3
0
0
0.3
0.3
0.6
Fig. 1.9
4
2 b/2
0
+b/ 2 2
4
0.6
4
(−) 2
2 b/2
0
+b/2 2
4
Symmetric ( +), left panel, and antisymmetric (−), right panel, linear combinations of singleparticle orbitals: the probability densities ψ (±) (x )2 are shown by the red line for the (+) and the blue line for the (−) and the differences δ n(±) ( x) between each of those and the average occupation of states φ1( x), φ2 (x) by black dashed lines; the green lines show the attractive potential of the two ions located at ±b/ 2 (positions indicated by thin vertical lines). In this example b = 2.5a and x is given in units of a.
13
1.2
Forming Bonds Between Atoms
−b/2 < x < +b /2. In the case of ψ (+) more electronic charge is accumulated in the
region between the two ions (the dashed black line is mostly positive), contributing to enhanced bonding. In the case of ψ (−) , electronic charge is depleted from the region between the two ions (the black dashed curve is mostly negative), which is detrimental to the bonding between the ions. The charge is of course conserved, so the amount of electronic charge accumulated (or depleted) between the two ions is compensated by corresponding changes in the amount of charge near the position of each ion and in the regions farther to the left of the left ion or to the right of the right ion. To make this argument a bit more quantitative, we deﬁne the change in potential energy for the combined system versus the two isolated ions: ³V
≡ ψ³ (±) [V1 (x ) + V2( x)] ψ (±) ´ −21 [³φ1 V1(x )φ1 ´ + φ2³V2(x )φ2 ´]
(1.17)
where we have deﬁned the potentials associated with the two ions, V1 (x ), V2 (x ): V1 (x )
2 = x −−eb/ 2 ,
V2 (x)
2 = x +−eb /2
A common approximation is to take the symmetric and antisymmetric combinations to be deﬁned as: 1 (±) ψ (x ) = √ [φ1 (x) ± φ2(x )] 2 that is, N (±) = 2, which is reasonable in the limit b µ a . In this limit, we can show (either analytically or by numerical integration) that the change in potential energy (+) ³V is always negative for ψ and always positive for ψ (−); moreover, the kinetic (+) energy is reduced for ψ and increased for ψ (−). All these considerations support the picture of ψ (+) corresponding to a bonding state and ψ (−) to an antibonding state. The preceding discussion can be generalized to the case of many atoms and more than one valence state per atom, especially when these states have pronounced lobes pointing in different directions in space. An example of this situation is shown in Fig. 1.10: here, for the purposes of illustration, we consider a hypothetical atom with two valence states, each having pronounced lobes which point in orthogonal directions in space. As in the case of the diatomic molecule discussed above, new levels are created when two such atoms are in close proximity, with energy lower than (bonding states) or higher than (antibonding states) the energy of the original states in the isolated atom. The bonding and antibonding states from a pair of atoms are separated by an energy difference, to which we refer as an “energy gap.” The presence of more ions creates a sequence of bonding states and a corresponding sequence of antibonding states, separated by a gap in energy. Assuming that the isolated atoms have one electron per valence state available in their neutral conﬁguration, the bonding states will be fully occupied by the valence electrons and the antibonding states will be empty. This leads to a lowerenergy, stable structure for the assembly of atoms relative to the isolated atoms, since the occupation of bonding states by valence electrons reduces their energy. As the number of atoms in the system increases, this pattern will evolve into a large set of bonding states and antibonding states, with the former occupied
14
1
From Atoms to Solids
E
noitcudnoC
0
d
Eb
ygrenE
Ec
a
gap
b
ecnelaV
b
Distance Fig. 1.10
Illustration of covalent bonding between many atoms: Left: The binding energy Eb of the solid as a function of the distance between the ions; E c is the Coulomb repulsion between the ions and ²b is the energy of the bonding combination of orbitals of the isolated neutral atoms. The insets indicate schematically the charge distribution, with red circles representing the ions and blue clouds representing the valence electrons leading to directed covalent bonds in which the electronic charge is distributed predominantly between nearestneighbor pairs of ions. Right: The corresponding energylevel diagram. The original N degenerate levels of the isolated individual atoms (at large distances) form bonding and antibonding combinations (with energies ²b , ²a ) which evolve into a distribution of states in the solid, each of which covers a wide energy range as the distance decreases. In this distribution, valence and conduction states are separated by an energy gap.
by valence electrons and the latter empty, but always separated by a gap in the energy due to their very different nature. This is the essence of a covalently bonded solid, also discussed at length in following chapters. Figure 1.10 illustrates the behavior of the binding energy per atom (left panel) and the distribution of electronic energy levels (right panel) as a function of the distance between the ions. The main differences between this situation and the case of metallic bonding is the nonuniform distribution of electron charge in space, which forms the directed covalent bonds between ions, and the presence of an energy gap in the distribution of energy levels, separating the ﬁlled bonding (also referred to as “valence”) states from the empty antibonding (also referred to as “conduction”) states.
1.2.3
Other Types of Bonding in Solids
The metallic and covalent bonding that we have described so far are the dominant types that produce stable crystals. There are other types of bonding, generally weaker than the metallic and covalent bonding, that are also encountered in solids. One type of bonding, that can actually be quite strong and is responsible for the stability of many solids encountered in everyday life, is ionic bonding. In this case, there are two (or sometimes more) kinds of ions in the solid, one that is positively charged having lost some of its valence electrons and one that is negatively charged having gained some electrons due to its higher electronegativity. This type of bonding is encountered, for example, in sodium chloride (NaCl), common salt. Another type of generally weaker but quite common
15
1.3
The Architecture of Crystals
bonding is the socalled van der Waals bonding, due mostly to dipolar interactions between neutral atoms or small atomic units. Yet another type of bonding, encountered in solids that contain hydrogen atoms and certain highly electronegative elements (like oxygen and nitrogen), is called hydrogen bonding, and has to do with the fact that the hydrogen atom has no core electrons and its core essentially consists of a proton which is very small on the atomic scale. In many solids, especially those composed of several kinds of atoms, the cohesion is due to a combination of different types of bonding, occasionally including all of the types mentioned. We discuss these other types of bonding in solids and their combinations in more detail below, when we deal with speciﬁc examples of solids where they are encountered.
1.3
The Architecture of Crystals
The atomic structure of materials is typically discussed in terms of the properties of crystals. There is good reason for this. A crystal, from a mathematical point of view, is a perfectly periodic arrangement of atoms in space which extends to inﬁnite size; in practice, crystals are large enough when measured in units of interatomic distances that the mathematical notion of the crystal can be adopted as a very good approximation. Although no real material is a perfect crystal, in a wide range of materials the atoms are organized in a fairly regular manner, approximating the order inherent in the mathematical deﬁnition of the crystal. In some cases, the similarity is quite spectacular, as in precious stones that can be cut in ways which reveal the underlying symmetry of the atomic arrangement. In other cases the similarity is not so obvious but still exists in very deep ways, as in the cases of chocolate bars, ice, candles, and many other objects familiar in everyday life. In many cases, the overall shape of a material is due to the atomic structure of the crystal, as we will show through some examples in this chapter. The structure of crystals can be understood by a close look at the properties of the atoms from which they are composed. We can identify several broad categories of atoms, depending on the nature of the valence electrons that participate actively in the formation of the solid. Accordingly, we will discuss below the crystal structure of various solids based on the properties of the valence electronic states of the constituent atoms. We are only concerned here with the basic features of the crystal structures that the various atoms form, such as their coordination number (number of nearest neighbors) and the nature of the bonds they form, without paying close attention to the details; these will come later. Finally, we will only concern ourselves with lowtemperature structures, which correspond to the lowestenergy static conﬁguration; dynamical effects, which can produce a different structure at higher temperatures, will not be considered. 4 We begin our discussion with those solids formed by atoms of one element only, called elemental solids, and then proceed to more complicated structures involving several types of atoms. Some basic properties of the elemental solids are collected in the Periodic Table. There is no information for the elements H and He (atomic numbers 1 and 2) because these elements 4 J. Friedel, J. de Phys. (Paris) 35, L59 (1974).
16
1
a
c
c a
a
b b a
Fig. 1.11
From Atoms to Solids
a a
c
c
b
a a
a
a
a
Shapes of the unit cells in some lattices that appear in the Periodic Table. The corners drawn in thin black lines indicate right angles between edges. The lattices are discussed in more detail in Chapter 3 (see Section 3.3).
do not form solids under normal conditions: H forms a molecular solid at sufﬁciently low temperature or high pressure, while He remains liquid at temperatures very close to absolute zero. For the rest of the elements, we list:
•
• • • •
The crystal structure of the most common phase. The acronyms for the crystal structures that appear in the Periodic Table stand for: BCC = body centered cubic, FCC = face centered cubic, HCP = hexagonal close packed, GRA = graphite, TET = tetragonal, DIA = diamond, CUB = cubic, MCL = monoclinic, ORH = orthorhombic, RHL = rhombohedral, TRI = triclinic. Selected shapes of the corresponding crystal unit cells are shown in Fig. 1.11. For crystals which can be characterized by a single structural parameter, the lattice constant, the value of this parameter is given in units of angstroms. Such crystals are, for example, FCC, BCC, HCP. For other crystal types, more structural parameters are required to fully specify the unit of the crystal. The melting temperature (K). We note here that typical values of the cohesive energy of solids are in the range of a few electronvolts (1 eV = 11,604 K), which means that the melting temperature is only a small fraction of the cohesive energy, typically a few percent. The atomic concentration of the most common crystal phase in 1022 cm−3. The electrical resistivity (in units of µ±·cm); for most elemental solids the resistivity is of order 1–100 in these units, except for some good insulators which have resistivities 103 , 10 6, or 10 9 times higher. 1.3.1
Atoms with No Valence Electrons
The ﬁrst category consists of those elements which have no valence electrons. These are the atoms with all their electronic shells completely ﬁlled, which are chemically inert and are referred to as the “noble elements,” He, Ne, Ar, Kr, Xe. When these atoms are brought together to form solids, they interact very weakly. Their outer electrons are not disturbed much, since they are essentially core electrons. The weak attractive interaction between such atoms is the result of slight polarization of the electronic wavefunction in one atom due to the presence of other atoms around it. This interaction is referred to as a “ﬂuctuating dipole” or van der Waals interaction. Since the interaction is weak, the solids are not very stable and they have very low melting temperatures, well below room temperature. The main concern of the atoms in forming such solids is to have as many neighbors as possible,
17
Fig. 1.12
1.3
The Architecture of Crystals
Illustration of the face centered cubic (FCC) crystal structure. Left : The conventional cubic cell of the FCC crystal, shown in thin red lines, with atoms at the corners of the cube and at the centers of the cube faces. Right: Several planes (outlined by thin colored lines) of closepacked spheres in the FCC crystal, and the six nearest neighbors of one atom indicated by yellow arrows.
in order to maximize the cohesion, since all interactions are attractive. The crystal structure that corresponds to this type of atom is one of the closepacking geometries, that is, atomic arrangements in space which allow the closest packing of hard spheres. The particular crystal structure that nobleelement atoms assume in solid form is FCC. Each atom has 12 equidistant nearest neighbors in this crystal, which lie on different equivalent planes. For example, an atom at the center of a particular cube face has four neighbors at the corners of the same cube face and eight more neighbors, four each on a plane parallel to, and on either side of, this face. Alternatively, atoms can be viewed as having six neighbors on a plane and six more, three each on a plane parallel to and on either side of it. These structural features are shown in Fig. 1.12. Thus, in the simplest case, atoms that have no valence electrons at all behave like hard spheres, which attract each other with weak forces, but are not deformed. They form weakly bonded solids in the FCC crystal structure, in which the attractive interactions are optimized by maximizing the number of nearest neighbors in a closepacking arrangement. The only exception to this rule is He, in which the attractive interaction between atoms is so weak that it is overwhelmed by the zeropoint motion of the atoms. Except when external pressure is applied to enhance this attractive interaction, He remains a liquid. This is an indication that in some cases it will prove unavoidable to treat the nuclei as quantum particles (see also the discussion below about hydrogen). The other closepacking arrangement of hard spheres is the hexagonal structure (HCP), with 12 neighbors which are separated into two groups of six atoms each: the ﬁrst group forms a planar sixmember ring surrounding an atom at the center, while the second group consists of two equilateral triangles, one above and one below the sixmember ring, with the central atom situated above or below the geometrical center of each equilateral triangle, as shown in Fig. 1.13. The HCP structure bears a certain relation to FCC: we can view both structures as planes of spheres closely packed in two dimensions, which gives a hexagonal lattice; for close packing in three dimensions the successive planes must be situated so that a sphere in one plane sits directly above the center of a triangle formed by three spheres in the previous plane. There are two ways to form such a stacking of hexagonal closepacked planes: . . .ABCABC . . . and . . .ABABAB . . ., where A , B , C represent the three possible
18
1
IA
H
s1
IIA 1
Hydrogen
Li
From Atoms to Solids
s2
He
2
Be
4
PERIODIC
Helium
3
BCC 3.51 453.7 4.70 9.4
HCP 2.29 1560 12.1 3.3
Na
Mg
11
Sodium
Li
Symbol Name Crystal structure Melting point Atomic concentration Resistivity
Beryllium
Lithium
12
3
Lithium
BCC 3.51 Lattice constant (Å) 453.7 (K) 4.70 (10 22/cm3 ) 9.4 (mWcm)
Magnesium
BCC 4.29 370.9 2.65 4.75
HCP 3.21 923 4.30 4.46
K
Ca
19
Potassium
20
BCC 5.33 336.5 1.40 21.6
FCC 5.59 1115 2.30 3.7
Rb
Sr
37
s d 2
Sc
1
21
Scandium
Calcium
Rubidium
IIIB
38
s d 2
2
Ti
22
Titanium
HCP 3.31 1814 4.27 51
Y
IVB
39
HCP 2.95 1941 5.66 47.8
Zr
40
VB
s d 2
V
3
23
VIB
s d 2
4
VIIB
s d 2
Cr* 24 Mn
5
25
Vanadium
Chromium
Manganese
BCC 3.03 2183 7.22 24.8
BCC 2.91 2944 8.33 12.9
CUB 1519 8.18 139
Niobium
Molybdenum
Technetium
Nb* 41 Mo* 42 Tc
VIII
s d 2
6
Fe
26
Iron
s2 d 7
Co
27
Cobalt
BCC 2.87 1811 8.50 9.71
43
VIII
HCP 2.51 1768 8.97 6.34
Ru* 44 Rh* 45
Strontium
Yttrium
Zirconium
BCC 5.59 312.5 1.15 12.1
FCC 6.08 1050 1.78 22.8
HCP 3.65 1799 3.02 60
HCP 3.23 2128 4.29 41.4
BCC 3.30 BCC 3.15 HCP 2.74 HCP 2.71 FCC 3.80 2750 2896 2430 2607 2237 5.56 6.42 7.04 7.36 7.26 15.2 5.17 14 7.2 4.5
Cs
Ba
La
Hf
Ta
55
Cesium
BCC 6.14 301.6 0.91 20
56
Barium
BCC 5.03 1000 1.60 50
57
Lanthanum
HCP 3.77 1193 2.70 80
72
Hafnium
73
Tantalum
HCP 3.20 2506 4.52 35.1
W
74
Wolframium
Re
75
Rhenium
Ruthenium
Os
76
Osmium
Rhodium
Ir
77
Iridium
BCC 3.30 BCC 3.17 HCP 2.76 HCP 2.73 FCC 3.84 3290 3695 3459 3306 2739 5.55 6.30 6.80 7.14 7.06 13.5 5.6 19.3 8.1 5.1
s2 d 0 f 2 s2 d 0 f 3 s2 d 0 f 4 s2 d 0 f 5 s 2 d 0 f 6 s 2 d 0 f 7
Ce
58
Cerium
HCP 3.62 1068 2.91 85.4
Pr
59
Nd
60
Praseodymium Neodymium
HCP 3.67 HCP 3.66 1208 1297 2.92 2.93 68 64.3
Pm
61
Promethium
Sm
Samarium
TRI 1345 3.03 105
62
Eu
63
Europium
BCC 4.58 1099 3.04 91
19
1.3
TABLE
The Architecture of Crystals
IIIA
s2 p 1
B
IVA
5
Boron
Al
s d
8
Ni
28
IB
s d 2
9
IIB
s 2 d 10
Cu* 29 Zn
30
6
s2 p 3
N
VIA 7
Nitrogen
13
O
VIIA 8
Oxygen
Si
14
Silicon
P
15
Phosphorus
31
Ge
32
S
33
F
16
Cl
Se
34
Br
Arsenic
Selenium
Bromine
FCC 3.61 1357 8.45 1.67
HCP 2.66 693 6.55 5.92
ORH 303 5.10
DIA 5.66 1211 4.42 47 X 106
TRI 1090 4.65 12 X 106
MCL 494 3.67
OR H 266 2.36
Silver
Cadmium
Indium
Tin
Antimony
FCC 3.89 1828 6.80 9.93
FCC 4.09 1235 5.85 1.63
HCP 2.98 594 4.64 6.83
TET 430 3.83 8.37
TET 505 2.91 11
TRI 904 3.31 39
Pt *
Au* 79 Hg
FCC 3.52 1728 9.14 6.84
Pd*
46
Palladium
78
Platinum
FCC 3.92 2041 6.80 9.85
Ag* 47 Cd* 48 In
Gold
Mercury
FCC 4.08 1337 7.14 2.12
RHL 234 7.06 96
80
Tl
49
81
Thallium
Sn
Pb
50
82
Lead
Sb
51
Bi
Te
52
Tellurium
83
Bismuth
I
Gadolinium
Terbium
ORH 387 2.36
HCP 3.64 HCP 3.60 1585 1629 3.02 3.22 131 114.5
66
HCP 3.59 1680 3.17 92.6
Ho
Holmium
67
Er
68
Erbium
HCP 3.58 HCP 3.56 1734 1770 3.22 3.26 81.4 86.0
Tm
69
Thulium
Po
At
HCP 3.54 1818 3.32 67.6
Yb
70
85
Astatine
Lu
36
Xe
54
FCC 6.20 161 1.64
HCP 3.46 FCC 4.95 MCL 577 601 544 3.50 3.30 2.82 18 20.6 107
Dysprosium
Kr
Xenon
s 2 d 1 f 7 s 2 d 1 f 8 s 2 d 0 f 10 s 2 d 0 f 11 s 2 d 0 f 12 s 2 d 0 f 13 s 2 d 0 f 14 s 2 d 1 f 14
Gd* 64 Tb* 65 Dy
18
FCC 5.71 116 2.17
53
TRI 723 2.94 160 X 103 Polonium
Ar
Krypton
Iodine
84
10
FCC 5.26 83.8 2.66
35
Germanium
Ne
Argon
ORH 172
Gallium
s2 p 6
Neon
17
Zinc
Noble
FCC 4.43 24.6 4.36
Chlorine
Copper
Nickel
9
MCL 53.5
ORH 388
As
s2 p 5
Fluorine
Sulfur
FCC 4.05 DIA 5.43 TCL 933 1687 317 6.02 5.00 230 X 109 2.67
Ga
s2 p 4
GRA 2.46 HCP 3.86 MCL 3800 63 54.8 17.6 3.5 X 103
Aluminum
2
C
VA
Carbon
RHL 2349 13.0 4 X 10 6
VIII
s2 p 2
71
Ytterbium
Lutetium
FCC 5.48 1097 3.02 25.1
HCP 3.50 1925 3.39 58.2
Rn Radon
86
20
Fig. 1.13
Fig. 1.14
1
From Atoms to Solids
Illustration of the hexagonal close packed (HCP) crystal structure. Left: One atom and its 12 neighbors in the HCP crystal; the size of the spheres representing atoms is chosen so as to make the neighbors and their distances apparent. Right: The stacking of closepacked planes of atoms in the HCP crystal.
Illustration of two interpenetrating FCC (left) or HCP (right) lattices; the two original lattices are denoted by sets of white and yellow spheres. These structures correspond to the diamond lattice if the two atom types are the same or the zincblende lattice if they are different (left), and to the wurtzite lattice (right). The lattices are viewed from the side, with the vertical direction corresponding to the direction along which closepacked planes of the FCC or HCP lattices would be stacked.
relative positions of spheres in successive planes according to the rules of close packing. The ﬁrst sequence corresponds to the FCC lattice, the second to the HCP lattice. An interesting variation of the closepacking theme of the FCC and HCP lattices is the following: consider two interpenetrating such lattices, that is, two FCC or two HCP lattices, arranged so that in the resulting crystal the atoms in each sublattice have as nearest equidistant neighbors atoms belonging to the other sublattice. These arrangements give rise to the diamond lattice or the zincblende lattice (when the two original lattices are FCC) and to the wurtzite lattice (when the two original lattices are HCP). This is illustrated in Fig. 1.14. Interestingly, in both cases each atom ﬁnds itself at the center of a tetrahedron with exactly four nearest neighbors. Since the nearest neighbors are exactly the same, these two types of lattices differ only in the relative positions of second (or farther) neighbors. It should be evident that the combination of two closepacked lattices cannot produce another closepacked lattice. Consequently, the diamond, zincblende, and wurtzite lattices are encountered in covalent or ionic structures in which fourfold coordination is preferred. For example: tetravalent group IV elements like C, Si, Ge form the diamond lattice; combinations of two different group IV elements or complementary elements (like group
21
Fig. 1.15
1.3
The Architecture of Crystals
Three different views of the regular icosahedron: the left view is along one of the ﬁvefold symmetry axes; in the middle view, a ﬁvefold axis is along the vertical direction; the right view is along a random orientation.
III–group V, group II–group VI, group I–group VII) form the zincblende lattice; certain combinations of group III–group V elements form the wurtzite lattice. These structures are discussed in more detail below. A variation of the wurtzite lattice is also encountered in ice and is due to hydrogen bonding. Yet another version of the closepacking arrangement is the icosahedral structure. In this case an atom has again 12 equidistant neighbors, which are at the apexes of an icosahedron. The icosahedron is one of the Platonic solids in which all the faces are perfect planar shapes; in the case of the icosahedron, the faces are 20 equilateral triangles. The icosahedron has 12 apexes arranged in ﬁvefold symmetric rings,5 as shown in Fig. 1.15. In fact, it turns out that the icosahedral arrangement is optimal for close packing of a small numbers of atoms, but it is not possible to ﬁll 3D space in a periodic fashion with icosahedral symmetry. This fact is a simple geometrical consequence (see also Chapter 3 on crystal symmetries). Based on this observation it was thought that crystals with perfect ﬁvefold (or tenfold) symmetry could not exist, unless defects were introduced to allow for deviations from the perfect symmetry. 6 The discovery of solids that exhibited ﬁvefold or tenfold symmetry in their diffraction patterns, in the mid1980s, 7 caused quite a sensation. These solids were named “quasicrystals,” and their study created a new exciting subﬁeld in condensed matter physics. 1.3.2
Atoms with s Valence Electrons
The second category consists of atoms that have only s valence electrons. These are Li, Na, K, Rb, and Cs (the alkalis) with one valence electron, and Be, Mg, Ca, Sr, and Ba with two valence electrons. The wavefunctions of valence electrons of all these elements extend far from the nucleus. In solids, the valence electron wavefunctions at one site 5 An nfold symmetry means that rotation by 2π/ n around an axis leaves the structure invariant. 6 F. C. Frank, Proc. Roy. Soc. A 215, 43 (1952); F. C. Frank and J. S. Kasper, Acta Cryst. 11, 184 (1958); Acta
Cryst. 12, 483 (1959). 7 D. Shechtman, I. Blech, D. Gratias, and J. W. Cahn, Phys. Rev. Lett. 53, 1951 (1984). D. Shechtman was
awarded the 2011 Nobel Prize in Chemistry for this discovery.
22
1
From Atoms to Solids
have signiﬁcant overlap with those at the nearestneighbor sites. Since the s states are spherically symmetric, the wavefunctions of valence electrons do not exhibit any particular preference for orientation of the nearest neighbors in space. For the atoms with one and two s valence electrons, a simpliﬁed picture consists of all the valence electrons overlapping strongly, and thus being shared by all the atoms in the solid forming a “sea” of negative charge. The nuclei with their core electrons form ions which are immersed in this sea of valence electrons. The ions have charge +1 for the alkalis and +2 for the atoms with two s valence electrons. The resulting crystal structure is the one which optimizes the electrostatic repulsion of the positively charged ions with their attraction by the sea of electrons. The actual structures are BCC for all the alkalis, and FCC or HCP for the twos valence electron atoms, except Ba, which prefers the BCC structure. In the BCC structure each atom has eight equidistant nearest neighbors, as shown in Fig. 1.16, which is the second highest number of nearest neighbors in a simple crystalline structure, after FCC and HCP. In Ba, which is the heaviest of the column IIA elements, the ﬁlledshell electrons start having wavefunctions that extend far from the nucleus, simply because they correspond to large principal quantum numbers, and thus are no longer unaffected by the presence of other nearby atoms; the interactions between such electronic states lead to the BCC structure being more stable than the FCC structure for this element. One point deserves further clariﬁcation: we mentioned that the valence electrons have signiﬁcant overlap with the electrons in neighboring atoms, and thus they are shared by all atoms in the solid, forming a sea of electrons. It may seem somewhat puzzling that we can jump from one statement – the overlap of electron orbitals in nearby atoms – to the other – the sharing of valence electrons by all atoms in the solid. The physical symmetry which allows us to make this jump is the periodicity of the crystalline lattice. This symmetry is the main feature of the external potential that the valence electrons feel in the bulk of a crystal: they are subjected to a periodic potential in space, in all three dimensions, which for all practical purposes extends to inﬁnity – an idealized situation we discussed earlier. The electronic wavefunctions must transform according to the symmetry operations of the hamiltonian, as we will discuss in detail in later chapters; for the purposes of the
Fig. 1.16
Illustration of the body centered cubic (BCC) crystal structure. Left : The conventional cubic cell (shown in thin red lines) with one atom and its eight neighbors in the BCC crystal. Right: The stacking of closepacking planes, indicated by thin colored lines, in the BCC crystal; the four nearest neighbors of an atom on such a plane are shown by yellow arrows.
23
1.3
The Architecture of Crystals
present discussion, this implies that the wavefunctions themselves must be periodic, up to a phase. The mathematical formulation of this statement is called Bloch’s theorem. A periodic wavefunction implies that if two atoms in the crystal share an electronic state due to overlap between atomic orbitals, then all equivalent atoms of the crystal share the same state equally, that is, the electronic state is delocalized over the entire solid. This behavior is central to the physics of solids, and represents a feature that is qualitatively different from what happens in atoms and molecules, where electronic states are localized (except in certain large molecules that possess symmetries akin to lattice periodicity).
1.3.3
Atoms with s and p Valence Electrons
The next level of complexity in crystal structure arises from atoms that have both s and p valence electrons. The individual p states are not spherically symmetric, so they can form linear combinations with the s states that have directional character: a single p state has two lobes of opposite sign pointing in diametrically opposite directions. The s and p states, illustrated in Fig. 1.17, can then serve as the new basis for representing electron wavefunctions and their overlap with neighboring wavefunctions of the same type can lead to interesting ways for arranging the atoms into a stable crystalline lattice (see Appendix C on the character of atomic orbitals). In the following we will use the symbols s( r), pl (r) (l = x , y , z ) and d m (r) (m = xy , yz , zx , x 2 − y 2 , 3z2 − r 2 ) to denote atomic orbitals as they would exist in an isolated atom, which are functions of r. When they are related to an atom A at position RA, these
z
z
z
y
z
y
y x
x
s
px z
y x
py y
x
pz y
y x
d 3z 2 r2 Fig. 1.17
x
d x2 y 2
x
d xy
Representation of the character of s, p, d atomic orbitals. The lobes of positive sign in the px, py , pz and d3z2 −r2 , dx2 −y2 , dxy orbitals are shown shaded. The dyz, dzx orbitals are similar to the dxy orbital, but lie on the y, z and z, x planes.
24
1
From Atoms to Solids
become functions of r − RA (the origin is translated by −RA so that the new orbital is centered at the position of the nucleus) and these will be denoted as s A (r) = s (r − RA ), A A pA l (r) = pl (r − RA ), and dm (r) = d m (r − RA ). We will use the symbols φi (r) (i = 1, 2, ...) for states that are linear combinations of the atomic orbitals s A , p Al , d Am at site A , and the symbols ψ n(r) (n = a , b ) for combinations of the φiX (r)s (X = A , B , ...; i = 1, 2, ...) which are appropriate for the description of electronic states in the crystal. Our ﬁrst example concerns a twodimensional (2D) crystal of carbon atoms, which, when stacked together with many other such planes, forms graphite. In this case, the ﬁrst three orbitals, φ1A, φA2 , φ3A , belonging to a carbon atom labeled A , point along three directions on the x , y plane separated by 120◦ , while the last one, φ4A , points in a direction perpendicular to the x , y plane, as shown in Fig. 1.18 and deﬁned in Table 1.1. If the orbitals s A , pA i (i = x , y , z ) have energies ²s and ²p , then the states φk (k = 1, 2, 3) have energy (²s + 2²p )/3 (see Problem 5); these states, since they are composed of one s and two p atomic orbitals, are called sp 2 orbitals. Imagine now a second identical atom, which we label B , with the linear combinations shown in Fig. 1.18 and deﬁned in Table 1.1 as B B B B φi (i = 1 − 4). The orbitals φ1 , φ2 , φ3 also point along three directions on the x , y plane ◦ separated by 120 , but in the opposite sense (rotated by 180◦ ) from those of atom A . For example, φ1A points along the −ˆx direction, while φB1 points along the +ˆx direction. Now imagine that we place atoms A and B next to each other along the x axis, ﬁrst atom A and to its right atom B , at a distance a. We arrange the distance so that there is signiﬁcant overlap between orbitals φ1A and φ1B , which are pointing toward each other, thereby maximizing the interaction between these two orbitals. Let us assume that in the neutral isolated state of the atom we can occupy each of these orbitals by one electron; note that this is not √ the b ground state of the atom. We can form two linear combinations, ψ1 = (φ1A + φB ) / 2 1 √ and ψ1a = (φ1A − φ1B )/ 2, of which the ﬁrst maximizes the overlap and the second has a node at the midpoint between atoms A and B . As usual, we expect the symmetric linear combination of singleparticle orbitals (called bonding state) to have lower energy than the antisymmetric one (called antibonding state) in the system of the two atoms; this is a general feature of how combinations of singleparticle orbitals behave (see Problem 4), as was discussed in our earlier heuristic model of two atoms with one valence electron each (see Fig. 1.8 and related discussion). The exact energy of the bonding and antibonding states will depend on the overlap of the orbitals φA1 , φ1B . We can place two electrons, one from each atomic orbital, in the symmetric linear combination because of their spin degree of freedom; this is based on the assumption that the spin wavefunction of the two electrons is antisymmetric (a spin singlet), so that the total wavefunction, the product of the spatial and spin parts, is antisymmetric upon exchange of their coordinates, as it should be due to their fermionic nature. Through this exercise we have managed to lower the energy of the system, since the energy of ψ b is lower than the energy of φA1 or φ1B . This is the essence of the chemical bond between two atoms, which in this case is called a covalent σ bond, as already mentioned in relation to the simple model of Fig. 1.10. Imagine next that we repeat this exercise: we take another atom with the same linear combinations √ of orbitals as B , which we will call B 1 , and place it in the direction of the vector (xˆ − 3yˆ ) /2 relative to the position of atom A , and at the same distance a as atom B B from A . Due to our choice of orbitals, φ2A and φ2 1 will be pointing toward each other. We
25
Fig. 1.18
1.3
The Architecture of Crystals
Illustration of covalent bonding in a single plane of graphite, called “graphene.” Top: Example of the formation of hybrid sp2 orbitals from linear combinations of s and p orbitals, with relative 2 weights 1 and 2, respectively: this is the hybrid orbital labeled φB 1 in Table 1.1. Middle: The sp linear combinations of s and p atomic orbitals corresponding to the atoms labeled A and B, as deﬁned in Table 1.1. Bottom : The energylevel diagram for the s, p atomic states, their sp2 linear a b B combinations (φA i s and φi s), and the bonding (ψ i s) and antibonding (ψ i s) states (up–down arrows indicate electron spins). The shaded regions indicate the broadening of the individual energy levels over a range of values into the valence and conduction bands.
26
1
Table 1.1 the
sp2
From Atoms to Solids
The linear combinations of
s
and
hybrids for the two atoms, labeled
p A
atomic orbitals that form and
B
, per unit cell in
the graphite structure.
√
√
A 1
= √13 sA − √23 pAx
φ
B 1
= √13 sB + √23 pBx
A 2
= √13 sA + √16 pAx − √12 pAy
φ
B 2
= √13 sB − √16 pBx + √12 pBy
A 3
= √13 sA + √16 pAx + √12 pAy
φ
B 3
= √13 sB − √16 pBx − √12 pBy
A 4
= pAz
φ
B 4
= pBz
φ
φ
φ
φ
can form symmetric and antisymmetric combinations from them, occupy the symmetric (lowerenergy) one with two electrons as before, and create a second σ bond between atoms A and B 1. Finally, we repeat this procedure with a third atom B 2 placed along the direction √ of the vector (xˆ + 3yˆ )/2 relative to the position of atom A , and at the same distance a as the previous two neighbors. Through the same procedure we can form a third σ bond between atoms A and B 2, by forming the symmetric and antisymmetric linear combinations of the orbitals φ3A and φ3B2 . Now, as far as atom A is concerned, its three neighbors are exactly equivalent, so we consider the vectors that connect them as the repeat vectors at which equivalent atoms in the crystal should exist. If we place atoms of type B at all the possible integer multiples of these vectors, we form a lattice. To complete the lattice we have to place atoms of type A also at all the possible integer multiples of the same vectors, relative to the position of the original atom A . The resulting lattice is called the honeycomb lattice. Each atom of type A is surrounded by three atoms of type B and vice versa, as illustrated in Fig. 1.18. Though this example may seem oversimpliﬁed, it actually corresponds to the structure of graphite, one of the most stable crystalline solids. In graphite, planes of C atoms in the honeycomb lattice are placed on top of each other to form a 3D solid, as illustrated in Fig. 1.19, but the interaction between planes is rather weak (similar to the van der Waals interaction). An indication of this weak bonding between planes compared to the ˚ inplane bonds is that the distance between nearestneighbor atoms on a plane is 1.42 A, ˚ a factor of 2.36 larger. whereas the distance between successive planes is 3.35 A, What about the orbitals pz (or φ4), which so far have not been used? If each atom had only three valence electrons, then these orbitals would be left empty since they have higher energy than the orbitals φ1, φ2 , φ3, which are linear combinations of s and p orbitals (the original s atomic orbitals have lower energy than p). In the case of C, each atom has four valence electrons so there is one electron left per atom when all the σ bonds have been formed. These electrons remain in the pz orbitals which are perpendicular to the x , y plane and thus parallel to each other. Symmetric and antisymmetric combinations of neighboring pAz and p Bz orbitals can also be formed (the states ψ4b , ψ4a respectively), and the energy can be lowered by occupying the symmetric combination. In this case the overlap between neighboring p z orbitals is signiﬁcantly smaller and the corresponding gain in energy signiﬁcantly less than in σ bonds. This is referred to as a π bond, which is
27
Fig. 1.19
Fig. 1.20
1.3
The Architecture of Crystals
Illustration of atomic arrangement in graphite in a top view (left) and a perspective view (right): atoms form planes with every atom on a plane having three neighbors bonded by strong covalent bonds, and the planes are stacked on top of each other. The atoms on a single plane are shown in the same color but are colored differently in successive planes (blue and red), which are shifted relative to each other. The next plane in the sequence would be exactly above the ﬁrst (blue) one, along the direction perpendicular to the plane, repeating the pattern to very large distances. Bonding between the planes is relatively weak, due to van der Waals interactions, and is not shown in this representation.
The structure of the C60 molecule or “buckyball” (left), consisting of pentagonal and hexagonal rings of C atoms, and of carbon nanotubes (right), consisting of hexagonal rings of C atoms as in a plane of graphite, but wrapped into a cylinder (for more details on these and similar structures, see Chapter 5).
generally weaker than a σ bond. Carbon is a special case, in which the π bonds are almost as strong as the σ bonds. An intriguing variation of this theme is a structure that contains pentagonal rings as well as the regular hexagons of the honeycomb lattice, while maintaining the threefold coordination and bonding of the graphitic plane. The presence of pentagons introduces curvature in the structure, and the right combination of pentagonal and hexagonal rings produces the almost perfect sphere, shown in Fig. 1.20. This structure actually exists in nature! It was discovered in 1985 and has had a great impact on carbon chemistry and physics – its discoverers, R. F. Curl, H. W. Kroto, and R. E. Smalley, received the 1996 Nobel Prize for Chemistry. Many more interesting variations of this structure have also been produced, including “onions” – spheres within spheres – and “tubes” – cylindrical arrangements of threefoldcoordinated carbon atoms. The tubes in particular seem promising for applications in technologically and biologically relevant systems. These structures have been nicknamed after Buckminster Fuller, an American scientist
28
1
Table 1.2 the
sp3
From Atoms to Solids
The linear combinations of
s
and
hybrids for the two atoms, labeled
p A
atomic orbitals that form and
B
, per unit cell in
the diamond structure.
φ
A 1
= 21
φ
A 2
= 21
φ
A 3
= 21
φ
A 4
= 21
º º º º
A A sA − pA x − py − pz A A sA + pA x − py + pz A A sA + pA x + py − pz A A sA − pA x + py + pz
» φ
B 1
= 12
φ
B 2
= 12
φ
B 3
= 12
φ
B 4
= 12
» » »
º
»
º
»
º
»
º
»
B B s B + pB x + py + pz B A s B − pB x + py − pz B B s B − pB x − py + pz B B s B + pB x − py − pz
and practical inventor of the early twentieth century, who designed architectural domes based on pentagons and hexagons; their nicknames are buckminsterfullerene or buckyball for C60, buckyonions, and buckytubes. There is a different way of forming bonds between C atoms: consider the following linear combinations of the s and p atomic orbitals for atom A , deﬁned in Table 1.2 as φA i (i = 1 − 4). The energy of these states, which are degenerate, is equal to (²s + 3 ² p)/4, where ²s , ²p are the energies of the original s and p atomic orbitals (see Problem 5); the new states, which are composed of one s and three p orbitals, are called sp 3 orbitals. These orbitals point along the directions from the center to the corners of a regular tetrahedron, as illustrated in Fig. 1.21. We can now imagine placing atoms B , B 1 , B 2, B 3 at the corners of the tetrahedron, with which we associate linear combinations of s and p orbitals just like those for atom A , but having all the signs of the p orbitals reversed, deﬁned in Table 1.2 as φiB ( i = 1 − 4). Then we will have a situation where the φ orbitals on neighboring A and B atoms will be pointing toward each other, and we can form symmetric and antisymmetric combinations of those, ψ b, ψ a respectively, to create four σ bonds around atom A . The exact energy of the ψ orbitals will depend on the overlap between the φA and φB orbitals; for sufﬁciently strong overlap, we can expect the energy of the b a ψ states to be lower than the original s atomic orbitals and those of the ψ states to be higher than the original p atomic orbitals, as shown schematically in Fig. 1.21. The vectors connecting the equivalent B , B 1 , B 2, B 3 atoms deﬁne the repeat vectors at which atoms must be placed to form an inﬁnite crystal. By placing both A type and B type atoms at all the possible integer multiples of these vectors, we create the diamond lattice shown in Fig. 1.22. This is the other stable form of bulk C; an experimental image of this structure taken with a transmission electron microscope (TEM) is shown in Fig. 1.23. Since C has four valence electrons and each atom at the center of a tetrahedron forms four σ bonds with its neighbors, all electrons are taken up by the bonding states. This results in a very stable and strong 3D crystal. Surprisingly, graphite has a somewhat lower internal energy than diamond, that is, the thermodynamically stable solid form of carbon is the soft, black, cheap graphite rather than the very strong, brilliant, expensive diamond crystal (which means that diamonds are deﬁnitely not forever)!
29
Fig. 1.21
1.3
The Architecture of Crystals
Illustration of covalent bonding in the diamond lattice. Top: Example of the formation of hybrid sp3 orbitals from linear combinations of one s and three p orbitals: this is the hybrid orbital labeled φB 1 in Table 1.2. Middle: The sp 3 linear combinations of s and p atomic orbitals corresponding to the atoms labeled A and B, as deﬁned in Table 1.2. Bottom : The energylevel diagram for the s, p b B atomic states, their sp 3 linear combinations (φA i s and φi s), and the bonding (ψi s) and antibonding ( ψia s) states (up–down arrows indicate electron spins). The shaded regions indicate the broadening of the individual energy levels over a range of values into the valence and conduction bands.
The diamond lattice, with four neighbors per atom, is relatively open compared to the closepacked lattices. Its stability comes from the very strong covalent bonds formed between the atoms. Two other elements with four valence s and p electrons, namely Si and Ge, also crystallize in the diamond, but not the graphite, lattice. There are two more elements with four valence s and p electrons in the Periodic Table, Sn and Pb. Sn forms crystal structures that are distorted variants of the diamond lattice, since its σ bonds are
30
Fig. 1.22
Fig. 1.23
1
From Atoms to Solids
The diamond crystal. Left : The conventional cube, outlined in red lines, with C atoms at the cube corners and face centers, forming a regular FCC lattice. A second FCC lattice is formed by C atoms at the centers of tetrahedra deﬁned by the atoms of the ﬁrst FCC lattice – one such tetrahedron is outlined in yellow lines. The two interpenetrating FCC lattices are displaced relative to each other by 1/4 of the main diagonal of the cube. Right: Perspective view of larger portion of the crystal.
The structure of the diamond lattice as revealed by the transmission electron microscope (TEM) [adapted from F. Hosokawa, H. Sawada, Y. Kondo, K. Takayanagi, and K. Suenaga, “Development of Cs and Cc correctors for transmission electron microscopy,” Microscopy 62, 2341 (2013)]. The ﬁgure on the upper right shows an intensity scan along the vertical dashed line in the main ﬁgure, ˚ The lowerleft corner with peaks corresponding to the atomic positions separated by 89 pm (0.89 A). of the TEM image contains a simulated image of the structure. The ﬁgure on the lower left shows a ballandstick representation of the crystal oriented along the same crystallographic direction.
not as strong as those of the other groupIVA elements, and it can gain some energy by increasing the number of neighbors (from four to six) at the expense of perfect tetrahedral σ bonds. Pb, on the other hand, behaves more like a metal, preferring to optimize the number of neighbors and form the FCC crystal. Interestingly, elements with only three valence s and p electrons, like B, Al, Ga, In, and Tl, do not form the graphite structure, as alluded to above. They instead form more complex structures in which they try to optimize bonding given their relatively small number of valence electrons per atom. Some examples: the common structural unit for B is the icosahedron, shown in Fig. 1.15, and such units are close packed to form the solid; Al forms the FCC crystal and is the representative metal with s and p electrons and a closepacked structure; Ga forms quite complicated crystal structures with six or seven near neighbors (not all of them at the same distance); In forms a distorted version of the cubic close packing in which the 12 neighbors are split into a
31
Fig. 1.24
1.3
The Architecture of Crystals
Typical layer structures that groupV elements form, with all atoms threefold coordinated as in a graphitic plane, but with bond angles between nearest neighbors being close to 90◦ , representative of porbital bonds. The planes are stacked on top of each other to form the 3D solids. Left: A layer of blue phosphorus. Right: A layer of black phosphorus (also referred to as “phosphorene”).
group of four and another group of eight equidistant atoms. None of these structures can easily be described in terms of the notions introduced above to handle s and p valence electrons, demonstrating the limitations of this simple approach. Of the other elements in the Periodic Table with s and p valence electrons, those with ﬁve electrons, N, P, As, Sb, and Bi, tend to form complex structures where atoms have three σ bonds to their neighbors but not in a planar conﬁguration. A characteristic pattern is one in which the three p valence electrons participate in covalent bonding while the two s electrons form a ﬁlled state which does not contribute much to the cohesion of the solid; this ﬁlled state is called the “lone pair” state. If the covalent bonds were composed of purely p orbitals, the bond angles between nearest neighbors would be 90◦; instead, the covalent bonds in these structures are a mixture of s and p orbitals with predominant p character, and the bond angles are somewhere between 120◦ (sp 2 bonding) and 90◦ (pure p bonding), as illustrated in Fig. 1.24. As an example, two different structures of solid P are represented by this kind of local bonding arrangement. In one structure, blue phosphorus, the covalent bonds are arranged in puckered hexagons which form planes. In another structure, black phosphorus, the atoms form bonded chains along one direction, displaced in the other two directions so that the resulting arrangement is a layer with the chains slightly above and below the average position in the direction perpendicular to the plane of the layer. In both structures, the layers are stacked on top of each other to form the solid. The interaction between layers is much weaker than that between atoms in a single layer: an indication of this difference in bonding is the fact that the distance between nearest neighbors in a ˚ while the closest distance between atoms on successive layer of blue phosphorus is 2.17 A, ˚ layers is 3.87 A, almost a factor of 2 larger. The structures of As, Sb, and Bi follow the same general pattern with threefold bonded atoms, but in those solids there exist additional covalent bonds between atoms in different layers so that the structure is not as clearly layered as in the case for P. An exception to this general tendency is nitrogen, the lightest element with ﬁve valence electrons, which forms a crystal composed of nitrogen molecules since the N2 unit is particularly stable. The elements with six s and p valence electrons, O, S, Se, Te, and Po, tend to form molecularlike ring or chain structures with two nearest neighbors per atom, which are
32
1
From Atoms to Solids
then packed to form 3D crystals. These rings or chains are puckered and form bonds at angles that try to satisfy bonding requirements analogous to those described for the solids with four s and p valence electrons. Since these elements have a valence of 6, they tend to keep four of their electrons in one ﬁlled s and one ﬁlled p orbital and form covalent bonds to two neighbors with their other two p orbitals. This picture is somewhat oversimpliﬁed, since signiﬁcant hybridization takes place between s and p orbitals that participate in bonding, so that the preferred angles between the bonding orbitals are not 90◦ , as pure p bonding would imply, but range between 102 ◦ and 108◦. Typical distances ˚ for S, 2.32 A ˚ for Se, between nearestneighbor atoms in the rings or chains are 2.06 A ˚ and 2.86 A for Te, while typical distances between atoms in successive units are 3.50 ˚ for S, 3.46 A ˚ for Se, and 3.74 A ˚ for Te; that is, the ratio of distances between A atoms within a bonding unit and across bonding units is 1.7 for S, 1.5 for Se, and 1.3 for Te. An exception to this general tendency is oxygen, the lightest element with six valence electrons, which forms a crystal composed of oxygen molecules; the O2 unit is particularly stable. The theme of diatomic molecules as the basic unit of the crystal, already mentioned for nitrogen and oxygen, is common in elements with seven s and p valence electrons also: chlorine, bromine, and iodine form solids by close packing of diatomic molecules.
1.3.4
Atoms with s and d Valence Electrons
This category includes all the atoms in the middle columns of the Periodic Table, that is, columns IB to VIIB and VIII. The d orbitals in atoms have directional nature like the p orbitals. However, since there are ﬁve d orbitals it is difﬁcult to construct linear combinations with s orbitals that would neatly point toward nearest neighbors in 3D space and produce a crystal with simple σ bonds. Moreover, the d valence orbitals typically lie lower in energy than the s valence orbitals and therefore do not participate as much in bonding (see for example the discussion about Ag in Chapter 5). Note that d orbitals can form strong covalent bonds by combining with p orbitals of other elements, as we discuss in a subsequent section. Thus, elements with s and d valence electrons tend to form solids where the s electrons are shared among all atoms in the lattice, just like elements with one or two s valence electrons. This is particularly true for the elements Cu, Ag, and Au (called the “noble elements” due to their relatively chemically inert nature), which have electronic shells of the type d 10 s 1, that is, a ﬁlled d shell and one s electron outside it; the d states, however, are close in energy to the s state, and there is signiﬁcant interaction between them. The predominantly d electron elements form spaceﬁlling closepacked crystals, of the FCC, HCP, and BCC types. There are very few exceptions to this general tendency, namely Mn which forms a very complex structure with a cubic lattice and a very large number of atoms (58) in the unit cell, and Hg which forms a lowsymmetry rhombohedral structure. Even those structures, however, are slight variations of the basic closepacking structures already mentioned. For instance, the Mn structure, in which atoms have from 12 to 16 neighbors, is a slight variation of the BCC structure. The crystals formed by most of these elements typically have metallic character.
33
1.3
1.3.5
The Architecture of Crystals
Atoms with s , d , and f Valence Electrons
The same general trends are found in the rare earth elements, which are grouped in the lanthanides (atomic numbers 58–71) and the actinides (atomic numbers 90 and beyond). Of those we discuss brieﬂy the lanthanides as the more common of the rare earths that are found in solids. In these elements the f shell is gradually ﬁlled as the atomic number increases, starting with an occupation of two electrons in Ce and completing the shell with 14 electrons in Lu. The f orbitals have directional character, which is even more complicated than that of d orbitals. The solids formed by these elements are typically closepacked structures like FCC and HCP, with a couple of exceptions (Sm which has rhombohedral structure and Eu which has BCC structure). They are metallic solids with high atomic densities. More interesting are structures formed by these elements and other elements of the Periodic Table, in which the complex character of the f orbitals can be exploited in combination with orbitals from neighboring atoms to form strong bonds. Alternatively, these elements are used as dopants in complicated crystals, where they donate some of their electrons to states formed by other atoms. One such example is discussed in the following sections.
1.3.6
Solids with Two Types of Atoms
Some of the most interesting and useful solids involve two types of atoms, which in some ways are complementary. One example that comes immediately to mind are solids composed of atoms in the ﬁrst (groupIA) and seventh (groupVIIA) columns of the Periodic Table, which have one and seven valence electrons, respectively. Solids composed of such elements are referred to as “alkali halides.” It is natural to expect that the atom with one valence electron will lose it to the more electronegative atom with seven valence electrons, which then acquires a closed electronic shell, completing the s and p levels. This of course leads to one positively and one negatively charged ion, which are repeated periodically in space to form a lattice. The easiest way to arrange such atoms is at the corners of a cube, with alternating corners occupied by atoms of the opposite type. This arrangement results in the sodium chloride (NaCl) or rocksalt structure, one of the most common crystals. Many combinations of groupIA and groupVIIA atoms form this kind of crystal. In this case each ion has six nearest neighbors of the opposite type. A different way to arrange the ions is to have one ion at the center of a cube formed by ions of the opposite type. This arrangement forms two interpenetrating cubic lattices and is known as the cesium chloride (CsCl) structure. In this case each ion has eight nearest neighbors of the opposite type. Several combinations of groupIA and groupVIIA atoms crystallize in this structure. Since in all these structures the groupIA atoms lose their s valence electron to the groupVIIA atoms, this type of crystal is representative of ionic bonding. Both of these ionic structures are shown in Fig. 1.25. Another way of achieving a stable lattice composed of two kinds of ions with opposite sign is to place them in the two interpenetrating FCC sublattices of the diamond lattice, described earlier. In this case each ion has four nearest neighbors of the opposite type, as
34
Fig. 1.25
Fig. 1.26
1
From Atoms to Solids
Illustration of cubic crystals formed by ionic solids. Left: The rocksalt, NaCl structure, in which the ions of each type form an FCC lattice with each ion surrounded by six neighbors of the opposite type; the two interpenetrating FCC lattices are displaced relative to each other by 1/2 of the main diagonal of the cube. Middle: The CsCl structure, in which the ions of each type form a simple cubic lattice with each ion surrounded by eight neighbors of the opposite type. The two interpenetrating cubic lattices are displaced relative to each other by 1/2 of the main diagonal of the cube. Right: NaCl crystals exhibiting the characteristic cubic shape dictated by the atomicscale structure of the crystal [source: Wikimedia CC BYSA 3.0, https://commons.wikimedia.org/w/index.php?curid=227730].
The zincblende lattice in which every atom is surrounded by four neighbors of the opposite type. Left: The conventional cubic cell is outlined in thin red lines and a tetrahedron of green atoms is outlined in yellow lines. Right: Perspective view of a larger portion of the zincblende crystal.
shown in Fig. 1.26. Many combinations of atoms in the IB column of the Periodic Table and groupVIIB atoms crystallize in this structure, which is called the zincblende structure from the German term for ZnS, the representative solid with this lattice. The elements in the IB column have a ﬁlled d shell (10 electrons) and one extra s valence electron, so it is natural to expect them to behave in some ways similarly to the alkali metals. However, the small number of neighbors in this structure, as opposed to the rocksalt and cesium chloride structures, suggest that the cohesion of these solids cannot be attributed to simple ionic bonding alone. In fact, this becomes more pronounced when atoms from the second (groupIIB) and sixth (groupVIA) columns of the Periodic Table form the zincblende structure (ZnS itself is the prime example). In this case we would have to assume that the groupII atoms lose their two electrons to the groupVI atoms, but since the electronegativity difference is not as great between these two types of elements as
35
1.3
The Architecture of Crystals
between groupIA and groupVIIA elements, something more than ionic bonding must be involved. Indeed, the crystals of groupII and groupVI atoms in the zincblende structure are good examples of mixed ionic and covalent bonding. This trend extends to one more class of solids: groupIIIA and groupVA atoms also form zincblende crystals, like AlP, GaAs, InSb, etc. In this case, the bonding is even more tilted toward covalent character, similar to the case of groupIV atoms which form the diamond lattice. Finally, there are combinations of two groupIV atoms that form the zincblende structure; some interesting examples are SiC and GeSi alloys. A variation on this theme is a class of solids composed of Si and O. In these solids, each Si atom has four O neighbors and is situated at the center of a tetrahedron, while each O atom has two Si neighbors, as illustrated in Fig. 1.27. In this manner the valence of both Si and O is perfectly satisﬁed, so that the structure can be thought of as covalently bonded. Due to the large electronegativity of O, the covalent bonds are polarized to a large extent, so that the two types of atoms can be considered partially ionized. This results again in a mixture of covalent and ionic bonding. The tetrahedra of Si–O atoms are very stable units and the relative positions of atoms in a tetrahedron are essentially ﬁxed. The position of these tetrahedra relative to each other, however, can be changed with little cost in energy, because this type of structural distortion involves only a slight bending of bond angles, without changing bond lengths. This freedom in relative tetrahedron orientation produces a very wide variety of solids based on this structural unit, including amorphous structures, like the common glass illustrated in Fig. 1.27, and structures with many open spaces in them, like the zeolites. Yet another category of solids composed of two types of atoms are the socalled transitionmetal chalcogenides. In these materials, the transitionmetal atom contributes to the bonding with its partially ﬁlled d states (typical elements are Sn, Fe, Mo, Ta, W) and the chalcogen atom contributes to the bonding with its p electrons (typical elements are S, Se, Te). Some materials involve a onetoone ratio of the metal to the chalcogen atoms (the transitionmetal monochalcogenides, like SnS, FeSe), while in others the ratio is onetotwo (the transitionmetal dichalcogenides, like MoS2 , WSe2 ). What is
Fig. 1.27
Example of an ioniccovalent amorphous structure, the silicondioxide glass. Left: Illustration of an amorphous network of SiO2, with every Si atom (yellow spheres) having four O neighbors and every O atom (red spheres) having two Si neighbors. Right: An enlargement of a small part of the amorphous SiO 2 network, in which the local bonding between Si and O atoms is clearly seen.
36
Fig. 1.28
1
From Atoms to Solids
Illustration of the atomic and electronic structure of a layered transitionmetal dichalcogenide crystal, molybdenum disulﬁde. Top row: A single layer of the MoS2 solid, with yellow spheres representing the S atoms and brown spheres representing the Mo atoms: top, side, and perspective views. Bottom row: Schematic representation of the energy levels of atomic orbitals of Mo and S atoms, the symmetric S hybrid orbitals, and their combination into bonding and antibonding bands.
interesting about these solids is that they consist of layers within which the atoms are strongly bonded, while the interlayer bonding is much weaker, of van der Waals type. A typical example, molybdenum disulﬁde (MoS2 ), is shown in Fig. 1.28. In this case, the corresponding energylevel diagram of atomiclike states and their bonding and antibonding combinations produces a band gap when the bands are ﬁlled by the available valence electrons. Many of these materials behave like semiconductors, with band gaps in the range of 2–3 eV. For this layer, which has a mirrorplane symmetry on the plane of the metal atoms, the states of the chalcogen atoms that participate in the bonding within one layer are symmetric (even and odd) linear combinations of the atomic p orbitals. The bonding between these hybrid p orbitals and the d orbitals of the metal atom involves both covalent and ionic character. The 3D crystal is formed by stacking of such layers. The layered nature of these materials makes them very good lubricants. The possibility of extracting a single layer of one material, and combining it with one or more layers of another similar material, has opened up new exciting avenues for manipulating the properties of solids to achieve
37
1.3
The Architecture of Crystals
interesting electronic and optical responses. The hope of employing these structures in the fabrication of novel electronic and optical devices has sparked intensive research into their properties. Equally exciting is the prospect of exploring the physics of electrons conﬁned in these 2D layered heterostructures, including quantum Hall effects, topologically protected edge states that can carry spin currents, and superconductivity; all of these topics are under intense investigation at the time of writing. 1.3.7
Hydrogen: A Special One s ValenceElectron Atom
So far we have left H out of the discussion. This is because H is a special case: it has no core electrons. Its interaction with the other elements, as well as between H atoms is unusual, because when H tries to share its one valence s electron with other atoms, what is left is a bare proton rather than a nucleus shielded partially by core electrons. The proton is an ion much smaller in size than the other ions produced by stripping the valence electrons from atoms: its size is 10−15 m, ﬁve orders of magnitude smaller than typical ions which ˚ It also has the smallest mass, which gives it a special character: have a size of order 1 A. in all other cases (except He) we can consider the ions as classical particles, due to their large mass, while in the case of hydrogen, its light mass implies a large zeropoint motion which makes it necessary to take into account the quantum nature of the proton’s motion. Yet another difference between hydrogen and all other elements is the fact that its s valence electrons are very strongly bound to the nucleus: the ionization energy is 13.6 eV, whereas typical ionization energies of valence electrons in other elements are in the range 1–2 eV. Due to its special character, H forms a special type of bond called a “hydrogen bond.” This is encountered in many structures composed of molecules that contain H atoms, such as organic molecules and water. The solid in which hydrogen bonding plays the most crucial role is ice. Ice forms many complex phases.8 In its ordinary phase called Ih , the H2O molecules are placed so that the O atoms occupy the sites of a wurtzite lattice (see Fig. 1.14), while the H atoms are along lines that join O atoms.9 There are two H atoms attached to each O atom by short covalent ˚ while the distance between O atoms is 2.75 A. ˚ There is one H bonds (of length 1.00 A), atom along each line joining two O atoms. The bond between a H atom and an O atom to which it is not covalently bonded is called a hydrogen bond, and in this system, has length ˚ it is these hydrogen bonds that give stability to the crystal. This is illustrated in 1.75 A; Fig. 1.29. The hydrogen bond is much weaker than the covalent bond between H and O in the water molecule: the energy of the hydrogen bond is 0.3 eV, while that of the covalent H–O bond is 4.8 eV. There are many ways of arranging the H atoms within these constraints for a ﬁxed lattice of O atoms, giving rise to a large conﬁgurational entropy. Other forms of ice have different lattices, but this motif of local bonding is common. Within the atomic orbital picture discussed earlier for solids with s and p electrons, we can construct a simple argument to rationalize hydrogen bonding in the case of ice. The O atom has six valence electrons in its s and p shells and therefore needs two more 8 N. H. Fletcher, The Chemical Physics of Ice (Cambridge University Press, Cambridge, 1970). 9 J. D. Bernal and R. H. Fowler, J. Chem. Phys. 1, 515 (1933).
38
Fig. 1.29
1
From Atoms to Solids
Illustration of hydrogen bonding between water molecules in ice: the O atom (red larger circles) is at the center of a tetrahedron formed by other O atoms, and the H atoms (white smaller circles) are along the directions joining the center to the corners of the tetrahedron. The O–H covalent bond ˚ (thicker black lines), while the H–O hydrogen bond distance is distance is a = 1.00 A ˚ (denoted by dashed thinner lines). This is the structure of Ih ice in which the O atoms sit b = 1.75 A at the sites of a wurtzite lattice (cf. Fig. 1.14) and the H atoms are along the lines joining O atoms; there is one H atom along each such line, and two H atoms bonded by short covalent bonds to each O atom. On the right, a picture of a snowﬂake exhibiting the characteristic sixfold symmetry of the underlying ice crystal.
electrons to complete its electronic structure. The two H atoms that are attached to it to form the water molecule provide these two extra electrons, at the cost of an anisotropic bonding arrangement (a completed electronic shell should be isotropic, as in the case of Ne, which has two more electrons than O). The cores of the H atoms (the protons), having lost their electrons to O, experience a Coulomb repulsion. The most favorable structure for the molecule which optimizes this repulsion would be to place the two H atoms in diametrically opposite positions relative to the O atom, but this would involve only one p orbital of the O atom to which both H atoms would bond. This is an unfavorable situation as far as formation of covalent bonds is concerned, because it is not possible to form two covalent bonds with only one p orbital and two electrons from the O atom. A compromise between the desire to form strong covalent bonds and the repulsion between the H cores is the formation of four sp 3 hybrids from the orbitals of the O atom, two of which form covalent bonds with the H atoms, while the other two are ﬁlled by two electrons each. This produces a tetrahedral structure with two lobes which have more positive charge (the two sp 3 orbitals to which the H atoms are bonded) than the other two lobes (the two sp 3 orbitals which are occupied by two electrons each) which have more negative charge. It is natural to expect that bringing similar molecular units together would produce some attraction between the lobes of opposite charge in neighboring units. This is precisely the arrangement of molecules in the structure of ice discussed above and shown in Fig. 1.29. This rationalization, however, is somewhat misleading as it suggests that the hydrogen bond, corresponding to the attraction between oppositely charged lobes
39
1.3
The Architecture of Crystals
of the H2 O tetrahedrons, is essentially ionic. In fact, the hydrogen bond has signiﬁcant covalent character as well: the two types of orbitals pointing toward each other form bonding (symmetric) and antibonding (antisymmetric) combinations, leading to covalent bonds between them. This point of view was originally suggested by L. Pauling10 and has remained controversial until recently, when sophisticated scattering experiments and quantummechanical calculations provided convincing evidence in its support.11 The solid phases of pure hydrogen are also unusual. At low pressure and temperature, H is expected to form a crystal composed of H2 molecules in which every molecule behaves almost like an inert unit, with very weak interactions to the other molecules. At higher pressure, H is supposed to form an atomic solid when the molecules have approached each other enough so that their electronic distributions are forced to overlap strongly. 12 However, the conditions of pressure and temperature at which this transition occurs, and the structure of the ensuing atomic solid, are still a subject of active research.13 The latest estimates are that it takes more than 5 Mbar of pressure to form the atomic H solid, which can only be reached under very special conditions in the laboratory. There is considerable debate about what the crystal structure at this pressure should be, and although the BCC structure seems to be the most likely phase by analogy to all other alkalis, this has not been unambiguously proven to date. 1.3.8
Solids with More Than Two Types of Atoms
If we allow several types of atoms to participate in the formation of a crystal, many more possibilities open up. There are indeed many solids with complex composition, but the types of bonding that occur in these situations are variants of the types we have already discussed: metallic, covalent, ionic, van der Waals, and hydrogen bonding. In many situations, several of these types of bonding are present simultaneously. One interesting example of such complex structures is the class of ceramic materials in which hightemperature superconductivity (HTSC) was observed in the mid1980s (this discovery, by J. G. Bednorz and K. A. M¨uller, was recognized by the 1987 Nobel Prize for Physics). In these materials, strong covalent bonding between Cu and O forms 1D or 2D structures where the basic building block is oxygen octahedra; rare earth atoms are then placed at hollow positions of these backbond structures and become partially ionized, giving rise to mixed ionic and covalent bonding (see for example Fig. 1.30). The motif of oxygen octahedra with a metal atom at the center to which the O atoms are covalently bonded, supplemented by atoms which are easily ionized, is also the basis for a class of structures called “perovskites.” The chemical formula of perovskites is ABO3, where A is the easily ionized element and B the element which is bonded to the oxygens. The basic unit is shown in Fig. 1.30: bonding in the xy plane is accomplished through the overlap between the px and py orbitals of the ﬁrst (O1 ) and second (O2) oxygen atoms, 10 L. Pauling, J. Am. Chem. Soc. 57, 2680 (1935). 11 E. D. Isaacs, A. Shukla, P. M. Platzman, et al. , Phys. Rev. Lett. 82, 600 (1999). 12 E. Wigner and H. B. Huntington, J. Chem. Phys. 3 , 764 (1935); I. F. Silvera, Rev. Mod. Phys. 52 , 393 (1980);
H. K. Mao and R. J. Hemley, Am. Sci. 80, 234 (1992). 13 R. P. Dias and I. F. Silvera, Science, 355, 715 (2017).
40
1
From Atoms to Solids
O3 O2 O1 B
A
z
pz
O3
y z a a
py y
c
O1 B d x2 y 2
Fig. 1.30
O2
px
x
x
B d3z 2r 2
Illustration of the structure and bonding in perovskite crystals. Top, left: A Cu atom (cyan sphere, labeled B) surrounded by six O atoms (red spheres, three of them labeled O1, O2, O3 ), which form an octahedron (shown in yellow); the Cu–O atoms are bonded by strong covalent bonds. The green spheres at the cube corners (labeled A ) represent ionized metal atoms. Top, right: Cornersharing O octahedra, forming a 2D square lattice; when joined at the remaining apexes with other octahedra they form a 3D lattice. Bottom: The px , py , pz orbitals of the three O atoms (labeled O1, O2, O3 in red) and the dx2 −y2 , d3z2 −r 2 orbitals of the Cu atoms (labeled B in cyan) that participate in the formation of covalent bonds in the octahedron are shown schematically.
respectively, and the dx2 −y2 orbital of B; bonding along the z axis is accomplished through the overlap between the p z orbital of the third (O3 ) oxygen atom and the d 3z2 −r2 orbital of B (see Fig. 1.17 for the nature of these p and d orbitals). The A atoms provide the necessary number of electrons to satisfy all the covalent bonds. Thus, the overall bonding involves both strong covalent character between B and O, as well as ionic character between the B–O units and the A atoms. The complexity of the structure gives rise to several interesting properties, such as ferroelectricity, that is, the ability of the solid to acquire and maintain an internal dipole moment. The dipole moment is associated with a displacement of the
41
1.4
Bonding in Solids
B atom away from the center of the octahedron, which breaks the symmetry of the cubic lattice. These solids have very intriguing behavior: when external pressure is applied on them it tends to change the shape of the unit cell of the crystal and therefore produces an electrical response since it affects the internal dipole moment; conversely, an external electric ﬁeld can also affect the internal dipole moment and the solid changes its shape to accommodate it. This coupling of mechanical and electrical responses is very useful for practical applications, such as sensors and actuators and nonvolatile memories. The solids that exhibit this behavior are called piezoelectrics; some examples are CaTiO3 (calcium titanate), PbTiO3 (lead titanate), BaTiO3 (barium titanate), and PbZrO3 (lead zirconate). Another example of complex solids is the class of crystals formed by fullerene clusters and alkali metals: there is strong covalent bonding between C atoms in each fullerene cluster, weak van der Waals bonding between the fullerenes, and ionic bonding between the alkali atoms and the fullerene units. The clusters act just like the groupVII atoms in ionic solids, taking up the electrons of the alkali atoms and becoming ionized. It is intriguing that these solids also exhibit superconductivity at relatively high temperatures!
1.4
Bonding in Solids
In our discussion on the formation of solids from atoms we encountered ﬁve general types of bonding in solids: 1. Van der Waals bonding , which is formed by atoms that do not have valence electrons available for sharing (like the noble elements) and is rather weak; the solids produced in this way are not particularly stable. 2. Metallic bonding , which is formed when electrons are shared by all the atoms in the solid, producing a uniform “sea” of negative charge; the solids produced in this way are the usual metals. 3. Covalent bonding , which is formed when electrons in welldeﬁned directional orbitals, which can be thought of as linear combinations of the original atomic orbitals, have strong overlap with similar orbitals in neighboring atoms; the solids produced in this way are semiconductors or insulators. 4. Ionic bonding , which is formed when two different types of atoms are combined, one that prefers to lose some of its valence electrons and become a positive ion, and one that prefers to grab electrons from other atoms and become a negative ion. Combinations of such elements are I–VII, II–VI, and III–V. In the ﬁrst case bonding is purely ionic, in the other two there is a degree of covalent bonding present. 5. Hydrogen bonding , which is formed when H is present, due to its lack of core electrons, light mass, and high ionization energy. For some of these cases, it is possible to estimate the strength of bonding without involving a detailed description of the electronic behavior. Speciﬁcally, for van der Waals bonding and for purely ionic bonding it is sufﬁcient to assume simple classical models. For van der Waals bonding, one assumes that there is an attractive potential between the
42
1
From Atoms to Solids
atoms which behaves like ∼ r −6 with distance r between atoms (this behavior can actually be derived from perturbation theory, see Problem 8). The potential must become repulsive at very short range, as the electronic densities of the two atoms start overlapping, but electrons have no incentive to form bonding states (as was the case in covalent bonding) since all electronic shells are already ﬁlled. For convenience the repulsive part is taken to be proportional to r −12, which gives the famous Lennard–Jones 6–12 potential: VLJ (r )
= 4²
¶´ µ12 a r
−
´ a µ6¹
(1.18)
r
with ² and a constants that determine the energy and length scales. These have been determined for the different elements by referring to the thermodynamic properties of the noble gases; the values of these parameters for the usual noble gas elements are shown in Table 1.3. Use of this potential can then provide a quantitative measure of cohesion in these solids. One measure of the strength of these potentials is the vibrational frequency that would correspond to a harmonic oscillator potential with the same curvature at the minimum; this is indicative of the stiffness of the bond between atoms. In Table 1.3 we present the frequencies corresponding to the Lennard–Jones potentials of the common noble gas elements (see following discussion and Table 1.4 for the relation between this frequency
Table 1.3
Parameters for the Lennard–Jones potential for noble gases
(for original sources see Ashcroft and Mermin, mentioned in Further Reading). For the calculation of
h¯ ω
using the Lennard–Jones parameters
see the following discussion and Table 1.4.
(meV) ˚ a ( A) h¯ ω (meV)
²
Table 1.4
Ne
Ar
Kr
Xe
3.1 2.74 2.213
10.4 3.40 2.310
14.0 3.65 1.722
20.0 3.98 1.510
VLJ ( r), Morse VM (r ), and VHO (r ). The relations between the parameters that ensure the three potentials
Comparison of the three eﬀective potentials, Lennard–Jones
harmonic oscillator
have the same minimum and curvature at the minimum are also given (the parameters of the Morse and harmonic oscillator potentials are expressed in terms of the Lennard–Jones parameters).
VLJ (r ) Potential
Vmin rmin
V¶¶ (rmin ) Relations
4²
−²
º( ) a 12 r
1 (2 6 ) a
1
−
( a )6 » r
(72/2 3 )(²/a2 )
VM (r) º
²
e−2(r −r 0 )/b
−²
− 2e−(r−r0) b /
»
VHO (r )
−² + 12 mω2 (r − r0 )2 −²
r0
r0
2( ²/b2)
m ω2
r0
r0
= (2 61 )a 1 b = (2 6 /6) a
= (2 61 )a ¼ 1 ω = (432 3 ) ²/ma 2
43
1.4
Bonding in Solids
and the Lennard–Jones potential parameters). The vibrational frequency ω is related to the spring constant κ of the harmonic oscillator by the expression ω
∼
´ κ µ1/2 m
where m is the mass of the oscillating particle. For comparison, the vibrational frequency of the H 2 molecule, the simplest type of covalent bond between two atoms, is about 500 meV, a factor of ωH /ωNe ∼ 200 larger, while the masses of the Ne and H atoms give a √ factor of m Ne /m H ∼ 3; we conclude from this comparison that the spring constant for Ne–Ne interactions must be about four orders of magnitude smaller than that of the H–H bond, that is, the Lennard–Jones potentials for the noble gases correspond to very soft bonds indeed! A potential of similar nature, also used to describe effective interactions between atoms, is the Morse potential: V M (r )
=²
º
e−2(r −r0 )/ b − 2e−(r −r0 )/b
»
(1.19)
where again ² and b are the constants that determine the energy and length scales and r 0 is the position of the minimum energy. It is instructive to compare these two potentials to the harmonic oscillator potential which has the same minimum and curvature, given by: VHO( r )
= −² + 21 m ω 2(r − r 0 )2
(1.20)
with ω the frequency, m the mass of the particle in the potential, and r 0 the position of the minimum. The deﬁnitions of the three potentials are such that they all have the same value of the energy at their minimum, namely −². The relations between the values of the other parameters which ensure that the minimum in the energy occurs at the same value of r and that the curvature at the minimum is the same are given in Table 1.4; a plot of the three potentials with these parameters is given in Fig. 1.31. The harmonic oscillator potential is what we would expect near the equilibrium of any normal interaction potential. The other two potentials extend the range far from the minimum; both potentials have a much sharper increase of the energy for distances shorter than the equilibrium value, and a much weaker increase of the energy for distances larger than the equilibrium value, relative to the harmonic oscillator. The overall behavior of the two potentials is quite similar. One advantage of the Morse potential is that it can be solved exactly, by analogy to the harmonic oscillator potential (see Appendix C). This allows a comparison between the energy levels associated with this potential and the corresponding energy levels of the harmonic oscillator; the latter are given by: E nHO
=
·
¸
n
+ 21 h¯ ω
whereas those of the Morse potential are given by: EM n
=
·
n
¸
¶
+ 21 h¯ ω 1 − h¯4ω²
(1.21)
· n
+ 12
¸¹ (1.22)
44
1
From Atoms to Solids
1.2 0.9
LennardJones Morse Harmonic
0.6 0.3
)r(V
0
0.3 0.6 0.9 1.2
0.8
1
1.2
1.4
1.6
1.8
2
r Fig. 1.31
The three effective potentials discussed in the text, Lennard–Jones [Eq. (1.18)], Morse [Eq. (1.19)], and harmonic oscillator [Eq. (1.20)], with the same minimum and curvature at the minimum. The energy is in units of ² and the distance in units of a, the two parameters of the Lennard–Jones potential.
for the parameters deﬁned in Table 1.4. We thus see that the spacing of levels in the Morse potential is smaller than in the corresponding harmonic oscillator, and that it becomes progressively smaller as the index of the levels increases. This is expected from the behavior of the potential mentioned above, and in particular from its asymptotic approach to zero for large distances. Since the Lennard–Jones potential has an overall shape similar to the Morse potential, we expect its energy levels to behave in the same manner. For purely ionic bonding, one assumes that what keeps the crystal together is the attractive interaction between the positively and negatively charged ions, again in a purely classical picture. For the ionic solids with rocksalt, cesium chloride, and zincblende lattices discussed already, it is possible to calculate the cohesive energy which only depends on the ionic charges, the crystal structure, and the distance between ions. This is called the Madelung energy. The main difﬁculty in evaluating this energy is that the summation converges very slowly, because the interaction potential (Coulomb) is long range. In fact, formally this sum does not converge, and any simple way of summing successive terms gives results that depend on the choice of terms. The formal way to treat periodic structures using the concept of reciprocal space, which we will develop in detail in Chapter 2, makes the calculation of the Madelung energy through the Ewald summation trick much more efﬁcient. For an example of the difﬁculties of calculating the Madelung energy in simple cases, see Problem 2. We will revisit this issue in Chapter 4 in much more detail, once we have developed all the methodology for handling the ionic energy contribution accurately and efﬁciently (see Section 4.10). The other types of bonding, metallic, covalent, and mixed bonding, are much more difﬁcult to describe quantitatively. For metallic bonding, even if we think of the electrons as a uniform sea, we need to know the energy of this uniform “liquid” of fermions, which
45
Further Reading
is not a trivial matter. In addition to the electronic contributions, we have to consider the energy of the positive ions that exist in the uniform negative background of the electron sea. This is another Madelung sum, which converges very slowly. As far as covalent bonding is concerned, although the approach we used by combining atomic orbitals is conceptually simple, much more information is required to render it a realistic tool for calculations, and the electron interactions again come into play in an important way. This will also be discussed in detail in subsequent chapters. The descriptions that we mentioned for the metallic and covalent solids are also referred to by more technical terms. The metallic sea of electrons paradigm is referred to as the “jellium” model in the extreme case when the ions (atoms stripped of their valence electrons) are considered to form a uniform positive background; in this limit the crystal itself does not play an important role, other than it provides the background for forming the electronic sea. The description of the covalent bonding paradigm is referred to as the linear combination of atomic orbitals (LCAO) approach, since it relies on the use of a basis of atomic orbitals in linear combinations that make the bonding arrangement transparent, as was explained above for the graphite and diamond lattices. We will revisit these notions in more detail in the following chapters.
Further Reading
1. Solid State Physics , N. W. Ashcroft and N. D. Mermin (Saunders College Publishing, Philadelphia, PA, 1976). This is a comprehensive and indispensable source on the physics of solids; it provides an inspired coverage of most topics that had been the focus of research up to its publication. 2. Introduction to Solid State Theory , O. Madelung (SpringerVerlag, Berlin, 1981). This book represents a balanced introduction to the theoretical formalism needed for the study of solids at an advanced level; it covers both the singleparticle and the manybody pictures. 3. Basic Notions of Condensed Matter Physics , P. W. Anderson (BenjaminCummings Publishing, Menlo Park, CA, 1984). 4. Quantum Theory of Solids , C. Kittel (Wiley, New York, 1963). 5. Solid State Theory , W. A. Harrison (McGrawHill, New York, 1970). 6. Principles of the Theory of Solids , J. M. Ziman (Cambridge University Press, Cambridge, 1972). 7. The Nature of the Chemical Bond and the Structure of Molecules and Solids , L. Pauling (Cornell University Press, Ithaca, NY, 1960). This is a classic treatment of the nature of bonding between atoms; it discusses extensively bonding in molecules but there is also a rich variety of topics relevant to the bonding in solids. 8. Crystal Structures , R. W. G. Wyckoff (Wiley, New York, 1963). This is a very useful compilation of all the structures of elemental solids and a wide variety of common compounds.
46
1
From Atoms to Solids
9. Physics of Solids , E. N. Economou (SpringerVerlag, Berlin, 2010). This is a careful and intuitive introduction to the physics of solids with many useful examples. 10. Condensed Matter Physics , M. P. Marder (Wiley, Hoboken, NJ, 2010). This is a comprehensive and modern treatment of the physics of solids. Problems
1.
An important consideration in the formation of crystals is the socalled packing ratio or ﬁlling fraction. For each of the elemental cubic crystals (simple cubic, FCC, BCC), calculate the packing ratio, that is, the percentage of volume occupied by the atoms modeled as touching hard spheres. For the NaCl and CsCl structures, assuming that each type of ion is represented by a hard sphere and the nearestneighbor spheres touch, calculate the packing ratio as a function of the ratio of the two ionic radii and ﬁnd its extrema and the asymptotic values (for the ratio approaching inﬁnity or zero, that is, with one of the two ions being negligible in size relative to the other one). Using values of the atomic radii for the different elements, estimate the ﬁlling fraction in the actual solids.
2.
The three ionic lattices, rocksalt, cesium chloride, and zincblende, discussed in this chapter are called bipartite lattices, because they include two equivalent sites per unit cell which can be occupied by the different ions so that each ion type is completely surrounded by the other. Describe the corresponding bipartite lattices in two dimensions. Are they all different from each other? Try to obtain the Madelung energy for one of them, and show how the calculation is sensitive to the way in which the inﬁnite sum is truncated.
3.
Consider the singleparticle hamiltonian:
ˆ sp =
H
where p is the momentum operator m the mass of the particle, and
p=
p2 2m
+ V (r)
−ih¯ ∇r
V (r)
the potential energy. Show that the commutator of the hamiltonian with the potential energy term, deﬁned as [Hˆ sp , V (r)] = Hˆ sp V (r) − V (r)Hˆ sp
is not zero, except when the potential is a constant V (r) = V 0. Based on this result, provide an argument to the effect that the energy eigenfunctions can be simultaneous eigenfunctions of the momentum operator only for free particles. 4.
In the example of bond formation in a 1D molecule, using the deﬁnitions of the wavefunctions for the isolated atoms, Eq. (1.14), and the bonding and antibonding states, Eq. (1.15), show that:
47
Problems
(a) The difference in the probability of an electron being in the bonding or antibonding states, rather than in the average of the two isolatedatom wavefunctions, is given by the expression in Eq. (1.16). (b) The change in the potential energy for the combined system versus the two isolated ions, given by Eq. (1.17), is negative for the ψ (+) state and positive for the ψ (−) state (take b = 2.5a and perform a numerical integration). (c) The change in the kinetic energy for the combined system versus the two isolated ions is negative for the ψ (+) state and positive for the ψ (−) state (take b = 2.5a and perform a numerical integration). 5.
Derive the value of the energy of sp 2 and sp 3 hybrids in terms of the values of the energy of the s and p orbitals, ²s and ²p . What are the assumptions that you need to make in order for these expressions to be valid?
6.
Produce an energylevel diagram for the orbitals involved in the formation of the covalent bonds in the water molecule. Provide an argument of how different combinations of orbitals than the ones discussed in the text would not produce as favorable a covalent bond between H and O. Describe how the different orbitals combine to form hydrogen bonds in the solid structure of ice.
7.
Consider a simple excitation of the ground state of the freeelectron system, consisting of taking an electron from a state with momentum k 1 and putting it in a state with momentum k2 ; since the ground state of the system consists of ﬁlled singleparticle states with momentum up to the Fermi momentum k F , we must have k1  ≤k F and k2 > k F. Removing the electron from state k1 leaves a “hole” in the Fermi sphere, so this excitation is described as an “electron–hole pair.” Discuss the relationship between the total excitation energy and the total momentum of the electron–hole pair; show a graph of this relationship in terms of reduced variables, that is, the excitation energy and momentum in units of the Fermi energy ²F and the Fermi momentum k F . (At this point we are not concerned with the nature of the physical process that can create such an excitation and with how momentum is conserved in this process.)
8.
In order to derive the attractive part of the Lennard–Jones potential, we consider two atoms with Z electrons each and ﬁlled electronic shells. In the ground state, the atoms will have spherical electronic charge distributions and, when sufﬁciently far from each other, they will not interact. When they are brought closer together, the two electronic charge distributions will be polarized because each will feel the effect of the ions and electrons of the other. We are assuming that the two atoms are still far enough from each other so that their electronic charge distributions do not overlap, and therefore we can neglect exchange of electrons between them. Thus, it is the polarization that gives rise to an attractive potential; for this reason this interaction is sometimes also referred to as the “ﬂuctuating dipole interaction.”
48
1
From Atoms to Solids
To model the polarization effect, we consider the interaction potential between the two neutral atoms: 2 2
Vint
= R Z−e R  − 1
±
2
i
Ze 2
r(1) i − R2 
−
± j
Ze 2
r(2) j − R1  (1)
+
± ij
e2
(2) r(1) i − rj 
(2)
where R1, R2 are the positions of the two nuclei and ri , rj are the sets of electronic coordinates associated with each nucleus. In the above equation, the ﬁrst term is the repulsion between the two nuclei, the second term is the attraction of the electrons of the ﬁrst atom to the nucleus of the second, the third term is the attraction of the electrons of the second atom to the nucleus of the ﬁrst, and the last term is the repulsion between the two sets of electrons in the two different atoms. The summations over i, j run from 1 to Z . From secondorder perturbation theory, the energy change due to this interaction is given by: ³E
=³´0(1) ´0(2) Vint ´0(1) ´0(2) ´ ½ ½2 ± + E −1 E ½½³´0(1)´0(2)Vint ´n(1)´m(2)´½½ nm
(1)
0
(1.23)
nm
(2)
where ´0 , ´0 are the groundstate manybody wavefunctions of the two atoms, (1) (2) ´ n , ´m are their excited states, and E 0 , E nm are the corresponding energies of the twoatom system in their unperturbed states. We deﬁne the electronic charge density associated with the ground state of each atom through: (I )
n0 (r)
=Z =
² ½ ½2 ½ (I ) ½ ´ ( r , r , r , ..., r ) ½ 0 2 3 Z ½ d r2d r3 · · d r· Z
Z ² ± i=1
δ (r
½
½2
− ri ) ½½´0(I) (r1 , r2 , ..., rZ )½½
d r1d r2 ·
(1.24)
· d r· Z
with I = 1, 2 (the expression for the density n(r) in terms of the manybody wavefunction ´ ´ is discussed in detail in Appendix C). Show that the ﬁrstorder term in ³ E corresponds to the electrostatic interaction energy between the charge ( r), n(2) (r). Assuming that there is no overlap between these density distributions n(1) 0 0 two charge densities, show that this term vanishes (the two charge densities in the unperturbed ground state are spherically symmetric). The wavefunctions involved in the secondorder term in ³E will be negligible, unless the electronic coordinates associated with each atom are within the range of nonvanishing charge density. This implies that the distances r(1) i − R1 and (2) rj − R2 should be small compared to the distance between the atoms R2 − R1 , which deﬁnes the distance at which interactions between the two charge densities
49
Problems
become negligible. Show that expanding the interaction potential in the small (1) (2) quantities  ri − R1 / R2 − R1  and  rj − R2 / R2 − R1  gives, to lowest order: e2
− R − R  2 1 e2
+ R − R  2 1
(2) ± (r(1) (rj − R2) · (R2 − R1) i − R1 ) · (R2 − R1)
3
·
(R2 − R1 )2
ij
(R2 − R1 )2
(2) ± (r(1) i − R1 ) · (rj − R2)
(1.25)
(R2 − R1 )2
ij
Using this expression, show that the leadingorder term in the energy difference ³E behaves like  R2 − R1 −6 and is negative. This establishes the origin of the attractive term in the Lennard–Jones potential. 9.
We wish to determine the eigenvalues of the Morse potential, Eq. (1.19). One method is to consider an expansion in powers of (r − r 0 ) near the minimum and relate it to the harmonic oscillator potential with higherorder terms. Speciﬁcally, the potential V( r)
= 21 m ω 2(r − r 0 )2 − α(r − r 0 )3 + β (r − r 0)4
has eigenvalues ²n
= (n +
where γ
3
= 2 hω ¯
¶
(1.26)
¹
1 1 )h¯ ω 1 − γ (n + ) 2 2
·
¯
h
¸2 ¾
mω
5 α2 2 m ω2
−β
¿
First, check to what extent the expansion (1.26) with up to fourthorder terms in (r − r 0 ) is a good representation of the Morse potential; what are the values of α and β in terms of the parameters of the Morse potential? Use this approach to show that the eigenvalues of the Morse potential are given by Eq. (1.22). 10.
An important simple model that demonstrates some of the properties of electron states in inﬁniteperiodic solids is the socalled Kronig–Penney model.14 In this model, a particle of mass m experiences a 1D periodic potential with period a :
= 0, 0 < x < (a − l ) = V0 , (a − l) < x < a V (x + a ) = V (x) V (x )
where we will take V0
>
0. The wavefunction ψ (x ) obeys the Schr¨odinger equation
¾
−¯
h2 d 2
2m dx 2
+ V (x)
¿
ψ (x)
14 R. de L. Kronig and W. G. Penney, Proc. Roy. Soc. (London), A
= ²ψ ( x)
130 , 499 (1931).
50
1
From Atoms to Solids
(a) Choose the following expression for the particle wavefunction: ψ (x )
= ei kx u(x )
and show that the function u(x ) must obey the equation d2 u(x ) dx 2
+ 2ik dud(xx)
¶
2m V (x )
2m ²
¹
+ 2 u (x ) = 0 h¯ ¯ Assuming that u (x) is ﬁnite for x → ±∞ , the variable k must be real so that the −
k
2
−
h2
wavefunction ψ (x ) is ﬁnite for all x. (b) We ﬁrst examine the case ² > V0 > 0. Consider two solutions u 1(x ), u2 (x ) for the ranges 0 < x < (a − l ) and (a − l) < x < a , respectively, which obey the equations d2u 1 (x) dx 2
+ 2ik dud1x(x ) − [k 2 − κ 2]u 1( x) = 0,
0 0 and (² − V0 ) equations can be written as:
À
( a − l)
0. Show that the solutions to these
−k)x + d 1 e−i(κ +k)x , 0 < x < (a − l)
u1 (x )
= c 1ei(
u2 (x )
= c 2 ei( −k)x + d 2 e−i( +k)x ,
κ
r c ; this is known as the cutoff function. In this case, consistency requires that we adopt a similar expression for the hamiltonian matrix elements: tµν
= f (r ij)tmj,li(r ij)
(2.92)
which are cut off for r > rc by the same function f (r ). The larger r c is, the more matrix elements we will need to calculate (or ﬁt), and the approximation becomes more computationally demanding. Multicenter Integrals
The formulation of the TBA up to this point assumed that the TBA hamiltonian matrix elements depend only on two singleparticle wavefunctions centered at two different atomic sites. For example, we assumed that the hamiltonian matrix elements depend only on the relative distance and orientation of the two atomiclike orbitals between which we calculate the expectation value of the singleparticle hamiltonian. This is referred to as the twocenter approximation, but it is obviously another implicit approximation, on top of restricting the basis to the atomiclike wavefunctions. In fact, it is plausible that in the environment of the solid, the presence of other electrons nearby will affect the interaction of any two given atomiclike wavefunctions. In principle, we should consider all such interactions. An example of such terms is a threecenter matrix element of the hamiltonian in which one orbital is centered at some atomic site, a second orbital at a different atomic site, and a term in the hamiltonian (the ionic potential) includes the position of a third atomic site. One way of taking into account these types of interactions is to make the hamiltonian matrix elements environment dependent. In this case, the value of a twocenter hamiltonian matrix element, involving explicitly the positions of only two atoms, will depend on the position of all other atoms around it and on the type of atomic orbitals on these other atoms. To accomplish this, we need to introduce more parameters to allow for the ﬂexibility of having several possible environments around each twocenter matrix element, making the approach much more complicated. The increase in realistic representation of physical systems is always accompanied by an increase in complexity and computational cost. ExcitedState Orbitals in Basis
Finally, we can consider our basis as consisting not only of the valence states of the atoms, but including unoccupied (excited) atomic states. This is referred to as going beyond the minimal basis. The advantages of this generalization are obvious, since including more
99
2.6
General BandStructure Methods
basis functions always gives a better approximation (by the variational principle). This, however, presents certain difﬁculties: the excited states tend to be more diffuse in space, with tails extending farther away from the atomic core. This implies that the overlap between such states will not fall off fast with distance between their centers, and it will be difﬁcult to truncate the nonorthogonal overlap matrix and the hamiltonian matrix at a reasonable distance. To avoid this problem, we perform the following operations. We orthogonalize ﬁrst the states in the minimal basis. This is accomplished by diagonalizing the nonorthogonal overlap matrix and using as the new basis the linear combination of states that corresponds to the eigenvectors of the nonorthogonal overlap matrix. Next, we orthogonalize the excited states to the states in the orthogonal minimal basis, and ﬁnally we orthogonalize the new excited states among themselves. Each orthogonalization involves the diagonalization of the corresponding overlap matrix. The advantage of this procedure is that with each diagonalization, the energy of the new states is raised (since they are orthogonal to all previous states), and the overlap between them is reduced. In this way we create a basis that gives rise to a hamiltonian which can be truncated at a reasonable cutoff distance. Nevertheless, the increase in variational freedom that comes with the inclusion of excited states increases the computational complexity, since we will have a larger basis and a correspondingly larger number of matrix elements that we need to calculate or obtain from ﬁtting to known results. This extension is suggestive of a more general approach: we can use an arbitrary set of functions centered at atomic sites to express the hamiltonian matrix elements. A popular set is composed of normalized gaussian functions (see Appendix A) multiplied by the appropriate spherical harmonics to resemble a set of atomiclike orbitals. We can then calculate the hamiltonian and overlap matrix elements using this set of functions and diagonalize the resulting secular equation to obtain the desired eigenvalues and eigenfunctions. To the extent that these functions represent accurately all possible electronic states (if the original set does not satisfy this requirement we can simply add more basis functions), we can then consider that we have a variationally correct description of the system. This is the more general LCAO method. It is customary in this case to use an explicit form for the singleparticle hamiltonian and calculate the hamiltonian and overlap matrix elements exactly, either analytically, if the choice of basis functions permits it, or numerically. The number of basis functions is no longer determined by the number of valence states in the constituent atoms, but rather by variational requirements.
2.6
General BandStructure Methods
Since the early days of solidstate theory, a number of approaches have been introduced to solve the singleparticle hamiltonian and obtain the eigenvalues (band structure) and eigenfunctions. These methods were the foundation on which modern approaches for electronic structure calculations have been developed. We review the basic ideas of these methods next.
100
2
Electrons in Crystals: Translational Periodicity
Cellular or linearized mufﬁntin orbital (LMTO) method : This approach, originally 4 developed by Wigner and Seitz, considers the solid as made up of cells (the Wigner–Seitz or WS cells), which are the realspace analog of the Brillouin zones; a simple example is shown in Fig. 2.25 for a 2D hexagonal lattice. In each cell, the potential felt by the electrons is the Coulomb potential of the atomic nucleus, which is spherically symmetric around the nucleus. However, the boundaries are those of the WS cell, whose shape is dictated by the crystal. Due to the Bloch character of wavefunctions, the following boundary conditions must be obeyed at the boundary of the WS cell denoted by rb :
= e−i k·Rψk(rb + R) nˆ (rb) · ∇ψk (rb) = − e−ik ·R nˆ (rb + R) · ∇ψk (rb + R) ψk (rb)
(2.93)
where nˆ ( rb ) is the vector normal to the surface of the WS cell at rb ; the minus sign on the righthand side of the second equation is a consequence of the convention that the surface normal vector always points outward from the volume enclosed by the surface. Since the potential inside the WS cell is assumed to be spherical, we can use the standard expansion in spherical harmonics Y lm(rˆ ) and radial wavefunctions φkl (r ) (for details see Appendix C) which obey the following equation:
¼
− 2¯m
Â
h2 e
d2 dr 2
+
2 d r dr
Ã
+ V (r ) + r+2 1) l(l
½
φk (r )
= ±kφk(r )
(2.94)
where the dependence of the radial wavefunction on k enters through the eigenvalue ±k . In terms of these functions, the crystal wavefunctions become: ψk (r)
=
µ lm
ˆ
α klm Y lm (r)φkl (r )
(2.95)
Taking matrix elements of the hamiltonian between such states creates a secular equation which can be solved to produce the desired eigenvalues. Since the potential cannot be truly spherical throughout the WS cell, it is reasonable to consider it to be spherical within a sphere which lies entirely within the WS, and to be zero outside that sphere. This gives rise to a potential that looks like a mufﬁntin, hence the name of the method. This method is used for calculations of the band structure of complex solids. The basic assumption of the method is that a spherical potential around the nuclei is a reasonable approximation to the true potential experienced by the electrons in the solid. Augmented plane wave (APW) method : This method, introduced by J. C. Slater,5 consists of expanding the wavefunctions in plane waves in the regions between the atomic spheres, and in functions with spherical symmetry within the spheres. Then the two expressions must be matched at the sphere boundary so that the wavefunctions and their ﬁrst and second derivatives are continuous. For core states, the wavefunctions are essentially unchanged within the spheres. It is only valence states that have signiﬁcant weight in the regions outside the atomic spheres.
4 E. Wigner and F. Seitz, Phys. Rev. 43, 804 (1933). 5 J. C. Slater, Phys. Rev. 51, 846 (1937).
101
2.6
General BandStructure Methods
y
y
x
x
a
Fig. 2.25
Left: Illustration of the Wigner–Seitz cell for a 2D hexagonal lattice, shown as a shaded hexagon around each atom (blue circle). The periodicity (red arrows) is captured as boundary conditions on the wavefunctions at the edges of the WS cell. Right: Illustration of the mufﬁntin potential, in which a region (greenshaded area) around each atom represents the atomiclike spherical potential and the rest of the space is at a constant potential (white). The red arrows are the primitive lattice vectors of the lattice.
Both the LMTO and the APW methods treat all the electrons in the solid, that is, valence as well as core electrons. Accordingly, they are referred to as “allelectron” methods. The two methods share the basic concept of separating space in the solid into the spherical regions around the nuclei and the interstitial regions between these spheres. In the APW method, the spheres are touching while in the LMTO method, they are overlapping. In many cases, especially in crystal structures other than the closepacked ones (FCC, HCP, BCC), this separation of space leads to inaccuracies, which can be corrected by elaborate extensions described as “full potential” treatment. There is also an allelectron electronic structure method based on multiple scattering theory known as the Korringa– Kohn–Rostocker (KKR) method. A detailed exposition of these methods falls beyond the scope of this book; they are discussed in specialized articles or books (see for example the book by D. Singh),6 often accompanied by descriptions of computer codes which are necessary for their application. In the remainder of this section we will examine other band structure methods in which the underlying concept is a separation between the electronic core and valence states. This separation makes it possible to treat a larger number of valence states, with a relatively small sacriﬁce in accuracy. The advantage is that structures with many more atoms in the unit cell can then be studied efﬁciently. Orthogonalized plane wave (OPW) method : This method, due to C. Herring,7 is (v) an elaboration on the APW approach. The basis states φk µ for expanding the valence wavefunctions are written at the outset as a combination of plane waves and core states:
µ
φk(v) µ =kµ +
c±
(c± )
βk
6 D. Singh, Planewaves, Pseudopotentials and the LAPW Method 7 C. Herring, Phys. Rev. 57 , 1169 (1940).
±
ψk(c )µ
(2.96)
(Kluwer Academic, Boston, MA, 1994).
102
2
Electrons in Crystals: Translational Periodicity
where k µ represents a plane wave of wavevector k and ψk(c) (r)µ are Bloch states formed out of core states:
µ
ψk(c) µ =
R
eik· R φR
(c )
µ
(2.97)
with  µ a core state centered at R. In essence, we are assuming that the core states φ(c) (r) can easily be obtained at the level of individual atoms, and that they do not change when the atoms are in the crystal environment, a reasonable approximation. We can then use those core states in a Bloch sum to construct the appropriate electronic states in the crystal that correspond to core electrons. For the valence states, we created a basis which, in addition to core states, includes plane waves. With the choice of the parameters (c ) φR
(c)
βk
= −´ψk(c) kµ
(v)
we make sure that the basis functions φk (r) are orthogonal to the core Bloch states:
µ
±
±
´φk(v) ψk(c) µ = k´ψk(c) µ − ´kψk(c ) µ´ψk(c ) ψk(c) µ =0
(2.98)
c±
(c± )
where we have used ´ψk ψk µ =δcc± to reduce the sum to a single term. We can then use these states as the basis for the expansion of the true valence states: (c)
µ
ψk(v) µ =
G

(v)
α k (G) φk G
+
µ
(2.99)
Taking matrix elements between such states produces a secular equation which can be diagonalized to obtain the eigenvalues of the energy. Pseudopotential plane wave (PPW) method : We can manipulate the expression in the last equation to obtain something quite interesting. First notice that:
µ
ψk(c+) Gµ = and with this, we obtain:
µ
ψk(v) µ = =
¼
αk (G)
G
Â µ
R
ei(k+ G)· R φR
(c )
k + Gµ − ´ψk(c+) G k + Gµψk(c+) Gµ
k + Gµ −
G
(2.100)
µ
Ã
α k (G)
µ =ψk(c )µ
c
µ c
´
(c) ψk

Â µ
½ Ã
k + Gµ ψk(c)µ
αk ( G)
G
which, with the deﬁnition
µ
φ˜ k(v)µ = can be rewritten as:
G
ik ·r
µ
V
G
k + Gµ →φ˜k(v) (r) = e√
α k (G)
µ
α k (G)e
ψk(v)µ = φ˜k(v) µ − ´ψk(c) φ˜ k(v)µψk(c) µ c
iG·r
(2.101)
(2.102)
103
2.6
General BandStructure Methods
This is an interesting expression, because it tells us that we can express the true valence (v) (v) wavefunctions ψk in terms of the auxiliary functions φ˜ k from which the overlap with the core states has been subtracted out. These are known as “pseudowavefunctions” and they obey a singleparticle Schr¨odinger equation with a modiﬁed potential, known as the “pseudopotential,” ﬁrst introduced by Phillips and Kleinman8 (see also Chapter 4, (v) Section 4.9, for a more extensive discussion). Notice that the pseudowavefunction φ˜ k (r) is given as an expansion over plane waves only, Eq. (2.101), while it involves exactly the (v) same coefﬁcients αk (G) as the true valence wavefunction ψk (r). This implies that ﬁnding (v) these coefﬁcients by solving the appropriate equation obeyed by φ˜ k (r) is equivalent to solving the full problem for the original valence wavefunction; the advantage of dealing (v) (v) with φ˜k rather than with ψk is that the former is quite simple, since it only involves plane waves. The concepts of the pseudowavefunction and the pseudopotential are very important for realistic calculations in solids, and we will return to them in Chapter 4, where a more thorough justiﬁcation of these ideas and their applications will be presented. 2.6.1
Crystal Pseudopotentials
Having developed pseudopotentials for individual atoms, we return to the discussion of valence electron states in crystals. The crystal potential that the pseudowavefunctions experience is given by:
˜ xtl (r) =
V
µ R,i
˜ ion(r − ti − R)
(2.103)
V
where V˜ ion (r − ti ) is the pseudopotential of a particular atom in the unit cell, at position ti . We can expand the crystal pseudopotential in the planewave basis of the reciprocal lattice vectors:
˜ xtl (r) = µ V˜ xtl (G)eiG·r
(2.104)
V
G
It turns out that the pseudopotential is much smoother than the true Coulomb potential of the ions, and therefore we expect its Fourier components V˜ xtl (G) to fall fast with the magnitude of G. To simplify the situation, we will assume that we are dealing with a solid that has several atoms of the same type in each unit cell; this is easily generalized to the case of several types of atoms. Using the expression from above in terms of the atomic pseudopotentials, the Fourier components take the form (with NV PUC the volume of the crystal):
˜ xtl (G) = V
´
1 NV PUC
1 µ
=N
R,i
˜ xtl (r)e−iG·r dr = µ V
ei G·ti
¶
1 V PUC
´
R,i
´
1 NV PUC
˜ ion (r − ti − R)e−iG·r dr
V
·
˜ ion (r)e−iG·r dr = V˜ ion(G) µ ei G·t
V
8 J. C. Phillips and L. Kleinman, Phys. Rev. 116, 287 (1959).
i
i
(2.105)
104
2
Electrons in Crystals: Translational Periodicity
where we have eliminated a factor of N (the number of PUCs in the crystal) with a ∑ summation R , since the summand at the end does not involve an explicit dependence on R. We have also deﬁned the Fourier transform of the atomic pseudopotential V˜ at (G) as the content of the square brackets in the nexttolast expression in the above equation. The sum appearing in the last step of this equation: S (G)
=
µ
eiG·ti
(2.106)
i
is called the “structure factor.” Depending on the positions of atoms in the unit cell, this summation can vanish for several values of the vector G. This means that the values of the crystal pseudopotential for these values of G are not needed for a bandstructure calculation. From the above analysis, we conclude that relatively few Fourier components of the pseudopotential survive, since those corresponding to large G are negligible because of the smoothness of the pseudopotential, whereas among those with small  G , several may be eliminated due to vanishing values of the structure factor S (G). The idea then is to use a basis of plane waves exp(iG · r) to expand both the pseudowavefunctions and the pseudopotential, which will lead to a secular equation with a relatively small number of nonvanishing elements. Solving this secular equation produces the eigenvalues (band structure) and eigenfunctions for a given system. To put these arguments in quantitative form, consider the singleparticle equations which involve a pseudopotential (we neglect for the moment all the electron interaction terms, which are anyway isotropic; the full problem is considered in more detail in Chapter 4):
¼
½
− 2¯m ∇ 2 + V˜ xtl (r) φ˜ (kn) (r) = ±k(n) φ˜k(n)(r) h2
e
(2.107)
These must be solved by considering the expansion for the pseudowavefunction in terms of plane waves, Eq. (2.101). Taking matrix elements of the hamiltonian with respect to planewave states, we arrive at the following secular equation:
µ G±
ˆ sp (G, G± )αk(n)(G± ) = ±k(n)α(kn) (G)
Hk
(2.108)
ˆ sp , which contains the ionic where the matrix elements of the singleparticle hamiltonian H pseudopotential V˜ ion, are given by: ˆ sp (G, G± ) = h¯
Hk
2
(k + G)2 ± ˜ ion(G − G±) S (G − G± ) δ (G − G ) + V 2m e
(2.109) (n )
Diagonalization of the hamiltonian matrix gives the eigenvalues of the energy ±k and (n ) corresponding eigenfunctions φ˜ k (r). Obviously, Fourier components of V˜ ion(r) which are multiplied by vanishing values of the structure factor S (G) will not be of use in the above equation.
105
2.7
2.7
Localized Wannier Functions
Localized Wannier Functions
Up to this point we have emphasized the description of the singleparticle states for electrons in terms of planewavelike functions ψk(n) (r), or “band states,” which are delocalized. Often, it is desirable to use localized states to describe the electrons, especially when we want to determine the effect of localized perturbations on the properties of the solid. These localized states are referred to as “Wannier functions.” There is a onetoone correspondence between such states and the delocalized wavelike states with which we are familiar. We derive these relations here and comment on the usefulness of the localized (n ) states. We denote as φR (r) the Wannier function that is localized in the unit cell deﬁned by the Bravais lattice vector R. We deﬁne the Wannier functions as follows: (n )
φR
(r) =
µ
√1
N
k
e−ik ·R ψk (r) (n )
(2.110)
We can obtain the band states from the Wannier functions by a similar linear transformation, namely: 1 µ i k·R ± (n) (n ) ψk (r) = √ e φR ± (r) (2.111) N
R±
To show that the two transformations are equivalent, we begin with the last expression and multiply both sides by e−ik ·R and sum over all k:
µ −ik ·R (n) 1 µ −i k·R µ (n) i k·R ± e φ ± (r)e e ψ (r) = √ k
k
N
R±
k
R
µ µ −ik ·(R−R± ) (n) e φ ± (r)
= √1
N
k
R±
R
In the last expression, the sum of the complex exponentials over all values of k gives a δ function in the lattice vectors: 1 µ −i k·(R−R ± ) e
N
k
= δ(R − R± )
which, with the summation over R± , produces the desired relation, that is, Eq. (2.110). Similarly, we can show straightforwardly that the Wannier functions are orthonormal:
´φR(m± ) φR(n) µ =N1 = N1
µ −ik· R −ik± · R± (m ) (n) e e ´ψ ±  ψ µ kk±
k
k
µ −ik· R ik± · R± ± e e δkk± δ mn = δ (R − R )δmn kk±
where we have used the orthonormality of the band states, ´ψk±  ψk µ =δkk± δ mn . We discuss next some interesting aspects of the Wannier functions. The ﬁrst one has to do with the degree of localization of Wannier functions. Using our familiar expression for the Bloch function: µ −i k·R (n) ik ·r (n ) (n) i k·r ψk (r) = u k (r)e ⇒ φR(n)(r) = √1 e u k (r)e (m )
N
k
(n)
106
2
Electrons in Crystals: Translational Periodicity
and taking u (kn)(r) ≈ u(0n)(r) to be approximately independent of k : (n ) φR (r)
(n)
u 0 (r) µ
= √
N
k
e−ik ·R eik· r ∝
´
k∈BZ
e−ik ·(R−r) dk
with the integration over k in the ﬁrst BZ, which has a typical radius of k max ∼ π/a, where a is the lattice constant. This last integral then, assuming spherically symmetric BZ, gives:
´
k∈BZ
´
e−ik ·(R−r) dk ∝
kmax
0
k2
e−ik R−r − eik R−r −ik R − r dk
∝ R −1 r2
where we have neglected numerical factors to obtain the qualitative dependence of the (n ) integral on R − r. The last expression shows that the Wannier function φr (r) is reasonably localized around the position R of the unit cell. A much better degree of localization can be obtained by taking advantage of the fact that the Bloch functions can include an arbitrary phase ϕn(k ): (r) = eiϕ n(k) uk (r)ei k·r
(n)
(n )
ψk
This freedom in the deﬁnition of the Bloch function can be exploited to produce the socalled “maximally localized Wannier functions,” as originally proposed by N. Marzari and D. Vanderbilt. 9 These functions have found wide use in understanding the results of electronic structure calculations in a more physically transparent manner. The second aspect is the usefulness of the Wannier functions in dealing with localized perturbations of the crystal lattice. Suppose we have the hamiltonian Hˆ sp that includes ˆ sp0 , which is the familiar ideal crystal and a weak, localized, timedependent the part H perturbation potential:
ˆ sp = Hˆ 0sp + V (r, t)
H
(n )
We can then use the Wannier functions of the unperturbed hamiltonian, φR ( r), as the basis to express the solution of the timedependent Schr¨odinger equation for the full hamiltonian:
ˆ sp ψ (r, t ) = ih¯ ∂ ψ ( r, t),
H
∂t
ψ (r, t )
=
µ n,R
(n )
(n)
c R (t )φR (r)
(2.112)
Inserting the expression for ψ (r, t ) in the timedependent Schr¨odinger equation and multiplying both sides by φ∗R(±m )(r) and integrating over r we obtain:
µ n,R
(n )
(n)
(m)
µ ´φ(Rm± ) Hˆ 0sp + V (r, t)φ(Rn) µ =i h¯ ∂ c ∂Rt (t ) ´φR(m± )φ(Rn) µ =i h¯ ∂ c R∂±t (t)
c R ( t)
n ,R
where we have taken advantage of the orthogonality of Wannier functions, namely:
´φ(Rm± )φR(n)µ =δ(R − R± )δmn
9 N. Marzari and D. Vanderbilt, Phys. Rev. B , 56 , 12847 (1997).
107
2.8
Density of States
Using the Bloch eigenfunctions of Hˆ 0 , ψk(n) (r), their eigenvalues ±k(n) , and their relation to sp
the Wannier functions,
ˆ sp
(n )
H0 φ R
(r) =
√1
N
(n )
φR
(r), in the above equation we arrive at:
µ −i k·R (n) (n) e ± ψ ( r) ⇒ k
k
k
´R(m± ) Hˆ sp0 φR(n)µ =N1
φ
µ −ik ·(R−R ± ) (n) e ± δ k
k
mn
(m)
The earlier equation for the time derivative of c R± (t) then becomes: ih¯
∂c
(m) (t ) R± ∂t
µ
=
n ,R
(n)
c R (t)
º
(n ) R −R±
δ mn ±
»
(nm) + VRR ± (t)
(2.113)
with the deﬁnitions ±
(n) R−R ±
= N1
µ k
(n )
±k
±
e−ik ·(R−R ),
V
(nm) (t ) RR±
= φ´ (Rm± )V(r, t )φR(n) µ
Equation (2.113) for the time evolution of the expansion coefﬁcients is a useful expression for a perturbing potential V ( r, t) that is well localized, because then very few matrix (nm ) elements VRR ± (t ) survive, since the Wannier functions are also well localized. The resulting (n )
system of a few coupled equations for the time evolution of the coefﬁcients cR (t) can easily be solved. If instead we had used the Bloch states of the unperturbed hamiltonian to express the wavefunction ψ (r, t), we would need to employ a very large number of coupled equations to solve for the time evolution of the system, since a localized perturbation like V (r, t) would require a large number of Fourier components, the matrix elements ´ψk(m± ) V( r, t)ψk(n) µ, for its accurate representation.
2.8
Density of States
An important feature of the electronic structure of a solid is the density of electronic states as a function of the energy. This is a key quantity in describing many of the electrical and optical properties of solids. This is the quantity measured experimentally in a number of situations, like in tunneling experiments or in photoemission and inverse photoemission experiments. The density of states, g (± ), for energies in the range [±, ± + d±] is deﬁned as the sum over all states labeled by n with energy ±n in that range, per volume V of the system: g(± )d±
= V1
µ n, ±n ∈ [± ,± +d± ]
1 ⇒ g (± ) =
1 µ V
n
δ (±
− ± n)
(2.114)
where the last expression is obtained by taking the limit d± → 0, in which case the unit under the sum is replaced by a δ function in the energy ±, centered at the value ±n . The units of the density of states g( ±) are 1/[Energy][Volume ]. The index of the energy states n can take the usual expressions, for example, a set of discrete values for a ﬁnite system, the momentum p = h¯ k for a system of free particles with eigenstates ±k , or the crystal
108
2
Electrons in Crystals: Translational Periodicity
momentum k in the ﬁrst BZ. The case of eigenstates characterized by a twocomponent wavevector k = (kx , ky ) and parabolic bands
= h¯2mk∗ 2
±k
2
is illustrated in Fig. 2.26. We will examine the other cases in more detail below.
Example 2.8 Tunneling at metal–semiconductor junction To give an example of how the density of states appears in expressions that are related to physically measurable quantities, we discuss tunneling at a contact between a metal and a semiconductor which has a band gap ±gap . For an intrinsic semiconductor without any impurities, the Fermi level will be in the middle of the band gap (see Chapter 5). At equilibrium the Fermi level on both sides of the contact must be the same. When a voltage bias V b is applied to the metal side, all its states are shifted by +eV b . In general, the current ﬂowing from side 2 to side 1 of a contact will be given by: I 2→1
º
µ
= − Tkk± 2 1 − fk(1) kk±
»
(2)
(2.115)
f k±
where Tkk± is the tunneling matrix element between the relevant singleparticle states (1) (2) and f k , f k± are the Fermi occupation numbers on each side. The overall minus sign comes from the fact that the expression under the summation accounts for electrons transferred from side 2 to 1, whereas the standard deﬁnition of the current involves transfer of positive charge. We will assume that, to a good approximation, the tunneling matrix elements are independent of k, k ± . We can turn the summations over k and k± into integrals over the energy, but this requires careful handling of the number of available states: speciﬁcally, we must take into account the number of available states at each inﬁnitesimal energy interval [±, ± + d± ], which arises from all the states with wavevectors k whose energy lies in this interval. This quantity is deﬁned as the DOS g (± ); the situation we are discussing is illustrated in Fig. 2.27.
k
+d
ky
0
g(
)
kx Fig. 2.26
Illustration of the calculation of the density of states: states with energy in the range ±k ∈ [± , ± + d± ], which include all states with k values in the shaded ring on the (kx , ky ) plane, contribute to the value of g(± ). When the bin size d ± → 0, g(± ) becomes a smooth function of ± (solid black line).
109
2.8
Density of States
With these assumptions, applying the above expression for the current to the semiconductor–metal contact (with each side now identiﬁed by the superscript (S) or (M) for semiconductor and metal, respectively) we obtain: I M→S
= −T 2
I S→M
= −T 2
´ ∞ ´−∞ ∞
−∞
g
(S)
º
»
(±) 1 − f (S) (±) g (M)(± − eV b)f (M)(± − eV b)d±
g (S) (±)f (S) (±)g (M) (±
º
»
− eV b ) 1 − f (M) (± − eV b )
d±
where we have also taken the metal side to be under a bias voltage V b , so that at a given energy ± the density of states sampled is g (M) (± − eV b). Subtracting the two expressions to obtain the net current ﬂowing through the contact we ﬁnd: I
= −T 
2
´ ∞
−∞
g
(S)
º
»
(± )g(M) (± − eV b ) f (S) (±) − f (M)(± − eV b) d±
(2.116)
We will assume that the gap is sufﬁciently small to consider the DOS in the metal as being approximately constant over a range of energies at least equal to ±gap around
Metal
Semiconductor
Conduction gap
F
Valence
g (M) Fig. 2.27
g (S)
0 0
Illustration of the simple model for tunneling between a metal (left side) and a semiconductor (right side).
the Fermi level. What is usually measured experimentally is the socalled differential conductance, given by the derivative of the current with respect to applied voltage: dI dV b
= T 
2
´ ∞
−∞
g
(S)
(± )g
(M)
(± − eV b)
¶
∂f
(M)
(± − eV b) ∂ Vb
· d±
(2.117)
where we have taken g(M) (± − eV b ) to be independent of V b in the range of order ± gap around the Fermi level, consistent with our assumption about the behavior of the metal DOS. At zero temperature the Fermi occupation number has the form: f (M)(± )
= 1 − θ (± − ±F)
110
2
Electrons in Crystals: Translational Periodicity
where θ (± ) is the Heavyside stepfunction and therefore its derivative is a δ function (see Appendix A): ∂f
(M)
(± − eV b ) ∂ Vb
(M)
±
= −e ∂ f ∂ ± (± ± ) = e δ(±± − ±F )
where we have introduced the auxiliary variable ± ± = ± − eV b. Using this result in the expression for the differential conductance we ﬁnd:
¶
dI dV b
·
T =0
= e T 2 g(S)(±F + eV b)g (M) (±F )
(2.118)
which shows that by scanning the voltage V b , one samples the DOS of the semiconductor. Thus, the measured differential conductance will reﬂect all the features of the semiconductor DOS, including the gap. 2.8.1
FreeElectron Density of States
To illustrate the calculation of the DOS for real systems, we consider ﬁrst the freeelectron model in three dimensions. Since the states are characterized by their wavevector k , we simply need to add up all states with energy in the interval of interest. Taking into account the usual factor of 2 for spin degeneracy and applying the general expression of Eq. (2.114), we get: (3D) g FE (±)d±
µ
1
=V
k ,±k ∈[±,± +d± ]
2=
´
2 (2π )3
±k
∈[± ,±+d± ]
dk =
1 π2
k 2 dk
(2.119)
where we used spherical coordinates in kspace to obtain the last result as well as the fact that in the freeelectron model the energy does not depend on the angular orientation of the wavevector:
= h¯2mk ¶⇒ k dk = m2e d±, e h¯ 2
±k
for ±k ∈ [±, ± dimensions:
2
k
=
¸
2m e ±
¹ 1/2
¯
h2
(2.120)
+ d±]. These relations give, for the DOS in this simple model in three (3D)
g FE (± )
= 2π1 2
¸
2m e
¹3/2 ±
¯
h2
1/2
(2.121)
To facilitate comparison, we deﬁne ﬁrst a length scale a (which could be, for example, the lattice constant of a crystal), and in terms of this an energy scale ±˜ : 2 ˜ = 2mh¯ a 2
±
(2.122)
e
in terms of which the DOS in three dimensions becomes: (3D)
gFE (± )
± ²1/2
= 2π1 2 ±˜1a3 ±±˜
which has the dimensions of number of states per energy per volume.
(2.123)
111
2.8
3D
Density of States
2D
0D
1D
~(±−±0)1/2
0 Fig. 2.28
g(3D) FE
0
0
(2D) gFE
g(1D) FE
0
g(0D) FE
Illustration of the behavior of the DOS as a function of the energy ± , in the freeelectron model in three, two, one, and zero dimensions; the shapes in gray indicate schematically a 3D, 2D, 1D, and 0D (ﬁnite size) solid (the arrows show the directions in which the solid in each case extends to macroscopic size).
By analogous arguments we ﬁnd that in two and one dimensions the corresponding densities of states are given by: (2D)
gFE (± )
= π1
¸
me
¹
¯
h2
± ²0
= 21π ±˜ a12 ±±˜
(2.124)
which has the dimensions of number of states per energy per area, and (1D)
gFE (±)
= π1
¸
2m e
¯
h2
¹1/ 2 ±
± ² −1/2 = 1 1 ± −1/ 2
˜
π ±a
˜
±
(2.125)
which has the dimensions of number of states per energy per length. Finally, for a structure which is ﬁnite in all dimensions, that can be considered a 0D structure, the energy spectrum consists of discrete energy levels and the corresponding DOS consists of a series of δ functions at the values of the energy levels, with dimensions of number of states per energy. As is evident from these expressions, the dependence of the DOS on energy is a very strong function of dimensionality, as illustrated in Fig. 2.28. 2.8.2
Local Density of States
For systems where the electrons are localized, as opposed to the uniform density of the freeelectron model, an important concept is the “localized density of states” or “projected density of states” (PDOS). This concept makes it possible to resolve the total density into components related to speciﬁc local orbitals in the system. This becomes intuitively clear in cases where the basis for expanding electronic states consists of localized orbitals, hence the term “localized density of states,” as in the case of the tightbinding approximation or the Wannier functions. In such situations, suppose that the state ψnµ can be expressed in
112
2
Electrons in Crystals: Translational Periodicity
the basis of the orthonormal localized orbitals  φiµ:
µ
ψnµ =
i
(n )
ci
µ
φi µ, ´φj φi µ =δij ⇒ ψ´ nψn µ = c (i n)2 = 1 i
Inserting the last expression in the deﬁnition of the density of states g(± ) we get: g(± )
1µ
=V
δ (±
n
− ±n )
µ i
¼ µ 1µ
c(i n) 2 =
V
i
n
½
c (i n)2δ( ± − ±n ) =
µ
gi (± )
i
where we have deﬁned the PDOS, g i (± ), corresponding to the orbital φi µ, as: g i (±)
= V1
µ n
c (i n) 2 δ(± − ±n)
(2.126)
This quantity gives the density of states at the value ± that is related to the speciﬁc orbital φi µ in the basis. 2.8.3
Crystal DOS: Van Hove Singularities
(n)
In a crystal we need to use the full bandstructure calculation for ±k with n the band index and k the reciprocalspace vector in the ﬁrst BZ, in the expression for the density of states, which takes the form: g (± )
1µ
=V
n ,k
2
= (2π )3
2δ (± −
(n) ±k )
µ´ n
2
= (2π )3 1
( n) k
±
=±
∇k±(kn) 
µ´
δ (±
n
− ±k(n))dk
dS k
(2.127) (n )
where the last integral is over a surface in k space on which ±k is constant and equal to ±. The last step in the above equation can be proven by using the properties of the δ function, see Appendix A. In this ﬁnal expression, the roots of the denominator are of ﬁrst order and therefore contribute a ﬁnite quantity to the integration over a smooth 2D surface represented by S k ; these roots introduce sharp features in the function g(± ), which are called “van Hove singularities.” For the values k0 where ∇k ±k = 0, we can expand the energy in a Taylor expansion (from here on we consider the contribution of a single band and drop the band index for simplicity): [∇k ±k ]k=k 0
= 0 ⇒ ±k = ±k + 0
d µ i=1
α i (k i
− k 0,i )2
(2.128)
The expansion is over as many principal axes as the dimensionality of our system: in three dimensions (d = 3) there are three principal axes, characterized by the symbols αi , i = 1, 2, 3. Depending on the signs of these coefﬁcients, the extremum can be a minimum (0 negative coefﬁcients, referred to as “type 0 critical point”), two types of saddle point (“type 1 and 2 critical points”), or a maximum (“type 3 critical point”). There is a useful theorem that tells us exactly how many critical points of each type we can expect.
113
2.8
Table 2.4
Symbols (
l, Ml
= d ! /l! (d − l)! = 1, 2, 3 d=3
), multiplicity
αi , i
behavior of the coeﬃcients
Density of States
, type, and characteristic
along the principal axes for critical points in
dimensions.
l
Symbol
Multiplicity
Type
0 1 2 3
M0 M1 M2 M3
1 3 3 1
minimum saddle point saddle point maximum
Coefﬁcients α1 , α2 , α3 >
0 0, α3 α1 > 0, α2 , α3 α1 , α2 , α3 < 0
α1 , α2 >
<
0, i = 1, 2, 3. In order to perform the kspace integrals involved in the DOS we ﬁrst make the following changes of variables: in the neighborhood of the critical point at k 0 ±k
− ±k = α1k 21 + α2 k 22 + α3k 23 0
(2.129)
where k is measured relative to k0 . We can choose the principal axes so that α1 , α2 have the same sign; we can always do this since there are at least two coefﬁcients with the same sign (see Table 2.4). We rescale these axes so that α1 = α2 = β after the scaling and introduce cylindrical coordinates for the rescaled variables k 1, k2 : q
2
= k12 + k 22,
θ
= tan−1 (k 2/ k1 )
(2.130)
With these changes, the DOS function takes the form: g(± )
= (2πλ )3
´
δ (±
− ±k − β q2 − α3 k32) dk 0
(2.131)
where the factor λ comes from rescaling the principal axes 1 and 2. We can rescale the variables q, k3 so that their coefﬁcients become unity, to obtain: g(± )
=
´
λ
δ (±
1/2
(2π )2 β α3
− ±k − q2 − k 23 ) q dq dk 3 0
(2.132)
Now we can consider the expression in the argument of the δ function as a function of k 3: f (k3 )
= ± − ±k − q 2 − k 23 ⇒ f ± (k 3 ) = −2k3 0
(2.133)
and we can integrate over k 3 with the help of the expression for δ function integration Eq. (A.61) (derived in Appendix A), which gives: g(± )
= λ0
´
0
Q
(± − ±k0
1
− q 2)1 2 q dq /
(2.134)
114
2
Electrons in Crystals: Translational Periodicity
where the factor λ0 embodies all the constants in front of the integral from rescaling and integration over k 3, and we have dropped primes from the remaining variable of integration for simplicity. The upper limit of integration Q for the variable q is determined by the condition k32
= ± − ±k − q 2 ≥ 0 ⇒ Q = (± − ±k )1 2 0
(2.135)
/
0
and with this we can now perform the ﬁnal integration to obtain: g (±)
= −λ0
º
(± − ±k 0 − q 2) 1/ 2
»(± −±k0 )1 2 /
= λ0(± − ±k )1 2
(2.136)
/
0
0
This result holds for ± > ±k 0 . For ± < ±k0 , the δ function cannot be satisﬁed for the case we are investigating, with αi > 0, i = 1, 2, 3, so the DOS must be 0. By an exactly analogous calculation, we ﬁnd that for the maximum M 3 , with αi < 0, i = 1, 2, 3, the DOS behaves like: g (±)
= λ3( ±k − ± )1 2
(2.137)
/
0
for ± < ±k0 and it is 0 for ± > ±k0 . For the other two cases, M 1 , M 2, we can perform a similar analysis. We outline brieﬂy the calculation for M 1 : in this case, we have after rescaling α1 = α2 = β > 0 and α3 < 0, which leads to: g (± )
=
´
λ
δ( ±
1/ 2
(2π )2 β α3
→ λ1
´
Q2
0
1
(q 2
Q1
− ±k − q 2 + k 23 ) q dq dk 3
+ ±k − ±)1 2 /
0
q dq
(2.138)
and we need to specify the limits of the last integral from the requirement that q2 + ±k 0 − ± ≥ 0. There are two possible situations: (i) For ± < ±k 0 the condition q2 + ±k 0 − ± ≥ 0 is always satisﬁed, so that the lower limit of q is Q 1 = 0, and the upper limit is any positive value Q 2 = Q > 0. Then the DOS becomes:
º
»Q
= λ1 (q2 + ±k − ± )1 2 0 = λ1(Q 2 + ±k − ± )1 2 − λ1 (±k − ±)1 2 (2.139) For ± → ±k , expanding in powers of the small quantity ( ±k − ± ) gives: (2.140) g (±) = λ1 Q − λ 1(±k − ± )1 2 + O (±k − ± ) (ii) For ± > ±k the condition q 2 +±k −± ≥ 0 is satisﬁed for a lower limit Q 1 = (± −±k )1 2 and an upper limit being any positive value Q 2 = Q > (± − ±k )1 2 > 0. Then the g(± )
0
/
0
/
0
0
/
0
0
0
0
DOS becomes: g(± )
For ±
/
0
= λ1
0
0
º
(q2 + ±k 0 − ± )1/2
»Q (±−± k0 )1/2
/
/
= λ1 (Q 2 + ±k − ±)1 2 /
0
(2.141)
→ ±k , expanding in powers of the small quantity ( ±k − ± ) gives: 0
0
g (±)
= λ1Q + 2λQ1 (±k − ± ) + O [(±k − ±)2 ] 0
0
(2.142)
115
Further Reading
maximum
minimum
saddle point 1
~(± −±0 )1/2
saddle point 2
0
0 Fig. 2.29
g( ±)
0
0
0
The behavior of DOS, g( ±), near critical points of different type in three dimensions.
By an exactly analogous calculation, we ﬁnd that for the other saddle point M 2 , with 0, α3 > 0, the DOS behaves like:
α 1, α2
±k 0 . The behavior of the DOS for all the critical points is summarized graphically in Fig. 2.29. We should caution the reader that very detailed calculations are required to resolve these critical points. In particular, methods must be developed that allow the inclusion of eigenvalues at a very large number of sampling points in reciprocal space, usually by interpolation between points at which electronic eigenvalues are actually calculated.11
Further Reading
1. Wave Propagation in Periodic Structures , L. Brillouin (McGrawHill, New York, 1946). This is a classic book on wave and periodic structures, introducing the notion that has become known as “Brillouin zones,” with excellent illustrative examples. 2. Electronic Structure and the Properties of Solids , W. A. Harrison (W.H. Freeman, San Francisco, 1980). This book contains a general discussion of the properties of solids based on the tightbinding approximation. 3. Physics of Solids , E. N. Economou (SpringerVerlag, Berlin, 2010). This book contains a careful discussion of the physics of the tightbinding approximation and its many applications. 4. Handbook of the Band Structure of Elemental Solids , D. A. Papaconstantopoulos (Plenum Press, New York, 1989). This is a comprehensive account of the tightbinding approximation and its application to the electronic structure of elemental solids.
11 O. Jepsen and O. K. Andersen, Solid State Comm.
54 , 469 (1972).
9, 1763 (1971); G. Lehmann and M. Taut, Phys. Stat. Solidi
116
2
Electrons in Crystals: Translational Periodicity
Problems
1.
(a) Calculate the reciprocal lattice vectors for the crystal lattices given in Table 2.1. (b) Determine the lattice vectors, the positions of atoms in the primitive unit cell, and the reciprocal lattice vectors, for the NaCl, CsCl, and zincblende crystal structures discussed in Chapter 1.
2.
(a) Show that the singleparticle equation obeyed by u k (r), the part of the wavefunction which has full translational symmetry, is Eq. (2.22). (b) Show that the coefﬁcients αk (G) in the Fourier expansion of u (kn) (r) obey Eq. (2.44).
3.
We want to derive the expression for the energy at wavevector k0 + k in terms of the energy and wavefunctions at wavevector k0 , as given in Eq. (2.48). The simplest way to do this is to work with the part of the wavefunctions that are fully symmetric in the lattice periodicity, u (kn) (r), and the corresponding hamiltonian for ˆ sp (pˆ + h¯ k) [see Eq. (2.22)]. Consider as the unperturbed which they are solutions, H ˆ 0sp = Hˆ sp (pˆ + h¯ k0 ), with the known hamiltonian the one corresponding to k 0, H (n ) (n ) solutions u k0 (r), ±k 0 , and then consider the hamiltonian at (k 0 + k): the latter has extra terms relative to
ˆ sp
H0
which can be identiﬁed as the perturbation (n ± )
ˆ sp . We
H1
assume that there are no band degeneracies (±k0 ³= ±k 0 for n ³= n± ), so that we can use nondegenerate perturbation theory (see Appendix C). From the result for the energy at k0 + k , derive the expression for the inverse effective mass, given in Eq. (2.51). (n)
4.
For the 2D square lattice with lattice constant a , with one atom per unit cell, in the freeelectron approximation, ﬁnd the Fermi momentum and Fermi energy if there is one valence electron per atom. Show the Fermi sphere and draw carefully the occupied portions of the various BZs.
5.
(a) Determine the ﬁrst Brillouin zone of the FCC lattice. In order to do this, ﬁnd the ﬁrst set of reciprocal space vectors with the lowest magnitude, draw these vectors and the planes that are perpendicular to them at their midpoints. What shape does the envelope of these planes produce in reciprocal space? Then, ﬁnd the set of reciprocalspace vectors that have the next higher magnitude, and the planes that bisect these vectors. Describe the intersection of one of these planes with the corresponding planes of the ﬁrst set. This should be sufﬁcient to fully determine by symmetry the ﬁrst BZ. Compare your result to what is shown in Fig. 2.12. (b) Draw the ﬁrst few freeelectron bands for the 3D FCC lattice along the highsymmetry lines shown in Fig. 2.12, in units of (h¯ 2 /2m e )(2π/a )2 ; compare your results to those shown in Fig. 2.12. (c) For an FCC crystal with one atom per unit cell, which has Z = 3 valence electrons, estimate the position of the Fermi level on the bandstructure plot and describe the features of the resulting 3D Fermi sphere qualitatively.
117
Problems
6.
Prove that the orthogonality relation, Eq. (2.57), holds in general (not only in the context of the tightbinding approximation).
7.
The relationship between the band width and the number of nearest neighbors, Eq. (2.71), was derived for the simple chain, square, and cubic lattices in one, two, and three dimensions, using the simplest tightbinding model with one atom per unit cell and one s like orbital per atom. For these lattices, the number of neighbors z is always 2d , where d is the dimensionality. Consider the same simple tightbinding model for the closepacked lattices in two and three dimensions, that is, the simple 2D hexagonal lattice and the 3D FCC lattice, and derive the corresponding relation between the band width and the number of nearest neighbors.
8.
Prove the Bloch statement for the manybody wavefunction, that is, show that the manybody wavefunction will have Blochlike symmetry: µK (r1
+ R, r2 + R, ...) = eiK· RµK (r1, r2, ...)
(2.145)
Then relate the value of the wavevector K to the singleparticle wavevectors ki , i = 1, . . ., N , when the manybody wavefunction is written as a product of singleparticle states. 9.
For a Bloch state deﬁned as: (n )
φk,s (r)
ik·r
= e√
V
(n)
u k (r)λs
where λ s is a twocomponent spaceindependent spinor, ﬁnd the hamiltonian in the weakly relativistic limit [see Appendix C, Eq. (C.80)] that applies to the space(n ) dependent part of the wavefunction uk (r). 10.
Derive the density of states for the freeelectron model in two dimensions, Eq. (2.124) and one dimension, Eq. (2.125).
11.
Derive the type, multiplicity, and behavior of the DOS at critical points in one and two dimensions.
12.
Derive the behavior of the DOS near the Dirac point in one, two, and three dimensions, where the energy is given by Eq. (2.85).
13.
For the simple model of the graphene lattice, which consists of one pz like orbital per atom in the 2D honeycomb lattice, described in Section 2.5: (a) Show that the energy of the two bands is given by Eq. (2.87). (b) Show that at the corner of the Brillouin zone (K point) this expression leads to Dirac behavior, Eq. (2.85). (c) Calculate numerically the DOS near the critical points ³ , M, and K and show that it has the expected behavior.
118
2
14.
Electrons in Crystals: Translational Periodicity
Consider the following 2D model: the lattice is a square of side a with lattice vectors a1 = a xˆ and a2 = ayˆ ; there are three atoms per unit cell, one Cu atom and two O atoms at distances a1 /2 and a2 /2, as illustrated in Fig. 1.30. We will assume that the atomic orbitals associated with these atoms are orthogonal. (a) Although there are ﬁve d orbitals associated with the Cu atom and three p orbitals associated with each O atom, only one of the Cu orbitals (the dx2 −y2 one) and two of the O orbitals (the p x one on the O atom at a1/2 and the p y one on the O atom at a2/2) are relevant, because of the geometry; the remaining Cu and O orbitals do not interact with their neighbors. Explain why this is a reasonable approximation, and in particular why the Cu–d 3z2 −r2 orbitals do not interact with their nearestneighbor O–p z orbitals. (b) Deﬁne the hamiltonian matrix elements between the relevant Cu–d and O–p nearestneighbor orbitals and take the onsite energies to be ±d and ±p , with ± p < ±d . Use these matrix elements to calculate the band structure for this model. (c) Discuss the position of the Fermi level for the case where there is one electron in each O orbital and one or two electrons in the Cu orbital.
Historical note: Even though this model may appear artiﬁcial, it has been used extensively to describe the basic electronic structure of the copper oxide–rare earth materials, which are hightemperature superconductors.12 12 L. F. Mattheis, Phys. Rev. Lett. 58 , 1028 (1987).
3
Symmetries Beyond Translational Periodicity
In the previous chapter we discussed in detail the effects of lattice periodicity on the singleparticle wavefunctions and the energy eigenvalues. We also touched on the notion that a crystal can have symmetries beyond the translational periodicity, such as rotations around axes, reﬂections on planes, and combinations of these operations with translations by vectors that are not lattice vectors, called “nonprimitive” translations. All these symmetry operations are useful in calculating and analyzing the physical properties of a crystal. There are two basic advantages to using the symmetry operations of a crystal in describing its properties. First, the volume in reciprocal space for which solutions need to be calculated is further reduced, usually to a small fraction of the ﬁrst Brillouin zone, called the “irreducible” part; for example, in the FCC crystals with one atom per unit cell, the irreducible part is 1/48 of the full BZ. Second, certain selection rules and compatibility relations are dictated by symmetry alone, leading to a deeper understanding of the physical properties of the crystal as well as to simpler ways of calculating these properties in the context of the singleparticle picture; for example, using symmetry arguments it is possible to identify the allowed optical transitions in a crystal, which involve excitation or deexcitation of electrons by absorption or emission of photons, thereby elucidating its optical properties. In this chapter we address the issue of crystal symmetries beyond translational periodicity in much more detail. To achieve this, we must make an investment in the mathematical ideas of group theory. We restrict ourselves to the bare minimum necessary to explore the effects of symmetry on the electronic properties of the crystal. In several cases, we will ﬁnd it useful to state and prove theorems to the extent that this exercise provides insight into how the theory actually works. When we give proofs, we shall mark their end by the symbol ±, as is commonly done in mathematical texts; this may be useful in case the reader wishes to skip the proofs and continue with the exposition of the theory.
3.1
TimeReversal Symmetry for Spinless Fermions
In addition to the symmetries a crystal has in real space, there is also another type of symmetry in reciprocal space which allows us to connect the properties of states with wavevector k to those with wavevector −k. This is called “inversion symmetry” and holds irrespective of whether the realspace crystal possesses the corresponding symmetry or not. In real space, inversion symmetry implies r → − r, that is, the crystal remains 119
120
3
Symmetries Beyond Translational Periodicity
invariant if we move every point in space to its inverse with respect to some properly chosen origin. The corresponding operation in reciprocal space is k → −k, that is, the properties of the crystal are invariant if we replace every value of the wavevector with its opposite. The inversion symmetry in reciprocal space always holds, even if the crystal does not have inversion in real space. This remarkable property is a consequence of timereversal symmetry, that is, the fact that the hamiltonian of a solid does not change if we change the sign of the time variable, t → −t. Evidently, when a term in the hamiltonian breaks timereversal symmetry (e.g. an external magnetic ﬁeld), the inversion in reciprocal space is also broken. We discuss this symmetry ﬁrst, and then turn our attention to the description of all other crystal symmetries beyond periodicity. For spinless fermions, since the hamiltonian is real, that is, the system is timereversal invariant, we must have for any state characterized by the wavevector k:
Kramers’ Theorem
(n )
±k
= ±−(mk)
(3.1)
To prove Kramers’ theorem, we take the complex conjugate of the singleparticle Schr¨odinger equation
Proof
ˆ sp ψk(n) (r) = ±k(n)ψk(n) (r) ⇒ Hˆ sp ψk∗(n)(r) = ±k(n)ψk∗(n) (r)
(3.2)
H
∗(n)
(n )
(n )
that is, the wavefunctions ψk (r) and ψk (r) have the same (real) eigenvalue ±k . But we (m) ∗(n) can identify ψk (r) with ψ−k (r), because: (m )
ψ k (r)
−
−ik ·r ±
= e√
V
G
(m )
α k (G)e
−
iG·r
and
−ik·r ± ∗(n) ∗(n) (r) = e√ iG·r αk (−G)e V −G
ψk
(3.3)
where in the second sum we have used −G as the symbol for the summation over the inﬁnite set of reciprocal lattice vectors. In the above expressions, the two sums contain exactly the same exponentials, term by term, with the same overall wavevector −k, as determined by the exponential outside the sum. Therefore, the second wavefunction must be one of the set of wavefunctions corresponding to the wavevector −k, that is:
∗(n)(−G) = α(m) (G) ⇒ ψ ∗(n)(r) = ψ (m )(r) ⇒ ±(m) = ± (n) −k k −k −k k
αk
as desired.
(3.4)
±
The identiﬁcation of the two wavefunctions may require a change in the band labels, but this is inconsequential since those labels are purely for keeping track of all the solutions at each wavevector value and have no other physical meaning. This theorem is relevant to electrons in crystals when each state characterized by k is occupied by both spinup and spindown particles, in which case the spin does not play a major role, other than doubling the occupancy of the klabeled states. For systems with equal numbers of up and down spins, Kramers’ theorem amounts to inversion symmetry in reciprocal space. A more detailed analysis which takes into account spin states explicitly reveals that for spin1/2 particles, without spin–orbit coupling, Kramers’ theorem becomes:
− ↓ = ±k,↑ , (m )
± k,
(n)
∗(n) (m) − ↓ (r) = i σy ψk ,↑ (r)
ψ k,
(3.5)
121
3.2
Crystal Groups: Deﬁnitions
where σy is a Pauli matrix (see Appendix C). This will be discussed in more detail in Chapter 9.
3.2
Crystal Groups: Deﬁnitions
Taking full advantage of the crystal symmetries requires the use of group theory. This very interesting branch of mathematics is particularly well suited to reduce the amount of work by effectively using group representations in the description of singleparticle eigenfunctions. Here, we will develop some of the basic concepts of group theory including group representations, and we will employ them in simple illustrative examples. We ﬁrst deﬁne the notion of a group: it is a ﬁnite or inﬁnite set of operations, which satisfy the following four conditions. 1. Closure : if P and Q are elements of the group, so is R = PQ . 2. Associativity: if P , Q , R are members of a group, then (PQ )R = P (QR ). 3. Unit element: there is one element E of the group for which EP = PE = P , where P is any other element of the group. 4. Inverse element: for every element P of the group, there exists another element called its inverse P −1 , for which PP −1 = P −1 P = E . A subgroup is a subset of operations of a group which form a group by themselves (they satisfy the above four conditions). Two groups are called isomorphic when there is a onetoone correspondence between their elements P 1 , P 2 , ..., P n and Q 1 , Q 2 , ..., Q n, such that P 1P 2
= P 3 ⇒ Q 1Q 2 = Q 3
(3.6)
Finally, we deﬁne the notion of a class. A subset of elements Q j of the group G constitutes a class C if, for all elements Q i of the group, the following relation holds:
−1 = Q k
Si Qj Si
(3.7)
that is, when we multiply an element of the class Q j by any other group element S i (on the 1 left) and by its inverse S − i (on the right), the result is an element Q k which also belongs to the class. In practical terms, we choose an element of the group Q j and go through all 1 the other elements of the group S i , multiplying Q j by S i and S − i , to produce the entire class C to which Q j belongs. Implicit in this deﬁnition is the fact that a true class cannot be broken into subclasses. We will give examples of groups and classes below, for speciﬁc crystals; the notion of a class plays an important role in group representations, which we will discuss in a later section. For a crystal, we can deﬁne the following groups. (a)
: the space group, which contains all symmetry operations that leave the crystal invariant. (b) R : the translation group, which contains all the translations that leave the crystal invariant, that is, all the Bravais lattice vectors R. R is a subgroup of S . S
122
3
(c)
Symmetries Beyond Translational Periodicity
: the point group, which contains all spacegroup operations with the translational part set equal to 0. Q is not necessarily a subgroup of S , because when the translational part is set to 0, some operations may no longer leave the crystal invariant if they involved a translation by a vector not equal to any of the Bravais lattice vectors.
Q
The space group can contain the following types of operations.
• • • • •
Lattice translations (all the Bravais lattice vectors R), which form R. Proper rotations by 0 degrees (which corresponds to the identity or unit element, {E  0}) and by the special angles π3 , π2 , 23π , π , 43π , 32π , 53π around an axis. Improper rotations: inversion (denoted by I ), or reﬂection on a plane (denoted by σ ). Screw axes, which involve a proper rotation and a translation by t ±= R, parallel to the rotation axis. Glide planes, which involve a reﬂection about a plane and a translation by t ±= R along that plane.
Some general remarks on grouptheory applications to crystals are in order. We saw that Q consists of all spacegroup operators with the translational part set equal to 0. Therefore, Q × R ±= S in general, because several of the group symmetries may involve nonlattice vector translations t ±= R. The point group leaves the Bravais lattice invariant but not necessarily the crystal invariant (recall that the crystal is deﬁned by the Bravais lattice and the atomic basis in each unit cell). If the crystal has glide planes and screw rotations, that is, symmetry operations that involve {U t} with t ±= 0 and {E  t} ∈/ R, then Q does not leave the crystal invariant. So why do we bother to consider the point group Q at all? As we shall see in the next section, even if Q does not leave the crystal invariant, it does leave the (n ) energy spectrum ±k invariant! Groups that include such symmetry operations are referred to as nonsymmorphic groups. A symmorphic group is one in which a proper choice of the origin of coordinates eliminates all nonlattice translations, in which case Q is a true subgroup of S . Finally, all symmetry operators in the space group commute with the hamiltonian, since they leave the crystal, and therefore the external potential, invariant.
Example 3.1 Honeycomb lattice with basis of two different atoms: √ C3v group 3√ xˆ + y ], ˆ a2 = This model is described by the realspace lattice vectors a = ( a / 2)[ 1 √ √ (a/ 2)[ ]ˆ and reciprocalspace vectors b1 = (2π/ 3a )[xˆ + 3ˆy], b2 = √ 3xˆ − y √ (2π/ 3a )[xˆ − 3yˆ ], with the positions of the two atoms within the PUC given by t1 = 0, t2 = (a1 + a2 )/3. As illustrated in Fig. 3.1, the symmetries of this model are:
• • • • • •
the identity E rotation by 2π/3 around an axis perpendicular to the plane, C 3 rotation by 4π/3 around an axis perpendicular to the plane, C 23 reﬂection on the xaxis, σ1 reﬂection on the axis at θ = 2π/3 from the x axis, σ2 reﬂection on the axis at θ = 4π/3 from the x axis, σ3 .
123
3.2
Crystal Groups: Deﬁnitions
b1
σ2
σ2
Ν
C3 a1 a2
C32
Κ
C3
σ1
C
2 3
Μ σ1
Γ
σ3 σ3
ky
y x
Fig. 3.1
kx
b2
Left: The symmetry operations of the 2D honeycomb lattice with a basis of two different atoms (circles colored red and blue). These operations form the C3v group and are labeled 2 σ1 , σ 2, σ3 for the reﬂections and C 3, C for the rotations, which are indicated by the curves 3 with arrows. The red arrows labeled a1, a2 show the primitive lattice constants. Right: The irreducible Brillouin zone (yellow rhombus) for the 2D honeycomb lattice with C 3v symmetry; the special points are labeled ² , M, K, N. The green arrows labeled b1, b2 show the reciprocalspace lattice constants. Table 3.1
Symmetry operations and group multiplication table for symmetries of the
C3v
group:
each entry in the table is the result of taking the product of two operations, with the operation on the left of the row acting
ﬁrst and the operation at the top of the column acting
second. The
√ √ u = [ x − 3 y ] / 2, u2 = [x + 3y ]/2, 1 √ √ v1 = [ 3x − y]/ 2, v2 = [ 3x + y] /2
horizontal and vertical lines in the multiplication table separate the group into the three classes
C1 , C2 , C 3 . We have used the deﬁnitions:
.
U E C3 C23 σ1 σ2 σ3
{U0} (x, y )
( x, y) (−u1 , −v2 ) (−u2, v1 ) ( x, − y) ( u1 , −v2 ) ( u 2 , v1 )
Oˆ {U 0} (x , y) ( x, y) ( −u2 , v1 ) (−u1, −v2) ( x, −y) ( u 1 , − v2 ) ( u 2 , v1 )
C1
C2 C3 C23 E
C32 E C3
σ1
σ3
σ2
σ2
σ1
σ3
σ3
σ2
σ1
E C3 C23
C3 σ1
σ2
σ3
σ2
σ3
σ1
σ3
σ1
σ2
E C3 C23
E C3
C3 C23 E
C 23
These symmetries constitute the point group Q for this physical system, called C 3v . We assume that the origin is at the position of one of the two different atoms, so that the group is symmorphic. This point group has the group multiplication table given in Table 3.1: an entry in this table is the result of multiplying the element at the top of its column with the element at the left of its row. The deﬁnition of each element in terms of its action on an arbitrary vector (x , y ) on the plane is also given in the left half of Table 3.1. This group multiplication table can be used to prove that all the group properties are satisﬁed. It is also very useful in identifying the classes in the group:
124
3
Symmetries Beyond Translational Periodicity
the element E is in a class by itself, as is always the case for any group; the elements C 3, C 23 form a second class; the elements σ1, σ2, σ3 form a third class. The separation of the group into these three classes can easily be veriﬁed by applying the deﬁnition in Eq. (3.7).
3.3
Symmetries of 3D Crystals
In three dimensions there are 14 different types of Bravais lattices, 32 different types of point groups, and a total of 230 different space groups, of which 73 are symmorphic and 157 are nonsymmorphic. The 14 Bravais lattices are grouped into six crystal systems called triclinic, monoclinic, orthorhombic, tetragonal, hexagonal, and cubic, in order of increasing symmetry. The hexagonal system is often split into two parts, called the trigonal and hexagonal subsystems. The deﬁnitions of these systems in terms of the relations between the sides of the unit cell (a , b , c ) and the angles between them (with α = the angle between sides a , c ; β = the angle between sides b , c ; and γ = the angle between sides a, b) are given in Table 3.2. Figure 3.2 shows the conventional unit cells for the 14 Bravais lattices. Each corner of the cell is occupied by sites that are equivalent by translational symmetry. When there are no other sites equivalent to the corners, the conventional cell is the same as the primitive cell for this lattice and it is designated P. When the cell has an equivalent site at its geometric center (a body centered cell) it is designated I for the implied inversion symmetry; the primitive unit cell in this case is onehalf the conventional cell. When the cell has an equivalent site at the center of one face it is designated C (by translational symmetry it must also have an equivalent site at the opposite face); the primitive unit cell in this case is onehalf the conventional cell. When the cell has an equivalent site at the center of each face (a face centered cell) it is designated F; the
Table 3.2
The seven crystal systems (ﬁrst column) and the associated 32 point groups (last column) for
crystals in three dimensions. The relations between the cell sides shown and the corresponding lattices are labeled
F
P R
= face centered,
(a, b, c) I
= primitive,
and cell angles
= body centered,
C
(α , β , γ )
are
= side centered,
= rhombohedral.
System
Cell sides
Cell angles
Lattices
Point groups
Triclinic Monoclinic Orthorhombic Tetragonal
a ±= a ±= a ±= a=
±= β ±= γ = β = 2 ±= γ α = β = γ = 2 α = β = γ = 2
P P, C P, I, C, F P, I
Trigonal Hexagonal
a= b= c a = b ±= c
Cubic
a= b= c
C1 , Ci C2 , Cs , C 2h D 2 , D 2 h , C2 v C4 , S4 , C 4h , D4 , C4v , D2d , D4h C3 , C3i , C3v , D3 , D3d C6 , C3h , C 6h , C6v, D3h, D6, D6h T , T h, O, Td , Oh
b ±= b ±= b ±= b ±=
c c c c
α
α
π
π
π
= β = γ ±= 2 , γ = 23 α = β = 2 π
α
π
π
α
=β=γ = 2
π
P P, R P, I, F
125
3.3
Triclinic
Orthorhombic
z
b
c
y
a
x
b P
ay x
Cubic
z
z c
c a P
a y x
a a
a
P
y x
a P
a y
Monoclinic I c
x
Hexagonal
z
c
P
z
Tetragonal
z
β α γ x
Symmetries of 3D Crystals
I
R
I
a y
b
P
C
F C Fig. 3.2
F
The conventional unit cells of the 14 Bravais lattices in the six systems in three dimensions; the trigonal system unit cell is included in the conventional cell of the hexagonal system. The dots indicate equivalent sites in the unit cell: those at the corners are equivalent by translational symmetry, the rest indicate the presence of additional symmetries implying a primitive unit cell smaller than the conventional one. Dashed lines within the cells connect equivalent points for easier visualization. The cells are labeled P, I, C, F, R, according to the convention of Table 3.2. For the cells labeled P in each system, we also indicate the cartesian coordinate axes, labeled x, y, z , and the length of the unit cell sides, as a, b, c; in the triclinic cell, we also show the cell angles α, β, γ between the cell sides.
primitive unit cell in this case is onequarter the conventional cell. Finally, in the hexagonal system there exists a lattice which has two more equivalent sites inside the conventional cell, at height c /3 and 2c/3 along the main diagonal (see Fig. 3.2), and it is designated R for rhombohedral; the primitive unit cell in this case is onethird the conventional cell. A number of possible point groups are associated with each of the 14 Bravais lattices, depending on the symmetry of the basis. There are 32 point groups in all, denoted by the following names:
• • • •
C for “cyclic,” when there is a single axis of rotation; a number subscript m indicates the m fold symmetry around this axis (m can be 2, 3, 4, 6). D for “dihedral,” when there are twofold axes at right angles to another axis. T for “tetrahedral,” when there are four sets of rotation axes of threefold symmetry, as
in a tetrahedron (see Fig. 3.3). O for “octahedral,” when there are fourfold rotation axes combined with perpendicular twofold rotation axes, as in an octahedron (see Fig. 3.3).
126
3
(a) Fig. 3.3
Symmetries Beyond Translational Periodicity
(b )
(c)
(d)
Illustration of symmetry axes, shown as doubleheaded red arrows, of the tetrahedron and the octahedron. (a) A threefold rotation axis of the regular tetrahedron passes through one of its corners and the geometric center of the equilateral triangle directly across it; there are four such axes in the regular tetrahedron, each passing through one of its corners. One symmetry plane, passing through one of the tetrahedron edges and the center of the opposite edge, is highlighted in pink. (b) Two tetrahedra (in this case not regular ones) with a common axis of threefold rotational symmetry in the cube are identiﬁed by thicker red lines; the triangular bases of these tetrahedra, which lie entirely within the cube, are highlighted in pink. There are four pairs of such tetrahedra in the cube, whose threefold rotational symmetry axes are the main diagonals of the cube. (c) Three different symmetry axes of an octahedron; when the edges of the horizontal square are not of the same length as the other edges, the vertical axis corresponds to fourfold rotation, while the two horizontal axes correspond to twofold rotation. When all edges are of equal length, all three axes correspond to fourfold rotational symmetry. (d) One such octahedron, with all edges equal and three fourfold rotation axes, shown in thicker lines, is inscribed in the cube.
In all these cases the existence of additional mirrorplane symmetries is denoted by a second subscript which can be h for “horizontal,” v for “vertical,” or d for “diagonal” planes relative to the rotation axes. Inversion symmetry is denoted by the letter subscript i. In the case of a onefold rotation axis, when inversion symmetry is present the notation C i is adopted (instead of what would normally be called C 1i ), while when a mirrorplane symmetry is present the notation C s is used (instead of what would normally be called C 1h). Finally, the group generated by the symmetry operation of π/2 rotation followed by reﬂection on a vertical plane, the socalled “rotoreﬂection” group, is denoted by S4 (this is different from C 4v , in which the π/2 rotation and the reﬂection on a vertical plane are independently symmetry operations). This set of conventions for describing the 32 crystallographic groups is referred to as the Schoenﬂies notation; the names of the groups in this notation are given in Table 3.2. There is a somewhat more rational set of conventions for naming crystallographic point groups described in the International Tables for Crystallography . This scheme is more complicated; we refer the interested reader to those tables for further details. There exists a useful way of visualizing the symmetry operations of the various point groups, referred to as “stereograms.” These consist of 2D projections of a point on the surface of a sphere and its images generated by acting on the sphere with the various symmetry operations of the point group. In order to illustrate the action of the symmetry operations, the initial point is chosen as some arbitrary point on the sphere, that is, it does not belong to any special axis or plane of symmetry. The convention for the equivalent
127
Fig. 3.4
3.3
Monoclinic
T etragona l
C2
C4
Cs
Symmetries of 3D Crystals
Trigonal
H exagona l
Cubic
C3
C6
T
S4
C 3i
C 3h
Th
C 2h
C 4h
C 3v
C 6h
Td
Orthorhombic
C 4v
D3
C 6v
O
C 2v
D4
D 3d
D6
Oh
D2
D 2d
D 3h
D 2h
D 4h
D 6h
Stereograms for 30 point groups in three dimensions. The lines within the circles are visual aids, which in several cases correspond to reﬂection planes. The trigonal and hexagonal subsystems are shown separately, and the triclinic system (groups C1 and Ci ) is not shown at all since it has trivial representations.
points on the sphere is that those in the northern hemisphere are drawn as open circles, while those in the southern hemisphere are shown as solid dots and the sphere is viewed from the northern pole. In Fig. 3.4 we show the stereograms for 30 point groups belonging to six crystal systems; the stereograms for the triclinic system (point groups C 1 and C i ) are not shown because they are trivial: they contain only one point each, since these groups do not have any symmetry operations other than the trivial ones (identity and inversion). As an illustration, we discuss brieﬂy the symmetries of the cube, which has the highest degree of symmetry compatible with 3D periodicity. When only twofold, threefold, and fourfold rotations are allowed, as required by 3D periodicity (see Problem 1), there are 24
128
3
Table 3.3
Symmetries Beyond Translational Periodicity
The 24 symmetry operations of the cube that involve rotations by
π/3 (the class C 3 ), π/2 (the class C 4 ), and
2π
(the identity
(−x , − y, −z)
E
π
(the classes
, which forms a class
C1
symmetry operations can be generated by combining each of the rotations with inversion corresponds to
C1 C5
E
x
Ux/ 2
x
−y
−x −x
−y
U1
y
U1
z
Uy/ 2 Uz /2
U2
C3
y
z
U3
−y −z
U3
y
U2
U4 U4
−y −z
Ux/ 4
x
U x/4
x
Uy/ 4
−z
z
U y/4
z
z
x
Uz /4
y
x
y
U z/ 4
y
−x −z x
−z z
−x
C4
−y x
−y −x −x y
I
, which
, that is, a change of all signs.
z
−z −z
C 5 and C2 ),
by itself ). 24 more
C2
z
−z y y
−x
Ux/ 2 Ux² / 2
−y −x −x
Uy/ 2
z
y/ 2
−z
−z −y −y
Uz /2
y
x
U² U²
z /2
−y
x z
−x
−y y x
−x z z y
−y x
−x −z −z
images of an arbitrary point in space (x , y, z ): these are given in Table 3.3. The associated 24 operations are separated into ﬁve classes: 1. The identity E . 2. Twofold ( π ) rotations around the axes x , y , z denoted as a class by C24 and as individual operations by U ν/ 2 (ν = x , y, z ). 3. Fourfold (2π/4) rotations around the axes x , y , z denoted as a class by C4 and as individual operations by U ν/ 4 (ν = x , y , z ) for counterclockwise or by U ν/4 for clockwise rotation. 4. Threefold (2π/3) rotations around the main diagonals of the cube denoted as a class by C3 and as individual operations by U n (n = 1, 2, 3, 4) for counterclockwise or by U n for clockwise rotation. 5. Twofold ( π ) rotations around axes that are perpendicular to the x , y , z axes and bisect the inplane angles between the cartesian axes, denoted as a class by C2 and as individual ² with the subscript indicating the cartesian axis operations by U ν/2 (ν = x , y , z ) or U ν/ 2 perpendicular to the rotation axis. These symmetry operations are represented schematically in Fig. 3.5. When inversion is added to these operations, the total number of images of the arbitrary point becomes 48, since inversion can be combined with any rotation to produce a new operation. It is easy to rationalize this result: there are 48 different ways of rearranging the three cartesian components of the arbitrary point, including changes of sign. The ﬁrst coordinate can be any of six possibilities (³x , ³y , ³z ), the second coordinate can be any of four possibilities, and the last coordinate any of two possibilities.
129
3.4
z
Symmetries of the Band Structure
z
3
z
z
4
x
x
y 2
1
z
y y
y
1
y
2
x 4
x
3
x
y
x
(b)
(a) Fig. 3.5
z
(c)
Symmetry operations of the cube. (a) The rotation axes for the C 4 (fourfold rotations) and C 5 (twofold rotations) classes, for rotations around axes that pass through the centers of opposite faces of the cube. (b) The C3 class consisting of threefold rotation axes which correspond to the main diagonals of the cube (arrows labeled 1–4). (b) The C 2 class consisting of twofold rotation axes that are perpendicular to the cartesian axes, and bisect the angles between them. All rotation axes are shown as doubleheaded arrows and the points at which they intersect the cube [face centers in (a), corners in (b), edge centers in (c)] are indicated by small red circles.
If these 48 operations are applied with respect to the center of the cube, then the cube remains invariant. Therefore, in a crystal with a cubic Bravais lattice and a basis that does not break the cubic symmetry (such as a single atom per unit cell referred to as simple cubic, or an FCC or a BCC lattice), all 48 symmetry operations of the cube will leave the crystal invariant and therefore all these operations form the point group of the crystal. This is the largest point group compatible with 3D periodicity. There are other, larger point groups in three dimensions but they are not compatible with 3D periodicity. For example, the icosahedral group has a total of 120 operations, but its ﬁvefold symmetry is not compatible with translational periodicity in three dimensions.
3.4
Symmetries of the Band Structure
To apply symmetry operations on various functions, we introduce the operators corresponding to the symmetries. These will be symbolized by {U  t}, where U corresponds to a proper or improper rotation and t to a translation. These operators act on realspace vectors according to the rule
{U t}r ≡ U r + t
(3.8)
In terms of these operators, the translations can be described as {E R} (where E is the identity, or unit element), while the pure rotations (proper or improper) are described as {U 0}. The ﬁrst set corresponds to the translation group R, the second to the point group Q. We note that the proper or improper rotations leave the Bravais lattice invariant, that is:
{U 0}R = U R = R² ,
R, R²
∈R
(3.9)
130
3
Symmetries Beyond Translational Periodicity
For any two symmetry operators belonging to the space group:
{U 1 t1 }{U 2 t2 }r = U{ 1 t1}[U 2 r + t2 ] = U 1 U 2r + U 1t2 + t1 (3.10) which means that the operator {U 1U 2 U 1 t2 + t1 } corresponds to an element of the space
group. Using this rule for multiplication of operators, we can easily show that the inverse of {U t} is:
{U t}−1 = U{ −1  −U −1t} (3.11) The validity of this can be veriﬁed by applying {U −1− U −1 t}{U t} on r, whereupon we get back r. We can use the expression for the inverse of {U t} to prove the following relation for the inverse of a product of operators in terms of their inverses:
{U 2 t2 }−1{U 1t1}−1 = [{U 1 t1 }{U 2 t2 }]−1
(3.12)
which can easily be proved from the deﬁnition of the inverse element in Eq. (3.11). In the following we will need to apply symmetry operations to functions of the space variable r, so we deﬁne a new set of operators whose effect is to change r:
ˆ{
 } f (r) ≡ f ({U t}−1r)
(3.13)
OUt
In this deﬁnition of Oˆ {U t} , the action is always on the vector r itself. Theorem
{U t}. Proof
The group formed by the operators
ˆ{
 } is
O Ut
isomorphic to the group of operators
We note that
ˆ{
 } ˆ {  } f (r) = Oˆ {U1 t1} f ({U 2 t2 }−1 r) = Oˆ {U 1t1 } g(r) = g ({U 1t1}−1r) = g(r² )
O U1 t1 O U2 t2
where we have introduced the deﬁnitions g (r)
= f ( {U 2 t2 }−1 r)
and r²
= U{ 1 t1 }−1 r
to facilitate the proof. Using these deﬁnitions, we have
²
g (r )
= f ({U 2 t2 }−1 r²) = f ({U 2 t2}−1 {U 1 t1 }−1 r) = f ([ {U 1 t1 }{U 2t2}]−1 r) = Oˆ {U t }{U t } f (r) ⇒ Oˆ {U t } Oˆ {U t } = Oˆ {U t }{U t } 1 1
1 1
2 2
1 1
2 2
2 2
(3.14)
The last equality in Eq. (3.14) proves the isomorphism between the groups {U t} and ˆ {Ut} , since their elements satisfy the condition of Eq. (3.6) in an obvious correspondence O between elements of the two groups. ± Having deﬁned the basic formalism for taking advantage of the crystal symmetries, we will now apply it to simplify the description of the eigenfunctions and eigenvalues of the singleparticle hamiltonian.
131
3.4
Symmetries of the Band Structure
{ } ∈
For any element of the space group U t S , when we apply it to an eigenstate (n ) (n) of the hamiltonian ψk (r) with eigenvalue ±k , we obtain a new state which we will denote
Theorem
as
˜ (n) (r) with eigenvalue ±˜q(n) such that: (n) (n) (n ) (n) (n) (n) ±˜q = ± Uk = ± k and ψ˜ q(n) (r) = Oˆ {U t} ψk ( r) = ψ˜ Uk ( r) = ψk (U −1r − U −1 t)
ψq
(3.15)
We need to prove ﬁrst, that ψk(n) (r) and ψ˜ q(n) (r) are eigenstates of the hamiltonian with the same eigenvalue and second, that ψ˜ q(n)(r) is a Bloch state of wavevector q = U k. We ﬁrst note that the symmetry operators of the space group commute with the hamiltonian, by their deﬁnition (they leave the crystal, hence the total potential invariant):
Proof
ˆ{
²
³
³
²
²
³
ˆ sp ψk(n) (r) = Oˆ {Ut} ±k(n)ψk(n) (r) ⇒ Hˆ sp Oˆ {Ut} ψk(n)( r) ² ³ = ±k(n) Oˆ {Ut} ψk(n) (r) (n ) (n) which shows that ψk (r) and ψ˜ q (r) are eigenfunctions with the same eigenvalue, proving the ﬁrst relation in Eq. (3.15). To prove the second relation, we apply the operator Oˆ {E− R} (n ) to the function ψ˜ q (r): this is simply a translation operator (E is the identity), and therefore changes the argument of a function by +R. We expect to ﬁnd that this function is then changed by a phase factor exp[iU k · R], if indeed it is a Bloch state of wavevector U k . To }
OUt
H
prove this we note:
{U t}−1{E  −R}{U t} = U {t }−1 {U t − R} = U{−1  −U −1 t}{U t − R} = E{ U −1 t − U −1 R − U −1t} = E { −U −1 R} and multiplying the initial and ﬁnal parts of this equation by {U t} from the left, we get {E  −R}{ U t} = U {t}{ E  −U −1R} ⇒Oˆ { E−R}{Ut} = Oˆ {Ut}{E−U− R} due to isomorphism of the groups {U t } and Oˆ {U t} . When we apply the operators in this 1
(n)
last equation to ψk (r), we ﬁnd:
ˆ{
OE
(n ) (n) −R} Oˆ {U t} ψk (r) = Oˆ {U t} Oˆ {E −U −1R } ψk (r) ⇒ ˆ {E−R} ψ˜ (n)(r) = Oˆ {Ut} ψ (n)(r + U −1 R) O
q
k
(n)
Using the fact that ψk (r) is a Bloch state, we obtain:
= ei k·U− Rei k·r u (n) (r + U −1 R) = eik· U− Reik· r u(n)(r + R² ) = ei Uk·Rψk(n) (r) where we have used the fact that k · U −1 R = U k · R, that is, a dot product of two vectors (n )
ψk
(r + U −1R)
1
1
does not change if we rotate both vectors by U . We have also taken advantage of the fact that the operation {U  0}−1 on R produces another Bravais lattice vector R² , Eq. (3.9), and that u (n) (r) is the part of the Bloch state that has the full periodicity of the Bravais lattice, u (n) (r + R² ) = u(n)( r). When the last result is substituted in the previous equation, we get:
ˆ{
−R } ψ˜ q(n) (r) = eiUk· R ψ˜ q(n) (r)
O E
132
3
which proves that
Symmetries Beyond Translational Periodicity
˜ (n)(r), deﬁned in Eq. (3.15), is indeed a Bloch state of wavevector
ψq
q = U k . Therefore, the corresponding eigenvalue must be ±Uk , which is equal to ±k (n ) (n) since we have already proven that the two Bloch states ψk (r) and ψ˜ q (r) have the same (n) eigenvalue. Thus, the energy spectrum ±k has the full symmetry of the point group Q = [{U  0}]. Furthermore, we have shown that the two Bloch states at k and U k are related by: (n )
(n)
˜ (n) = Oˆ {Ut} ψk(n) (r) = ψk(n)({U t}−1r) = ψk(n) (U −1 r − U −1 t)
ψUk (r)
±
which completes our proof of the relations in Eq. (3.15).
The meaning of the theorem we just proved is that from the states and their eigenvalues at the wavevector value k we can obtain the states and corresponding eigenvalues at the wavevector values U k, related to the original value by the elements of the point group Q = {{ U 0}}. The set of vectors U k for {U  0} ∈Q is called the star of k. Another way to connect the eigenvalues and eigenstates at k to those at U k is through the hamiltonian that applies to u (kn) (r), the part of the Bloch wavefunction that has the full translational symmetry of the Bravais lattice:
´
(p + h¯ k )2 2m e
µ
+ V( r)
(n )
u k (r)
= Hˆ spk u (kn)(r) = ±k(n)u (kn) (r)
(3.16)
with V (r) the singleparticle potential that has the full symmetry of the crystal. We ﬁrst note that since {U t } ∈S , Oˆ { U t} leaves the potential invariant: Oˆ { U t} V (r) = V (U −1r−U −1 t) = V ( r). We will ﬁnd the following three relations useful: (i) because p =
ˆ{
 } p = U −1 p
O Ut
−i h¯ ∇r , which means that the translation by t does not affect p; (ii) k · (U −1p ) = (U k ) · p
because when both vectors k and U −1p are rotated by U , their dot product does not change; (iii) (U a)2
= (U −1 a)2 = a2
since the magnitude of a vector does not change when it is rotated by any proper or improper rotation operator U (or by its inverse U −1). We apply the operator Oˆ {U t} to ˆ spk f (r) where f (r) is an arbitrary function, and use the invariability of the potential term H and the relations (i), (ii), (iii) derived above to ﬁnd:
ˆ{
}
OU t
²
ˆ
³
sp Hk f (r)
= =
´
´
h k (U −1p )
p2 2m e
+ ¯ ·m
p2 2m e
+¯
⇒ˆ
e
e
ˆ = ˆ ˆ
sp O{U  t} Hk
e
sp HUk O{U t}
f (U −1r
µ
· + h¯ 2 (U k)2 + V (r) 2m
h (U k ) p me
µ
+ ¯2m + V( r) h 2k 2
²
ˆ{
− t)
 } f (r)
³
OUt
(3.17)
This result shows that Oˆ {U t} does not commute with Hˆ k , because it changes the value of k to U k ; we can use this to obtain the same relations between the eigenvalues and sp
133
3.4
Symmetries of the Band Structure
eigenfunctions at the two values, k and U k, as those that we derived earlier, Eq. (3.15) – we leave the proof of this to the reader (see Problem 5) We note that for the group of operations {U  0} that leave k invariant up to a reciprocal space vector G, U k = k + G, the sp hamiltonian Hˆ k , deﬁned in Eq. (3.16), is also left invariant. The statements we have proved above on the symmetries of the band structure offer a way to achieve great savings in computation, since we need only solve the singleparticle equations in a small portion of the Brillouin zone which can then be used to obtain all the remaining solutions. This portion of the Brillouin zone, which can be “unfolded” by the symmetry operations of the point group to give us all the solutions in the entire Brillouin zone, is called the irreducible Brillouin zone (IBZ).
Example 3.2 Square lattice with one atom per unit cell: C 4v group The symmetries for this model, described by the realspace lattice vectors a1 axˆ , a2 = a yˆ and reciprocalspace vectors b1 = (2π/a) ˆx, b2 = (2π/a)yˆ are:
• • • • • • • •
=
The identity E . Rotation by (2π )/4 around an axis perpendicular to the plane, C 4. Rotation by (2π )/2 around an axis perpendicular to the plane, C 2. Rotation by 3(2 π )/4 around an axis perpendicular to the plane, C 43. Reﬂection on the x axis, σx . Reﬂection on the y axis, σx . Reﬂection on the axis at θ = π/4 from the xaxis, σ1. Reﬂection on the axis at θ = 3π/4 from the x axis, σ3 .
These symmetries constitute the point group Q for this physical system. We assume that the origin is at the position of the atom, so that the group is symmorphic. This point group has the group multiplication table given in Table 3.4: an entry in this table is the result of multiplying the element at the top of its column by the element at the left of its row. The deﬁnition of each element in terms of its action on an arbitrary vector (x, y ) on the plane is also given in the left half of Table 3.4. This group multiplication table can be used to prove that all the group properties are satisﬁed. It is also very useful in identifying the classes in the group: the element E is in a class by itself, as is always the case for any group; the elements C 4, C 34 form a second class; the element C 2 is in a class by itself; the elements σx , σy form a fourth class; the elements σ1 , σ3 form a ﬁfth class. The separation of the group into these three classes can easily be veriﬁed by applying the deﬁnition in Eq. (3.7). For this system the point group is a subgroup of the space group, because it is a symmorphic group and therefore the space group S is given by S = Q × S , where S is the translation group. Using these symmetries we deduce that the symmetries of the point group give an IBZ which is 1/8 that of the ﬁrst BZ, shown in Fig. 3.6. There are a few highsymmetry points in this IBZ (in (k x , k y ) notation): (1) ² = (0, 0), which has the full symmetry of the point group. (2) M = (1, 1)(π/a), which also has the full symmetry of the point group.
134
3
Table 3.4
Symmetries Beyond Translational Periodicity
Group multiplication table for symmetries of the 2D square lattice: each entry
in the table is the result of taking the product of two operations, with the operation on the left of the row acting
ﬁrst and the operation at the top of the column acting
second.
The horizontal and vertical lines in the multiplication table separate the group into the ﬁve classes,
U E C2 C4 C43 σx σy σ1 σ3
Fig. 3.6
C1 , C2 , C 3 , C 4 , C5 .
{U0} (x, y) Oˆ { U 0} (x, y) C1 C2 C 3 ( x, y) ( − x, − y) ( −y, x ) ( y, −x ) ( x, − y) ( −x, y) ( y, x) ( − y, − x)
( x, y ) ( −x, −y) ( y, − x) (−y, x) ( x, − y) (−x, y) ( y, x ) ( −y, −x)
C4
E C2 C4 C34
C2 E C34 C4
C4 C 34 C2 E
C 34 C4 E C2
σx
σy
σ1
σ3
σy
σx
σ3
σ1
σ1
σ3
σy
σx
σ3
σ1
σx
σy
C5
σx
σy
σ1
σy
σx
σ3
σ1
σ3
σ1
σx
σy
σ1
σ3
E C2 C34 C4
C2 E C4 C 34
σy
σx
C4 C34 E C2
σ3
C34 C4 C2 E
Left: The symmetry operations of the 2D square lattice; the thick straight lines indicate the reﬂections (labeled σx , σy , σ1, σ3 ) and the curves with arrows the rotations (labeled C4, C2 , C34). These operations form the C4v group. Right: The IBZ (yellow triangle) for the 2D square lattice with C4v symmetry; the special points are labeled ² , ³ , ´, M, Z, X.
(3) X = (1, 0)(π/a ), which has the symmetries E , C 2, σx , σy . (4) ´ = (k , 0)(π/a ), 0 < k < 1, which has the symmetries E , σx . (5) ³ = (k , k )( π/a), 0 < k < 1, which has the symmetries E , σ 1. (6) Z = (1, k )(π/a), 0 < k < 1, which has the symmetries E , σy . Any point inside the IBZ that is not one of the highsymmetry points mentioned above does not have any symmetry, other than the identity E .
To summarize the discussion so far, we have found that the symmetry properties of the energy spectrum and the singleparticle wavefunctions simplify the task of obtaining the band structure considerably, by requiring that we solve the singleparticle Schr¨odinger equations in the IBZ only. Furthermore, both the energy and the wavefunctions are smooth
135
3.5
Application: Special kPoints
functions of k, which in the limit of an inﬁnite crystal is a continuous variable, so we can understand the behavior of the energy bands by considering their values along a few highsymmetry directions: the rest interpolate in a smooth fashion between these directions. One important point to keep in mind is that Kramers’ theorem always applies, which for systems with equal numbers of spinup and spindown electrons implies inversion symmetry in reciprocal space . Thus, even if the crystal does not have inversion symmetry as one of the point group elements, we can always use inversion symmetry, in addition to all the other point group symmetries imposed by the lattice, to reduce the size of the irreducible portion of the BZ. In many cases, another symmetry operation is actually equivalent to inversion symmetry, so we do not have to add it explicitly in the list of symmetry operations when deriving the size of the IBZ. In the following, since we will be dealing with the point group symmetries that apply to the properties in reciprocal space, we will denote the arbitrary proper or improper rotation that belongs to this group simply by U .
3.5
Application: Special k Points
Another useful application of group theory arguments is in the simpliﬁcation of reciprocalspace integrations. Very often we need to calculate quantities of the type g
1 ±
=N
k ∈BZ
g (k)
V PUC
= (2π )3
¶
g (k ) dk
(3.18)
where k ∈ BZ stands for all values of the wavevector k inside a Brillouin zone (it is convenient to assume that we are dealing with the reduced zone scheme and the ﬁrst BZ). For example, when calculating the electronic number density n (r) in the singleparticle picture we have to calculate the quantities n k (r)
=
± (j ) j ,±k ³0); the latter two are the states deﬁned in Eq. (4.15). The vertical dashed lines at ´b/ 2 indicate the positions of the protons and the green lines indicate the Coulomb potential of the nuclei in the isolated atoms and in the molecule.
the midpoint of the distance between the two protons (the center of the molecule). There are two possibilities for singleparticle states with the proper symmetry under inversion: 1 ψ0 (r) = √ [φ1(r) + φ2(r)] 2 1 (4.15) ψ1 (r) = √ [φ1(r) − φ2(r)] 2 the ﬁrst being a symmetric and the second an antisymmetric wavefunction, upon inversion with respect to the center of the molecule; these are illustrated in Fig. 4.1. The energy that corresponds to these two states is obtained by calculating the expectation value of the hamiltonian Hˆ sp in the wavefunctions ψ0(r) and ψ1 (r). Obviously, these expectation values will be expressed in terms of matrix elements of Hˆ sp in the basis orbitals, that is, ²φi Hˆ sp  φj ³ (i, j = 1, 2) (the bra ²φi  and ket  φi ³ notation for singleparticle states and its extension to manyparticle states constructed as products of singleparticle states are discussed in Appendix C). In order to express the results in more compact and transparent notation, we deﬁne the matrix element of this hamiltonian in the orbital φ1 (r) or φ2 (r) to be: ³ ≡ φ ²1 Hˆ sp φ1 ³ = φ2²Hˆ sp φ2 ³ (4.16) Notice that φ1(r) or φ2(r) are not eigenstates of Hˆ sp (r), and ³ ±= ³0, because φi (r) is an eigenstate of the hamiltonian hi (r) (i = 1, 2), which contains only one proton (at the position Ri ) attracting the electron. However, the wavefunctions φi (r) are fairly localized and die exponentially as a function of the distance from the position of the proton where they are centered, therefore the extra terms that appear in the evaluation of ³ due to the presence of the other proton in Hˆ sp , that is, the terms
169
4.2
The Hydrogen Molecule
2 ²φ1 R−e− r φ1 ³ 2
and
2 ²φ2  R−e− r φ2 ³ 1
are very small, so to a good approximation we may take ³ ≈ ³0 (to be more precise, since the contributions of the above two terms are strictly negative, ³ < ³0). We also deﬁne the socalled “hopping” matrix elements of the singleparticle hamiltonian in the atomic orbital basis: t
ˆ sp φ1³ ≡ −²φ1 Hˆ sp φ2 ³ = −² φ2 H
(4.17)
where we can choose the phases in the wavefunctions φ1(r), φ2(r) to make sure that t is a real positive number. These matrix elements describe the probability of one electron “hopping” from state φ1 (r) to φ2 (r) (or vice versa), within the singleparticle hamiltonian ˆ sp (r); this hopping enhances the kinetic energy of the electrons. The expectation values H ˆ sp in terms of the ψi (r), which we deﬁne as ³b and ³a for i = 0 and i = 1, of H respectively, are:
= ψ² 0Hˆ sp (r)ψ0³ =³ − t ³a = ψ ² 1Hˆ sp (r)ψ1³ =³ + t
³b
(4.18)
ˆ sp ; they We emphasize that the wavefunctions ψ0 (r), ψ1(r) are not eigenfunctions of H are simply singleparticle states with the proper spatial symmetry, and as such more appropriate for describing the state of electrons in the singleparticle hamiltonian than the original atomic orbitals φi ( r) ( i = 1, 2). The results we have derived so far are quite instructive. As seen from Fig. 4.1, the state ψ0(r), with energy expectation value ³ b < ³0 , has more weight in the region near the center of the molecule, which contributes to its stability by enhancing the attraction between negative (electrons) and positive (protons) charges; this was designated as the “bonding” state in the general discussion on bonding in Chapter 1. In contrast to this, the other state, ψ1(r), with energy expectation value ³a > ³0 , has a node at the midpoint between the two protons, and as a consequence has more electronic charge on the regions farther away from the proton positions; this is the state that was designated as “antibonding” in Chapter 1, and does not contribute to the cohesion of the molecule. To complete the picture, we might consider putting two electrons in each of the singleparticle states, taking advantage of their spin degree of freedom by assuming that the spins of the two electrons are opposite when they are in the same spatial wavefunction. More precisely, we take the total spin state to be antisymmetric (a “singlet,” we return to this in more detail shortly) so that the only possibility for the spatial part of the twobody wavefunction is to be totally symmetric with respect to interchange of the electron coordinates, r1 , r2 . These assumptions lead to the following twoelectron wavefunctions: H
(r1 , r2 ) H ±1 (r1 , r2 ) ±0
= ψ0(r1 )ψ0 (r2) = ψ1(r1 )ψ1 (r2)
(4.19) (4.20)
We use the superscript H to denote these twobody wavefunctions, in anticipation of the discussion in the next section; a generalization of this approach is the socalled “Hartree”
170
4
From Many Particles to the SingleParticle Picture
approximation. Since we are now dealing with two electrons, we can write the total hamiltonian as:
ˆ
H(r1, r2 )
2
= Hˆ sp (r1 ) + Hˆ sp (r2 ) + r −e r  1 2
(4.21)
We call the very last term in this expression, the electron–electron repulsion, the “interaction” term. The expectation values of the total hamiltonian in terms of the ±iH (r1, r2 ) H twoelectron wavefunctions, which we deﬁne as E H 0 and E 1 for i = 0, 1, respectively, are:
= ±² 0HHˆ (r1, r2 )±0H³ =2(³ − t ) + U2 H E1 = ± ² 1HHˆ (r1, r2 )±1H³ =2(³ + t ) + U2 E 0H
(4.22) (4.23)
where we have deﬁned the “onsite” repulsive interaction between two electrons, which arises from the interaction term when the two electrons are placed at the same orbital, as: 2
U
≡ φ² i (r1 )φi (r2) r −e r  φi (r1 )φi (r2 )³, 1 2
i
= 1, 2
(4.24)
From its deﬁnition, U is a real, positive number. Other terms arising from the interaction term and oneelectron states at different positions will be considered much smaller in magnitude than U and will be neglected. A model based on these physical quantities, the hopping matrix element t, and the onsite Coulomb repulsion energy U , was introduced originally by J. Hubbard.1 The model contains the bare essentials for describing electronelectron interactions in solids, and has found many applications, especially in highly correlated electron systems. Despite its apparent simplicity, the Hubbard model has not been solved analytically and the effort to determine the physics of this simple but powerful model remains an active area of research. The picture we have constructed so far is quite useful but not entirely satisfactory. The main problem is the very casual treatment of the spin degrees of freedom, and consequently of the symmetry of the twoelectron wavefunction in terms of electron exchange properties. Speciﬁcally, we know that the twoelectron wavefunction must be antisymmetric with respect to exchange of the electron degrees of freedom, including position and spin. This symmetry should not be confused with the symmetry that applies to spatial degrees of freedom, which is imposed by the nature of the hamiltonian, in the present case the inversion symmetry with respect to the center of the molecule. In fact, both types of symmetry should be obeyed by the twoelectron wavefunction. In order to achieve this, we will start over, attempting to build these symmetries into the twoelectron trial wavefunctions from the beginning, in all the ways that this is possible with our chosen basis of the two singleparticle orbitals φ1(r), φ2 (r). Having done this, we will then try to ﬁgure out the optimal linear combination of such trial wavefunctions which gives the lowest total energy for the twoelectron system. The generalization of this type of approach is known as the “Hartree–Fock” approximation. 1 J. Hubbard, Proc. Roy. Soc. A 276, 238 (1963); Proc. Roy. Soc. A 277, 237 (1964); Proc. Roy. Soc. A 281, 401
(1964).
171
4.2
The Hydrogen Molecule
We begin with a discussion of the spin part of the twoelectron wavefunction. As discussed in more detail in Appendix C, the spins of two spin1/2 fermions can be combined in states with total spin S and z projection Sz . Of these states, the one with total spin S = 0, called the spin “singlet,” is antisymmetric with respect to exchange of the fermions, whereas the three states with total spin S = 1 and S z = 0, ´1, called the spin “triplet,” are symmetric with respect to exchange of the electrons. For example, the S z = 0 states for the spin singlet and the spin triplet are: singlet :
], √1 [↑↓ − ↓↑
triplet :
2
] √1 [↑↓ + ↓↑ 2
with the convention that the ﬁrst up or down arrow in each pair corresponds to the particle with label 1 and the second to the particle with label 2. Having built the spin part of the twofermion wavefunction with a speciﬁc symmetry upon exchange, we must next build the spatial part so that the total wavefunction, which is a product of the spatial and spin parts, will be totally antisymmetric upon exchange. Consequently, the part accompanying the spinsinglet state must be symmetric in the spatial coordinates and the part accompanying the spintriplet state must be antisymmetric in the spatial coordinates. Taking into account the symmetry imposed by the hamiltonian, that is, inversion symmetry upon exchange of the electron positions due to the symmetry of the molecule, we ﬁnd that the following twoelectron trial wavefunctions are allowed in terms of the singleparticle orbitals, φ1 (r), φ2(r): (s)
²0
(r1 , r2 ) =
√1
2
[φ1(r1) φ2 (r2) + φ1(r2 )φ2 (r1)]
= φ1(r1 )φ1(r2) = φ2(r1 )φ2(r2) 1 (t) ² (r1 , r2 ) = √ [φ1(r1) φ2 (r2) − φ1(r2 )φ2 (r1)] (s)
(r1 , r2 ) (s) ²2 (r1 , r2 ) ²1
2
(4.25) (4.26) (4.27) (4.28)
(s)
The wavefunction ²0 (r1, r2) is also known as the Heitler–London approximation. Since the three singlet states have exactly the same symmetries, both spatial and electronexchange, any linear combination of them will also have the same symmetries. Therefore, in order to ﬁnd the optimal combination which will give the lowest energy, we need to (s) ˆ (s) construct matrix elements of the twoparticle hamiltonian Hˆ ij = ² ² (s) i  H²j ³ for all possible values of the indices i, j, which produces a 3 × 3 matrix. We then diagonalize this matrix to ﬁnd its eigenvalues and eigenstates. This exercise shows that the three eigenvalues are given by:
²
µ
³
¶
µ
·
= 2³ + 2t λ − λ2 + 1 = 2 ³ − t λ2 + 1 + U2 (s) E 1 = 2³ + U ² ³ ¶ · U µ µ (s) E 2 = 2³ + 2t λ + λ 2 + 1 = 2 ³ + t λ 2 + 1 + 2 (s)
E0
(4.29) (4.30) (4.31)
172
4
From Many Particles to the SingleParticle Picture
and the corresponding twoelectron wavefunctions are: (s) ± 0 (r1, r2) (s)
±1
(s)
±2
1
=N
0
(r1, r2) =
√1
(r1, r2) =
1
2
¸
√
²
(s) 2²0 (r1 , r2 )
(s)
²1
¸
√
N2
+
(s)
²1
(r1 , r2) + ²(s) 2 (r1, r2 ) λ
+
√
³
2²(s) 0 (r1 , r2 ) +
(s)
²1
(4.33)
(r1 , r2) + ²2 (r1, r2 ) λ
−
(4.32)
1 + λ2
(r1 , r2) − ²2 (r1, r2) (s)
¹
√
(s)
1 + λ2
¹ (4.34)
where λ = U / 4t and N 0, N 2 are normalization constants. As far as the triplet state is concerned, since there is only one possibility for the spatial part, namely ²(t) (r1, r2 ), deﬁned in Eq. (4.28), the corresponding energy is: E
(t)
= ²² (t)Hˆ ²(t) ³ =2³
(4.35)
The order of the totalenergy values for the twoelectron states, within what we called heuristically the Hartree–Fock approximation, is: (s)
E0
³(c) (valence states have, by deﬁnition, higher energy than core states). Thus, this term is repulsive and tends to push the corresponding states φ˜ (v) ³ outside the core. In this sense, the pseudopotential represents the effective potential that valence electrons feel, if the only effect of core electrons were to repel them from the core region. Therefore, the pseudowavefunctions experience an attractive Coulomb potential which is shielded near the position of the nucleus by the core electrons, so it should be a much smoother potential without the 1/r singularity due to the nucleus with Z protons at the origin. Farther away from the core region, where the core states die exponentially, the potential that the pseudowavefunctions experience is the same as the Coulomb potential of an ion, consisting of the nucleus plus the core electrons. In other words, through the pseudopotential formulation we have created a new set of valence states, which experience a weaker potential near the atomic nucleus, but the proper ionic potential away from the core region. Since it is this region in which the valence electrons interact to form bonds that hold the solid together, the pseudowavefunctions preserve all the important physics relevant to the behavior of the solid. The fact that they also have exactly the same eigenvalues as the original valence states indicates that they faithfully reproduce the behavior of true valence states. There are some aspects of the pseudopotential, at least as formulated above, that make it somewhat suspicious. First, it is a nonlocal potential: applying it to the state  φ˜ (v) ³ gives
±
(³
c
(v)
− ³ )ψ ³²ψ (c)
(c)
(c)
º
φ˜ (v)³ = V˜ ( r, rµ )φ˜ (v)( rµ )drµ
± ⇒ V˜ ( r, rµ ) = (³ (v) − ³(c) )ψ (c)∗ (rµ )ψ (c)(r) c
This nonlocality certainly complicates things. The pseudopotential also depends on the energy ³ (v ), as the above relationship demonstrates, which is an unknown quantity if we view Eq. (4.129) as the Scrh¨odinger equation that determines the pseudowavefunctions φ˜ (v) ³ and their eigenvalues. Finally, the pseudopotential is not unique. This can be demonstrated by adding any linear combination of ψ (c) ³ states to φ˜ (v) ³ to obtain a new state φˆ (v )³:
±
φˆ (v )³ =φ˜ (v) ³ +
cµ

γ cµ ψ
(cµ )
±
³ ⇒φ˜ (v)³ = φˆ v³ −
cµ

γ cµ ψ
(c µ )
³
(4.133)
where γcµ are constants. Using the new expression for  φ˜ (v) ³ in Eq. (4.129), we obtain:
¸
ˆ sp +
H
± c
¹ ¸
φˆ (v) ³ −
(³(v) − ³(c) )ψ (c) ³²ψ (c) 
¸
±
= ³ (v) φˆ (v) ³ − µ
cµ

γ cµ ψ
(cµ )
³
±
¹
cµ

γ cµ ψ
(c µ )
³
¹
∑ ∑
We can now use ²ψ (c) ψ (c ) ³ =δ ccµ to reduce the double sum c cµ on the lefthand side of this equation to a single sum, and eliminate common terms from both sides to arrive at:
¸
ˆ sp +
H
± c
¹
(³ (v) − ³ (c )) ψ (c )³²ψ (c) 
φˆ (v) ³ =³(v) φˆ (v)³
(4.134)
206
4
From Many Particles to the SingleParticle Picture
This shows that the state φˆ (v) ³ obeys exactly the same singleparticle equation as the state φ˜ (v)³, which means it is not uniquely deﬁned, and therefore the pseudopotential is not uniquely deﬁned. Practice, however, has shown that these features can actually be exploited to deﬁne pseudopotentials that work very well in reproducing the behavior of the valence wavefunctions in the regions outside the core, which are precisely the regions of interest for the physics of solids. As an example, we discuss next how typical pseudopotentials are constructed for modern calculations of the properties of solids.16 We begin with a selfconsistent solution of the singleparticle equations for all the electrons in an atom (core and valence). For each valence state of interest, we take the calculated radial wavefunction and keep the tail starting at some point slightly before the last extremum. When atoms are placed at usual interatomic distances in a solid, these valence tails overlap signiﬁcantly, and the resulting interaction between the corresponding electrons produces binding between the atoms. We want therefore to keep this part of the valence wavefunction as realistic as possible, and we identify it with the tail of the calculated atomic wavefunction. We call the radial distance beyond which this tail extends the “cutoff radius” r c , so that the region r < r c corresponds to the core. Inside the core, the behavior of the wavefunction is not as important for the properties of the solid. Therefore, we can construct the pseudowavefunction to be a smooth function, which has no nodes and goes to zero at the origin, as shown in Fig. 4.7. We can achieve this by taking some combination of smooth functions which we can ﬁt to match the true wavefunction and its ﬁrst derivative at r c , and approach smoothly to zero at the origin. This hypothetical wavefunction must be normalized properly. Having deﬁned the pseudowavefunction, we can invert the Schr¨odinger equation to obtain the potential which would produce such a wavefunction. This is by deﬁnition the desired pseudopotential: it is guaranteed by construction to produce a wavefunction which matches exactly the real atomic wavefunction beyond the core region (r > r c ), and is smooth and
~
(r) 0
r V
Z e /r 2
Fig. 4.7
nuc
(r)
0 ~
V
(r)
r ion
(r)
~ Z e /r V
2
Schematic representation of the construction of the atomic pseudowavefunction φ˜ (r ) and the atomic pseudopotential V˜ ion (r ) (right panel), beginning with the valence wavefunction ψ ( r) and the Coulomb potential of the nucleus V nuc( r) (left panel); the range of the core, beyond which ψ (r ) matches φ˜ (r ) and V˜ ion( r ) matches the Coulomb potential of the ion, is shown shaded in pink. 16 D. R. Hamann, M. Schl¨uter, and C. Chang, Phys. Rev. Lett. 43, 1494 (1979).
207
4.9
The Pseudopotential
nodeless inside the core region, giving rise to a smooth pseudopotential. We can then use this pseudopotential as the appropriate potential for the valence electrons in the solid. This is illustrated schematically below. Basic steps in constructing a pseudopotential
1. Solve 2. Fix 3. Construct
ˆ sp ψ (v)(r ) = [Fˆ sp + V nuc (r )]ψ (v) (r ) = ³(v) ψ (v)( r ) (v) (v ) φ (r ) = ψ (r ) for r ≥ r c (v) φ (r ) for 0 ≤ r < rc , under the following conditions:
H
(i) φ (v)(r ) : smooth, nodeless; (ii) (v)
4. Normalize
φ
5. Invert
[Fˆ
(r ) for 0 ≤ r
sp
0
0
x
V0
Reverse bias:Vb
0
x
0
x
0
x
0 or ²k(n² ) − ²k(n) < 0, which correspond to positive or negative values of the frequency ω. The physical meaning of this is that one case ω > 0 describes the absorption of radiation and the other case ω < 0 the emission of radiation of frequency ω. In the following we will develop expressions that describe the response of the solid to the absorption or emission of light of frequency ω in terms of quantities that can be measured experimentally, that is, the conductivity and the dielectric function. As expected from the above discussion, these quantities will involve the singleparticle states that capture the electronic structure of the solid and energyconserving δ functions. We also expect that the response of the solid will be most pronounced for frequencies ω that (n) (n² ) resonate with energy differences between occupied and unoccupied states, ²k² −²k = h¯ ω. The relevant interaction term Hˆ int (r, t ) is that which describes absorption or emission of photons, the carriers of the electromagnetic ﬁeld:
ˆ int (r, t ) =
H
e m ec
(n )
A(r, t) · p
(6.2)
with A(r, t ) the vector potential of the electromagnetic radiation ﬁeld and p = (h¯ / i)∇r the momentum operator, as discussed in more detail in Appendix C. To understand better what is involved in the photon absorption/emission processes, we will use the relations
ˆ 0, r] = [H
−mih¯ p, Hˆ 0 ψk(n) ³ =²k(n)ψk(n) ³ e
ˆ int (r, t) in Eq. (6.1) as: to rewrite the matrix elements of H ² ±ψk(n² ) Hˆ int ψk(n) ³ =i hec ¯
³
(n ² )
² k²
− ²k(n)
´
A(t ) ·
²
± (n ) rψk(n) ³
ψk²
(6.3)
282
6
Electronic Excitations
which gives for the absorption probability of Eq. (6.1): P i→f (ω)
2
² ±
±2
²
± = 2hπ ωc 2 ± k(n² )(er)ψk(n) ³±± ±A( t) · ψ ¯ k,k²,n,n²
(n ² )
δ (²k ²
− ²k(n) − h¯ ω )
(6.4)
This shows that the relevant quantity at the microscopic level is the expectation value of the dipole moment, expressed as the matrix elements of the operator dˆ = er between intital and ﬁnal states of the electons that are excited by the interaction with light. What is actually measured experimentally is the response of a physical system, such as a molecule or a solid, to the external ﬁeld, assuming that the ﬁeld produces a relatively small change to the state of the system, so that the response is linear in the ﬁeld. For an electromagnetic ﬁeld with electric component E(ω), the linear response is described by the polarizability α(ω), which relates the dipole moment d (ω) to the applied ﬁeld:
²
d (ω) = α (ω) · E(ω ) ⇒ d i (ω) =
α ij (ω )E j (ω)
j
In the last expression we have written out the polarizability as a tensor, with d i , E i the components of the dipole and the ﬁeld vectors. By using a ﬁeld with components only in one direction at a time, we can pick up the diagonal components αii , i = 1, 2, 3 of the polarizability, and deal with the average polarizability given by: α (ω)
= 31 Tr{αij(ω)} =13
²
α ii (ω)
i
which is independent of direction because the trace of the tensor is invariant under rotations. To measure the response of the system, as embodied in α(ω), we can excite the system by applying ﬁelds of strength E 0 and fequency ω, and measure the probability of absorption of this radiation ﬁeld, which experimentally is determined by the photoabsorption crosssection σ (ω):1 σ (ω )
∼ π2em2eh ω Im[α(ω)] ¯
This quantity will have sharp peaks when the frequency ω of the radiation ﬁeld coincides with a resonance of the physical system. Alternatively, we can excite the system with a ﬁeld that is a stepfunction in time,2 E (t) = E 0 θ (t), where θ (t ) is the Heaviside function (see Appendix A). Because this function changes very abruptly at t = 0, its Fourier transform contains all frequencies: E (ω)
=
µ ∞
−∞
E (t )eiω t dt
= E0
¶
π δ (ω)
− i ω1
·
With this expression for the ﬁeld, the imaginary part of the polarizability becomes: Im[α(ω)]
= ω Re[Ed (ω)] 0
1 See, for example, H. A. Bethe and E. E. Salpeter, Quantum Mechanics of One and TwoElectron Atoms and
Molecules (SpringerVerlag, Berlin, 1957). 2 A. Tsolakidis, D. SanchezPortal, and R. M. Martin, Phys. Rev. B 66, 235416 (2002).
283
6.1
Optical Excitations
This last expression gives us a recipe for determining the photoabsorption crosssection, through the Fourer transform d(ω ) of the timedependent dipole moment d (t) deﬁned by:
d (t) =
µ
r n (r, t)dr =
²
±ψk(n) (r, t )rψk(n) (r, t)³
k ,n,²k(n) ωp. We also show in Fig. 6.2 the more general case in which there are contributions from both free and bound electrons. These results make it evident that the dielectric function in the limit ω → 0, called the “static dielectric constant,” has divergent real and imaginary parts from the freeelectron component while from the boundcharge component the real part is a constant larger than unity and the imaginary part vanishes. We elaborate next on the two limiting cases, the freeelectron and boundelectron models.
288
6
25
Electronic Excitations
Free electrons
20
20
15
15
10
10
5
5
0
0
5
5
10
10
15 0
0.5
Bound electrons
25
1
1.5
15
0
0.5
1
1.5
Free & bound electrons
25 20 15 10 5 0 5 10 15 0
Fig. 6.2
0.5
1
1.5
Illustration of the general behavior of the real, ε1( ω) (cyan curves), and imaginary, ε2 (ω) (purple curves), parts of the dielectric function with frequency ω in units of the plasma frequency ωp , for the freeelectron case, ε(f) (ω) (topleft panel) and the boundelectron case, ε (b)( ω) (topright panel). The bottom ﬁgure shows a case where the contributions of the free and bound electrons are added to give the total. In these examples we have taken ω0 /ωp = 0.6 for the pole and η/ωp = 0.075.
The freeelectron result is known as the “Drude model” or the “longitudinal” component, because it refers to the motion of electrons as a uniform sea of charge along the direction of the external ﬁeld. This contribution is usually expressed as: ε
(f)
(ω) = 1 −
2
ωp ω(ω
+ i/τ )
(6.15)
where ωp is the plasma frequency and τ is the “relaxation time,” a quantity with dimensions of time, since it is the inverse of the width η. Since η is associated with the friction that electrons experience as they are moving through the solid, the relaxation time is a measure of the time scale associated with collisions that lead to damping of the oscillatory motion induced by the external ﬁeld. For a good conductor, the friction is very small or equivalently, on the time scale deﬁned by ω −1, the relaxation time is very large. This situation corresponds to: ωτ
µ 1 ⇒ τ1 ¶ ω ⇒ ωτ ¶ ω2
289
6.2
Conductivity and Dielectric Function
and in this limit the dielectric function takes the form ε
(f)
(ω)
2
= 1 − ω2p ω
(6.16)
The boundelectron result is known as the “Lorentz model” or “transverse” component, and is usually expressed as: ε
(b)
(ω) = 1 −
² i
2
λi ωp
(6.17)
2 (ω2 − ω0, i ) + iηi ω
with ωp the plasma frequency and ω0,i the poles in frequency, each associated with a width ηi and a weight λi . There are typically many pole values ω0, i , although in experimental measurements a few of the poles dominate because they are associated with a high density of states corresponding to electronic transitions that involve an energy difference equal to this frequency. This is reﬂected in the value of the weight λi . In the following sections we will explore in more detail the origin of the freeelectron and boundelectron behavior in metals and insulators. Before we delve into the detailed calculations, we present some examples of real solids, where the simple ideas discussed so far are already adequate to explain some of the important features of the dielectric function. In Fig. 6.3 we show the dielectric function of Al, our familiar freeelectronlike solid. In this case, the dielectric function is indeed dominated by the freeelectron component, as is evident by comparing the measured dielectric function to the simple result expected from the Drude model. The plasma frequency found in this case is h¯ ω = 15.2 eV. If we try to estimate the plasma frequency from the density of electrons in Al, taking into account that there are three valence electrons per atom, we ﬁnd h¯ ωp = 15.8 eV, reasonably close to the value obtained by ﬁtting the experimental result to the freeelectron model. In addition to the dominant freeelectron contribution, there is also a very small boundelectron contribution at h¯ ω0 = 1.4 eV, which is related to features of the band structure as indicated in Fig. 6.3; we will return to this later and explain its origin.
E3
E4
2
40
Al
100
2
ωp
0 40 1
1
10
80 0
4
E 3 E4
Fig. 6.3
8
12
16
Energy (eV)
20
Example of the behavior of the real and imaginary parts of the dielectric function, ε1 (ω ), ε2 (ω), for Al, a representative freeelectronlike solid. The value of the plasma frequency h¯ ωp = 15.2 eV is indicated. There is also a very small boundelectronlike contribution, from the features of the band structure (shown on the left) indicated by the symbols E 3 near the point W and E 4 near the point K. Adapted from H. Ehrenreich, H. R. Philipp, and B. Segall, Phys. Rev. 132, 1918 (1963).
290
6
Electronic Excitations
As another example, we consider the case of the noble metals Cu and Ag. In this case, there are 11 valence electrons per atom, which would give plasma frequencies h¯ ωp = 35.9 eV for Cu and 29.8 eV for Ag. However, we know from studying the electronic structure of these metals that the d electron bands are far below the Fermi level and they look almost like atomic states with very little dispersion, suggesting that the electrons in these states are not part of the freeelectron system; instead, they are closer to bound electrons. Indeed, the real part of the dielectric function ε1(ω ) for these two metals can be analyzed into freeelectron and boundelectron contributions, as shown in Fig. 6.4. The freeelectron contribution obtained from analyzing the experimental results gives a plasma frequency of 9.3 eV for Cu and 9.2 eV for Ag. If we consider only the s valence state as contributing to this behavior, which implies only one valence electron per atom, the estimates for the plasma frequency would be 10.8 eV for Cu and 9.0 eV for Ag, much closer to those obtained from experiment. Moreover, the boundelectron contribution from experimental results suggests a pole at h¯ ω0 ≈ 2 eV for Cu and ≈ 4 eV for Ag. The band structures of these two metals show that the highest d bands are about 2 eV and about 4 eV below the Fermi level for Cu and Ag, respectively, as shown in Fig. 6.4. These observations nicely explain the main features of the experimental results.
10 0
E0
ε1(b)
K UW
Γ
10
Γ
X W L
ωp
expt
ε1(f)
20
L
30 0
K UX
E0
2
4
0
E0
4
ε1(b)
Fig. 6.4
X W L
Γ
K UX
0
2
10
Ag
ωp
ε1(f)
12
Γ
8
expt
8
K UW
6
Energy (eV)
4
L
Cu
4
E0
6
Energy (eV)
8
10
Examples of the behavior of the real part of the dielectric function ε 1( ω) for Cu (top) and Ag (bottom): the main features are the pole at h¯ ω0 = 2 eV for Cu and 4 eV for Ag, and the value of the plasma frequency h¯ ωp = 9.3 eV for Cu and 9.2 eV for Ag. The corresponding band structures on the left show the feature (transitions from d bands to the Fermi surface, marked as E0 near the point L) responsible for the behavior near the pole. The experimental results and their analysis into the (f) (b) freeelectron ε1 and the boundcharge ε1 contributions are adapted from H. Ehrenreich and H. R. Philipp, Phys. Rev. 128 , 1622 (1962).
291
6.2
6.2.3
Conductivity and Dielectric Function
Connection to Microscopic Features
For the calculation of the conductivity, we will rely on the general result for the expectation value of a manybody operator Oˆ ({ri }), which can be expressed as a sum of singleparticle operators oˆ (ri ):
ˆ { } = ² oˆ (ri )
O ( ri )
i
in terms of the matrix elements in the singleparticle states, as derived in Appendix C. For simplicity, we will use a single index, the subscript κ , to identify the singleparticle states in the crystal, with the understanding that this index represents in shorthand notation both the band index and the wavevector index. From Eq. (C.21) we ﬁnd that the expectation value of the manybody operator O in the singleparticle states labeled by κ is:
²
±Oˆ ³ = oˆ ²
κ ,κ
κ ,κ
² γ κ ² ,κ
where oˆ κ,κ ² and γκ ,κ² are the matrix elements of the operator oˆ (r) and the singleparticle density matrix γ (r, r² ). We must therefore identify the appropriate singleparticle density matrix and singleparticle operator oˆ (r) for the calculation of the conductivity. As derived by Ehrenreich and Cohen3 to ﬁrstorder perturbation theory, the interaction term of the hamiltonian gives for the singleparticle density matrix: int
γκ ² ,κ
² = ² ² − ²f −−hf(ω + iη) ±ψ ² Hˆ int ψ ³ ¯ κ
κ
κ
κ
κ
κ
where fκ is the Fermi occupation number for the state with energy ²κ in the unperturbed system, and η is an inﬁnitesimal positive quantity with the dimensions of frequency. For the conductivity, the relevant interaction term Hˆ int (r, t ) is that which describes absorption or emission of photons, as mentioned earlier, Eq. (6.2):
ˆ int (r, t ) =
H
e m ec
A(r, t ) · p =
e
º
m ec
ei(q·r−ωt )A0 · p + c.c.
»
(6.18)
where h¯ q is the momentum and ω the frequency of the electromagnetic ﬁeld, A0 is the vector potential, and c.c. stands for complex conjugate. For the transverse component of the ﬁeld, we have the following relation between the transverse electric ﬁeld E t (∇r · Et = 0) and the vector potential At :
Et (r, t ) =
−c1 ∂∂At t ⇒ E t (q, ω) = icω At (q, ω) ⇒ At (q, ω ) = icω Et (q, ω )
(6.19)
With this, the interaction term takes the form
ˆ int (r, t) = −ie Et · p ⇒ ψ± ² Hˆ int ψ ³ =−ie Et ±ψ ² eiq·r et · pψ ³ m ω m ω
H
e
κ
κ
e
κ
κ
(6.20)
where we denote by et the unit vector along the direction of the ﬁeld, for which, since we are working with the transverse component, q · et = 0. 3 H. Ehrenreich and M. H. Cohen, Phys. Rev. 115, 786 (1959).
292
6
Electronic Excitations
The relevant singleparticle operator oˆ (r) is the current, since it describes the response of the physical system to the external ﬁeld. The singleparticle current operator is:
ˆj(q) = −e e−i q·r p ⇒ V me m eV Since in the end we want to use the relation J = σ E to obtain an expression for the ˆj(r) = −e
p
conductivity, assuming an isotropic medium, we will consider only the component of the current that is along the external ﬁeld, that is, its projection in the direction of the ﬁeld et :
−e e−iq·r e · p ⇒ j ² = −e ±ψ e−iq·r e · pψ ² ³ t t , m V m V
et · ˆj(q ) =
κ κ
e
κ
e
(6.21)
κ
Substituting the expressions from Eqs (6.20) and (6.21) into the expression for the expectation value of the current, and dividing by the magnitude of the external ﬁeld, we obtain for the conductivity: σt (q , ω)
2
= mie2 V e
±ψ ² eiq·r et · pψ ³2 ¼f ² − f ω ² ² − ² − h¯ (ω + iη ) , ²
²1
κ
κ
κ κ
½
κ
κ
, q · et
κ
κ
=0
(6.22)
This expression for the conductivity is known as the Kubo–Greenwood formula.4 From this result for the conductivity, and using the general relation derived earlier, Eq. (6.8), we ﬁnd for the dielectric function: 2
εt (q, ω)
= 1 − m42πVeω 2 e
² ±ψκ ² eiq· r et · pψκ ³2 ¼ κ ,κ
²
²κ²
− ² − h¯ (ω + iη)
fκ ²
κ
−f
½ κ
, q · et
=0
(6.23)
In the case of the longitudinal component of the ﬁeld, the derivation is similar, with the interaction hamiltonian being given by:
ˆ int (r, t) = (−e) ³(r, t) ⇒ (−e)³ (q, ω ) = −ie [el · E l (q, ω )], q
q · el
H
=q
as is easily seen from Eq. (6.7). This leads to the following expression for the longitudinal dielectric constant: εl (q, ω)
2
= 1 − 4Vqπ e2
² κ ,κ
²
±ψ ² ei q·r ψ ³2 ¼f ² − f ² − ² − h¯ (ω + i η)
²κ
½
κ
κ
κ
, q · el
κ
κ
=q
(6.24)
We will write explicitly the real and imaginary parts of the dielectric function, ε1 , ε2, as these are measured directly from the reﬂectivity, and one can be obtained from the other by the Kramers–Kronig relations. In the following we will make use of the mathematical identity 1
x
x
− iη = x 2 + η 2 + i
¾
x2
¿
+ η2 ⇒ η
lim
→0+
η
x
x2
1
+ η2 = P x ,
¾
lim
→0+
η
x2
¿
+ η2 = π δ (x ) η
(6.25) with P denoting the principal value, that is, the evaluation of the root x = 0 by approaching it symmetrically from the left and from the right. Applying Eq. (6.25) to the expression for 4 R. Kubo, J. Phys. Soc. Japan 12, 570 (1957); D. A. Greenwood, Proc. Phys. Soc. (London)
A71, 585 (1958).
293
6.2
Conductivity and Dielectric Function
the dielectric function, we ﬁnd:
² ±ψκ ² eiq ·r ψκ ³2 ¼
2
ε1,l (q , ω)
ε2,l (q , ω)
πe = 1 − 4Vq 2
2 2
= −4πVq e2
κ ,κ
² κ ,κ
− ² − h¯ ω
²κ ²
²
fκ ²
κ
−f
½
(6.26)
κ
±ψ ² eiq·r ψ ³2 δ(² ² − ² − h¯ ω ) κ
²
κ
κ
¼
κ
fκ ²
−f
½
(6.27)
κ
for the longitudinal component and similarly for the transverse one: ε1, t (q, ω)
ε2, t (q, ω)
2
= 1 − m42πVeω2 e
2 2
= −m4π2V eω2 e
²  et · κ ,κ
² κ ,κ
²
± eiq·r pψ ³2 ¼f ² − f ² ² −² −h ¯ω
²
ψκ ²
½
κ
κ
κ
(6.28)
κ
κ
et · ψ± ² ei q·r pψ ³2 δ(² ² − ² − h¯ ω) κ
κ
κ
¼
κ
fκ ²
−f
½ κ
(6.29)
Finally, we point out that in the limit of long wavelength, q → 0, which is the physically interesting situation as we shall discuss below, the longitudinal and transverse expressions for interband transitions (n ´= n ² ) become essentially the same, the only difference being in the direction of ﬁeld polarization, embodied in the vectors el , et . To see this, we start with the expression for the longitudinal dielectric constant and expand the exponential that appears in the matrix elements to lowest order in q : eiq·r
≈ 1 + iq · r
(6.30)
which we substitute in the matrix elements. Taking advantage of the facts that qˆ the longitudinal component and ±ψκ ψκ² ³ =δ κ,κ ² , we ﬁnd: lim [εl (q , ω)]
q→ 0
= 1 − 4πVe
2
±ψ ² el · rψ ³2 ¼f ² − f ² =´ ² ² − ² − h¯ (ω + iη)
²
κ
κ
κ
κ
½
κ
κ
= elˆ for
κ
κ
We can now use the relations between momentum and position operators, Eq. (6.3), to rewrite the above expression as: lim [εl (q , ω)]
q→ 0
2
= 1 − 4mπ2eV e
f ² −f el · ψ± ² pψ ³2 ² − ² − h ( ω + i η ) ² (² ² − ² )2 /h¯ 2 ¯ ´= ²
² κ
κ
κ
κ
κ
κ
κ
κ
κ
(6.31)
κ
Next we note that because of the denominators that appear under the matrix elements, the only signiﬁcant contributions come from values of h¯ ω very close to values of the energy differences (²κ ² − ²κ ). Indeed, if we set (²κ ² − ²κ ) ≈ h¯ ω in the denominator of the second factor under the summation in Eq. (6.31), we recover an expression which is the same as that for the transverse dielectric function, Eq. (6.23), in the limit q → 0, with the polarization vector el instead of et . For this reason, in the following, we deal only with the expression for the longitudinal dielectric function, which is simpler. 6.2.4
Implications for Crystals
The expressions that we derived above can be used to calculate the dielectric function of crystals, once we have determined the band structure, that is, solved for all the
294
6
Electronic Excitations
singleparticle eigenfunctions ψκ ³ and corresponding eigenvalues ²κ . We will need to introduce again the wavevector and band indices k, k² , n, n ² explicitly, so that the general expression reads: ε(q , ω)
=1−
²
±ψk(n² ) eiq· rψk(n) ³2 º (n² ) (n) » f k² − fk (n ² ) (n ) k,k ² ,n,n² ²k ² − ² k − h¯ (ω + i η)
4π e 2 ² Vq 2
(6.32)
We note ﬁrst that all the º expressions » we derived involve the difference between two Fermi (n ² ) (n) occupation numbers, fk² − fk . For low enough temperature (which is typically the case), these are either 1 or 0. The only terms that contribute to the sums involved in the expressions for the dielectric functions are those for which: (n ² ) (n) > ²F > ²k k²
⇒
²
º
(n ² )
fk²
= 0, f(kn) = 1
»
(n)
or
²k
(n ² ) k²
> ²F > ²
⇒
º ² (n ) fk ²
= 1, fk(n) = 0
»
that is, one of the states involved must be a valence state (occupied) and the other one a conduction state (unoccupied). We can then label the states explicitly by their band index, (v) (c) (c ) for conduction and (v ) for valence, with f k = 1 and f k² = 0. Taking into account the spin degeneracy of each level, we obtain for the real and imaginary parts: ε1 (q, ω)
ε2 (q, ω)
= 1+ =
16π e 2 ² Vq 2
²
2 2
8π e Vq 2
v,k,c,k²
v,k ,c,k²
±
(c) ψk²
iq· r
e 
³
À
(v) 2 ψk
±ψk(c² )eiq·r ψk(v)³2
º
²
(c)
(²k² (c)
δ (²k ²
−
−
(v) (c) ²k k² (v) ²k )2 (h ω)2
Á
− ¯
»
− ²k(v) − h¯ ω) − δ(²(kc²) − ²k(v) + h¯ ω)
Next, we take a closer look at the matrix elements involved in the expressions for the dielectric function. Since all electronic states in the crystal can be expressed in our familiar Bloch form: ei k·r (n) eik· r ² (n) (n ) iG· r ψk (r) = √ u k (r) = √ α k (G)e (6.33) V
V
G
we ﬁnd the following expression for the matrix element: (n ² ) ψk²
±
iq· r
e 
(n ) ψk
²º
³ =
GG²
»∗
(n² ) ² α k ² (G )
1 (n) α k (G) V
µ
²
²
ei(k−k +q +G−G )·r dr
The last integral produces a δ function in reciprocalspace vectors (see Appendix A): 1 V
µ
²
ei(k −k +q +G)·r dr = δ ( k − k² + q + G) ⇒ k²
= k+ q +G
However, taking into account the relative magnitudes of the wavevectors involved in this condition reveals that it boils down to k² ≈ k, or q → 0. The reason for this is that the momentum of radiation for optical transitions is given by  q =(2π/λ), with λ the ˚ while the crystal wavevectors have wavelength, which in the optical range is λ ∼ 10 4 A, ˚ Consequently, typical wavelength values of order the interatomic distances, that is, ∼ 1 A. ² the difference between the wavevectors k, k of the initial and ﬁnal states due to the photon momentum q is negligible. Taking the value q = 0 in the above equation, and constraining
295
6.2
Conductivity and Dielectric Function
the summation to the ﬁrst BZ (G = 0), leads to socalled “direct” transitions, that is, transitions at the same value of k in the BZ, and therefore between different bands, one occupied and one unoccupied. These are the only allowed optical transitions when no other excitations are present. When other excitations that can carry crystal momentum are present, such as phonons (see Chapter 7), the energy and momentum conservation conditions can be satisﬁed independently, even for indirect transitions, in which case the initial and ﬁnal photon states can have different momenta (see Chapter 8). The limit q → 0 is also useful in analyzing transitions between occupied and unoccupied states across the Fermi level of a metal, for the same band; in this case, the limit must be taken carefully for intraband transitions, as we discuss in detail below. Having established that the longwavelength (small q ) limit is the relevant range for optical transitions, we can now use the results derived earlier, Eq. (6.24), with q = k ² − k. To analyze the behavior of the dielectric function, we will consider two different situations: we will examine ﬁrst, transitions at the same wavevector k² = k but between different bands n ´= n ² and second, transitions within the same band n = n ² but at slightly different values of the wavevector k² = k + q . The ﬁrst kind correspond to interband or boundelectron transitions; they correspond to situations where an electron makes a direct transition by absorption or emission of a photon across the band gap in insulators or semiconductors. The second kind are called intraband or freeelectron transitions; they correspond to situations where an electron makes a transition by absorption or emission of a photon across the Fermi level by changing its wavevector slightly. In both cases, we will be assuming that we are working in the longwavelength limit q → 0. We consider ﬁrst the effect of direct interband transitions, that is, transitions for which k = k ² and n ´= n ² . To ensure direct transitions we introduce a factor δk ,k² in the double summation over wavevectors in the general expression for the dielectric function, Eq. (6.32), from which we obtain, from the transverse component of the dielectric function in the longwavelength ( q → 0) limit: ε
inter
(q, ω) = 1 −
4π e 2 ² ±±
¯ k,n´=n²
Vq 2h
±±
(n² ) iq ·r (n) ψk e ψk


±2 ³±±
(n² )
− fk(n) (n ² n ) ωk − (ω + i η) fk
(6.34)
where we have deﬁned
¯
(n ² n )
h ωk
²
= ²k(n ) − ²k(n)
There are two possible sets of values for the summation indices, giving rise to summation terms [n
= v , n² = c ] ⇒
[n
= c , n² = v ] ⇒
º ² (n ) fk
º ² (n ) fk
»
±
±2
= 0, fk(n) = 1 → ±±±ψk(c)eiq·r ψk(v)³±± »
±
(cv) ωk
±2
= 1, fk(n) = 0 → ±±±ψk(v)eiq·r ψk(c)³±±
−1 − (ω + i η) 1
(vc) ωk
− (ω + i η)
296
6
Electronic Excitations
With these contributions, and taking into account the spin degeneracy of each state, we ﬁnd: ε
inter
(q , ω)
= 1 + 16Vπhe ¯
2
±2 ² ±± (c) ±± ψk rψk(v) ³±± ³
k ,c,v
(cv )
ωk
´ (cv) 2 ωk
− (ω +
(6.35) iη) 2
where we have used the expansion of Eq. (6.30); the summation in the ﬁnal result is over k values in the ﬁrst BZ and (c, v) pairs of values of conduction and valence bands at the same k value. This last expression is the type of expression we mentioned before, Eq. (6.11), with ω0 ´= 0. The terms that appear under the summation in the expression for ε intra (q, ω ) (cv) give large contributions for ω ≈ ωk . For these values of ω, the expression reduces to the Lorentz expression, Eq. (6.17), mentioned earlier. In this expression, ω0,i are the special values for which there is a signiﬁcant portion of the BZ (many k values) with ω(kcv) = ω0,i . The expression for the imaginary part of the dielectric function in particular is very similar to the expressions that we saw earlier for the DOS. The main difference here is that what appears in ε2intra (q , ω) is the density of pairs of states that have energy difference h¯ ω0,i , rather than the DOS at given energy ² . This new quantity is called the “joint density of states” (JDOS), and its calculation is exactly analogous to that of the DOS. This is an important feature of the band structure, which to a large extent determines the behavior of ε2intra( q, ω ). This result corresponds to a material in which only interband transitions are allowed, that is, a material with a band gap. Representative examples of the dielectric function for semiconductors and insulators are shown in Fig. 6.5. We next work out what happens in the intraband transitions, that is, n = n ² and k ² = k + q. To simplify the notation, we deﬁne
¯
(n)
h ωk (q )
= ²(kn+) q − ²(kn) = q · ∇k²k(n) +
¯
h2
2m (n)(k )
q2 ,
1 m (n) (k)
≡
1
3h¯ 2
∇k2²k(n)
(6.36)
with the Taylor expansion in powers of q being valid in the limit q → 0; m (n)( k) is an average effective mass,5 deﬁned by the local (k dependent) curvature of the band. The expression for the dielectric function now takes the form ε
intra
(q, ω) = 1 −
4π e2 ² ±±
¯
Vq 2h
k,n
±±
(n ) ψk+q
i q·r
e 
(n) ψk
±2 ³±±
− f k(n) (n) ωk (q) − (ω + iη) (n )
fk +q
(6.37)
The difﬁculty in setting q = 0 in the present case lies in the fact that in this limit the term 1/ q2 in front of the summation blows up, but the numerator of the summands also vanishes (n ) and in the denominator, ωk (q ) → 0, so all these terms need to be considered together when taking the limit. Again, there are two possibilities for the values of the indices and the corresponding terms in the summation:
º
(n )
(n )
²k q > ²F , ²k
+
»
< ²F
º
»
±
±2
⇒ fk(n+)q = 0, f k(n) = 1 → ±±±ψk(n+) qeiq· r ψk(n)³±±
(n ) ωk (q )
−1 − (ω + i η)
5 To obtain this expression we have assumed that the curvature is isotropic, so that we can deﬁne its average,
and hence a scalar value for the effective mass, which otherwise would be a tensor.
297
Fig. 6.5
6.2
Conductivity and Dielectric Function
Representative examples of the interband contributions to the dielectric function (real and imaginary parts, ε 1inter and εinter , respectively), for semiconductors (Si, Ge, AlP, GaAs) and 2 insulators (C, SiC), obtained from the band structures calculated by DFT methods (calculations performed by G. A. Tritsaris).
º
(n)
(n)
² k q < ²F , ² k
+
» > ²F
º
⇒ fk(n+)q = 1,
(n )
fk
±
»
±2
= 0 → ±±±ψk(n+) qeiq·r ψk(n)³±±
1
(n) ωk (q)
− (ω + iη)
and changing the indices of the occupied and unoccupied states, we can rewrite the expression for the dielectric function as: ε
intra
(q , ω)
4π e2 ² ±±
= 1 + Vq 2h ¯
k,n
±
(n ) ± ψk+q
iq ·r
± ( n ) ±2 ψk ±
e 
³
À
(n)
(n )
ωk
2 fk
(q) − (ω + iη)
+
(n )
Using the expansion of Eq. (6.30) leads to:
±ψk(n+)q eiq· rψk(n) ³ ≈ ψ±k(n+) qψk(n) ³ =1,
for q → 0
Moreover, for q → 0 and any ﬁnite value of ω , we have: (n )
ωk
(q) → 0 ⇒ ωk (q)/ω (n)
¶1
(n)
ωk
2 fk
Á
(q ) + (ω + i η)
298
6
Electronic Excitations
and using Taylor expansions in the small quantity ωk(n) (q)/ω for the two terms in the square brackets, we arrive at: ε
intra
( q, ω )
= 1+ = 1−
¸
4 π e2
¯
Vq 2h
¸
¹
² k ,n
À
2fk(n)
−2ω(kn) (q) ω (ω + iη)
Á
⎛ ⎛ ⎞⎤ ⎞ ¹⎡ (n ) ² ² 4 4 π e2 2 h f ¯ k ⎠⎦ ⎣ q · ⎝ ∇k ²k(n) fk(n)⎠ + q2 ⎝
¯
Vq 2h
¯
h
k,n
m
k,n
(n)
(k)
1 ω(ω
+ iη )
(n)
We notice that, due to Kramers degeneracy, without taking spin into account, ²k must (n ) (n ) be an even function of k, since ²−k = ²k , and therefore its derivative with respect to k (n)
must be an odd function of k ; for the same reason, f k is also an even function of k. These observations imply that the term proportional to q in the above expression will vanish upon summing over k in the BZ. Thus, the only term remaining in the summation over k is the one proportional to q 2 = q2 , which leads to: ε
( q, ω ) = 1 −
¸
intra
4π e 2
¹
V
² 2f k(n) k ,n
1
m (n)(k )
ω(ω
+ iη )
At this point, we need to specify the values of k for which the summand does not vanish. The above derivation was based on the assumption that the band labeled n is such that a (n ) state with eigenvalue ²k +q is occupied (valence state) and another state with eigenvalue is empty (conduction state), or vice versa, in the limit q → 0. This means that the band labeled n must be intersected by the Fermi level. We therefore deﬁne a surface in reciprocal space, S(Fn), associated with this band and containing all the values of k at which the Fermi level intersects the band, that is, on this surface ²k(n) = ²F . The summation that appears in the last equation will then extend over all values of k on this surface. We deﬁne N ele , the number of k values that belong to all such surfaces of bands that are intersected by the Fermi level: (n )
²k
N ele
=
²² n
2
(6.38)
k∈
(n ) SF
which counts all the electronic states, including spin degeneracy, that belong to surfaces deﬁned by the Fermi level. With this deﬁnition, the expression for the dielectric function arising from intraband contributions takes the form
ε
intra
(q, ω) = 1 −
¸
4π e 2N m eV
¹ ele
⎡
⎢ 4 ² ² ⎣
N ele n m (n ) k ∈SF
⎤
me
(n)
(k )
⎥ ⎦
1 ω(ω
+ iη )
(6.39)
where we have set fk(n) = 1. The expression for the intraband dielectric function is precisely the type of expression we mentioned before, Eq. (6.11), with ω0 = 0. In the ﬁnal result we have also introduced a factor of m e /N ele inside the square brackets and its reciprocal factor outside, where m e is the electron mass, to produce more physically transparent expressions. Speciﬁcally, the quantity is parentheses is the square of the bare plasma frequency, while
299
6.2
Conductivity and Dielectric Function
the quantity in brackets is a dimensionless number, giving the average of the band curvature on the surface in reciprocal space where the band intersects the Fermi level, for each such band labeled n; this factor modiﬁes the bare plasma frequency to a value appropriate for the particular solid, whose dielectric behavior due to intraband transitions is determined by this set of bands. The remaining term in the expression for the dielectric function, namely 1/ω(ω + iη), determines its dependence on the frequency, a behavior equivalent to the Drude expression for the dielectric function discussed earlier, Eq. (6.15). The derivations outlined above show that the dielectric function of a metal with several bands will have intraband contributions, described by Eq. (6.39), for small values of ω, as well as interband contributions, described by Eq. (6.35), at higherfrequency values, depending on which pair of bands shows large JDOS, and the corresponding dipole matrix elements do not vanish. In contrast to this, the dielectric function of a semiconductor or insulator will derive only from interband contributions, described by Eq. (6.35), which also depends on large JDOS between pairs of bands and nonvanishing dipole matrix elements. We discuss next representative examples of each type. 6.2.5
Application: Optical Properties of Metals and Semiconductors
We address the behavior of the dielectric function of Al ﬁrst, shown in Fig. 6.3. We saw there that, in addition to the dominant freeelectron contribution, there was a boundelectron contribution at h¯ ω0 = 1.4 eV. This feature comes from direct transitions between occupied and unoccupied states near the W and K points of the BZ. In these regions, marked E 3 and E4 , there exist bands below the Fermi level and above the Fermi level that are almost parallel, hence there exists a large JDOS, and the energy difference between these pairs of bands is approximately 1.4 eV. In Fig. 6.6 we show the dielectric function of the noble metals Cu and Ag for a wide range of energies up to 20 eV. In addition to the boundelectron feature discussed earlier (see Fig. 6.4 and related comments), there are many other interesting features arising from transitions between states below and above the Fermi level that have similar dispersion, that is, their energies are nearly parallel. In the lowenergy region, a major feature is found around 5 eV, which is manifest as a broad peak in Cu and a broad shoulder in Ag. The transitions responsible for this feature span a range of energies, and are marked as E1 for those near the L point and as E2 for those near the X point in the BZ. This behavior closely matches the general behavior of the dielectric function as illustrated in Fig. 6.2. Other features at higher energies can similarly be explained by transitions between parallel bands, of which several examples can be found in different regions of the BZ. Data for the dielectric functions of Al, Cu, Ag, and various other metals are collected in Table 6.1. In this table we compare actual values of the plasma frequency h¯ ωp as extracted from experiments to those obtained from Eq. (6.12), which can be written as:
¯ =
h ωp
¶
16π nat n el ( a/a 0) 3
·1/2
× 13.6058 eV
(6.40)
the latter being an expression based on the number of electrons per unit volume available to partipate in plasmon oscillations; in this expression n at is the number of atoms in the
300
6
Electronic Excitations
4
E2
E1
2 0 2 4
L
K UW
Γ
X W L
Γ
K UX
ε1 E0
2
E2
E1,E 2
0
4
E1
Cu
ε2
5
10
Energy (eV)
E0
20
Ag
ε1
ε2
15
0 2
L Fig. 6.6
K UW
Γ
X W L
Γ
K UX
4
E1,E2 0
5
10
Energy (eV)
15
20
Examples of the behavior of the real and imaginary parts of the dielectric function ε1 (ω), ε2( ω) for Cu (top) and Ag (bottom). In addition to the dbandtoFermisurface feature, marked as E 0 and discussed in Fig. 6.4, other lowenergy features involve transitions near the L point marked as E 1 and transitions near the X point marked as E2 . The experimental results are adapted from H. Ehrenreich and H. R. Philipp, Phys. Rev.128 , 1622 (1962).
conventional unit cell (for the BCC, FCC, diamond, and zincblende crystals), a is the lattice constant of this unit cell in units of a 0 , and nel is the average number of valence electrons per atom. The agreement between these two quantities is quite reasonable when a meaningful value for the average number of valence electrons per atom is used: this means three electrons for Al, one electron for the alkalis (Na, K) and noble metals (Cu, Ag, Au), and just 0.5 electrons for Pt. For semiconductors, it is often easy to identify the features of the band structure which are responsible for the major peaks of the dielectric function. These features are typically related to transitions between occupied and unoccupied bands which happen to be parallel, that is, they have a constant energy difference over a signiﬁcant portion of the BZ, because this produces a large JDOS. We show in Fig. 6.7 the examples of Si and Ge. In the case of Si, for instance, there are two such sets of bands, one in which the highest occupied and lowest unoccupied bands differ by a constant energy of ∼ 3.5 eV near the ´ point, marked as E0 , and the L point, marked as E 1 in Fig. 6.7, and another where they differ by ∼ 4.2 eV near the X point, marked as E2 in Fig. 6.7. Indeed, a major feature in both the real and imaginary parts of the dielectric function of Si [a node in ε1(ω ) and the main peak in ε2(ω)] can be seen at h¯ ω ≈ 4.1 eV in Fig. 6.5. A second feature at h¯ ω ≈ 3.8 eV is seen as a shoulder to the left of the main peak. Similar features appear in the dielectric function of Ge: the peak near h¯ ω ≈ 2 eV is due to interband transitions near the L point, marked as E1 , and the peak near h¯ ω ≈ 4.5 eV is due to interband transitions near the X point, marked as E 2.
301
6.2
Table 6.1
Conductivity and Dielectric Function
Plasma frequencies for various metal and semiconductor
crystals (the crystal structure and lattice constant also included):
ωp
in units of
exp ωp
a0
are
is from
(1) ωp is from the zero of
ﬁtting the Drude model to experimental data,
(l) ε1 (ω ), ω p
a
is the estimate from Eq. (6.40),
is from the maximum of the energy loss function,
Eq. (6.41). All values of the frequencies and inverse relaxation times
h¯ /τ et al. (
) are in electronvolts. Data for metals are from M. A. Ordal
, Applied Optics
24
, 4493 (1985) and for semiconductors from
H. R. Philipp and H. Ehrenreich,
Metal Na (BCC) K (BCC) Al (FCC) Cu (FCC) Ag (FCC) Au (FCC) Pt (FCC) Semiconductor Si (DIA) Ge (DIA) GaAs (ZBL)
Phys. Rev.
129
a/ a0
nat
nel
h¯ ωp
8.11 10.07 7.65 6.82 7.73 7.71 7.4
2 2 4 4 4 4 4
1 1 3 1 1 1 0.5
5.91 4.27 15.77 10.82 8.97 9.00 6.76
a/ a0
nat
nel
h¯ ωp
10.26 10.70 10.68
8 8 8
4 4 4
16.60 15.60 15.63
, 1550 (1963).
h¯ ωp
exp
h¯ /τ
5.71 3.72 14.75 7.39 9.01 9.03 5.15
0.028 0.018 0.082 0.009 0.018 0.027 0.069
h¯ ωp
h¯ ωp
(1)
15.0 13.8 9.7
(l)
16.4 16.0 14.7
As these two examples of semiconductors show, at high enough energies (around 15 eV), the behavior of the dielectric function exhibits the general features expected from both the freeelectron and the boundelectron contributions, that is, ε1 (ω) crosses from negative to positive values. In the case of semiconductors, where the boundelectron contribution is dominant at low frequencies (see also the computed dielectric functions in Fig. 6.5), it is difﬁcult to assign a value to the plasma frequency ωp . This is in contrast to the case of metals, where the lowfrequency behavior clearly exhibits a freeelectron contribution that can be ﬁtted to yield a value for ωp . For semiconductors there are two alternative ways to (1) estimate ωp : from the value at which ε1 (ω) changes sign, which we denote by ωp , or from the value at which the socalled “energy loss” function, deﬁned as ε2 (ω)
ε(ω )2 = −Im (l)
¾
1 ε (ω)
¿
(6.41)
exhibits a maximum, which we denote by ωp ; the energy loss function gives a measure of the energy absorbed by the oscillations of the electron gas in response to the external ﬁeld. In Table 6.1 we show a comparison between the values of ωp obtained from Eq. (6.40) and (l) those of ω(1) p and ωp for the representative semiconductors Si, Ge, and GaAs. In general, (1) (l) the value of ωp appears to be an underestimate, while the value of ωp is higher and closer to ωp.
302
6
Electronic Excitations
Si
E2
E1
E2
40
E0
1.5 Im
2
20
1
1.0
0
E0,E1
p
1
5
10
Energy (eV)
15
Ge
E1
0
K Fig. 6.7
Im
2
10
10
1
0.8
p
1
E1 E2 5
10
0
1.2
20
E2
0.5
Energy (eV)
15
0.4 0
The dielectric function of Si (top) and Ge (bottom), real ε1 and imaginary ε2 parts. The band structures on the left show the excitations that produce the main features in the dielectric constant; these are labeled as E 0 for transitions near the ´ point, E1 for transitions near the L point, and E 2 for transitions near the X point. The value of the plasma frequency marked by ωp corresponds to (1)
, the root of ε1( ω). The experimental results are adapted from H. R. Philipp and H. Ehrenreich, Phys. Rev. 129, 1550 (1963); the quantity −Im ε −1 is shown on the right axis.
ωp
6.3
Excitons
Up to this point we have discussed how crystals can be excited from their ground state by absorption of light quanta, that is, photons; the reverse process, deexcitation of an excited state by emission of photons, is also possible. In treating these effects, we concentrated on dominant features of light absorption of emission, related to portions of the band structure of the crystal where there are many states that can contribute to such processes, namely, there is a large JDOS between occupied and empty bands that can participate in the excitations. In semiconductors and insulators there is another aspect of light absorption that is very important, the lowenergy excitations. This refers to energy values close to the band gap, since at least that much energy is needed to induce an excitation by photon absorption in semiconductors and insulators. In this range of energy, the excited electron and the hole left behind are oppositely charged quasiparticles, and as such interact by a screend Coulomb potential. Because their charges are opposite, the interaction is attractive, but the presence of all the other charged particles in the system provides the screening. The attraction between electron and hole quasiparticles leads to formation of bound states. The bound electron–hole pair is called an “exciton.” Its presence in the optical absorption spectra of semiconductors and insulators is ubiquitous, and can produce very interesting phenomena, such as condensation of these entities, which act like bosons.
303
6.3
Excitons
Moreover, the excitons must dissociate in order to produce free carriers (electrons or holes) that can carry current through the material; this process competes with recombination of the electron and the hole, producing emission of a photon. Thus, exciton dissociation is a process of great practical importance in devices like photovoltaics, that depend on electron excitation by light and subsequent motion of the charges (positive and negative) in the device. The creation and behavior of excitons involves both fascinating physics and important consequences for practical applications. In this section we explore the main ideas in the physics of excitons, ﬁrst through simple heuristic arguments, and then through more detailed models based on the picture of solids that we have developed so far. 6.3.1
General Considerations
Experimentally, the presence of excitons becomes evident when light is absorbed by the solid as individual photons, assuming that each absorbed photon creates an electron–hole pair. The signature of excitons appears in the optical absorption measurements. If there were no excitons, the lowest energy of a photon required to produce an excited electron, while leaving a hole behind, would be equal to the band gap. The presence of the exciton implies that the lowestenergy excitation induced by be absorption of light will correspond to photon energies smaller than the bandgap energy, as expected for an electron–hole pair that is bound by the Coulomb interaction. Quite often, several exciton peaks can be resolved experimentally, reﬂecting the features of the valence and conduction bands of the solid, as shown in Fig. 6.8. There is a wide range of excitons. The limiting cases concern electron–hole pairs that are strongly or weakly bound. In the tightly bound case, the binding energy is of order 1 eV. This is common in insulators, like ionic solids (for example, SiO2); these are referred to as “Frenkel excitons.”6 In the weakly bound case, the exciton is delocalized over a range of several angstroms, and with a small binding energy of order 0.001–0.1 eV (1–100 meV); these are referred to as Wannier or Mott–Wannier excitons 7 and are common in small bandgap systems, especially semiconductors. These two limiting cases are reasonably well understood, while intermediate cases are more difﬁcult to treat. In Table 6.2 we give some examples of materials that have Frenkel or Mott–Wannier excitons and the corresponding band gaps and exciton binding energies. The presence of excitons is a genuinely manybody effect, so we need to invoke the manybody hamiltonian to describe the physics. For the purposes of the following treatment, we will ﬁnd it convenient to cast the problem in the language of Slater determinants composed of singleparticle states, so that solving it becomes an exercise in dealing with singleparticle wavefunctions. We begin by writing the total manybody hamiltonian Hˆ in the form
ˆ {ri }) = ² hˆ ( ri ) + 1 ²
H(
i
2
i´=j
e2
 ri − rj 
,
2 2 ˆ = −h¯ ∇r2 + ² −Z I e 2m e  r − R − tI  R,I
h (r)
6 J. Frenkel, Phys. Rev. 37 , 1276 (1931). 7 N. Mott, Trans. Faraday Soc. 34, 500 (1938); G. Wannier, Phys. Rev. 52, 191 (1937).
(6.42)
304
6
Electronic Excitations
Table 6.2 Examples of Frenkel excitons in ionic solids and Mott–Wannier excitons in semiconductors; the band gap
²gap
and the binding energies of the ﬁrst excitonic state,
E1bin = ²gap − Eexc 1
, Eq. (6.48), are
given in units of electronvolts. [ Sources : M. Fox, Optical Properties of Solids (Oxford University Press, New York, 2001); K. Takahashi, A. Yoshikawa, and A. Sandhu, (Eds),
Wide Bandgap Semiconductors –
Fundamental Properties and Modern Photonic and Electronic Devices (SpringerVerlag, Berlin, 2007).]
Frenkel excitons ²gap
E bin 1
KI
6.3
0.4
KBr
7.4
KCl
8.7
KF
Mott–Wannier excitons ²gap
Ebin 1
²gap
E 1bin
NaI
5.9
0.3
0.7
NaBr
7.1
0.9
NaCl
8.8
10.8
0.9
NaF
RbCl
8.3
0.4
RbF
10.3
0.8
²gap
Ebin 1
ZnS
3.84
0.037
Si
1.17
0.015
0.4
ZnO
3.37
0.9
ZnSe
2.83
0.059
Ge
0.74
0.004
0.017
AlN
6.28
0.044
11.5
0.8
ZnTe
2.39
0.013
GaN
3.52
0.025
CsF
9.8
0.5
CdS
2.58
0.027
GaAs
1.52
0.004
LiF
13.7
0.9
CdSe
1.73
0.015
InP
1.42
0.005
CdTe
1.61
0.012
GaSb
0.80
0.002
k
Absorption (arb. units)
excitons Conduction
exc
E1
excitons gap F
Valence
0 gap Fig. 6.8
electron
exc
E1
hole
k
Left: Modiﬁcation of the absorption spectrum in the presence of excitons (solid red curve) relative to the spectrum in the absence of excitons (faint curve); in the latter case absorption begins at exactly the value of the intrinsic band gap, ²gap. In this example, we show four bound states for excitons, the sharp peaks below ²gap. Right: Schematic representation of the conduction and valence bands and the energy levels in the gap corresponding to electron–hole bound states. The exc bin energy of the ﬁrst exciton state is shown as Eexc 1 ; its binding energy is E1 = ²gap − E1 , see Eq. (6.48).
where R are the lattice vectors and tI are the positions of the ions in the unit cell. In this manner, we separate the part that can be dealt with strictly in the singleparticle framework, namely hˆ (r), which is the noninteracting part, and the part that contains all the complications of electron–electron interactions. For simplicity, in the following we will discuss the case where there is only one atom per unit cell, thus eliminating the index I for the positions of atoms within the unit cell. The manybody wavefunction will have Blochlike symmetry:
305
6.3
± K (r1
Excitons
+ R, r2 + R, ...) = eiK·R±K (r1, r2 , ...)
(6.43)
We will illustrate these issues for the cases of both strongly bound (Frenkel) excitons and weakly bound (Wannier) excitons. For the manybody wavefunctions, we choose to work with Slater determinants in the positions {r} and spins {s } of the electrons. To keep the notation simple and the discussion transparent, we will consider the band structure of a solid with a fully occupied valence band and an empty conduction band; generalization to more bands is straightforward. For a solid consisting of N atoms with two electrons per atom (so that we can have a fully occupied valence band), we then have the general manybody wavefunction
{r}, {s }) =
± K(
± (v) ± ψ (r1) ± k 1↑ ± (v) ± ψk 1↓ (r1) ± ± · ± 1 ± · √ (2N )! ±± · ± ± (v) ± ψkN ↑ (r1) ± (v) ± ψ (r1) kN ↓
±
· · ψ· k(v)↑ (r2N ) ±± · · ψ· k(v)↓ (r2N ) ±±± · · ±± · · ±± · · ±± (v) (v) ψk ↑ (r2) · · ψ ·k ↑ (r2N ) ±±± (v) ψk ↓ (r2) · · ψ ·k(v)↓ (r2N ) ± (v)
(r2) 1↑ (v) ψk ↓ (r2) 1
ψk
1
1
N
N
N
N
In the ground state, all the states corresponding to k values in the ﬁrst BZ will be occupied, and the total wavevector will be equal to 0, since for every occupied k state there is a corresponding −k state with the same energy. Similarly, the total spin will be 0, because of the equal occupation of singleparticle states with up and down spins. Our goal is to create excited states, starting from the groundstate wavefunction, by replacing a singleparticle valence wavefunction that is occupied in the ground state with a singleparticle conduction wavefunction that is empty in the ground state. When we do this, care must be taken to preserve the important features of the manybody wavefunction that should not be affected by the excitation. Speciﬁcally, as argued above, optical excitations involve direct k transitions, as explained in Section 6.2.4, that is, excitation by absorption (or deexcitation by emission) of a photon produces no change in the crystal momentum of electrons or the total spin. Because of the difference in the nature of holes and particles, we need to pay special attention to the possible spin states of the entire system. When the electron is removed from a state with spin s h , the manybody state has a total spin z component S z = − s h , since the original ground state had spin 0. Therefore, the new state created by adding a particle with spin s p produces a manybody state with total spin z component Sz = s p − s h . This reveals that when we deal with hole states, we must take their contribution to the spin as the opposite of what a normal particle would contribute. Taking into consideration the fact that the hole has the opposite wavevector of a particle in the same state, we conclude that the hole corresponds to the timereversed particle state, since the effect of the timereversal operator Tˆ on the energy and the wavefunction is:
ˆ
(n)
↑
T ²k
= ²−(nk) ↓ , Tˆ ψk(n↑)³ =ψ−(nk) ↓ ³
306
6
Table 6.3
Electronic Excitations
Spin conﬁgurations for a particle–particle
pair and a particle–hole pair for spin1/2 particles; in the latter case the ﬁrst spin refers to the particle, the second to the hole.
Spin state S Sz 1 1
1 0
1
−1
0
0
Particle–particle
Particle–hole
↑↑ ↑↓ 1 √2 (↑↑ − ↓↓ ↑↓ + ↓↑ ) ) ↓↓ ↓↑ 1 1 √ (↑↓ − ↓↑ √ (↑↑ + ↓↓ ) ) 2 2 √12 (
as discussed in Chapter 2. Notice that for the particle–hole system, if we start as usual with the highest S z state, which in this case is ↑↓, and proceed to create the rest by applying spinlowering operators (see Appendix C), there will be an overall minus sign associated with the hole spinlowering operator due to complex conjugation implied by time reversal. The resulting spin states for the particle–hole system, as identiﬁed by the total spin S and its z component Sz , are given in Table 6.3 and contrasted with the particle–particle spin states. With these considerations, we are now ready to construct speciﬁc models to capture the nature and behavior of excitons. But before we discuss such detailed models, we provide a heuristic picture that captures the essence of the problem; we will be able to justify this heuristic picture from the more detailed treatment that follows. We shall assume that we are dealing with two quantummechanical entities, a particle with effective mass m e and a hole with effective mass m h . These have been created by an excitation relative to the ground state, in which all states below the Fermi level are occupied and separated by an energy gap ²gap from the unoccupied states. We think of these as quasiparticles of opposite charge, −e for the particle and +e for the hole, interacting with a screened Coulomb potential: 2
V (rp, rh )
= −ε¯ r e − r  0 p h
where ε¯ 0 is the static dielectric constant of the medium in which they move. In this oversimpliﬁed picture, the details of the crystal potential that the particle and the hole experience have been subsumed in a few key features: the dielectric constant of the crystal and the effective masses, which are a consequence of the fact that they are derived from electronic states of the crystal. More speciﬁcally, these effective masses are determined by the curvature at the extrema of the relevant conduction and valence bands corresponding to the particle and hole states. The hamiltonian for this simple system is given by:
ˆ
H(rp, rh )
p2
2
2
= ²gap + 2mp + 2pmh − ε¯ r e − r  e h 0 p h
307
6.3
Excitons
with pp and ph the momentum operator for the particle and the hole. Since the energy is measured relative to the gound state, the hamiltonian includes a constant term ²gap to reﬂect the fact that the particle–hole excitation involves the transfer of an electron from an occupied state below the Fermi level to an unoccupied state above the Fermi level, which differ by this much energy. We now make the standard change of coordinates to the centerofmass R and the relative coordinate r:
R=
+ m h rh , me + mh
m e rp
r = rp − rh
(6.44)
in terms of which we rewrite the hamiltonian as:
ˆ
H(R, r)
2
2
2
= ²gap + 2PM + 2pµ − ε¯ er 0
with p0 and p the momentum operators for the centerofmass and the relative coordinate, and the two new variables for the masses, M and µ , deﬁned by: M
= m e + m h,
µ
= mm e+mmh e
(6.45)
h
Since the last expression of the hamiltonian includes only a kinetic energy term for the centerofmass coordinate, we can write the wavefunction of the system as:
= ±K (R, r) = √1
± K( rp , rh)
V
eiK·R ψ (r)
(6.46)
where we have separated out the centerofmass motion as a plane wave with wavevector K. The twobody Schr¨odinger equation then reads:
¸
ˆ
= ¸E exc K ± K( R , r ) ⇒ ¹ h¯ 2 K2 exc − ²gap − ψ (r) = E ψ (r)
H(R, r)± K(R,
2 2 2 − h¯2∇µr − ε¯ er 0
¹
r)
K
2M
(6.47)
The last expression is simply the Schr¨odinger equation for a hydrogenlike atom, with effective mass of the “electron” equal to µ and Coulomb potential between the “nucleus” and the “electron” screened by the dielectric constant ε¯0 . We have encountered this model before, in the case of dopant impurities in crystals, Section 5.5; by solving this problem, we recover the solutions corresponding to the hydrogen atom, with both the energy and the length scaled by appropriate factors that involve the dielectric constant ε¯ 0 and the effective mass µ. The sequence of energy levels from these solutions corresponds closely to the excitonic peaks found in experimental measurements, discussed in relation to Fig. 6.8. The difference between the value of the gap and the actual energy of the state with the electron–hole pair excitation, a positive quantity, is called the “binding energy” of the exciton, deﬁned as: E bin K, n
= ²gap − E exc K, n
(6.48)
for various states labeled by n . We shall return to these results and provide a detailed discussion of the implications once we have developed a more rigorous justiﬁcation of the origin of Eq. (6.47).
308
6
6.3.2
Electronic Excitations
Strongly Bound (Frenkel) Excitons
For strongly bound (Frenkel) excitons, it is convenient to use a unitary transformation to a new set of basis functions which are localized at the positions of the ions in each unit cell of the lattice. These socalled Wannier functions, discussed in Section 2.7, are deﬁned in (v) terms of the usual band states ψk,s (r) through the following relation: (v)
φs
(r − R)
= √1
N
² k
e−ik·R ψk ,s (r) (v )
(6.49)
Using this new basis, we can express the manybody wavefunction as:
{r}) =
±0 (
± (v) ± φ (r1 − R1) ± ↑ ± (v) ± φ↓ (r1 − R1) ± ± · ± 1 ± √ · (2N )! ±± · ± ± (v) ± φ↑ ( r1 − RN ) ± (v) ± φ ( r1 − RN )
↓
±
· · φ·↑(v) (r2N − R1 ) ±± · · φ·↓(v) (r2N − R1 ) ±±± ± · ± ± · ± ± · ± (v) · · φ·↑ ( r2N − RN ) ±±± · · φ·↓(v)( r2N − RN ) ±
(6.50)
In order to create an exciton wavefunction, we remove a single electron from state φs(vh )(r − (c) Rh) and put it in state φs p (r − Rp). We next construct Bloch states from the proper basis. Let us denote by
± (v) ± φ (r − R ) 1 ± ↑ 1 ± (v) ± φ↓ (r1 − R1) ± ± · ± ± ± ² λ(S,Sz )(s p ) ± (c) · (S,Sz ) ³R ({r}) = √(2N )! ±± φsp (r1 − Ri ) i sp ± · ± ± ± (v) · ± φ (r − R ) N ± ↑ 1 ± (v) ± φ↓ ( r1 − RN )
±
· · φ·↑(v) (r2N − R1 ) ±±± · · φ·↓(v) (r2N − R1 ) ±± ± · ± ± · ± (c) · · φ· s (r2N − Ri ) ±±± ± · ± ± · ± (v) · · φ·↑ ( r2N − RN ) ±±± · · φ·↓(v)( r2N − RN ) ± p
(6.51)
the manybody wavefunction produced by exciting one electron from a valence to a conduction singleparticle state at the unit cell identiﬁed by the lattice vector Ri . There ( S ,S ) are two differences between ³R i z and the groundstate wavefunction ±0 of Eq. (6.50): a valence singleparticle state φ (v )(r) has been changed into a conduction singleparticle state φ (c) (r) at the unit cell identiﬁed by Ri , and the spin of this singleparticle state is now s p, which can be different from the spin of the original singleparticle state, denoted by sh . The new manybody state has total spin S and z projection S z , produced by the combination ( S ,S ) of s p , s h , in the manner discussed above; in the ³Ri z wavefunction, λ(S,Sz) (s p) are the
309
6.3
Excitons
coefﬁcients corresponding to the (S , S z ) state for each s p value as given in Table 6.3. Then, the Bloch state obtained by appropriately combining such states is: N 1 ²
{r}) = √
( S ,S z ) ±K (
N i=1
eiK·R i ³Ri
(S,Sz )
({r})
(6.52) (S,S )
The choice we have made in writing down the manybody wavefunction ³Ri z , namely that the electron and the hole are localized at the same lattice site Ri , represents the extreme case of a localized Frenkel exciton. This can be generalized to a less restrictive situation, where the electron is created at a lattice site different from the hole position, that is, the particle state is at lattice vector Rj , j ´= i, and appears on the ith row of the Slater determinant (see Problem 10). The energy of the state corresponding to the choice of identical electron and hole positions is then: (S,Sz )
EK
² = ±± K(S,S )Hˆ ±K(S,S ) ³ =N1 ei K·(R−R² )±³R(S²,S )Hˆ ³(RS,S )³ z
z
z
z
(6.53)
R ,R ²
(S,S )
Now we can deﬁne the last expectation value as E R ² ,Rz , and obtain for the energy: (S,Sz )
EK
= = =
1 ² N
R,R²
1 ² N
R
( S ,S ) E0 z
²
eiK·(R−R ) E R² ,Rz ( S ,S )
E R,Rz
+ N1
( S ,S )
²² R R² ´=R
²
eiK·(R−R ) E R² ,Rz
( S ,S )
² + e−i K·RE (S,Sz)
(6.54)
R
R´=0
where we have taken advantage of the translational symmetry of the hamiltonian to write (S,S ) ( S ,S ) E R ² ,Rz = E R−Rz ² ; we have also eliminated summations over R² when the summand does not depend explicitly on R, together with a factor of (1/N ). (S,S ) (S,S ) We can express the quantities E 0 z , E R z in terms of the singleparticle states φ (v) (r) ( c ) and φ (r) as follows:
= E 0 + E˜ 0(c) − E˜ 0(v ) + U (0S) (6.55) where E 0 is the groundstate energy, E 0 = ± ± 0Hˆ ±0³, and the other terms that appear in (S,Sz )
E0
this equation are deﬁned as follows:
˜ (c ) = φ± (0c) hˆ φ0(c)³ +V˜ 0(c) , E˜ 0(v ) = φ± 0(v )hˆ φ0(v) ³ +V˜ 0(v) À Á ² e2 e2 ( c ) ( c ) ( v ) ( c ) ( v ) ( c ) ( v ) ( v ) ( c ) ˜0 = V 2±φ0 φR   r − r²  φ0 φR ³ − φ0± φR   r − r²  φR φ0 ³ R E0
˜ (v ) =
V0
(S )
U0
² R
À
2±φ0(v )φR(v)
e2
 r − r²   φ0 2
(v) (v) φR
e2
³ − φ(0±v) φR(v )  r − r²  φ(Rv) φ(0v) ³ 2
= 2δS,0 ±φ0(c)φ0(v)   r −e r²  φ0(v)φ0(c)³ − φ0(±c)φ0(v)   r −e r²  φ0(c )φ0(v)³
(6.56) (6.57)
Á (6.58) (6.59)
310
6
Electronic Excitations
In the expressions above, we have used the shorthand notation φR(n) (r) = φ (n) (r − R) with n = v or c for the valence or conduction states. We have not included spin labels in the singleparticle states φ (n) (r)R , since the spin degrees of freedom have explicitly been taken into account to arrive at these expressions. Hˆ ({ri }), hˆ (r) are the manybody and singleparticle hamiltonians deﬁned in Eq. (6.42). With the same conventions, the last term appearing under the summation over R in Eq. (6.54) takes the form (S,Sz )
ER
≡ U R(S) = ³± (RS,S ) Hˆ ³ (0S,S ) ³ 2 2 = 2δS,0 ±φR(v) φ0(c)   r −e r²  φR(c)φ0(v) ³ −φR(±v) φ0(c)   r −e r²  φ0(v)φR(c) ³ z
z
(6.60)
With these expressions, the energy of the excited state takes the form ( S ,S z )
EK
= E 0 + E˜ 0(c ) − E˜ 0(v) + U (0) 0 + = E 0 + E˜ 0(c ) − E˜ 0(v) +
² −iK·R (S,Sz ) e E R
R ´=0
² −iK·R (S) e U
(6.61)
R
R
( S ,S )
The interpretation of these results is the following: the energy E K z of the system with the exciton in a state of wavevector K and spin S with z component S z is equal to the (c) (v) energy of the ground state E 0 , plus the particle energy E˜ 0 minus the hole energy E˜ 0 ; (S) the last term, based on the deﬁnition of U R from Eq. (6.59) for R = 0 and Eq. (6.60) for R ´= 0, gives the particle–hole interaction. We note that the particle and hole energies, (c ) (v) E˜ 0 and E˜ 0 , represent quasiparticles and contain the contribution from the singleparticle (n) (n ) hamiltonian, ±φ0 hˆ φ0 ³, for n = c and n = v , as well as the interactions of the particle or the hole with all other electrons in the system, expressed by the terms V˜ 0(c) and V˜ 0(v) , respectively. All interaction terms are at the Hartree–Fock level and include the direct Coulomb and the exchange contributions, which is a natural consequence of our choice of a Slater determinant for the manybody wavefunction, Eq. (6.50). To analyze the effects of the presence of excitons, we will assume that K = 0, S = Sz = 0. We then ﬁnd for the energy of the ﬁrst excitation: E exc 1
= E 0(0,0) − E 0 = E˜ (0c) − E˜ (0v) +
² R
(0)
UR
= ²gap +
² R
(0)
UR
where we have deﬁned the bandgap energy ²gap as the difference between the particle and hole quasiparticle energies: ² gap
= E˜ (0c) − E˜ (0v)
From our assumption of localized functions for the singleparticle states φR(n) (r), we conclude that the interaction term is dominated by U 0(0) , that is, the Coulomb and exchange interactions between the particle and the hole situated in the same unit cell, which is given by Eq. (6.59). When the particle and the hole are situated in unit cells a distance R ´= 0 apart, the localized nature of the singleparticle states leads to a much weaker interaction, as shown in Fig. 6.9. In this schematic example, which is based on an ionic insulator composed of positive and negative ions, the excitation consists of taking an electron from
311
6.3
Excitons
+e
e +e
R
e Fig. 6.9
Comparison of Coulomb interaction contributions for excitonic states with the particle and hole situated in the same unit cell (left panel) and in different unit cells a distance R apart (right panel); the unit cells are identiﬁed by the dashed lines. White circles represent positive ions and black circles negative ions. Red and blue clouds represent the density of particle and hole distributions.
the neighborhood of a positive ion (white circle), where it would normally reside in the ground state, to the neighborhood of a negative ion (black circle), and leaving a hole behind. This involves an excitation energy equal to the band gap of the insulator minus the interaction energy between the two charges. Within the strongly bound picture of the exciton derived above, the ﬁnal result for the excitation energy is then: E exc 1
≈ ²gap − +2
µ µ
µ µ
2
φ0(c)( r)2 r −e r² φ0(v )(r² )2 dr dr²
(c)∗
φ0
( r)φ0(v)( r)
e2
(v)∗
r − r²  φ0
(r² )φ0(c) (r²)dr dr²
(6.62)
Since the states φ0(v)( r) and φ0(c )(r) are orthogonal, their overlap is very small, and therefore the second integral in the above equation has much smaller value than the ﬁrst one, which is evidently a positive quantity. This shows that the photon energy h¯ ω = E 1exc, at which there is the ﬁrst absorption peak, is lower than the energy gap by approximately the value of the ﬁrst integral, that is, the exciton binding energy deﬁned in Eq. (6.48). Excitations of higher energy can also be obtained, for instance, by creating a hole at some unit cell and a particle at a nearneighbor cell; this will have a lower binding energy, that is, the difference exc from the value of the gap will be smaller than E bin 1 = ²gap − E 1 , which conﬁrms the qualitative picture of excitons shown in Fig. 6.8. 6.3.3
Weakly Bound (Wannier) Excitons
(n )
For weakly bound (Wannier) excitons, we will use the Bloch states ψk,s (r), in terms of which we must express the manybody wavefunction. Our starting point is the expression for the manybody wavefunction of Eq. (6.44), in which we replace a valence state (v) (c) ψk ,s (r), which becomes the hole state, with a conduction state ψk ,s (r), which becomes h h p p the particle state. The value of k h can be any of the N values that span the ﬁrst BZ, while the value of k p must be such that K = kp − k h to satisfy the total momentum conservation condition; this can be implemented by choosing
312
6
Electronic Excitations
particle : k p = k +
K K , hole : k h = k − 2 2
(6.63)
The value of k, in addition to the value of K, will serve to label the new basis states for the (S) manybody wavefunction, which are now written as ±K (k ; {r}, {s }). We next construct a linear combination of all such wavefunctions with coefﬁcients ξ K( k): (S )
±K
({r}, {s })
=
² k
(S )
ξK
(k )±K (k ; {r}, {s }) (S)
(6.64)
which is our trial wavefunction for solving the problem. All that remains to be done is to (S ) determine the coefﬁcients ξK (k ). Our goal then will be to derive an equation obeyed by these coefﬁcients, so that we can ﬁnd their values. This will be accomplished by requiring (S) the state ±K ({r}, {s }) to be a solution of the Schr¨odinger equation:
ˆ
(S )
H± K
({r}, {s }) = E exc ±K ({r}, {s }) (S )
ˆ the manybody hamiltonian for the system. with H As we have explained earlier, physically relevant processes for photon absorption or emission do not change the total momentum K and total spin S state, since the photon momentum is negligible on the scale relevant to crystal electrons. Unless there is some other type of process that could change the total momentum, we must take K = 0 and S = 0. As an aside, we note that processes which change the momentum during an excitation are indeed relevant in certain cases, involving, for example, the scattering of a quantum of lattice vibrations, called a phonon; the nature of phonons and their interactions with electrons will be examined later, in Chapter 7. In the following discussion we assume that the proper linear combination of spin states is used to ensure that the total spin S = 0, and we consider only the K = 0 case. To simplify the notation, we will drop the superscript S = 0 for the total spin and the subscript K = 0 for the total momentum. The manybody Schr¨odinger equation then takes the form ˆ  ³ =E exc ± ³ ⇒² ξ (k²)±± (k)Hˆ ± (k² )³ =E exc ξ (k)
H ±
k²
(6.65)
where we have taken advantage of the fact that, by construction, the wavefunctions ± (k)³ are orthonormal. In order to determine the values of the coefﬁcients ξ (k), we have to diagonalize the hamiltonian matrix in this basis of states. To calculate the matrix elements that appear in Eq (6.65), we go through the same steps as in the case of the Wannier basis, Eq. (6.53). Fortunately, all the work we did to obtain the Wannier basis matrix elements can be adopted here, with the change in notation that the lattice vector we had labeled “0” maps to the wavevector k and the lattice vector R maps to the wavevector k² ; both k and k² span the ﬁrst BZ. We can then simply rewrite the expressions we found above in terms of the Bloch states  ψk ³, ψk² ³, to obtain for the diagonal matrix elements (k = k² ):
±± (k)Hˆ ± (k)³ =E 0 + E˜ k(c) − E˜ k(v ) + U k
313
6.3
Excitons
with E 0 the groundstate energy and the remaining quantities deﬁned as:
˜ (c) = ψ± k(c )hˆ ψk(c)³ +V˜ k(c) , E˜ (kv) = ψ± k(v) hˆ ψk(v) ³ +V˜ k(v) 2 2 ˜ k(c) = ² 2±ψk(c) ψk(v² )  e ² ψk(c)ψk(v²) ³ − ψ±k(c) ψk(v² ) e ² ψk(v² ) ψk(c) ³ V r − r  r − r  Ek
k²
˜ (v) = ² 2±ψk(v) ψk(v² )  e ² ψk(v)ψk(v²) ³ − ψ±k(v) ψk(v² ) e ² ψk(v² ) ψk(v) ³ r − r  r − r  2
Vk
(6.67)
2
k²
2
Uk
(6.66)
2
= 2±ψk(c) ψk(v)  r −e r²  ψk(v)ψk(c) ³ − ψ±k(c)ψk(v ) r −e r²  ψk(c) ψk(v) ³
while for the offdiagonal matrix elements, k ²
(6.68) (6.69)
´= k, we ﬁnd:
2
2
±±(k)Hˆ ±(k² )³ =2±ψk(c) ψk(v² ) r −e r²  ψk(v )ψk(c² ) ³ − ψk±(c)ψk(v² )  r −e r²  ψk(c² ) ψk(v)³ With these expressions, we can start evaluating the relevant integrals so that we can solve for the coefﬁcients ξ (k ) in Eq. (6.65). These integrals can in principle be evaluated (n ) numerically, since we assume that the singleparticle states ψk (r) are known. For a more transparent solution, we will make some simplifying assumptions. The ﬁrst is that we (n ) will treat the quasiparticle energies E˜ k as known, without having to evaluate either the (n ) singleparticle terms or the twoparticle contributions, V˜ k . In fact, we have seen in the previous chapter that reasonable quasiparticle energies can be obtained from ﬁrstprinciples calculations based on density functional theory or other similar approaches. We then need to concern ourselves only with the terms U k and the offdiagonal matrix elements of the hamiltonian, both of which involve two types of integrals, the Coulomb and the exchange interactions. We will use the familiar expression for the Bloch states, Eq. (6.33), with the assumption that the periodic part, u(kn)( r), is a slowly varying function of k. We then obtain, for the Coulomb integral: 2
1 V2
µ µ
±ψk(c) ψk(v² ) r −e r²  ψk(c² )ψk(v) ³ = (c)∗
uk
(v)∗
(r)uk ² (r² )
e2
(c) (v) ² −i(k−k ² )·(r−r² ) u k² (r)u k (r )e drdr² ² r − r 
The fastvarying part of this integral involves the complex exponential multiplied by the Coulomb potential, with the other parts being slowly varying. We can approximate the integral by taking out the slowly varying parts and replacing them by their averages, denoted by ±· · .·The ³ expression for the integral then becomes:
Â
2
±ψk(c) ψk(v² )  r −e r²  ψk(c² ) ψk(v )³ ≈ u (kc)∗ u(kc²)
Ã Â
(v)∗ (v)
u k² u k
Ã
VC (k
− k² )
with the last term that appears in this result being the Fourier transform of the Coulomb potential: V C( k)
≡ V1
µ
e−i k·r
e2
r dr
314
6
Electronic Excitations
The exchange integral is:
µ µ
2
±ψk(c) ψk(v² ) r −e r²  ψk(v )ψk(c² ) ³ =V12
(c)∗
(v)∗
u k (r)u k² ( r² )
e2
(v)
r − r² uk
(r)uk ² (r² )drdr² (c)
which, with the same approximations as above, takes the form
Â
(c)∗ (v) uk uk
Ã Â
Ã
(v)∗ (c ) 1 uk ² u k² V2
µ µ
e2
² r − r²  drdr
=
Â
(c)∗ (v)
uk uk
Ã Â
(v)∗ (c)
uk ² uk ²
Ã
VC (0)
but the orthogonality of the periodic parts of the Bloch wavefunctions gives:
Â
(c)∗ (v) uk uk
Ã
=
µ
(c)∗ (v ) uk (r)u k (r)dr
Â
= 0,
(v)∗ (c) uk ² uk ²
Ã
=
µ
(v)∗
(c)
u k² ( r)u k² (r)dr
=0
that is, the exchange integral does not contribute. Moreover, since the periodic part of the Bloch wavefunction is slowly varying with k , we can assume that for k² close to k the functions with the same superscipt index are approximately equal, which leads to:
Â
(c)∗ (c) u k u k²
Ã
≈
µ
(c ) (c)∗ uk (r)u k (r)dr
Â
= 1,
(v)∗ (v) uk ² uk
Ã
≈
µ
(v)∗
(v)
u k ( r)u k² (r)dr
=1
Putting all these results together, we ﬁnd for the hamiltonian matrix elements:
±± (k)Hˆ ± (k)³ =E 0 + E˜ k(c) − E˜ k(v ) − VC (0), ±± (k)Hˆ ± (k²) ³ = V−C(k − k² ) We can neglect the groundstate energy E 0 and the average Coulomb potential VC (0), since these are just constants that shift the spectrum. Also, a more careful treatment of manybody effects reveals that the Coulomb integral is modiﬁed by the dielectric function,8 which itself is energy and wavevector dependent, as shown in previous sections of this chapter. For the purposes of the present qualitative discussion, it sufﬁces to include just the static part of the dielectric function ε¯ 0, as an overall factor modifying the Coulomb integral, that is, we take V C (k
− k² ) = ε¯ 1V
˜ (c) − E˜ k(v )
Ek
»
ξ (k )
− ε¯ 1V 0
e2
r e
0
The matrix equation then becomes:
º
µ
−i(k−k ²)·r dr
² µ e 2 −i(k−k ² )·r e dr ξ (k² ) = E exc ξ (k )
r
k²
and turning as usual the summation over k ² values into an integral over the BZ, we arrive at:
º
˜ (c ) − E˜ (kv)
Ek
»
ξ (k)
− ε¯ (21π )3 0
µ µ
e2
r
²
e−i(k−k )·r dr ξ (k² ) dk²
= E exc ξ (k)
(6.70)
Next, we assume that the excitation is taking place across the band gap, between the two band extrema, as shown schematically in Fig. 6.8. In this case, we can write the
8 M. Rohlﬁng and S. G. Louie, Phys. Rev. B 62, 4927 (2000).
315
6.3
Excitons
quasiparticle energies near the band extrema as quadratic approximations in k, with the effective masses of the electron and the hole:
˜ (c) = ²F + ²gap + h¯
Ek
2
2 2 k
2m e
, E˜ k
(v)
h¯ k + = ²F − ²gap 2 2m
2 2
(6.71)
h
where we have assumed the Fermi level ²F to be in the middle of the band gap, as expected for an intrinsic semiconductor or insulator. The two expressions lead to:
º
»
˜ (c) − E˜ (kv) = ²gap + h¯ k 2µ
Ek
2 2
Finally, we introduce the Fourier transform of ξ (k ), which is a function of the realspace position r that we call ψ (r): ξ (k )
= V1
µ
ψ (r)e
−ik ·r dr ⇒ ψ (r) =
µ
1
ξ (k)e
(2π )3
ik ·r
dk
(6.72)
and substituting this in the equation for ξ (k ), we ﬁnd:
À
2 − ¯ 2µ∇ − ε¯ er 0
h 2 r2
Á
ψ (r)
= (E exc − ²gap)ψ ( r)
(6.73)
with µ the reduced mass of the particle–hole pair, deﬁned in Eq. (6.45). The last equation is precisely what we had anticipated based on a simple heuristic picture, Eq. (6.47), with K = 0, the case we have been analyzing here. The energy levels obtained from solving this equation are given by: E nexc
= ²gap −
µe
4
¯¯
2h 2ε20 n 2
= ²gap −
¸
m ee4
2h¯
¹
µ/ m e
1
ε2 0
n2
¯
2
n
= 1, 2, . . .
where the quantity in parentheses is equal to 1 Ry = 13.6058 eV, the energy scale for the actual hydrogen atom. This sequence of values is very similar to typical experimental results, as shown schematically in Fig. 6.8; it is the same sequence of energy values as in the hydrogen atom, scaled by the factor (µ/m e )/ε¯ 20 . Figure 6.10 shows a remarkable experimental demonstration of how reasonable this description is, for the case of the insulator Cu2 O, with the exciton states of index up to n = 25 clearly resolved. In this case, the factor (µ/m e )/ε¯ 02 = 0.00676, giving an “effective Rydberg” value of 92 meV; the static dielectric constant of Cu2O is ε¯ 0 = 7.5, and the effective mass µ = 0.38 m e . The eigenfunctions are also the same as in the case of a hydrogenlike atom, with effective electron mass µ and effective nuclear charge +e/ ε¯0 ; for instance, the lowest eigenfunction, for n = 1, is:
−r/a¯ , ψ1( r) = A 1 e
¯¯ = a¯ = µe 2 h 2 ε0
¸
¯
h2 m ee2
¹
¯ = a ε¯ 0 0 µ/m µ/ m ε0
e
e
(6.74)
where A 1 is the normalization constant and the quantity in parentheses is the Bohr radius, a 0, which sets the length scale for the actual hydrogen atom. From our discussion of the heuristic model, it follows that this is the wavefunction that describes the relative motion of the particle and the hole, while the centerofmass coordinate does not enter the picture
316
Fig. 6.10
6
Electronic Excitations
Left: Excitons in Cu2O, an insulator with a direct band gap ²gap = 2.17208 eV [adapted from “Giant Rydberg excitons in the copper oxide Cu2 O,” T. Kazimierczuk, D. Fr¨ohlich, S. Scheel, H. Stolz, and M. Bayer, Nature 514 , 343 (2014)]. Right: Schematic illustration of the wavefunction of an s state of the exciton, for a ﬁxed position of the hole (blue circle) and the distribution of the electron (red cloud) around it, according to the wavefunction of Eq. (6.74).
because we chose K = 0. Had we considered the case K ´= 0, we would have obtained a planewavelike behavior for the centerofmass coordinate; this case can be developed by following the same steps as above and taking the particle and hole wavevectors to be given by Eq. (6.63). The picture that emerges then is that the weakly bound particle–hole pair moves as a neutral entity with centerofmass momentum h¯ K, and the distribution of one charge relative to the other is described by hydrogenlike wavefunctions with the characteristic length scaled by a factor ε¯ 0/(µ/m e ) relative to the Bohr radius a0 , which, for example, in the case of Cu2 O mentioned above, is approximately 20. To visualize this behavior we show schematically in Fig. 6.10 the wavefunction for the electron–hole pair in the lowestenergy s like state described by Eq. (6.74), with the position of the hole ﬁxed at some point, for a ﬁctitious 2D square lattice. To obtain this picture, we start with the manybody wavefunction of Eq. (6.64), integrate out all the coordinates other than those of the particle rp and the hole rh, whence the expression of Eq. (6.46) emerges, and then plot the values of this effective twoparticle state as a function of rp for a ﬁxed value of rh, supressing the wavelike contribution from the dependence on the centerofmass coordinate R. The reverse picture as a function of rh, with the electron ﬁxed at some position rp , also holds.
Further Reading
1. Electronic Structure and Optical Properties of Semiconductors Chelikowsky (SpringerVerlag, Berlin, 1988).
, M. L. Cohen and J. R.
317
Problems
2. Electronic States and Optical Transitions in Solids , F. Bassani and G. Pastori Parravicini (Pergamon Press, Oxford, 1975). 3. H. Ehrenreich, “Electromagnetic transport in solids: Optical properties and plasma effects,” in J. Tauc (Ed.), Optical Properties of Solids (Course 34 of E. Fermi International Summer School, Varenna, Italy, 1966). This article presents a fundamental theory for solids and includes several examples, some of which were discussed in the text. 4. H. R. Philipp and H. Ehrenreich, “Ultraviolet optical properties,” in R. K. Willardson and A. C. Beer (Eds), Semiconductors and Semimetals , Vol. 3, p. 93 (Academic Press, New York, 1967). This is a general review article, including the theoretical background within the oneelectron framework, but with emphasis on the experimental side. 5. Optical Properties of Solids , F. Wooten (Academic Press, New York, 1972). This book contains a comprehensive treatment of optical properties of solids.
Problems
1.
Prove that if a uniform electron gas is displaced by a small amount in one direction relative to the uniform background of compensating positive charge and then is allowed to relax, it will oscillate with the plasma frequency, Eq. (6.12).
2.
Derive the expressions for the real and imaginary parts of the dielectric function as a function of frequency due to interband transitions, starting with the expression of Eq. (6.35).
3.
Derive the expressions for the real and imaginary parts of the dielectric function as a function of frequency due to intraband transitions, starting with the expression of Eq. (6.39).
4.
Compare the expression for the dielectric function due to interband transitions, Eq. (6.35), to the Lorentz result, Eq. (6.17), and identify the constants in the latter in terms of fundamental constants and the microscopic properties of the solid. Provide a physical interpretation for the constants in the Lorentz expression. Apply this analysis to the case of Si, whose band structure is shown in Fig. 6.7 and real and imaginary parts of the dielectric function are given in Fig. 6.5.
5.
Compare the expression for the dielectric function due to intraband transitions, Eq. (6.39), to the Drude result, Eq. (6.15), and identify the constants in the latter in terms of fundamental constants and the microscopic properties of the solid. Provide a physical interpretation for the constants in the Drude expression.
6.
From the general expression for the dielectric function due to interband transitions, Eq. (6.35), show that the static dielectric constant for semiconductors and insulators, εinter (ω = 0), is a real constant greater than 1.
318
6
7.
Electronic Excitations
An important check on the calculation of the dielectric function values is the socalled “sum rule”: µ ∞ π 2 (6.75) ω ε2 (q , ω) d ω = ω 2 p 0 where ωp is the plasma frequency, Eq. (6.12). We can prove this relation by the following steps. First, show that the double commutator of the hamiltonian Hˆ with e¸iq ·r gives: [Hˆ , eiq ·r ] = eiq ·r
¸
¯
h2 q2
2m e
¹
2 2 º » − i m¯ q · ∇r ⇒ e−iq·r , [Hˆ , eiq·r ] = h¯mq
h2
e
e
We can take the expectation value of the lefthand side in the last relation with respect ∑ to a state ψκ ³, and then insert a complete set of states 1 = κ² ψκ ² ³±ψκ ²  to obtain:
²º κ
±ψ ² eiq· rψ ³2 + ±ψ eiq·r ψ ² ³2 κ
²
κ
κ
»
κ
(²κ ² − ²κ ) =
¯
h 2q 2 me
Using this result, show that: 1 ²º V
κ ,κ
²
fκ
±ψ ² eiq·r ψ ³2 + f ² ±ψ eiq· r ψ ² ³2 κ
κ
κ
κ
κ
»
( ²κ ² − ²κ )
= h¯mq
2 2
N
e
2V
where N is the number of electrons in the solid, V is the total volume, and f κ are Fermi occupation numbers. By comparing this expression to that for the imaginary part of the dielectric function, Eq. (6.27), and integrating over ω, we can establish the sum rule, Eq. (6.75). 8.
Prove the expressions for the various terms in the energy of a Frenkel exciton represented by a Slater determinant of Wannier functions, given in Eqs (6.55)–(6.60).
9.
Using the Fourier transform of the coefﬁcients ξ (k), Eq. (6.72), in the exciton equation, Eq. (6.70), and the result of Eq. (6.71), prove the ﬁnal equation for the exciton wavefunction, Eq. (6.73).
10.
11.
Write the manybody wavefunction ³Ri ,Rz j ({r}, {s }) for a Frenkel exciton with the electron and hole at different lattice sites Ri and Rj . Using this expression, construct a manybody wavefunction with the proper Bloch character for a periodic solid as (S,S ) an expansion over ³ Ri ,Rzj ({r}, {s }) states with appropriate coefﬁcients. Compare this wavefunction with the expression of Eq. (6.52) and discuss the choice of expansion coefﬁcients that make the two manybody wavefunctions identical. ( S ,S )
Using data from Tables 5.2 and 5.3 for the static dielectric constants and effective masses of electrons and holes, estimate the binding energies of excitons for the semiconductors Si, Ge, GaAs, and compare with the experimental values given in Table 6.2.
7
Lattice Vibrations and Deformations
Up to now we have focused mainly on the behavior of electrons in a solid, given the ﬁxed positions of all the ions. This is justiﬁed in terms of the Born–Oppenheimer approximation, and allowed us to study a number of interesting phenomena, including the interaction of solids with light. We next move on to a detailed account of what happens when the ions in a solid move away from their positions at equilibrium, that is, the lowestenergy structure of the entire system. We will again employ the Born–Oppenheimer approximation which is valid for most situations since the typical time scale for motion of ions, 10 −15 sec (femtoseconds), is much slower than the relaxation time of electrons, 10−18 sec (attoseconds). We will examine two broad types of motion: the vibrations of atoms with small amplitude around their equilibrium positions, known as “phonon” modes, and the elastic deformation of a solid, that is, distortion by relatively small changes of atomic positions relative to equilibrium of a very large number of atoms that do not permanently change the shape of the solid. These topics will allow us to access some of the thermal properties of solids, which have to do with transport of mechanical energy by lattice vibrations, and some features of solids that characterize their response to external pressure, like bulk and elastic moduli.
7.1
Lattice Vibrations: Phonon Modes
At a nonzero temperature the atoms that form a crystalline lattice vibrate about their equilibrium positions, with an amplitude that depends on the temperature. Because a crystalline solid has symmetries, these thermal vibrations can be analyzed in terms of collective modes of motion of the ions. These modes correspond to collective excitations, which are typically called “phonons,”1 although strictly speaking phonons are the quanta of these excitations. Unlike electrons, phonons are bosons: their total number is not ﬁxed, nor is there a Pauli exclusion principle governing the occupation of any particular phonon state. This is easily rationalized, if we consider the real nature of phonons, that is, collective vibrations of the atoms in a crystalline solid which can be excited arbitrarily by heating (or hitting) the solid. We next discuss the physics of phonons and how they can be used to describe the thermal properties of solids. The vibrational motions of the atoms are typically discussed in the context of classical dynamics, while the quantum mechanics of the electrons is hidden in the interaction 1 The word phonon derives from the Greek noun 319
φωνη ,
“phoni,” for voice.
320
7
Lattice Vibrations and Deformations
potential between the ions, as discussed in detail in Chapter 4, Sections 4.1 and 4.10. Suppose that the positions of the ions in the crystalline solid at zero temperature are determined by the vectors
Rni
= Rn + ti
(7.1)
where the Rn are the Bravais lattice vectors and the ti are the positions of ions in one primitive unit cell, with the convention that ti  < Rn  for all nonzero lattice vectors. Then the deviation of each ionic position at nonzero temperature from its zerotemperature position can be denoted as:
= δRni
Sni
(7.2)
with n running over all the PUCs of the crystal and i running over all ions in the PUC. In terms of these vectors, the kinetic energy K of the ions will be: K
=
±1 n ,i
2
²
Mi
dS ni dt
³2
=
±1 niα
2
´
Mi
dSniα dt
µ2
(7.3)
where M i is the mass of ion i and α labels the cartesian coordinates of the vectors Sni (α = x, y, z in three dimensions). When ions move, the system has a potential energy in excess of the frozenion potential energy U ion , discussed earlier in Chapter 4. We denote this excess potential energy as ±U , and refer to it in the following as simply the “potential energy,” since this is the term of interest when atoms in the solid deviate from the ideal positions. ±U can be written as a Taylorseries expansion in powers of S ni . The harmonic approximation consists of keeping only the secondorder terms in this Taylor series, with the zerothorder term being a constant (which we can set to zero for convenience). We will also take the ﬁrstorder terms to be zero, since the system is expected to be in an equilibrium conﬁguration at zero temperature, which represents a minimum of the total energy. Higherorder terms in the expansion are considered negligible. In this approximation, the potential energy ±U is then given by: ±U
= 21
±
Sniα
n,i,α ;m ,j,β
∂ 2 E tot ∂ R niα ∂ R mjβ
S mjβ
(7.4)
where the total energy E tot depends on all the atomic coordinates Rni. We deﬁne the socalled forceconstant matrix by: F niα ,mj β
= ∂ R∂
2E tot
niα ∂ R mj β
(7.5)
which has the dimensions of a spring constant, [energy]/[length]2 . In terms of this expression, the potential energy becomes: ±U
= 21
±
n,i,α ;m,j,β
S niα F niα,mjβ Smj β
(7.6)
The size of the forceconstant matrix is d × n at × N , where d is the dimensionality of space (the number of values for α), n at is the number of atoms in the PUC, and N is the number of PUCs in the crystal. We notice that the following relations hold:
321
7.1
Lattice Vibrations: Phonon Modes
∂ 2 ±U ∂ S niα ∂ Smj β ∂ ±U ∂ S niα
=
= F ni ,mj = ∂ R∂ α
±
β
2E tot
(7.7)
niα ∂ R mj β tot
= ∂∂RE
F niα ,mj β S mjβ
(7.8)
niα
m,j,β
where the ﬁrst set of equations is a direct consequence of the deﬁnition of the forceconstant matrix and the harmonic approximation for the energy, while the second set of equations is a consequence of Newton’s third law, since the lefthand side represents the negative of the α component of the total force on ion i in the unit cell labeled by Rn. The motion of the ions will be governed by the following equations: Mi
d2 Sniα d t2
tot
±
niα
m,j,β
= −∂∂RE = −
F niα,mj β Smj β
(7.9)
where we have used Eq. (7.8). We can try to solve the equations of motion by assuming sinusoidal expressions for the time dependence of their displacements:
= √1M u˜ ni
S niα( t)
i
α
e−iωt
(7.10)
where ω is the frequency of oscillation and we have explicitly introduced the mass of the ions in the deﬁnition of the new variables u˜ niα . This gives, when substituted in the equations of motion: ± 2 ω u ˜ niα = F niα,mjβ ¶ 1 u˜ mjβ (7.11) M iM j
m,j,β
We deﬁne a new matrix, which we will call the dynamical matrix, through
˜
D niα,mj β
=¶1
MiM j
(7.12)
F niα,mj β
In terms of this matrix, the equations of motion can be written as:
±
˜
˜
D niα,mj β u mjβ
m,j,β
= ω2 u˜ ni ⇒ D˜ · u ˜= ω2 u˜ α
(7.13)
where we have used bold symbols for the dynamical matrix and the vector of ionic displacements in the last expression. This is an eigenvalue equation, the solution of which gives the values of the frequency and the vectors that describe the corresponding ionic displacements. The size of the dynamical matrix is the same as the size of the forceconstant matrix (i.e. d ×n at × N ). Obviously, it is impossible to diagonalize such a matrix for a crystal in order to ﬁnd the eigenvalues and eigenfunctions when N → ∞ . We need to reduce this eigenvalue equation to a manageable size, so that it can be solved. To this end, we note that from the deﬁnition of the dynamical matrix:
˜
D niα,mj β
=¶1
M iMj
F niα,mjβ
=¶
1 M iMj
∂
2 tot
E
∂ R niα ∂ R mj β
(7.14)
If both positions R niα , R mjβ were to be shifted by the same lattice vector R± , the result of differentiation of the energy with ionic positions must be the same because of the
322
7
Lattice Vibrations and Deformations
translational invariance of the hamiltonian. This leads to the conclusion that the dynamical matrix can only depend on the distance Rn − Rm and not on the speciﬁc values of n and m , that is:
˜
D niα,mjβ
= D˜ i ,j
α β
(Rn − Rm )
(7.15)
Accordingly, we can deﬁne the ionic displacements as follows:
˜
u niα (k)
= ui
α
( k) eik ·Rn
(7.16)
which gives for the eigenvalue equation:
±± j,β
m
˜
− Rm) e−ik·(R −R
˜
=
D iα,j β (Rn
n
m)
u jβ (k )
= ω2 u i
α
(k)
(7.17)
and with the deﬁnition D iα,jβ (k )
=
±
D iα,jβ (R) e−ik· R
R
±
e−ik· Rn ¶
n
∂ 2±U
1 MiM j
∂ S niα ∂ S0jβ
(7.18)
where the last expression is obtained with the use of Eq. (7.7), the eigenvalue equation takes the form
± j,β
D iα ,j β (k) ujβ ( k)
= ω2 ui
α
(k ) ⇒ D(k ) · uk
(l)
=
·
¸ (l ) 2
ωk
(l)
uk
(7.19)
Since D i α,jβ (k) has a dependence on the wavevector k , so will the eigenvalues ω and the eigenvectors u iα , both of which have now been labeled by the value of k. We have also introduced an additional “band” index for the eigenvalues and corresponding eigenvectors, needed for the reason explained below. The size of the new matrix is d × n at , which is a manageable size for crystals that typically contain few atoms per PUC. In transforming the problem to a manageable size, we realize that we now have to solve this eigenvalue problem for all the allowed values of k, which of course are all the values in the ﬁrst BZ. There are N distinct values of k in the ﬁrst BZ, where N is the number of PUCs in the crystal, that is, no information has been lost in the transformation. Arguments similar to those applied to the solution of the singleparticle hamiltonian for the electronic states can also be used here, to reduce the reciprocalspace volume where we need to obtain a solution down to the IBZ only. The solutions to the eigenvalue equation will need to be labeled by the additional “band” index l, which takes d × n at values at each k value, to take into account all the different ions in the PUC and the dimensionality of space in which they move. The solution for the displacement of ion j in the PUC at lattice vector Rn will then be given by: (l ) 1 (l) (l ) Snj (k, t) = ¶ eˆ kj eik ·Rn e−i ωk t (7.20) Mj
where ˆekj is the set of d components of the eigenvector that denote the displacement of ion j in d dimensions. The eigenvectors can be chosen to be orthonormal: (l)
±¹ j
º∗
±
(l) (l ) eˆ kj · ekj ˆ = δll±
(7.21)
323
7.1
Lattice Vibrations: Phonon Modes
In terms of these displacements, the most general ionic motion of the crystal can be expressed as: ± (l) 1 (l) ik ·R −iω(l)t S n,j (t) = ck ¶ eˆ kj e n e k (7.22) Mj
l,k
(l)
where the coefﬁcients c k correspond to the amplitude of oscillation of the mode with (l) (l) frequency ωk . We note that the eigenvalues of the frequency ωk obey the symmetry (l) (l) ωk+G = ωk , where G is any reciprocal lattice vector. This symmetry is a direct consequence of the property D iα,jβ ( k) = D i α,jβ (k + G), which is evident from the deﬁnition of the dynamical matrix, Eq. (7.18). The symmetry of the eigenvalue spectrum allows us to solve the eigenvalue equations for ω(kl) in the ﬁrst BZ only, just like we did for the electronic energies. In both cases the underlying symmetry of the crystal that leads to this simpliﬁcation is the translational periodicity. These analogies are summarized below.
Analogies between phonons and electrons in crystals
d2
S niα dt 2
±
= −
»
m,j ,β
S niα (t)
±
Phonons Mj Mi
˜
i
˜
m ,j,β
α ,j β
β
˜
u niα (k) D iα,jβ (k)
=
±
(l)
(1) (2) (3) (4) (5) (6) (7) (8)
α
(3)
(Rn − Rm ) (4)
= ui
α
(k)eik· Rn (5)
˜
D(k )uk Mj
e−iωt (2)
D iα,jβ (R) e−ik ·R (6)
R
1 S(njl )(k , t ) = ¶
α
= ω2 u˜ ni
D niα,mjβ u mjβ
D˜ ni ,mj = D˜ i α
∂ sp ¯ ∂ t ψ (r, t ) = Hˆ ψ (r, t)
D niα,mj β Smj β (1) ih
= √1M u˜ ni
˜
Electrons
=
·
¸ (l) 2 (l ) uk
ωk
(7)
eˆ (kjl) ei k·R n e−iωk t (8) (l)
ψ (r, t )
= ψ (r)e−i t h¯ ² /
ˆ sp ψ (r) = ²ψ (r)
H
V (r
+ R) = V (r)
ψk (r)
= u k(r)eik·r ,
u k (r
+ R) = uk(r)
ˆ sp = e−ik·r Hˆ sp eik· r
Hk
ˆ sp u (kn) (r) = ²k(n) u (kn) (r)
Hk
(n )
ψk
(r, t) = u (kn)(r)eik ·r e−i ²k
(n )
t/ h¯
Fundamental equation of motion. Separation of timedependent and timeindependent components. Eigenvalue equation for timeindependent component. Fundamental symmetry of operator acting on timeindependent component. Consequences of fundamental symmetry (Bloch states). Operator acting on periodic component of Bloch states. Eigenvalue equation for periodic component of Bloch states. General form of eigenvectors/eigenfunctions, including timedependent part.
324
7
Lattice Vibrations and Deformations
Finally, we can calculate a phonon density of states, just like we did for the electronic eigenvalues in a crystal. The expression for the phonon DOS, by analogy to that for electronic states, for a system in d dimensions is: g (ω)
1
= (2π ) d
±¼ k ,l
1
(l) ω k
=ω
∇kω(kl )
dS k
(7.23)
where S k is a surface in reciprocal space on which the condition ωk = ω is satisﬁed and the summation is over values of k in the ﬁrst BZ and over values of the index l of phonon branches at a given value of k. (l)
7.2
The Born ForceConstant Model
We present next a very simple model for calculating the dynamical matrix. In its ideal, zerotemperature conﬁguration, we can think of the crystal as consisting of atoms with “bonds” between them. These bonds can have covalent, ionic, or metallic character, and in the context of the very simple model we are considering, all the bonds are localized between pairs of atoms. For situations where this picture is reasonable, it is appropriate to consider an effective potential u(Ri , Rj ) between each pair of atoms at positions Ri , Rj (for simplicity of notation, we use here a single index, i or j, to denote the atomic position vectors, with the understanding that this index contains both the unit cell index and the basis index). The total potential energy ±U includes the contributions from all pairs of atoms: ±U
=
±
²ij ³
u (Ri , Rj )
where the notation ²ij ³ stands for summation over all the distinct nearestneighbor pairs. We shall assume that there are two types of distortions of the bonds relative to their ideal positions and orientations: 1. bond stretching, that is, elongation or contraction of the length of bonds, expressed as ± Ri − Rj  , and 2. bond bending, that is, change of the orientation of bonds relative to their original position, expressed as ±θij , where θij is the angle describing the orientation of the bond with respect to a convenient direction in the undistorted, ideal crystal. For the bondstretching term, ur (Ri , Rj ), we will take the contribution to the potential energy to be proportional to the square of the amount of stretching: ur (Ri , Rj )
∼ (±Ri − Rj )2
(7.24)
325
7.2
The Born ForceConstant Model
For the bondbending term, u θ (Ri , Rj ), we will take the contribution to the potential energy to be proportional to the square of the angle that describes the change in bond orientation: u θ (Ri , Rj )
∼ (±θij) 2
(7.25)
It is important to justify on physical grounds our choices for the behavior of the bondstretching and bondbending terms. First, we note that these choices are consistent with the harmonic approximation on which the entire model is based, as discussed in the previous section. The behavior of the bondstretching term is easy to rationalize: we think of bonds as simple harmonic springs, with a spring constant κr , implying that the force due to changes in the equilibrium bond length is proportional to the amount of extension or contraction, ±Ri − Rj , and hence the potential energy is quadratic in this variable, as expressed by Eq. (7.24). The behavior of the bondbending term is a little trickier to explain. This term is related to the preference of atoms to have certain angles between the bonds they form to nearest neighbors. For example, in tetrahedrally bonded solids, with bonds formed by interaction between sp 3 hybrid orbitals, the preferred bond angle is 109.47 o; in planar structures with bonds formed by interaction between sp 2 hybrid oribtals, the preferred bond angle is 120o (for examples of such solids, see Chapter 1). Any deviation from the preferred bond angle will lead to an increase in the potential energy, even if there are no changes in the bond lengths. The reason is that a deviation in angular orientation leads to changes in the nature of the hybrid orbitals that are involved in the bonding, which produces a less favorable (higher potential energy) structure. While these examples were picked from covalently bonded solids, similar arguments can be invoked in the general case. Thus, the bondbending contribution is really a threebody term, since we need three different atomic positions to deﬁne an angle between the two bonds. To see the connection of this threebody term to the bondbending model, we deﬁne the angle between the bonds of atom pairs ij and jk as θijk, with the apex at the middle atom j; similarly, the angle between the bonds of atom pairs ji and il is θjil , with the apex at the middle atom i . When atoms i and j move from their ideal crystal positions, it is these two bond angles that will be affected. We take, as is common, the energy cost for changing a bond angle from its preferred value, θ0 , in the ideal, undistorted crystal to be proportional to a trigonometric function of the new angle minus the value of this function at θ0; this difference is squared, to take into account the equal contributions to the energy for positive and negative changes in the value of the function relative to the ideal one. We will assume that the displacements of the atoms i and j and their neighbors are such that only the two bond angles with apex at those two atoms are affected, and take the energy cost to be: u θ (Ri , Rj )
∼
½¾
¿2
cos(θijk ) − cos( θ0 )
+
¾
¿2 À
cos(θjil ) − cos( θ0 )
As shown in the simple diagram of Fig. 7.1, we can write the angle θijk as θijk = θ0 − ±θij , where ±θij is the change in orientation of the ij pair bond relative to its orientation in the
326
7
Lattice Vibrations and Deformations
θ0 i
Si
k Rij
l
Rij
Δθij Fig. 7.1
θijk
The origin of the bondbending term in the forceconstant model: the open circles denote the positions of atoms in the ideal conﬁguration and the ﬁlled circles their displaced positions; Si , Sj are the atomic displacements; Rij (blue arrow) and R±ij (red arrow) are the original and the distorted relative distances between atoms labeled i and j; ±θij is the change in orientation of the bond between these two atoms, equal to the change in the bond angle between pair ij and pair jk, which has value θ0 in the undistorted conﬁguration.
i
b
R ij
Sj
Rij
Si
j
Δθij Fig. 7.2
Sj
j
Bond stretching and bond bending in the forceconstant model: open circles denote the positions of atoms in the ideal conﬁguration and ﬁlled circles their displaced positions; only the atoms labeled i and j have been displaced by Si , Sj ; Rij (blue arrow) is the original relative distance (Rij  =b), R±ij (red arrow) is the distorted relative distance, and ±θij is the change in orientation of the bond (the angular distortion). The thick blue lines indicate bonds, some of which are stretched or bent due to the displacement of atoms i and j.
ideal crystal. Expanding to lowest order in the small angle ±θij , we ﬁnd that the above expression for the potential energy cost takes the form
¾
¿2
cos( θijk ) − cos(θ0)
=
¾
¿2
cos( θ0 − ±θij ) − cos( θ0 )
≈ sin2(θ0)( ±θij)2
and the same result is found for the term involving the angle θjil. This result justiﬁes our choice for the dependence of the potential energy on the bondbending contribution, Eq. (7.25). A signiﬁcant advantage of this formulation is that now we have to deal with twobody terms, that is, terms that involve only pairs of atoms as opposed to triplets of atoms, needed to specify the bond angles θijk , θjil; this greatly simpliﬁes calculations, both analytical and numerical. One caveat is that this model is not invariant under zerofrequency global rotations as a crystal should be. Nevertheless, it can still provide a reasonable description at nonzero frequencies for small displacements of the atoms from their equilibrium positions. To determine the contributions of bond stretching and bond bending to the potential energy, we will use the diagram shown in Fig. 7.2. The bondstretching energy is given by: ±U r
= 21 κr
±(
²ij ³
)
Rij 2
±
(7.26)
327
7.2
The Born ForceConstant Model
where κr is the force constant for bond stretching, and ± Rij  is the change in the length of the bond between atoms i and j. If we assume that all the bonds are equal to b (this can easily be generalized for systems with several types of bonds), then the change in bond length between atoms i and j is given by ± Rij  =R±ij  −b , where R±ij is the new distance between atoms i and j. We will denote by Si the departure of ion i from its equilibrium ideal position, which gives for the new distance between displaced atoms i and j:
R±ij
¹(
= Sj − Si + Rij ⇒ R ±ij =
) º1/2
− Si + Rij 2
Sj
(7.27)
The displacements S i will be taken to be always much smaller in magnitude than the bond distances Rij , consistent with the assumption of small deviations from equilibrium, in which case the harmonic approximation makes sense. Using this fact, we can expand in powers of the small quantity S i − S j /b , which gives to lowest order:
R±ij =b
´
1+
Rij · (S i − S j )
µ
b2
⇒ ±Rij =R±ij  −b = Rˆ ij · (Si − Sj )
(7.28)
which in turn gives for the bondstretching energy: ±U r
= 21 κr
±¹
ˆ ij (S j − S i ) · R
² ij³
º2
(7.29)
By similar arguments we can obtain an expression in terms of the variables S i , Sj for the bondbending energy, deﬁned to be: ±U θ
±
= 21 κ
θ
²ij ³
b2
(
±θij
)2
(7.30)
with κθ the bondbending force constant and ±θij the change in the orientation of the bond between atoms i and j . Using the same notation for the new positions of the ions (see Fig. 7.2), and the assumption that the displacements Si are much smaller than the bond distances Rij , we obtain for the bondbending term:
R±ij · Rij
²
= R ±ijb cos(±θij) ≈
1 1 − (±θij ) 2 2
³
R± · R R±ijb ⇒ Rij ± bij = 1 − 21 (±θij)2 ij
(7.31)
For the lefthand side of this last equation, we ﬁnd:
R±ij · Rij
R±ijb =
¾
(S j − Si + Rij ) · Rij
²
= 1+
¿ 1 b2
³Á
Rij · (S j − Si ) b2
2 = 1 − Sj − Si  +
2 b2
¾
Á
1+
1+
( Si − Sj )2 b2
Rij · (S i − S j ) b2
(Sj − Si ) · Rij 2b 4
¿2
−
−
2Rij · (Si b2
− Sj )
1 (Si − Sj )2 2 b2
+
Â −1/ 2
3  Rij · (Si − Sj ) 2 2 b4
Â
where we have used the Taylor expansion of (1 + x )−1/2 (see Appendix A) and kept only terms up to second order in the small quantities Si − Sj  /b . This result, when compared to
328
7
Lattice Vibrations and Deformations
the righthand side of the previous equation, gives: (±θij )2 b2
= Sj − Si 2 −
¹
ˆ ij (Sj − Si ) · R
º2
(7.32)
which leads to the following expression for the bondbending energy: ±U θ
=
1 ± κθ 2
²ij³
²
¹
Sj − Si  − (Sj − Si ) · Rˆ ij 2
º2 ³
(7.33)
Combining the two contributions, Eqs (7.29) and (7.33), we obtain for the total potential energy: ² ³ ¹ º2 1± 2 ˆ (κr − κ θ ) (Sj − Si ) · Rij + κθ  Sj − Si  (7.34) ±U = 2
²ij³
where the sum runs over all pairs of atoms in the crystal that are bonded, that is, over all pairs of nearest neighbors.
7.3
Applications of the ForceConstant Model
We will apply next the forceconstant model to a few simple examples that include all the essential features to demonstrate the behavior of phonons, in 1D, 2D, and 3D systems. In each case we will need to set up and diagonalize the dynamical matrix D i α,j β (k) as deﬁned in Eq. (7.18). We take the unit cell of interest to correspond to the zero Bravais lattice vector, and consider nearestneighbor interactions only, in the spirit of the Born forceconstant model. The potential energy ±U then has contributions from all the pairs of atoms in the crystal that are nearest neighbors. We focus on contributions to ± U that involve the atoms of the unit cell corresponding to the zero lattice vector, and employ the full notation for the displacement of ions S niα , S 0j β : n labels the unit cells which contain atoms that are nearest neighbors to the atoms of the unit cell with zero lattice vector; i, j label the atoms in the unit cells, and α, β label the spatial coordinates (α , β = x in 1D, α , β = x or y in 2D, α , β = x, y , or z in 3D). For crystals with nat atoms per unit cell, there are 3× nat modes for each value of k . When nat > 1, there are two types of phonon modes: modes in which the motion of atoms within one unit cell is in phase are referred to as “acoustic,” and are lowerfrequency modes; modes in which the motion of atoms within one unit cell is π out of phase are referred to as “optical,” and are higherfrequency modes. For example, in three dimensions there are three acoustic and three optical modes for a crystal with two atoms per unit cell, and their frequencies in general are not degenerate, except when this is required by symmetry. In cases where there is only one atom per unit cell, there are only acoustic modes. In all cases, the acoustic modes have a frequency that is linear in the wavevector k near the center of the BZ (k → 0); the limit k = 0 corresponds to the translation of the entire crystal in one direction, so naturally the frequency of this motion is zero. The slope of the (n) linear behavior of the frequency ωk near k → 0 with respect to the wavevector gives the
329
7.3
Applications of the ForceConstant Model
velocity of acoustic (very long wavelength) waves in the crystal, which can be different along different crystallographic directions.
Example 7.1 Periodic chain in one dimension We ﬁrst apply the forceconstant model to investigate phonon modes in a 1D inﬁnite chain with one atom per unit cell and lattice constant a , as shown in Fig. 7.3. We assume ﬁrst that all motion is conﬁned in the direction of the chain, taken as xˆ . Since we are dealing with one atom per unit cell with mass M , we do not need to use the atom index i, which we omit for simplicity. The potential energy in this case, with Sn , S m (n = 0, m = ´ 1) having components only in the xˆ direction along the chain, is given by: ±U x
= κ2r
¹
º
(S 1¯ x − S 0x )2 + (S0x − S1x )2
Taking derivatives of this potential energy with respect to the atomic displacements gives the dynamical matrix D x,x (k x ) and its solution ω(1) kx : D x,x (k x )
1 ¹
=M
2κ r − κr (e
º
+ e−ikx a )
ikx a
⇒
(1) ωk x
=
Ã
2κr M
[1 − cos(k x a)]1/ 2
A plot of this expression is shown in Fig. 7.3. Next, we consider the situation in which motion of the atoms in the direction perpendicular to the chain, ˆy, is also allowed. In this case, the potential energy includes another contribution from the displacements in this direction, given by:
= κ2
¹
º
− S0y )2 + (S 0y − S 1y )2 Now we have to solve a dynamical matrix of size 2 × 2, since we have n at = ±U y
θ
(S 1¯y
2 independent directions and still one atom per unit cell, but the offdiagonal matrix elements of this matrix are zero because there are no terms in the potential energy that involve the variables x and y simultaneously. The new matrix element is: D y,y (k x )
= M1
¹
2κ θ
º
− κ (eik a + e−ik a ) θ
x
x
(1)
There are therefore two solutions, one ωkx exactly the same as before, and the second given by (2) ωk x
=
Ã
2κθ M
[1 − cos(k x a)] 1/ 2
which is also shown in Fig. 7.3, with κθ < κr . We calculate the DOS for the phonon modes as a function of the frequency ω, using Eq. (7.23). For the ﬁrst type of phonons corresponding to frequencies ω(1) kx , the DOS, (1) which we will call g (ω ), is given by: g
(1)
(ω) =
1± L
k
δ (ω
−
(1) ωk )
=
1 2π
Ä (1) Ä−1 Ä dω Ä Ä k x Ä dk Ä Ä x (1) Ä dk x Ä ω =ω k
¼
330
Fig. 7.3
7
Lattice Vibrations and Deformations
Illustration of the 1D chain with lattice constant a and one atom of mass M per unit cell, and spring constant κr for bondlength distortions along the chain and κθ for bondangle distortions. The frequency of the phonon modes for displacements along the chain, xˆ (1) (2) direction, labeled ωk (red curve) and perpendicular to it, yˆ direction, labeled ωk (green curve) are shown as functions of k = kx xˆ . The corresponding DOS are shown as functions of (1) ( ω) and a greenshaded curve for g(2) ( ω). The atomic ω, in a redshaded curve for g displacements of the modes with frequencies marked (a), (b), (c), (d) are shown in Fig. 7.4.
with the integral restricted to values of k x that satisfy the condition (1) Differentiating the expression of ωkx with respect to k x , we obtain: dω(1) kx dk x
1 · κr a ¸
=
(1)
M
ωk
x
(1)
We solve for sin(kx a ) under the condition ωkx cos(k x a)
·
sin(kx a )
= ω: 2
= 1 − (2κω/M ) ⇒ r
¸ 1/ 2
sin(k x a) = 1 − cos (k x a) 2
= (2κ /M )1 2 ω
Á
2−
/
r
and with this result we ﬁnd for the density of states: g(1) ( ω)
1
2
= π a (2κ /M )1 2 r
(1)
ωk
/
Á
2−
ω
2
(2κ r /M )
ω
2
(2κ r /M )
Â−1/ 2
Â 1/2
=
ω.
331
7.3
Applications of the ForceConstant Model
(a)
(b)
(c)
(d)
Fig. 7.4
The atomic displacements corresponding to phonon modes in the 1D chain with one atom per unit cell, with frequencies indicated by (a), (b), (c), (d) in Fig. 7.3 for motion along the chain direction (left) and perpendicular to the chain direction (right). The black dashed lines are plots of the function cos(kx a) for the corresponding values of the wavevector: (a) kx = 0, (b) kx = π/ 5a, (c) kx = π/2a, (d) kx = π/a.
where an extra factor of 2 comes from the fact that there are two values of k x in the (1) BZ for which the condition ωkx = ω is satisﬁed for every value of ω in the range (1)
[0, ω1 ]. The result is plotted in Fig. 7.3. Similarly, we can calculate the DOS g(2) (ω) for phonon modes of the second type, also shown in Fig. 7.3. In both cases the DOS is constant, equal to 2/π aω1(i ) for i = 1, 2, for the range of values where the phonon frequency is linear in k x , and it diverges near the maximum value of the frequency. Finally, it is instructive to analyze the actual motion of atoms that corresponds to different modes. This is done by solving for the eigenvectors of the dynamical matrix Dx ,x( kx )S kx
= 2Mκr [1 − cos(k x a )] Sk
x
which gives the trivial solution that S kx is a constant (which we will take to be unity) and the corresponding displacements of the ions at unit cells labeled by n at lattice vectors Rn = na xˆ are given by:
Sn (k x ) =
√1
M
ei k·R n xˆ
= √1
M
einkx a xˆ
These are shown in Fig. 7.4 for selected values of the k x wavevector. Allowing for motion in the y direction produces similar phonon modes with displacements in that direction, also shown in Fig. 7.4 for the same selected values of kx .
Example 7.2 Periodic chain with two different masses in one dimension An interesting variation of this model is the case when there are two ions per unit cell with different masses, M 1 µ= M 2. Now we need to use all three indices for the potential: n , m for the lattice vectors; i, j for the two ions; and x , y for the two directions of motion. We only discuss the case of motion along the x direction. The expression for the potential energy becomes: ±U x
= κ2r
¹
(S 1¯ 2x − S 01x )2 + (S01x − S 02x )2 + (S02x − S11 x )2
º
332
7
Lattice Vibrations and Deformations
This expression for the potential leads to a dynamical matrix with diagonal elements: D 1x,1x (k x )
= 2Mκr ,
and offdiagonal elements: D 2x,1x (k x )
1
·
= −√ κr µ
= 2Mκr 2
¸
1 + eikx a , D 1x,2x (k x)
M1 M 2
We deﬁne the reduced mass
D 2x,2x (k x )
= D ∗2x,1x( kx )
and the ratio of the masses ζ :
µ
= MM 1+MM2 1
2
,
ζ
= MM 2 1
and solve for the eigenvalues of this matrix to ﬁnd the phonon frequencies: (´)
ωk
x
=
Ã
Á
κr µ
Å
1´ 1−
4ζ
(1 + ζ ) 2
sin2
´
kxa
2
µÆ1/2 Â1/ 2
(7.35)
The phonon modes now have two branches, labeled with the superscripts (−), corresponding to lower frequencies and (+), corresponding to higher frequencies; these are the “acoustic” and “optical” branches, respectively. The plot for these two phonon branches as functions of the wavevector k x is shown in Fig. 7.3. By following the same procedure as in the previous example, we can also calculate the DOS for each branch as a function of ω, which is included in Fig. 7.3.
Fig. 7.5
Illustration of the 1D chain with lattice constant a and two atoms per unit cell with masses M1 , M 2 and spring constants κr for bondlength distortions along the chain xˆ between pairs of (−) (+) nearest neighbors. The corresponding acoustic, ωk (red curve) and optical, ωk (blue x x curve) phonon mode dispersions are also shown as functions of k = kx xˆ . The DOS of the two branches is shown as a function of ω on the right.
333
7.3
Applications of the ForceConstant Model
The frequencies near the center and near the edge of the BZ are of particular interest. We will use the subscript 0 for values of  k ≈0 and the subscript 1 for values of k ≈π/a . Near k x ≈ 0, the acoustic and optical branch frequencies become: (−) ω0
≈
»
²
2κ r µ
√ζ ³ ak x , 2(1 + ζ )
(+) ω0
≈
»
Á
2κr
1−
µ
ζ a 2 kx2
Â
8(1 + ζ )2
that is, the lower branch is linear in kx and the higher branch approaches a constant value as k x → 0. At k x = π/a , the frequencies of the two branches become: (−) ω1
=
»
2κ r
´
κθ or equivalently ζ < 1, since the cost of stretching bonds is typically greater than the cost√of bending bonds. The relevant direction in reciprocal space is the vector √ k1 = (k / 2)(xˆ + y),ˆ with 0 ≤ k ≤ π/a; in the perpendicular direction, k 2 = ( k / 2)(xˆ − y ),ˆ the eigenvalues have no dispersion. We analyze the behavior of the √ eigenvalues and the corresponding eigenvectors near the center, √ k = k (xˆ + y )ˆ/ 2, and near the edge of the BZ, k = [( π/a) − k ](xˆ + y)ˆ/ 2. This gives the following results, to leading order in the small quantity k ¶ π/a : at k =
k
√ (xˆ +ˆy) : 2
at k =
(−) ω0
=
»
(π/a ) − k
√
2
ζ κr
2M (1 + ζ ) (xˆ + y)ˆ :
ak ,
(−) ω1
(+) ω0
=
Ã
=
2κθ M
Ã
2(κr + κ θ ) M
,
(+) ω1
=
Ã
Á
1−
ζa
2 2
k
8(1 + ζ )2
2κ r M
(−)
We see that the lowest frequency at k ≈ 0, ω0 , is linear in k = k . From the eigenvector of this eigenvalue in the limit k → 0, we ﬁnd that this mode corresponds to motion of all the atoms in the same direction and by the same amount, that is, uniform translation of the crystal. This motion does not involve bond bending or bond stretching distortions. The eigenvector of the lower branch eigenvalue ω(1−) at k =(π/a ) corresponds to motion of the two ions which is in phase within one unit cell, but π out of phase in neighboring unit cells. This motion involves bond bending √ (−) distortions only, hence the frequency eigenvalue ω1 ∼ κθ . For the eigenvalue (+) ω0 , we ﬁnd an eigenvector which corresponds to motion of the ions against each other within one unit cell, while the motion of equivalent ions in neighboring unit cells is in phase. This mode involves both bond stretching and bond bending, hence √ (+) (+) the frequency eigenvalue ω0 ∼ κr + κθ . Finally, for the eigenvalue ω1 , we ﬁnd an eigenvector which corresponds to motion of the ions against each other in the same unit cell, while the motion of equivalent ions in neighboring unit cells is π out of phase. This distortion involves bond stretching only, hence the frequency eigenvalue (+) ω1 ∼ √κr. The motion of ions corresponding to these four modes is illustrated in Fig. 7.6. There are four other modes which are degenerate to these and involve similar motion of the ions in the yˆ direction. In this example we get two branches because we have two atoms per unit cell, so the inphase and outofphase motion of atoms in the unit cell produce two distinct modes. Moreover, there are doubly degenerate modes at each value of k because we are dealing with a 2D crystal which has symmetric couplings in the xˆ and yˆ directions. This degeneracy would be broken if the couplings between atoms were not symmetric in the different directions.
Example 7.4 2D square crystal As another example we consider the 2D square lattice with lattice constant a in the x and y directions, and one atom of mass M per unit cell. This is illustrated in Fig. 7.7.
Â
336
7
Lattice Vibrations and Deformations
S 0 1 ,x S 0 1 ,y
a2
S 1 0 ,y
S 00 ,y
S 1 0 ,x
S 1 0 ,x
S 00,x
S 1 0 ,y
a1
S 0 1 ,x
S 0 1 ,y Fig. 7.7
The 2D square lattice with lattice constants a1 = axˆ , a2 = ayˆ , with one atom per unit cell. The displacements of one atom at the center and its four nearest neighbors, that enter in the expressions for the dynamical matrix, are shown by arrows.
Since we now have two independent lattice vectors, a1 = a xˆ , a2 = a yˆ , we will employ a slightly modiﬁed notation to exemplify the setup: we denote the atomic displacements as S nm,α , where n and m are the indices identifying the multiples of vectors a1 and a2, respectively, that determine the unit cells, and α = x or y . For the unit cell at the origin, the atomic displacement has components S 00,x , S 00, y, while for its four nearest neighbors, the components are S nm,α with n = ´ 1 and m = ´ 1 (the values −1 are denoted as 1¯ in each case). The potential energy is given by: ±U
= 21 (κr − κ
θ
)[(S00, x − S 10,x )2 + (S00, x − S 1¯ 0,x )2 +
− S01,y )2 + (S 00,y − S01¯ ,y )2] + 12 κ [( S00,x − S 10,x )2 + ( S00,x − S 1¯ 0,x )2 + ( S00,y − S 10,y )2 + (S 00,y − S 1¯ 0,y )2 ] (S 00,y
θ
+ 21 κ [( S00,x − S 01,x )2 + ( S00,x − S 01¯ ,x )2 + ( S00,y − S 01,y )2 + (S 00,y − S 01¯ ,y )2 ] θ
Differentiating the potential energy, we obtain the matrix elements of the dynamical matrix:
= 2κr + 2κ − κr(eik a + e−ik a ) − κ D y,y (k ) = 2κr + 2κ − κr (eik a + e−ik a ) − κ
D x,x (k )
θ
θ
x
x
y
y
θ
(eiky a + e−iky a )
θ
(eikx a + e−ikx a )
with the offdiagonal matrix elements zero. Diagonalizing this matrix we ﬁnd the eigenvalues of the two frequencies: (1)
ωk
(2) ωk
= =
²
2κ r M
²
(1
− cos(k x a)) + 2Mκ
θ
(
³ ) (1/ 2)
1 − cos( ky a )
³(1/ 2)
) 2κθ 2κ r ( 1 − cos(k y a ) + ( 1 − cos(k x a) ) M
M
337
7.3
Applications of the ForceConstant Model
(c) (d)
4
4
(a) 3
3
2
2
(b)
1 0 M
Fig. 7.8
1
Y
X
M
DOS (arb.units)
( a)
( b)
(c)
(d) (1)
0
(2)
Top: The frequencies of the phonon modes ωk (red curve) and ωk (green curve) of the 2D square lattice along different highsymmetry directions of the BZ, M–Y–³–X–M–³, where the points ³, X, Y, M are deﬁned in terms of ( kx , ky ) components as: ³ = (0, 0), X = (π/ a, 0), Y = (0, π/ a), M = ( π/a, π/a). The two modes are degenerate (purple curve) along the ³ –M direction. The DOS is also shown on the right. Bottom: Atomic displacements of the phonon modes with frequencies marked as (a), (b), (c), and (d).
These are shown in Fig. 7.8 along the highsymmetry directions of the BZ. We also show the corresponding DOS of all phonon modes, which exhibits the characteristic features of a 2D system near the extrema (minimum at ³ and maximum at M) and saddle points (X and Y). As expected, since there is only one atom per unit cell, in
338
7
Lattice Vibrations and Deformations
this case we have only acoustic modes, both having linear behavior with k near the origin. However, there are two different slopes for the two different frequencies along the ³–X and ³–Y directions, due to different ways of displacing the atoms for a given k value. In Fig. 7.8 we also show the eigenvectors of the atomic displacements corresponding to the eigenmodes with frequencies labeled (a), (b), (c), and (d). We recognize in (a) a mode at the X point of the BZ that involves only bond stretching of half of the crystal bonds (those that lie in the xˆ direction) with the displacement of the atoms exclusively in the xˆ direction, and in (b) a mode also at the X point that involves only bond bending of half of the crystal bonds (those that originally lie in the xˆ direction) with the displacement of the atoms exclusively in the yˆ direction. There are corresponding modes with equal frequencies at the Y point of the BZ which involve motion of the atoms in the direction perpendicular to that of modes (a) and (b). The two modes labeled (c) and (d) at the M point of the BZ involve both bond stretching/compressing of half of the bonds and bond bending of the other half of the bonds. These two modes have the same frequency, since they are equivalent by a rotation of the crystal by π/2.
Example 7.5 Phonons in a 3D crystal As an illustration of the above ideas in a more realistic example, we discuss brieﬂy the calculation of phonon modes in Si. Si is the prototypical covalent solid, where both bondbending and bondstretching terms are very important. If we wanted to obtain the phonon spectrum of Si by a forceconstant model, we would need parameters that can describe accurately the relevant contributions of the bondbending and bondstretching forces. For example, ﬁtting the values of κr and κθ to reproduce the experimental values for the highestfrequency optical mode at ³, labeled LTO (³),a and the lowestfrequency acoustic mode at X, labeled TA(X), gives the spectrum shown in Fig. 7.9 (see also Problem 1). Although such a procedure gives estimates for the bondstretching and bondbending parameters, the model is not very accurate. For instance, the values of the other two phonon modes at X are off by +5% for the mode labeled TO(X) and −12% for the mode labeled LOA(X), compared to experimental values. Interactions with several neighbors beyond the nearest ones are required in order to obtain frequencies closer to the experimentally measured spectrum throughout the BZ. However, establishing the values of force constants for interactions beyond nearest neighbors is rather complicated and must rely on experimental input. Moreover, with such extensions the model loses its simplicity and the transparent physical meaning of the parameters. Alternatively, one can use the formalism discussed in Chapter 4 (DFT/LDA and its reﬁnements) for calculating total energies or forces, as follows. The atomic displacements that correspond to various phonon modes can be established either by symmetry (for instance, using group theory arguments) or in conjunction with simple
339
Fig. 7.9
7.3
Applications of the ForceConstant Model
Top: The phonon spectrum of Si along the highsymmetry directions L −³ −X, calculated within the forceconstant model. Bottom : Atomic displacements associated with the phonon modes in Si at the ³ and X points in the BZ; inequivalent atoms are labeled 1–4.
calculations based on a forceconstant model, as in the example discussed above. For instance, we show in Fig. 7.9 the atomic displacements corresponding to certain highsymmetry phonon modes for Si, as obtained from the forceconstant model. For a given atomic displacement, the energy of the system relative to its equilibrium structure, or the restoring forces on the atoms, can be calculated as a function of the phonon amplitude. These energy differences are then ﬁtted by a second or higherorder polynomial in the phonon amplitude, and the coefﬁcient of the secondorder term gives the phonon frequency (in the case of a force calculation the ﬁt starts at ﬁrst order in the phonon amplitude). Higherorder terms give the anharmonic contributions which correspond to phonon–phonon interactions. This straightforward method, called the “frozen phonon” approach, gives results that are remarkably close to experimental values. Its limitation is that only phonons of relatively high symmetry can be calculated, such as at the center, the boundaries, and a few special points
340
7
Table 7.1
Lattice Vibrations and Deformations
Frequencies of four highsymmetry phonon modes in
the center (
Si
(THz), at
³ ) and the boundary ( X ) of the BZ, as obtained by theoretical
calculations and by experimental measurements. DFT results are from: J. R. Chelikowsky and M. L. Cohen, “Ab initio pseudopotentials and the structural properties of semiconductors,” in P. T. Landsberg (Ed.),
Handbook on
Semiconductors, Vol. 1, p. 59 (North Holland, Amsterdam, 1992); M. T. Yin and
M. L. Cohen, Phys. Rev. B
26
√κ /M = 2.245 Si θ
√κ /M = 8.828 r Si
, 5668 (1982). The forceconstant model is based
on nearestneighbor interactions only, with
THz,
THz, values that were chosen to reproduce exactly
the experimental frequencies marked by asterisks. The atomic displacements corresponding to these modes are shown in Fig. 7.9.
DFT energy calculation DFT force calculation Forceconstant model Experiment
LTO( ³)
LOA(X)
TO(X)
TA(X)
15.16 15.14 15.53
12.16 11.98 10.83
13.48 13.51 14.65
4.45 4.37 4.49
12.32
13.90
15.53∗
4.49∗
within the BZ. The reason is that phonon modes with low symmetry involve the coherent motion of atoms across many unit cells of the ideal crystal; in order to represent this motion, a large supercell (a multiple of the ideal crystal unit cell) that contains all the inequivalent atoms in a particular phonon mode must be used. For instance, the unit cell for the LTO( ³) mode in Fig. 7.9 involves only two atoms, the same as in the PUC of the perfect crystal, while the supercell for all the modes at X involves four atoms, that is, twice as many as in the PUC of the perfect crystal. The computational cost of the quantummechanical calculations of energy and forces increases sharply with the size of the unit cell, making computations for large unit cells with many atoms intractable. However, the information from the few highsymmetry points can usually be interpolated to yield highly accurate phonon frequencies throughout the entire BZ. In Table 7.9 we compare the calculated frequenciesb for the phonon modes of Fig. 7.9 to experimental values. a “L” stands for longitudinal, “T” for transverse, “O” for optical, and “A” for acoustic. b M. T. Yin and M. L. Cohen, Phys. Rev. B26, 3259 (1982).
7.4
Phonons as Harmonic Oscillators
We next draw an analogy between the phonon hamiltonian and that of a collection of independent harmonic oscillators. We begin with the most general expression for the (l) displacement of ions, Eq. (7.22). In that equation, we combine the amplitude c k with the (l) (l ) timedependent part of the exponential exp[−iωk t] into a new variable Qk (t ), and express
341
7.4
Phonons as Harmonic Oscillators
the most general displacement of ions as:
Snj (t ) =
± l,k
1
(l)
Q k (t ) ¶
ˆ (l)
e e M j kj
ik· Rn
(7.37)
These quantities must be real, since they describe ionic displacements in real space. Therefore, the coefﬁcients of factors exp[ik · Rn ] and exp[i(−k) · Rn] that appear in the expansion must be complex conjugate, leading to the relation
¹
º∗
ˆ (l) = Q (−l)k(t )eˆ(−l )kj
(l)
Q k (t)ekj
(7.38)
and since this relation must hold for any time t , we deduce that:
¹
º∗
(l )
Qk (t )
¹
eˆ kj
= Q (−l)k(t ),
(l)
º∗
= e(−ˆl)kj
(7.39)
The kinetic energy of the system of ions, per unit cell of the crystal, will be given in terms of the displacements S nj (t) as: K N
=
± M j ´ dS nj µ2 n,j
2N
dt
=
±
(l ) (l) 1 ± ± dQ k dQ k ± (l) (l± ) i(k+k ± )·Rn eˆ · e ˆ± e 2N dt dt kj k j n,j kl,k ± l±
(7.40)
where N is the number of unit cells. Using the relations of Eq. (7.39) and the fact that the sum over the Bravais lattice vectors Rn represents a δ function in the k argument [see Appendix A, Eq. (A.70)], we obtain for the kinetic energy:
= 12
K N
±
± dQ (kl) dQ (kl )∗
dt k,l ,l ± ,j
dt
eˆ (kjl) · e(kj ˆl±)∗ = 21
± dQ (kl) dQ (kl)∗ k ,l
dt
(7.41)
dt
where we have set G = 0 in the argument of the δ function since the wavevectors k, k± lie in the ﬁrst BZ, and the last equality was obtained with the help of Eq. (7.21). The potential energy is also expressed in terms of the atomic displacements and the forceconstant matrix: ±U
N
±
= N1
1
±
2 M iM j
k,l ;k± ,l ±
¶
n,i,α ;m,j ,β
(l± ) (l± )
±
Q k ekiα eik ·Rn F niα,mjβ Q k ± ek± jβ eik · Rm
ˆ
ˆ
(l) (l)
We now follow the same steps as in the derivation of the kinetic energy result, after using the deﬁnition of the kdependent dynamical matrix in terms of the forceconstant matrix, (l± ) (l± ) and the fact that eˆ k ± jβ are its eigenvectors with eigenvalues ( ωk )2, to ﬁnd: ±U
N
= 21N = 21N = 21
±
±
n,i,α ; m,j,β k,l; k± ,l±
± ± ±
n i,α ;j,β k,l; k± ,l±
±± k ,l;l± i ,α
ˆ
(l) (l )
(l± ) (l ± )
±
±
Q k ekiα ei(k+k )·Rn D niα,mj β Q k± ek± j β ei k ·(R m −Rn )
ˆ
(l) (l )
ˆ
±
(l ± )
±
Q k ekiα ei(k+k )·Rn Q k± D i α,jβ (k± )ek ± jβ
ˆ
(l) (l )
(l± )
Q k ekiα Q −k
·
¸ (l ± ) 2 (l ± ) − e−kiα
ω k
ˆ
= 21
ˆ (l )
± k,l
(l)
(l)∗
Qk Qk
·
¸ (l) 2
ωk
342
7
Lattice Vibrations and Deformations
where we have also used the orthogonality relations of the eigenvectors, Eq. (7.21), and the relations of Eq. (7.39). Combining the expressions for the kinetic and potential energies, we obtain the total energy of a system of phonons that represents the vibrational state of the ions in the solid: E vib N
=
⎡Ä
1 ± ⎣ÄÄ dQ k Ä Ä dt 2
Ä Ä Ä Ä
(l) Ä2
k,l
+
·
(l) ωk
⎤ ¸2 ÄÄ ÄÄ2 (l) ⎦ ÄQ k Ä
(7.42)
which is formally identical to the total energy of a collection of independent harmonic (l ) (l) oscillators with frequencies ωk , where Q k is the free variable describing the motion of the harmonic oscillator. This expression also makes it easy to show that the kinetic and potential contribution to the total energy are equal, as expected for harmonic oscillators (see Problem 2). This analysis shows that a solid in which atoms are moving is equivalent to a number of phonon modes that are excited, with the atomic motion given as a superposition of the harmonic modes corresponding to the excited phonons. The total energy of the excitation is that of a collection of independent harmonic oscillators with the proper phonon frequencies. Notice that the Q (kl) s contain the amplitude of the vibration, as seen from Eq. (7.37), and consequently, the total energy involves the absolute value squared of the amplitude of every phonon mode that is excited. Since the atomic motion in the solid must be quantized, the harmonic oscillators describing this motion should be treated as quantummechanical ones. Indeed, in Eq. (7.42), Q (kl) can be thought of as the quantummechanical position variable and dQ (kl )/dt as the conjugate momentum variable of a harmonic oscillator identiﬁed by index l and wavevector k. The amplitude of the vibration, contained in Q (kl) , can be interpreted as the number of excited phonons of this particular mode. In principle, there is no limit for this amplitude, therefore an arbitrary number of phonons of each frequency can be excited; all these phonons contribute to the internal energy of the solid. The fact that an arbitrary number of phonons of each mode can be excited indicates that phonons must be treated as bosons. With this interpretation, Q (kl) and its conjugate variable dQ (kl )/dt obey the proper commutation relations for bosons. This implies that the vibrational total energy per unit cell, due to the phonon excitations, must be given by: E vib s
=
±´ k,l
(l) nk ,s
+
µ
1 (l) h¯ ωk 2
(7.43)
where n (kl,)s is the number of phonons of frequency ω(kl) that have been excited in a particular state (denoted by s ) of the system. This expression is appropriate for quantum harmonic (l) oscillators, with nk ,s allowed to take any nonnegative integer value. One interesting aspect of this expression is that, even in the ground state of the system when none of the phonon modes is excited, that is, n(kl)0 = 0, there is a certain amount of energy in the system due to the socalled zeropoint motion associated with quantum harmonic oscillators; this arises from the factors 21 which are added to the phonon occupation numbers in Eq. (7.43). We will see below that this has measurable consequences (see Chapter 8). In practice, if the atomic displacements are not too large, the harmonic approximation to phonon excitations is reasonable. For large displacements, anharmonic terms become
343
7.5
Application: Speciﬁc Heat of Crystals
increasingly important, and a more elaborate description is necessary which takes into account phonon–phonon interactions arising from the anharmonic terms. Evidently, this places a limit on the number of phonons that can be excited before the harmonic approximation breaks down.
7.5
Application: Speciﬁc Heat of Crystals
We can use the concept of phonons to determine the thermal properties of crystals, and in particular their speciﬁc heat. This is especially interesting at low temperatures, where the quantum nature of excitations becomes important, and gives behavior drastically different from the classical result. We discuss this topic next, beginning with a brief review of the result of the classical theory. 7.5.1
The Classical Picture
The internal energy per unit volume associated with the motion of a collection of classical particles at inverse temperature β = 1/k BT (where k B is Boltzmann’s constant) contained in a volume V is given by: E vib V
É
{dR}{Édp}E vib({r}, {p})e− E ({r} ,{p} ) V {dr}{dp}e− E ({r },{p} ) ³ ²¼ = −V1 ∂β∂ ln {dr}{ dp}e− E ({r },{p} ) =
1
β
β
vib
vib
β
vib
(7.44)
where {r} and {p } are the coordinates and momenta of the particles. In the harmonic approximation, the energy is given in terms of the displacements δ Rn from ideal positions as: 1± 1 ± p2n E vib = (7.45) δ Rn · F( Rn − Rn± ) · δ Rn± + 2 ± 2 n Mn n ,n
where F(Rn − Rn± ) is the forceconstant matrix, deﬁned in Eq. (7.5); the indices n , n± run over all the particles in the system. Since both the potential and the kinetic parts involve quadratic expressions, we can rescale all coordinates by β1/2 , in which case the integral in the last expression in Eq. (7.44) is multiplied by a factor of β−3Nat , where N at is the total number of atoms in 3D space. What remains is independent of β , giving for the internal energy per unit volume: E vib V
= 3NV at k B T
(7.46)
from which the speciﬁc heat per unit volume can be calculated: c(T )
= ∂T ∂
Á
E vib V
Â
= 3k B(N at/V )
(7.47)
344
7
Lattice Vibrations and Deformations
This turns out to be a constant independent of temperature. This behavior is referred to as the Dulong–Petit law, which is valid at high temperatures. 7.5.2
The QuantumMechanical Picture
The quantummechanical calculation of the internal energy in terms of phonons gives the following expression: E vib V
1
=V
∑ vib −βE vib s s Es e ∑ vib −β E s
e
(7.48)
s
where E svib is the vibrational energy per unit cell corresponding to a particular state of the system, which involves a certain number of excited phonons. We will take E vib s from Eq. (7.43) that we derived earlier. Just like in the classical discussion, we express the total internal energy as: E vib V
1
= −V ∂β ∂
Ç È ± −βE vib s ln e
(7.49)
s
There is a neat mathematical trick that allows us to express this in a more convenient form. Consider the expression
± −βE vib s e s
=
± s
⎡ exp ⎣−
± ´ β
k,l
(l)
nk ,s
µ
+ 21 h¯ ω(kl) ⎦ (l)
which involves a sum of all exponentials containing terms β (nk nonnegative integer values
∞ Ê± (l ) 1 e−β (n+ 2 )h¯ωk k ,l n=0
=
(l) of n k .
⎤ (7.50)
+ 21 )h¯ ω(kl) with all possible
Now consider the expression
´
−βh 1 ω(l1 ) −βh 3 ω(l1 ) e ¯ 2 k 1 + e ¯ 2 k1 +
µ´
· ·
−βh 1 ω(l2) −βh 3 ω(l2) e· ¯ 2 k2 + e ¯ 2 k2 +
µ
· ·· ·· ·
It is evident that when these products are expanded out we obtain exponentials with (l) exponents (n + 21 )β h¯ ωk with all possible nonnegative integer values of n. Therefore, the expressions in these two equations are the same, and we can substitute the second expression for the ﬁrst one in Eq. (7.49). Notice further that the geometric series summation gives:
∞ ± (l ) 1 e−β (n+ 2 )h¯ωk n=0
=
e−β h¯ ωk / 2 (l)
(7.51)
1 − e−β h¯ ωk
(l)
which leads to, for the total internal energy per unit volume: E vib V
1
= −V ∂β ∂
⎤ ⎡ µ ´ Ê e−β h¯ω(kl) /2 1 ± (l) (l) 1 ⎦ ⎣ = ln h¯ ωk n¯ k + (l ) k,l
1 − e−β h¯ωk
V
k,l
2
(7.52)
345
7.5
Application: Speciﬁc Heat of Crystals
where we have deﬁned n¯ (kl) as:
¯ (l)
n k (T )
=
1 e ¯
(l ) β hω k
(7.53)
−1
(l)
This quantity represents the average occupation of the phonon state with frequency ωk , at temperature T , and is appropriate for bosons (see Appendix D). From Eq. (7.52) we can now calculate the speciﬁc heat per unit volume: c (T )
= ∂T ∂
Á
Â
E vib V
= V1
± k ,l
¯
(l) ∂
h ωk
∂T
¯ (l )
nk (T )
(7.54)
We examine ﬁrst the behavior of this expression in the lowtemperature limit. In this limit, βh ¯ ωk(l ) becomes very large, and therefore n¯ (kl )(T ) becomes negligibly small, except when (l) (l) ωk happens to be very small. We saw in earlier discussion that ωk goes to zero linearly near the center of the BZ (k ≈ 0), for the acoustic branches. We can then write near the (l) (l) (l ) center of the BZ ωk = v ˆ k , where k = k is the wavevector magnitude and v ˆ is k
k
the sound velocity which depends on the direction of the wavevector kˆ and the acoustic (l ) (l) branch label l . For large β we can then approximate all frequencies as ωk = v ˆ k over the k entire BZ, since for large values of k the contributions are negligible anyway, because of (l) the factor exp[β h¯v ˆ k ] which appears in the denominator. Turning the sum into an integral k as usual, we obtain for the speciﬁc heat at low temperature: c (T )
= ∂T ∂
±¼ l
dk (2π )3
¯ (kl)
hv ˆ k
(l ) β hv k e ¯ kˆ − 1
(7.55)
We will change variables as in the case of the classical calculation to make the integrand (l ) (l) independent of inverse temperature β , by taking βh¯v ˆ k = t ˆ , which gives a factor of β−4 k k in front of the integral, while the integral has now become independent of temperature. In fact, we can use the same argument about the negligible contributions of large values of k to extend the integration to inﬁnity in the variable k , so that the result is independent of the BZ shape. Denoting by c 0 the value of the constant which is obtained by performing the integration and encompasses all other constants in front of the integral, we then ﬁnd: c (T )
= c 0 ∂∂T T 4 = 4c 0T 3
(7.56)
that is, the behavior of the speciﬁc heat at low temperature is cubic in the temperature and not constant as the Dulong–Petit law suggests from the classical calculation. (l) In the hightemperature limit, that is, when kB T ¸ h¯ ωk , the Bose occupation factors take the form kB T 1 ≈ (7.57) (l) (l) h¯ ωk eβ h¯ ωk − 1 and with this, the expression for the speciﬁc heat becomes: c(T )
= V1
± k,l
kB
= 3k B (N at/V )
(7.58)
346
7
Lattice Vibrations and Deformations
which is the same result as in the classical calculation. Thus, at sufﬁciently high temperatures the Dulong–Petit law is recovered.
7.5.3
The Debye Model
A somewhat more quantitative discussion of the behavior of the speciﬁc heat as a function of the temperature is afforded by the Debye model. In this model we assume all frequencies to be linear in the wavevector magnitude, as acoustic modes near k ≈ 0 are. For simplicity we assume we are dealing with an isotropic solid, so we can take ω = vk for all the different acoustic branches, with v (the sound velocity) being the same in all directions. The total number of phonon modes is equal to 3N at , where N at is the total number of atoms in the crystal, and for each value of k there are 3nat normal modes in three dimensions (nat being the number of atoms in the PUC). Strictly speaking, the Debye model makes sense only for crystals with one atom per PUC, because it assumes all modes to be acoustic in nature (they behave like ω ∼ k for k → 0). Just like in the case of electronic states, we can use a normalization argument to relate the density of the crystal, n = N at /V , to the highest value of the wavevector that phonons can assume (denoted by k D ):
± k
3nat
→ 3V
¼
kD
0
4π k 2 dk (2π )3
3
= 3N at ⇒ n = NVat = 6kπD2
(7.59)
from which the value of k D is determined in terms of n . Notice that k D is determined by considering the total number of phonon modes , not the actual number of phonons present in some excited state of the system, which of course can be anything since phonons are bosons. We can also deﬁne the Debye frequency ωD and Debye temperature ´D , through: ωD
= vk D,
´D
= h¯kωD
(7.60)
B
With these deﬁnitions, we obtain the following expression for the speciﬁc heat at any temperature: c (T )
= 9nk B
´
T ´D
µ3 ¼ 0
´ D /T
t4 e t
(e t − 1)2
dt
(7.61)
In the lowtemperature limit, with ´D much larger than T , the upper limit of the integral is approximated by ∞, and there is no temperature dependence left in the integral, which gives a constant when evaluated explicitly. This reduces to the expression we discussed above, Eq. (7.56). What happens for higher temperatures? Notice ﬁrst that the integrand is always a positive quantity. As the temperature increases, the upper limit of the integral becomes smaller and smaller, and the value obtained from integration is lower than the value obtained in the lowtemperature limit. Therefore, as the temperature increases, the value of the speciﬁc heat increases slower than T 3 , as shown in Fig. 7.10. As we saw above, at sufﬁciently high temperature the speciﬁc heat eventually approaches the constant value of the Dulong–Petit law.
347
7.5
Application: Speciﬁc Heat of Crystals
ωD
c (T)
9
3 nkB
6
3
~T 3 0
T Fig. 7.10
0.5
1
D
Left: Behavior of the speciﬁc heat c as a function of temperature T in the Debye model. The asymptotic value for large T corresponds to the Dulong–Petit law. Right: Comparison of the density of states in the Debye model as given by Eq. (7.64), shown by the red line and a realistic calculation [adapted from R. Stedman, L. Almqvist, and G. Nilsson, Phys. Rev. 162, 549 (1967)], shown by the shaded curve, for the Al crystal.
To explore the physical meaning of the Debye temperature, we note that from its deﬁnition: (l)
n k (T )
=
1 (l )
(ω k
e
/ωD )( ´D / T )
−1
all phonon modes are excited, that is, n¯ (kl )(T ) > 0 for all frequencies, while for (l) T < ´D the highfrequency phonon modes are frozen, that is, n¯ k (T ) ≈ 0 for those modes. The Debye model is oversimpliﬁed, because it treats the frequency spectrum as linearly dependent on the wavevectors, ω = vk for all modes. For a realistic calculation we need to include the actual frequency spectrum, which produces a density of states with features that depend on the structure of the solid, analogous to what we discussed for the electronic energy spectrum. An example, the Al crystal, is shown in Fig. 7.10. Within the Debye model, the density of phonon modes at frequency ω per unit volume of the crystal, g (ω), can easily be obtained starting with the general expression
For T
> ´D
g(ω )
1 ±
=V
k ,l
δ (ω
−
(l) ωk )
=
±¼ l
± dk (l) δ (ω − ωk ) = (2π )3 l
¼ ω
=
(l) ω k
1 dS k 3 (2π ) ∇k ω(l)  k
where the last expression involves an integral over a surface in kspace on which ωk = ω. (l) (l) In the Debye model we have ωk = v k , which gives ∇k ωk  =v, with v the average (l) sound velocity. For ﬁxed value of ω = ωk = v k , the integral over a surface in kspace that corresponds to this value of ω is equal to the surface of a sphere of radius  k =ω/v , and since there are three phonon branches in 3D space, all having the same average sound velocity within the Debye model, we ﬁnd for the density of states: (l)
g (ω)
= (2π3 )3 1v 4π
· ω ¸2 v
2
= 2π3 2 ωv 3
(7.62)
348
7
Lattice Vibrations and Deformations
If we calculate the total number of available phonon modes per unit volume N ph/ V up to the Debye frequency ωD , we ﬁnd: N ph V
=
¼
ωD
0
3
g( ω)dω
= 2π1 2 ωv D3 = 3 6π1 2 kD3
(7.63)
which, from Eq. (7.59), is equal to 3(N at /V ), exactly as we would expect for a 3D crystal containing N at atoms. Using the deﬁnition of the Debye frequency, we can express the density of states as: g (ω)ωD n
=9
´
µ2
ω
(7.64)
ωD
which is a convenient relation between dimensionless quantities. In Fig. 7.10 we show a comparison of the density of states in the Debye model as given by Eq. (7.64), and as obtained by a realistic calculation for the Al crystal. This comparison illustrates how simple the Debye model is relative to real phonon modes. Nevertheless, the model is useful in that it provides a simple justiﬁcation for the behavior of the speciﬁc heat as a function of temperature as well as a rough measure of the highest phonon frequency, ωD . In fact, the form of the speciﬁc heat predicted by the Debye model, Eq. (7.61), is often used to determine the Debye temperature, and through it the Debye frequency. Since this relation involves temperature dependence, a common practice is to ﬁt the observed speciﬁc heat at given T to one half the value of the Dulong–Petit law as obtained from Eq. (7.61), which determines ´ D . Results of this ﬁtting approach for the Debye temperatures of several elemental solids are given in Table 7.2.
Table 7.2
Debye temperatures
elemental solids. Values of
´D
´D (K) and frequencies ωD (THz) for several ωD were determined by ﬁtting the observed
and
value of the speciﬁc heat at a certain temperature to half the value of the Dulong–Petit law through Eq. (7.61). Source : J. de Launay, Solid State Physics, Vol. 2 (Academic Press, Boston, MA, 1956).
Element Li Be B C∗ As Cu Zn Cr Mn Ni
´D
ωD
400 1000 1250 1860 285 315 234 460 400 375
8.33 20.84 26.05 38.76 5.94 6.56 4.88 9.58 8.33 7.81
∗
In the diamond phase.
Element
´D
ωD
Na Mg Al Si Sb Ag Cd Mo Fe Pd
150 318 394 625 200 215 120 380 420 275
3.12 6.63 8.21 13.02 4.17 4.48 2.50 7.92 8.75 5.73
Element
´D
ωD
K Ca Ga Ge Bi Au Hg W Co Pt
100 230 240 350 120 170 100 310 385 230
2.08 4.79 5.00 7.29 2.50 3.54 2.08 6.46 8.02 4.79
349
7.5
7.5.4
Application: Speciﬁc Heat of Crystals
Thermal Expansion Coeﬃcient
An important physical effect which is related to phonon modes and to the speciﬁc heat is the thermal expansion of a solid. The thermal expansion coefﬁcient α is deﬁned as the rate of change of the linear dimension L of the solid with temperature T , normalized by this linear dimension, at constant pressure P : 1
≡L
α
´
∂L
µ
(7.65)
∂T
P
The linear dimension of the solid L is related to its volume V through L gives for the thermal expansion coefﬁcient in terms of the volume: α
=
1 3V
´
∂V
= V 1 3, which /
µ
(7.66)
∂T
P
This can also be expressed in terms of the bulk modulus B , the negative inverse of which is the rate of change of the volume with pressure, normalized by the volume, at constant temperature:
≡ −V1
B −1
´
µ
∂V
(7.67)
∂P
T
[see also the equivalent deﬁnition, Eq. (7.78)]. With the help of standard thermodynamic relations (see Appendix D), we obtain for the thermal expansion coefﬁcient in terms of the bulk modulus and the pressure: α
= 31B
´
∂P
µ
(7.68)
∂T
V
The pressure is given by the negative rate of change of the Helmholtz free energy F with volume, at constant temperature:
´
P
= − ∂∂ VF
µ
(7.69) T
where F = E − TS , with E the internal energy and S the entropy (see Appendix D). When changes in the internal energy E are due exclusively to phonon excitations, we can use E from Eq. (7.52), and with this derive the appropriate expression for S (see Problem 5), to obtain for the thermal expansion coefﬁcient: α
=
1 ± 3B k,l
Ç
(l) − ¯∂ V ∂ h ωk
È Ç T
¯ (l )
∂nk ∂T
È
(7.70) V
This involves the same quantities as the expression for the speciﬁc heat c , Eq. (7.54), that (l) (l) is, the phonon frequencies ωk and the corresponding average occupation numbers n¯ k at temperature T . In fact, it is customary to express the thermal expansion coefﬁcient in terms of the speciﬁc heat as: γ c(T ) (7.71) α = 3B
350
7
Lattice Vibrations and Deformations
where the coefﬁcient γ is known as the Gr¨uneisen parameter. This quantity is given by: γ
=
1 ± ∂ h¯ ωk − ∂V c (T )
(l)
k,l
⎤⎡
⎡
⎤−1
¯ (l) = −V ⎣± ∂ h¯ ω(kl) ∂ n¯ (kl) ⎦ ⎣± h ω(l) ∂ n¯ (kl) ⎦ ¯ k ∂T ∂T ∂V ∂T
∂ nk
k,l
(7.72)
k,l
We can simplify the notation in this equation by deﬁning the contributions to the speciﬁc heat from each phonon mode as: (l)
ck
= h¯ ωk(l) ∂∂n¯Tk
(l)
(7.73)
and the modespeciﬁc Gr¨uneisen parameters: (l)
γk
(l)
(l)
ωk ) = −V(l) ∂∂ωVk = −∂∂(ln (ln V )
(7.74)
ωk
in terms of which the Gr¨uneisen parameter takes the form
⎡
γ
=⎣
± k,l
⎤⎡
(l) (l) ⎦ ⎣ ck
γk
± k,l
⎤−1
(l) ⎦
ck
(7.75)
The Gr¨uneisen parameter is a quantity that can be measured directly by experiment. Important warning. We should alert the reader to the fact that so far we have taken into account only the excitation of phonons as contributing to changes in the internal energy of the solid. This is appropriate for semiconductors and insulators where electron excitation across the band gap is negligible for usual temperatures. For these solids, for temperatures as high as their melting point, the thermal energy is still much lower than the bandgap energy, the minimum energy required to excite electrons from their ground state. For metals, on the other hand, the excitation of electrons is as important as that of phonons; when it is included in the picture, it gives different behavior of the speciﬁc heat and the thermal expansion coefﬁcient at low temperature. These effects can be treated explicitly by modeling the electrons as a Fermi liquid, which requires a manybody picture; a detailed description of the thermodynamics of the Fermi liquid is given Fetter and Walecka. 2
7.6
Application: Mössbauer Eﬀect
Another interesting manifestation of the quantum nature of phonons is the emission of recoilless radiation from crystals, known as the M¨ossbauer effect. Consider a nucleus that can emit γ rays due to nuclear transitions. In free space, the energy and momentum conservation requirements produce a shift in the γ ray frequency and a broadening of the spectrum. Both of these changes obscure the nature of the nuclear transition. We can estimate the amount of broadening by the following argument: the momentum of the 2 Quantum Theory of ManyParticle Systems
, A. L. Fetter and J. D. Walecka (McGrawHill, New York, 1971).
351
7.6
Application: Mössbauer Eﬀect
emitted photon of wavevector K is h¯ K, which must be equal to the recoil of the nucleus M v, with M the mass of the nucleus (assuming that the nucleus is initially at rest). The recoil energy of the nucleus is E R = M v2/2 = h¯ 2K2 /2M , and the photon frequency is given by h¯ ω0/c = h¯  K , so that E R = h¯ 2 ω20 /2Mc 2. The broadening is then obtained by E R = h¯ ±ω , which gives: ±ω ω0
´
=
ER
µ1/2
2Mc 2
This can be much greater than the natural broadening which comes from the ﬁnite lifetime of nuclear processes that give rise to the γ ray emission in the ﬁrst place. When the emission of γ rays takes place within a solid, the presence of phonons can change things signiﬁcantly. Speciﬁcally, much of the photon momentum can be carried by phonons with low energy, near the center of the BZ, and the emission can be recoilless, in which case the γ rays will have a frequency and width equal to their natural values. We next develop this picture by treating phonons as quantum oscillators. The transition probability between initial ( i³) and ﬁnal (²f ) states is given by: P i→f
ÄË
ÌÄ
2 = ÄÄ f Oˆ (K, {p })i ÄÄ
where Oˆ (K, {p}) is the operator for the transition, K is the wavevector of the radiation, and {p} are nuclear variables that describe the internal state of the nucleus. Due to translational and galilean invariance, we can write the operator for the transition as:
ˆ
O (K,
{p}) = exp[−iK · r]Oˆ ({p })
where the last operator involves nuclear degrees of freedom only. We exploit this separation to write: P i →f
ÄË
ÌÄ
2 = ÄÄ f Oˆ ({p })i ÄÄ P 0→0
where the states ²f  ,  i³ now refer to nuclear states, and P 0→0 is the probability that the crystal will be left in its ground state, with only phonons of low frequency ωq→0 emitted. We next calculate P 0→0 using the quantum picture of phonons. The hamiltonian for the crystal degrees of freedom involved in the transition is simply the phonon energy, as derived in Eq. (7.42). For simplicity, in the following we assume that there is only one type of atom in the crystal and one atom per unit cell, so that all atoms have the same mass M i = M ; this can easily be extended to the general case. This allows us to exclude the √ (l) factor of 1/ M from the deﬁnition of the coordinates Q q (t) (since the mass is now the same for all phonon modes), distinct from what we did above, see Eq. (7.37); with this new deﬁnition, the quantities Q s have the dimension of length. To simplify the notation, we also combine the q and l indices into a single index s . With these deﬁnitions, the total energy of the phonons takes the form E
vib
=
± s
Á
1 2M
´
dQ s M dt
µ2
+
1 M ω2s Q 2s 2
Â
=
±² 1 s
2M
P 2s
+ 12 M ω2s Q 2s
³ , Ps
= M ddQt s
352
7
Lattice Vibrations and Deformations
which, as discussed before, corresponds to a set of independent harmonic oscillators, with P s the canonical momenta. The harmonic oscillator coordinates Q s are related to the atomic displacements S by:
±
S=
s
ˆ
Q s es
where eˆ s is the eigenvector corresponding to the phonon mode with frequency ωs . Each of the oscillators obeys the hamiltonian
Á
ˆ vib φ(ns)(Q ) = − h¯ ∇Q + 1 M ω2s Q 2 H 2M 2 2
2
Â
(s)
φn
(Q ) = ²n(s) φ(ns )(Q )
The wavefunction of each independent harmonic oscillator in its ground state is: (s) φ0 (Q s )
=
´
µ1/ 4
1 π r s2
e−Q s / 2r s
2
2
where the constant 1/r s = M ωs / h¯ (see Appendix C). With all these expressions we are now in a position to calculate the probability of recoilless emission in the ground state of the crystal, at T = 0, so that all oscillators are in their ground state before and after the transition. This probability is given by: P 0→ 0
∼ =
Ä Ä ÄÊ Ë ÌÄ2 Ä (s) iK·ˆes Qs (s) Ä φ0 ÄÄ = ÄÄ φ0 e s Ä ´ Ä2 ÄÊ 1 µ1/2 ¼ Ä Ê −(K·ˆe )2 r2 /2 Ä Ä − Q2s / r2s iK·ˆes Qs s s e d Q sÄ = e e Ä 2 Ä s π rs Ä s
ÄË Ä i K·S ÌÄÄ2 Ä 0 e 0 Ä
But there is a simple relation between r 2s /2 and the average value of Q 2s in the ground state of the harmonic oscillator: r 2s
2
=
¼ ´
1
µ1/2
π r2 s
Q 2s e−Q s / rs dQ s 2
with the help of which we obtain:
ÄË ÌÄ Ä 0 eiK·S 0 Ä2 Ä Ä
2
Á
= exp −
±( s
Ë
=
(s )
φ0
Ì
Q 2s φ0(s) = )2 Ë
K · esˆ
Q 2s
Ì
Ë
Q 2s
Ì
Â
(l)
Now we will assume that all the phonon modes l have the same average (Q q )2 , which, following the same steps as in Eq. (8.10), leads to:
ÄË Ä iK· S ÌÄÄ2 Ä 0e 0 Ä
⎡
= exp ⎣−
± q
⎤ Ì K2 Q 2q ⎦ Ë
By a similar argument, we obtain:
Ä2 Î Í ÄÄ Ä ± Ë 2Ì ± Ä Ä 2 (l) (l) Ä Ä Q q ⇒ P 0→0 S = Ä Q q ˆeq Ä = 3 Ä Ä q ,l q
Ë Ì
∼ e−K
2
Ï 2Ð S
/3
353
7.7
Elastic Deformations of Solids
For harmonic oscillators the average kinetic and potential energies are equal and each is half of the total energy (see Problem 2). This gives: 2 M ωs
Ë
Ì
Q s = 2
´
ns
+
1 2
µ
Ë
Ì
¯ h¯ ωs ⇒ Q s  = Mω 2
´
h
s
ns
+
1 2
µ
(7.76)
with ns the phonon occupation numbers. This result holds in general for a canonical distribution, from which we can obtain: 1 2 Ë 2Ì K S 3
= ¯2M
h 2 K2 2
3
± 1 ´ s
¯
h ωs
ns
+
1 2
µ
=
2 ± 1 ER hω 3 s ¯ s
´ ns
+
1 2
µ
with E R the recoil energy as before, which is valid for a system with a canonical distribution at temperature T . At T = 0, n s vanishes and if we use the Debye model with ωs = vk (that is, we take an average velocity v s = v ), we obtain: 1 2 Ë 2Ì K S 3
= 13 E R
± 1 q
¯
hvk
from which we can calculate explicitly the sum over q by turning it into an integral with upper limit k D (the Debye wavevector), to obtain:
²
3 ER P 0→0 ∼ exp − 2 k B´D
³
(7.77)
with ´D the Debye temperature. As we have seen before, energy conservation gives E R = h¯ ω20/ 2Mc 2, which is a ﬁxed value since the value of ω0 is the natural frequency of the emitted γ rays. This last expression shows that if the Debye temperature is high enough (k B´ D ¸ E R ), then P 0→0 ∼ 1, in other words, the probability of the transition involving only nuclear degrees of freedom, without having to balance the recoil energy, will be close to 1. This corresponds to recoilless emission.
7.7
Elastic Deformations of Solids
As we have seen in Chapter 4, totalenergy calculations allow the determination of the optimal lattice constant of any crystalline phase of a material, its cohesive energy, and its bulk modulus. The totalenergy vs. volume curves for different phases of a material, like those for Si shown in Fig. 4.8, exhibit a quadratic behavior of the energy near the minimum. A simple polynomial ﬁt to the calculated energy as a function of volume near the minimum readily yields estimates for the equilibrium volume V 0 , and hence the lattice 1/ 3 constant a 0 ∼ V 0 , that corresponds to the lowestenergy structure. The standard way to ﬁt the totalenergy curve near its minimum is by a polynomial in powers of V 1/ 3, where V is the volume. The bulk modulus B of a solid is deﬁned as the change in the pressure P when the volume V changes, normalized by the volume (in the present calculation we are
354
7
Lattice Vibrations and Deformations
assuming zerotemperature conditions): B
≡ −V ∂∂ VP
(7.78)
Using the relation between the pressure and the total energy at zero temperature, we obtain for the bulk modulus: 2
P
= −∂∂ VE ⇒ B = V ∂∂ VE2
(7.79)
which is easily obtained from the totalenergy vs. volume curves, as the curvature at its minimum. A quadratic behavior of the energy as a function of the lattice constant is referred to as “harmonic” or “elastic” behavior. It implies simple harmonicspringlike forces that restore the volume to its equilibrium value for small deviations from it. This is behavior found in all materials. It implies that the solid returns to its original equilibrium state once the agent (external force) that produced the deviation is removed. If the distortion is large, then the energy is no longer quadratic in the amount of deviation from equilibrium and the solid cannot return to its equilibrium state; it is permanently deformed. This is referred to as “plastic” deformation. The elastic (harmonic) deformation can be described in much the same terms as the small deviation of individual atoms from their equilibrium positions on which we based the theory of lattice vibrations. In the case of elastic deformation a great number of atoms are moved from their equilibrium positions in the same direction in different parts of the solid. The amount of deformation is called strain and the resulting forces per unit area are called stress. These are both tensors because their values depend on the direction in which atoms are displaced and crystals are not necessarily isotropic. The theory that describes the effects of elastic deformation is called “elasticity theory.” 7.7.1
Phenomenological Models of Solid Deformation
Before we develop the basic concepts of elasticity theory and how they apply to simple cases of elastic deformation of solids, we discuss two phenomenological models that predict with remarkable accuracy some important quantities related to the energetics of solid deformations. The ﬁrst, developed by M. L. Cohen3 and based on the arguments of J. C. Phillips4 about the origin of energy bands in semiconductors, deals with the bulk modulus of covalently bonded solids. The second, developed by Rose, Smith, Guinea, and Ferrante,5 concerns the energyvs.volume relation and asserts that, when scaled appropriately, it is a universal relation for all solids; this is referred to as the universal binding energy relation (UBER). We discuss these phenomenological theories in some detail, because they represent important tools, as they distill the results of elaborate calculations into simple, practical expressions.
3 M. L. Cohen, Phys. Rev. B 32, 7988 (1985). 4 Bonds and Bands in Semiconductors , J. C. Phillips (Academic Press, New York, 1973). 5 J. H. Rose, J. R. Smith, F. Guinea, and J. Ferrante, Phys. Rev. B 29, 2963 (1984).
355
7.7
Elastic Deformations of Solids
Cohen’s theory gives the bulk modulus of a solid which has average coordination ²N c ³, as: B
= ²N4c ³ (1971 − 220I )d −3.5GPa
(7.80)
˚ and I is a dimensionless number which describes the where d is the bond length (A) ionicity: I = 0 for the homopolar crystals C, Si, Ge, Sn; I = 1 for III–V compounds (where the valence of each element differs by 1 from the average valence of 4); and I = 2 for II–VI compounds (where the valence of each element differs by 2 from the average valence of 4). The basic physics behind this expression is that the bulk modulus is intimately related to the average electron density in a solid where the electrons are uniformly distributed, as discussed in Chapter 4, Problem 5. For covalently bonded solids, the electronic density is concentrated between nearestneighbor sites, forming the covalent bonds. Therefore, in this case the crucial connection is between the bond length, which provides a measure of the electron density relevant to bonding strength in the solid, and the bulk modulus. Cohen’s argument produced the relation B ∼ d −3.5 , which, dressed with the empirical constants that give good ﬁts for a few representative solids, leads to Eq. (7.80). Later in this section we give actual values of bulk moduli B of several representative semiconductors (see Table 7.4); as can be checked from these values, the bulk moduli of semiconductors are captured with an accuracy which is remarkable, given the simplicity of the expression in Eq. (7.80). In fact, this expression has been used to predict theoretically solids with very high bulk moduli,6 possibly exceeding those of naturally available hard materials like diamond. The UBER theory gives the energyvs.volume relation as a twoparameter expression:
= E cohE (a ) E (a ) = − [1 + a + 0.05a 3] exp( −a) a = (a − a 0 )/l E (a )
(7.81)
where a is the lattice constant (which has a very simple relation to the volume per atom, depending on the lattice), a0 is its equilibrium value, l is a length scale, and E coh is the cohesive energy; the latter two quantities are the two parameters that are speciﬁc to each solid. This curve has a single minimum and goes asymptotically to zero for large distances; the value of its minimum corresponds to the cohesive energy. For example, we show in Fig. 7.11 the ﬁt of this expression to DFT/GGA values for a number of representative elemental solids, including metals with s (Li, K, Ca) and sp (Al) electrons, sd electron metals with magnetic (Fe, Ni) or nonmagnetic (Cu, Mo) ground states, and semiconductors (Si) and insulators (C). As seen from this example, the ﬁt to this rather wide range of solids is quite satisfactory; the values of the lattice constant and cohesive energy a 0 and E coh, extracted from this ﬁt, differ somewhat from the experimental values but this is probably related more to limitations of the DFT/GGA formalism than the UBER theory. The degree to which this simple expression ﬁts theoretically calculated values for a wide range of solids, as well as the energy of adhesion, molecular binding, and chemisorption of 6 A. Y. Liu and M. L. Cohen, Phys. Rev. B 41, 10727 (1990).
356
7
Lattice Vibrations and Deformations
ygrene gnidnib delacS Scaled separation Fig. 7.11
Fit of calculated total energies of various elemental solids to the universal binding energy relation; the calculations are based on DFT/GGA.
gas molecules on surfaces of metals, is remarkable. The UBER expression is very useful for determining, with a few electronic structure calculations of the total energy, a number of important quantities like the cohesive energy (or absorption, chemisorption, adhesion energies, when applied to surface phenomena), bulk modulus, critical stresses, etc. 7.7.2
Elasticity Theory: The Strain and Stress Tensors
Elasticity theory considers solids from a macroscopic point of view, and deals with them as an elastic continuum. The basic assumption is that a solid can be divided into small elements, each of which is considered to be of macroscopic size, that is, very large on the atomic scale. Moreover, it is also assumed that we are dealing with small changes in the state of the solid with respect to a reference conﬁguration, so that the response of the solid is well within the elastic regime, in other words, the amount of deformation is proportional to the applied force just like in a spring. Although these assumptions may seem very restrictive, limiting the applicability of elasticity theory to very large scales, in most cases this theory is essentially correct all the way down to scales of order a few atomic distances. This is due to the fact that it takes a lot of energy to distort solids far from their equilibrium reference state, and for small deviations from that state solids behave very similarly to elastic springs. We begin with the deﬁnitions of the strain and stress tensors in a solid. The reference conﬁguration is usually taken to be the equilibrium structure of the solid, on which there are no external forces. We deﬁne strain as the amount by which a small element of the solid is distorted with respect to the reference conﬁguration The arbitrary point in the solid at
357
Fig. 7.12
7.7
Elastic Deformations of Solids
Deﬁnition of the strain tensor for the cartesian ( x, y, z ) coordinate system: the arbitrary point in the solid at r = xxˆ + yyˆ + zˆz in the reference conﬁguration moves to r± = r + δ r = ( x + uxˆ + ( y + v) ˆy + (z + w)zˆ under the action of external forces, F, indicated by blue arrows, on the solid (in this example the left part is under compression and the right part is under tension). The undistorted shape and position are shown as dashed lines.
(x , y , z ) cartesian coordinates moves to (x + u, y + v , z + w ) when the solid is strained, as illustrated in Fig. 7.12. Each of the displacement ﬁelds u , v , w is a function of the position in the solid: u(x , y , z), v (x , y , z ), w (x , y, z ). The normal components of the strain are deﬁned to be: ² xx
= ∂∂ux ,
² yy
= ∂∂ vy ,
² zz
= ∂∂wz
(7.82)
These quantities represent the simple stretch of the solid in one direction in response to a force acting in this direction, if there were no deformation in the other two directions. A solid, however, can be deformed in various ways, beyond the simple stretch along the chosen axes x , y , z . In particular, it can be sheared as well as stretched. Stretching and shearing are usually coupled, that is, when a solid is pulled (or pushed) not only does it elongate (or contract) by stretching, but it also changes size in the direction perpendicular to the pulling (or pushing). The shear itself will induce strain in directions other than the direction in which the shearing force acts. To describe this type of deformation we introduce the shearstrain components given by: ² xy
= 21
´
∂u
∂v + ∂y ∂x
µ
,
²yz
= 12
´
∂v
∂w + ∂z ∂y
µ
,
²zx
= 12
´
∂w
∂u + ∂x ∂z
µ
(7.83)
which are symmetric, ²yx = ²xy , ²zy = ²yz , ²xz = ²zx. Thus, we need a secondrank tensor to describe the state of strain, which is a symmetric tensor with diagonal elements ²ii (i = x , y , z ) and offdiagonal elements ²ij (i , j = x, y, z ). We also introduce, for future use, the rotation tensor ξ xy
= 12
´
∂u
− ∂∂ vx ∂y
µ
,
ξyz
= 12
´
∂v
− ∂∂wy ∂z
µ
,
ξ zx
= 12
´
∂w ∂x
− ∂∂uz
µ
(7.84)
which describes the inﬁnitesimal rotation of the volume element at (x , y , z ). This is an antisymmetric tensor, ξji = − ξij (i , j = x, y, z ).
358
7
Lattice Vibrations and Deformations
There is a different notation which makes the symmetric or antisymmetric nature of the strain and rotation tensors more evident: we deﬁne the three cartesian axes as x 1 , x 2, x3 (instead of x , y , z ) and the three displacement ﬁelds as u 1, u2 , u 3 (instead of u , v , w ). Then the strain tensor takes the form ² ij
= 21
´
∂ui ∂ xj
+ ∂∂ ux j
µ
(7.85)
i
which holds for both the diagonal and offdiagonal components. This form makes the symmetric character of the strain tensor obvious. Similarly, the rotation tensor with this alternative notation takes the form ´ µ 1 ∂ui ∂uj ξij = − ∂x (7.86) 2 ∂xj i which is obviously an antisymmetric tensor. This notation becomes particularly useful in the calculation of physical quantities when other multipleindex tensors are also involved, as we will see below. For the moment, we will use the original notation in terms of x , y , z and u, v, w , which makes it easier to associate the symbols in 3D space with the corresponding physical quantities. It is a straightforward geometrical exercise to show that, if the coordinate axes x and y are rotated around the axis z by an angle ´, then the strain components in the new coordinate frame (x ± y ± z± ) are given by: 1 1 (²xx + ²yy ) + (²xx − ²yy ) cos 2´ + ²xy sin 2´ 2 2 1 1 (²xx + ²yy ) − (²xx − ²yy ) cos 2´ − ²xy sin 2´ ² y± y± = 2 2 1 (²yy − ²xx ) sin 2´ + ²xy cos 2 ´ (7.87) ² x± y± = 2 The last expression is useful, because it can be turned into the following equation: ² x± x±
=
tan 2´
= ² ²−xy ² xx yy
(7.88)
through which we can identify the rotation around the z axis which will make the shear components of the strain ²xy vanish. For this rotation, only normal strains will survive; the rotated axes are called the principal strain axes. Using this rotation angle, we ﬁnd that the normal strains along the principal strain axes are given by: ²x ± x±
= ²xx +2 ²yy +
Ñ
(²xx − ²yy )2 + 4²2xy
,
² y± y±
= ²xx +2 ²yy −
Ñ
(²xx
− ²yy )2 + 4²xy2
2 2 Next we deﬁne the stress tensor. The deﬁnition of stress is a generalization of the deﬁnition of pressure (i.e. force per unit area). We take the small element of the solid on which the external forces act to be an orthogonal parallelepiped with the directions normal to its surfaces deﬁning the axis directions ˆx, yˆ, ˆz . The forces that act on these surfaces can have arbitrary directions: for example, the force on the surface identiﬁed by +ˆx can have F x , F y, F z components. Consequently, we need a secondrank tensor to describe stress, just like for strain. We deﬁne the diagonal elements of the stress tensor
359
Fig. 7.13
7.7
Elastic Deformations of Solids
Deﬁnition of the stress tensor for the cartesian ( x, y, z ) coordinate system. The blue arrows labeled F denote the forces acting on the three faces of the cube. The resulting stress components are denoted as σij = Fj /A i , with F j the force components and Ai the area elements, i, j = x, y, z .
as σii = F i /A i (i = x , y, z ), where F i is the component of the force that acts on the surface in the ˆi direction and A i is the area of this surface of the volume element (see Fig. 7.13). Similarly, the offdiagonal components of the stress are denoted by σij and are given by σij = F j /A i . Care must be taken in deﬁning the sign of the stress components: the normal directions to the surfaces of the volume element are taken to always point outward from the volume enclosed by the parallelepiped. Thus, if the force applied to a surface points outward, the stress is positive (called tensile stress), while if it is pointing inward, the stress is negative (called compressive stress). The stress tensor is also symmetric, σji = σij (i , j = x , y , z), which is a consequence of torque equilibrium. Similar deﬁnitions and relations hold for the cylindrical polar coordinate system (r , θ , z ), ¶ 2 which is related to the cartesian coordinate system (x, y , z ) through r = x + y 2 and −1 (y /x ). θ = tan Just like in the analysis of strains, a rotation of the x , y coordinate axes by an angle θ around the z axis gives the corresponding relations between stresses in the old (σxx , σyy , σxy ) and new (σx± x± , σy± y± , σx± y± ) coordinate systems: σx± x±
=
σy± y±
=
σx± y±
=
1 1 (σxx + σyy ) + (σxx − σyy ) cos 2´ + σxy sin 2´ 2 2 1 1 (σxx + σyy ) − (σxx − σyy ) cos 2´ − σxy sin 2´ 2 2 1 (σyy − σ xx ) sin 2´ + σxy cos 2´ 2
(7.89)
From these relations we can determine the angle ´ that will give vanishing shear stress σx± y± in the new coordinate system, through the relation tan 2´ =
2σxy σ xx
− σyy
(7.90)
which determines the principal stress axes. On the planes that are perpendicular to the principal stress axes, the shear stress is zero, and only the normal component of the stress survives. There are two possible values of the angle ´ that can satisfy the equation for the principal stress, which differ by π/2. The two values of the normal stress from Eq. (7.89)
360
7
are given by: σx± x ±
=
σxx
+ σyy +
Ñ
Lattice Vibrations and Deformations
2 (σxx − σ yy )2 + 4σxy
2
2
,
σy ± y±
=
σxx
+ σyy −
Ñ
(σxx
− σyy )2 + 4σxy2
2
2
(7.91) which turn out to be the maximum and minimum values of the stress. The condition of equilibrium, for a volume element on which an arbitrary force f is exerted, is:
⎛
f = ⎝−
⎞
±
∂ σxj
j =x,y,z
∂j
⎛
⎠ xˆ + ⎝−
⎞
±
∂ σyj
j=x,y,z
∂j
⎛
⎠ yˆ + ⎝−
⎞
±
∂ σzj
j=x,y,z
∂j
⎠ zˆ
(7.92)
where the vector f has dimensions of force/volume. The equilibrium in terms of torque is assured by the fact that the stress tensor is symmetric, σij = σji (i , j = x, y, z ). The stress and strain tensors are useful in describing the response of a solid to an external load. In the simplest expression, we assume that only a normal stress is acting in the x direction, in response to which the solid is deformed by: ²xx
= Y1 σxx
(7.93)
that is, if the stress is compressive (negative), the solid is compressed in the x direction and if the stress is tensile (positive), the solid is elongated. The amount of elongation or contraction is determined by the positive coefﬁcient 1/Y , where the constant Y is called Young’s modulus. The above equation is the familiar Hooke’s law for elastic strain. For an arbitrary stress applied to the solid, we need to invoke all of the strain components to describe its state of deformation; the corresponding general form of Hooke’s law is referred to as a constitutive relation. The traditional way of doing this is through the elastic constants of the solid. These are represented by a tensor of rank 4, C ijkl , with each index taking three values corresponding to x , y , z, but not all of the combinations of the four subscripts give independent elastic constant values. For the independent values, a contracted version of this tensor is used, which is a matrix with only two indices C ij , each of which takes six values (this is referred to as Voigt notation). The connection between the two sets of elastic constants is made through the following identiﬁcation of indices: 1 → xx ,
2 → yy ,
3 → zz ,
4 → yz ,
5 → zx ,
6 → xy
The constitutive law relating stress to strain, in terms of the contracted elastic constants, is:
⎛
σxx
⎞
⎜σ ⎟ ⎜ yy ⎟ ⎜σ ⎟ ⎜ zz ⎟ = ⎜ ⎟ ⎜ σyz ⎟ ⎜ ⎟ ⎝ σzx ⎠ σxy
⎡
C 11 ⎢C ⎢ 12 ⎢C ⎢ 13 ⎢ ⎢ C 14 ⎢ ⎣ C 15 C 16
C 12 C 22 C 23 C 24 C 25 C 26
C 13 C 23 C 33 C 34 C 35 C 36
C 14 C 24 C 34 C 44 C 45 C 46
C 15 C 25 C 35 C 45 C 55 C 56
⎤⎛
⎞
² xx C 16 ⎟ ⎥ ⎜ C 26 ⎥ ⎜ ²yy ⎟ ⎥⎜ ⎟ C 36 ⎥ ⎜ ²zz ⎟ ⎥⎜ ⎟ C 46 ⎥ ⎜ ²yz ⎟ ⎥⎜ ⎟ C 56 ⎦ ⎝ ²zx ⎠ ² xy C 66
(7.94)
The symmetry of the strain tensor further constrains the 36 components of the matrix C ij , leaving only 21 independent values in the most general case: these are the six diagonal
361
7.7
Elastic Deformations of Solids
elements (corresponding to i = j) and the 15 offdiagonal ones on the upper triangle only (corresponding to j < i ), with those on the lower triangle (corresponding to j > i) related by symmetry, C ij = C ji , as indicated explicitly in Eq. (7.94). These equations imply that the solid is linear elastic, that is, its deformation is linear in the applied stress. This is valid for many physical situations if the deformation is sufﬁciently small. The use of the more general tensor of rank 4, C ijkl , simpliﬁes the constitutive equations when the Einstein repeatedindex summation convention is employed; this convention consists of summing over all the allowed values of indices which appear more than once on one side of an equation. For example, the abovementioned linear elastic constitutive relations are written as: σ ij
= C ijkl ²kl
(7.95)
where summation over the values of the indices k and l on the righthand side is implied because they appear twice (they are repeated) on the same side of the equation. Of course, not all the values of C ijkl are independent, because of symmetry; speciﬁcally, the symmetries we have already mentioned, ²ij = ²ji and σ ij = σji , imply that C ijkl = C jikl = C ijlk = C jilk , which makes many of the components of the fourindex tensor C ijkl identical. In the most general case, there are 21 independent components, just like for the contracted notation with two indices. Additional symmetries of the solid further reduce the number of independent values of the elastic constants. For example, in an isotropic solid, many of the components vanish, and of the nonvanishing ones only two are independent. Similarly, in a solid of cubic symmetry, there are only three independent elastic constants, as we show in the examples below. 7.7.3
Strain Energy Density
Next, we make the connection between energy, stress, and strain. We will calculate the energy per unit volume in terms of the applied stress and the corresponding strain, which is called the strain energy density (the repeated index summation is implied in the following derivation). We assume that the energy is at its lowest value, taken to be zero, at the initial state of the system before stress is applied. The rate of change of the energy will be given by: ¼ ¼ dE ∂ ui ∂ui = fi dV + σij nj dS (7.96) dt ∂t ∂t V S
where we have used the alternative notation u 1 = u , u 2 = v , u 3 = w and x 1 = x , x 2 = y , x 3 = z , employed in Eqs (7.85) and (7.86). The ﬁrst term in Eq. (7.96) is due to volume distortions, with f i the i component of the force on the volume element dV . The second term in Eq. (7.96) is due to surface distortions: the surface contribution involves the vector n with components ni (i = 1, 2, 3), which is the unit vector normal to a surface element dS ; the product σij n j represents the i component of the force on the surface element. By turning the surface integral to a volume one through the divergence theorem, we obtain: dE dt
=
¼ ² V
fi
∂ ui ∂t
+ ∂∂x
´
j
σij
∂ ui ∂t
µ³
dV
(7.97)
362
7
Newton’s law of motion F
Lattice Vibrations and Deformations
= m (d2 r/dt 2 ) applied to the volume element takes the form ρ
∂
2
ui
= fi + ∂∂σxij
∂ t2
(7.98)
j
where ρ is the density. In this equation fi is the component of the external force exerted on the volume element and ∂ σij /∂ x j is the contribution of the stress, which also amounts to a force on the volume element [see also Eq. (7.92), where the corresponding relation for equilibrium conditions is given]. From the deﬁnitions of the strain and rotation tensors, Eqs (7.85) and (7.86), we have:
´
∂ ∂t
∂ ui
µ
= ∂∂t
∂xj
(
²ij
+ ξij
)
(7.99)
Using Eqs (7.98) and (7.99) to simplify the expression for the change in the energy, Eq. (7.97), we obtain: dE dt
=
d (K dt
+ U) =
¼ Á
ρ
V
∂2ui ∂ui ∂ t2
Â
+
dV
∂t
¼ ² V
σij
∂ ²ij
³
∂t
dV
(7.100)
where we have taken advantage of the symmetric and antisymmetric nature of the stress and the rotation tensors to set σij ξ ij = 0. In Eq. (7.100), the ﬁrst term on the righthand side represents the kinetic energy K and the second the potential energy U . To obtain the kinetic energy K , we integrate over time the ﬁrst term on the righthand side of the last equation: K
²
¼
= 21
V
ρ
∂ ui
³2
dV
∂t
(7.101)
The strain energy density, denoted by µ, is deﬁned as the potential energy per unit volume;7 from the expression of the second term on the righthand side of Eq. (7.100), µ takes the form ¼ U
=
V
µ dV
⇒ ∂∂µt = σij ∂∂²tij ⇒ σij = ∂∂ µ²
(7.102)
ij
Now we can use the Taylor expansion for the strain energy density in terms of small strains: µ
= µ0 +
1 2
Á
2
Â
∂ µ
(7.103)
²ij ² kl
∂ ²ij ∂ ²kl
0
where the ﬁrstorder term is omitted on the assumption that we are referring to changes from an equilibrium state. Taking a derivative of this expression with respect to ²mn, we obtain: σmn
= =
∂µ ∂ ²mn
1 2
Á
=
1 2
Á
2
∂ µ ∂ ²mn ∂ ²kl
Â
∂ 2µ ∂ ²ij ∂ ²kl
Â
² kl
0
+
( δimδ jn ²kl 0
1 2
Á
+ δkmδln ²ij)
2
∂ µ ∂ ²mn ∂ ²ij
Â ² ij
0
=
Á
2
∂ µ ∂ ²mn ∂ ²ij
Â ²ij
(7.104)
0
7 Depending on the conditions, we can identify U as the internal energy if the loading process is adiabatic, that is,
without exchange of heat, or as the Helmholtz free energy if the loading process is isothermal, that is, quasistatic reversible under constant temperature.
363
7.7
Elastic Deformations of Solids
which, by comparison to Eq. (7.95), yields: C ijkl
=
Á
Â
2
∂ µ ∂ ²ij ∂ ²kl
(7.105) 0
This last equation demonstrates that the elastic constant tensor can be obtained by calculating the variations to second order in the potential energy density with respect to small strains. Using this expression, we can write the strain energy density as: µ
= µ0 + 21 C ijkl ²ij²kl = µ0 + 12 σij²ij
(7.106)
which shows that the strain energy density due to elastic deformation is obtained by multiplying the stress with the strain tensors. Another interesting result that this expression reveals is that the strain energy density is quadratic in the strain tensor ²ij . The relations we have just described within continuum elasticity and the corresponding general relations between forces F and the time derivatives of the position r or spatial derivatives of the potential energy U (r) are summarized below.
Correspondence between classical mechanics and continuum elasticity
Mechanics (1)
F=m
(2)
F=
2
d 2r d t2
(3)
−∇r U (r) F= − κ (r − r0)
(4)
U (r)
(1) (2) (3) (4)
Elasticity fi
+ ∂∂σxij = ρ ∂∂ tu2i j
= ∂² ij σij = C ijkl² kl ∂µ
σij
= U 0 + 12 κ (r − r0)2
µ
= µ0 + 21 C ijkl ²ij²kl
Equation of motion. Force from potential energy gradient/stress from strain energy density. Hooke’s law: linear spring force/linear stress–strain relation. Harmonic approximation: potential energy/strain energy density.
7.7.4
Isotropic Solid
We next examine the case of an isotropic, elastic solid, that is, a solid in which the elastic response in different directions is the same, and hence the corresponding elastic constants are equivalent. First, when a normal strain σxx is applied in the x direction, the solid not only deforms according to Eq. (7.93), but also deforms in the y, z directions according to: ² yy
= ²zz = −ν²xx = −ν σYxx
(7.107)
364
7
Lattice Vibrations and Deformations
where ν is called Poisson’s ratio. Poisson’s ratio is a positive quantity: when a material is pulled in one direction its crosssection perpendicular to the pulling direction becomes smaller (a rod gets thinner when pulled along its length).8 From this we conclude that if three normal stresses σxx , σyy , σzz are applied to an element which is an orthogonal parallelepiped with faces normal to the x, y, z axes, its state of strain will be given by: ² xx
= Y1 [ σxx − ν ( σyy + σzz )], ²yy = Y1 [σyy − ν (σxx + σzz )], ²zz = Y1 [σzz − ν (σ xx + σyy )]
(7.108) An analogous expression holds for shear stresses. Namely, if a shear stress σxy (or σyz , σzx ) is applied to a solid, the corresponding shear strains are given by: ² xy
= 21μ σxy ,
²yz
= 21μ σyz,
² zx
= 21μ σzx
(7.109)
In these expressions the shear modulus μ is used to relate strain to stress for the offdiagonal (shear) components. Of the three elastic constants introduced so far, Young’s modulus Y , Poisson’s ratio ν , and shear modulus μ , only two are independent, because they obey the relation Y
= 2μ(1 + ν ) ⇒ μ = 2(1 Y+ ν )
(7.110)
The relations for the strain can be written compactly with use of the Kronecker δ and the Einstein summation convention, as: ² ij
= 1 +Y ν σ ij − δij Yν ( σxx + σyy + σzz ),
i, j
= x, y, z
(7.111)
These equations can be inverted to give the stresses in terms of the strains: σij
= 2μ²ij + δijλ(²xx + ²yy + ²zz),
i, j
= x, y, z
(7.112)
where the quantity λ is deﬁned as: λ
Yν 2μν = (1 + ν )(1 = − 2ν ) 1 − 2ν
(7.113)
and is known as Lam´e’s constant. In cartesian coordinates, the above equation represents the following set of relations: Y = 2μ²xx + λ(²xx + ²yy + ²zz ) = (1 + ν )(1 − 2ν )
¾
(1 − ν )²xx + ν (²yy
+ ²zz )
¾
(1 − ν )²yy + ν (²xx
+ ²zz )
Y = 2μ²zz + λ(²xx + ²yy + ²zz) = (1 + ν )(1 − 2ν ) σxy = 2μ²xy , σyz = 2 μ²yz , σzx = 2 μ²yz
¾
σxx σyy σzz
Y = 2μ²yy + λ(²xx + ²yy + ²zz ) = (1 + ν )(1 − 2ν )
¿ ¿
¿
(1 − ν )²zz + ν (²xx + ²yy )
8 It is often mentioned that in certain exceptional solids, like cork, Poisson’s ratio can be negative. Cork actually
has a very small (near zero) Poisson ratio, but recently some materials have been synthesized that do have negative Poisson ratio.
365
7.7
Table 7.3
ν
Elastic Deformations of Solids
Values of the shear modulus
μ, Lamé’s constant λ, and Poisson’s ratio
for representative covalent and ionic solids (left column) and metals (right
column).
λ and ν
are given in megabars (1 Mbar = 100 GPa);
ν
is dimensionless.
The crystals in each category are ordered by their shear modulus value in decreasing order. Source: Hirth and Lothe, mentioned in Further Reading.
Covalent and ionic solids Crystal μ λ
Metals ν
C Si Ge
5.36 0.681 0.564
0.85 0.524 0.376
0.068 0.218 0.200
MgO LiF PbS NaCl KCl AgBr
1.29 0.515 0.343 0.148 0.105 0.087
0.68 0.307 0.393 0.146 0.104 0.345
0.173 0.187 0.267 0.248 0.250 0.401
Crystal W Mo Cr Ni Fe Cu Ag Au Al Pb Na K
μ
λ
ν
1.6 1.23 1.21 0.947 0.860 0.546 0.338 0.310 0.265 0.101 0.038 0.017
2.01 1.89 0.778 1.17 1.21 1.006 0.811 1.46 0.593 0.348 0.025 0.029
0.278 0.305 0.130 0.276 0.291 0.324 0.354 0.412 0.347 0.387 0.201 0.312
Values of the shear modulus, Lam´e’s constant, and Poisson’s ratio for representative solids are given in Table 7.3. Finally, we use these expressions to obtain an equation for the strain energy density, starting from Eq. (7.106), and setting the constant term µ0 = 0. Inserting the expressions we found for the stresses σij in terms of the strains ²ij above, we arrive at: µiso
= μ1(1−−2νν ) (²xx2 + ²yy2 + ²2zz) + 2μ( ²xy2 + ²yz2 + ²zx2 ) + λ(²xx ²yy + ²yy ²zz + ²zz ²xx )
(7.114)
an expression that will prove useful in the following derivations.
Isotropic Solid under Hydrostatic Pressure
We use the expressions derived so far to analyze the effects of hydrostatic pressure applied to an isotropic solid. We consider an orthogonal parallelepiped element in the solid which experiences stresses: σxx
= σyy = σzz = −p,
σxy
= σyz = σzx = 0
(7.115)
with the change in hydrostatic pressure p > 0. The ensuing strains are then given by: ² xx
= ²yy = ²zz = −1 −Y 2ν p ,
² xy
= ²yz = ²zx = 0
(7.116)
The change in volume of the element will be given by: dx (1 + ²xx ) × dy(1 + ²yy ) × dz (1 + ²zz)
= (1 + ²xx + ²yy + ²zz )dx dy dz
(7.117)
366
7
Lattice Vibrations and Deformations
where we neglect terms higher than ﬁrst order in the strains. We deﬁne the total fractional change in volume ²¯ = ²xx + ²yy + ²zz , and ﬁnd from the above equation that:
¯ = −Y3 (1 − 2ν )p
²
But the total fractional change in volume is also given as:
¯ = ±VV = −1B p
²
where B is the bulk modulus of the solid, as deﬁned in Eq. (7.78). This relationship reveals that the bulk modulus is expressed in terms of Young’s modulus and Poisson’s ratio as: B
μ (1 + ν ) 2 = λ+ μ = 3(1 −Y 2ν ) = 23(1 − 2ν ) 3
(7.118)
where we have also used the deﬁnition of Lam´e’s constant, Eq. (7.113). We can take advantage of this result to express various quantities in terms of the bulk modulus. Speciﬁcally, for the stress–strain relations we ﬁnd: σij
= B ²kk δij + 2μ
´
²ij
−
1 ²kk 3
µ
which for the diagonal terms becomes: σxx
= B ²¯ + 2μ
´
² xx
− 3²¯
µ
,
σyy
= B ²¯ + 2μ
= B ²¯δij + 2μ
´ ² yy
− ²3¯
´
µ ,
σzz
µ ¯ ² ij − 3 ²
= B ²¯ + 2μ
´ ²zz
− 3²¯
µ
By adding these three expressions and deﬁning the volume stress σ¯ = (σxx + σ yy + σzz )/3 (which is also called the hydrostatic component of stress), we obtain:
¯ = B1 σ¯
(7.119)
²
The result of Eq. (7.119) applies to any state of stress, and the quantities ²¯ , σ¯ are both invariant with respect to orthogonal transformations of the coordinate axes. The reason for this simple relation is that the shear strains, which in the present example are zero, do not contribute to any changes in the volume. We can also use the expressions derived so far to express the strain energy density in a form that provides some insight into the different contributions. We start with our expression from Eq. (7.114) and use the relations between B , μ, λ from Eq. (7.118) to write the strain energy density as: µiso
=
´
µ
3 2 B − λ (²xx 2
+ ²yy2 + ²zz2 ) + 2μ(²xy2 + ²2yz + ²zx2 ) + λ(²xx ²yy + ²yy ²zz + ²zz ²xx )
but we also have from Eq. (7.118): 3 B 2
− λ = 21 λ + μ
and
1 λ 2
= 12 B − 13 μ
and combining terms to form a perfect square, we ﬁnd µiso
=
´
µ
1 1 2 B − μ (²xx + ²yy + ²zz )2 + μ (²2xx + ²yy + ²zz2 ) + 2μ(²xy2 2 3
+ ²yz2 + ²zx2 )
367
7.7
Elastic Deformations of Solids
which can be written in a more compact and elegant form using Einstein notation: µ iso
=
1 B (²kk )2 + μ 2
²
² ij ² ij
−
1 (²kk )2 3
³
(7.120)
This is an interesting expression because it clearly shows that the ﬁrst term, which is quadratic in the volume change captured by ²¯ = (²xx + ²yy + ²zz ), is multiplied by the coefﬁcient (1/2)B and corresponds to the energy cost for uniform volume expansion or contraction, while the rest of the contribution is related to shear, and contains all the offdiagonal terms of the strain.
Stress Waves in Isotropic Solid
Finally, we calculate the speed of different types of stress waves through an isotropic solid. To this end, we use similar manipulations as above for the strain energy density to rewrite the general equilibrium condition of Eq. (7.98), for the case of an isotropic solid with no external forces, as: 2
(λ
2
2
+ μ) ∂∂x ∂uxj + μ ∂∂x ∂uxi = ρ ∂∂ tu2i i
j
j
j
or equivalently, in vector notation: 2
(λ
+ μ) ∇r (∇r · u) + μ∇r2 u = ρ ∂∂ t2u
(7.121)
This last expression allows us to ﬁnd the speed with which waves can propagate in an isotropic solid. We assume that the displacement ﬁeld u has a wave form
u( r, t) = ef (q · r − ct )
(7.122)
where e is the polarization of the wave, q is the direction of propagation, and c is its speed. Using this expression for u (r, t) in Eq. (7.121), we obtain (λ
+ μ) f ±± (q · r − ct )(e · q)q + μef ±± (q · r − ct )q2 = c 2 ρef ±± (q · r − ct )
where f ±± (x ) is the second derivative of f (x ) with respect to its argument. For dilatational waves, e ¹ q , we then ﬁnd that the speed of the wave is given by: cd
=
»
λ
+ 2μ =
»´
µ
B
ρ
+ 43 μ
1 ρ
(7.123)
while for shear waves, e ⊥ q, the speed of the wave is given by: cs
=
Ã
μ ρ
(7.124)
Note that in order to make the expression given above an identity for any function f (x ), for either dilatational or shear waves, we must have q 2 = 1; this implies that there is no length scale for the wave, that is, no natural scale to set the wavelength. We also note that on the surface of the solid there can only exist shear waves; the speed of propagation of these waves, called the Rayleigh speed c R , is typically c R ≈ 0.9c s .
368
7
Lattice Vibrations and Deformations
7.7.5
Solid with Cubic Symmetry
We examine next the case of a solid which has cubic symmetry, which is quite common in crystals. The minimal symmetry in such a case consists of axes of threefold rotation, which are the major axes of the cube, as illustrated in Fig. 3.5(a). The rotations by 2π/3 around these symmetry axes lead to the following permutations of the x, y, z axes:
→y→z→x 2 : x→z→ − y→x 3 :x→ − z→y→x 4 :x→ − y→ − z→x 1 :x
(7.125)
as described in Chapter 3, Table 3.3. Now we can use these general symmetries of the solid to deduce relations between the elastic constants. The simplest way to derive these relations is to consider the strain energy density expression of Eq. (7.106), which must be invariant under any of the symmetry operations. This expression for the energy is quadratic in the strains, so that the terms appearing in it can have one of the following forms: 2
²ii ,
2
²ii ²jj ,
²ij ,
²ii ² ij ,
² ii ² jk ,
² ij ² jk
(7.126)
with (i, j, k ) = (x , y , z ). Each type of the ﬁrst three terms in Eq. (7.126) gives a contribution to the energy that must be the same for all possible values of the indices, since the three 2 axes x, y, z are equivalent due to the cubic symmetry. Speciﬁcally, the contribution of ²xx 2 2 2 must be the same as that of ²yy and that of ²zz , and similarly for the terms ²ij and ²ii ²jj . These considerations imply: C 11
= C 22 = C 33,
C 12
= C 13 = C 23,
C 44
= C 55 = C 66
so there are at least three independent elastic constants, as claimed earlier. Moreover, the ﬁrst three terms in Eq. (7.126), when summed over the values of the indices, are unchanged under the symmetry operations of Eq. (7.125), while the last three terms change sign. For example, the term 2
² xx
+ ²yy2 + ²2zz
[which corresponds to the ﬁrst term in Eq. (7.126), since C 11 = C 22 = C 33 ] is unchanged under any of the operations in Eq. (7.125). In contrast to this, the term ²xx ²xy under the third operation in Eq. (7.125) is transformed into:
→ ²z¯¯z²¯zx = −²zz ²zx (where we have used the notation ¯z = − z for the subscripts of the strain), which is ² xx ²xy
another term of the same character but opposite sign. The coefﬁcients of terms that change sign must vanish, since otherwise, for an arbitrary state of strain, the energy would not be invariant under the symmetry operations. This implies vanishing of the following coefﬁcients: C 14
= C 15 = C 16 = 0,
C 24
= C 25 = C 26 = 0,
C 34
= C 35 = C 36 = 0
369
7.7
Elastic Deformations of Solids
and similar considerations lead to: C 45
= C 46 = C 56 = 0
leaving as the only independent coefﬁcients C 11 , C 12, C 44. This result leads to the following expression for the strain energy density of a solid with cubic symmetry: µcubic
=
· 1 2 C 11 ²xx 2 (
+C 12
¸
+ ²2yy + ²zz2 + 2C 44 ) ² xx ²yy + ² yy ²zz + ²zz ² xx
·
2
²xy
+ ²yz2 + ²zx2
¸
(7.127)
where we have taken the constant term µ0 to be zero for simplicity. This expression is also useful for calculating the elastic constants C 11 , C 12, C 44, using totalenergy calculations of the type discussed in detail in Chapter 4. Speciﬁcally, for C 11 it sufﬁces to distort the solid so that of all the strain components, only ²xx is nonzero, and then calculate the total energy as a function of the magnitude of ²xx and ﬁt it with a secondorder term in this variable: the coefﬁcient of this term is 21 C 11 . In a similar fashion, one can obtain values for C 12 and C 44. The diagonal components of the strain correspond to the change in volume, so ²xx corresponds to a volume change due to elongation or contraction of the solid in one direction only. In this sense, the elastic constant C 11 is related to the response of the solid to elongation or contraction in one direction only. The strains ²ij , i µ= j describe pure shear distortions of the solid without changes in the volume, so that the elastic constant C 44 is related to the response of the solid to shear forces. The elastic constant C 12 involves two different diagonal components of the strain, so that it is related to simultaneous distortions (elongation or contraction but not shear) along two different orthogonal axes. From this information, we can also deduce that the bulk modulus of a solid with cubic symmetry is related to the elastic constants C 11 and C 12 only (see Problem 12). In Table 7.4 we give the values of the elastic constants of some representative cubic solids. 7.7.6
Thin Plate Equilibrium
We consider next the case of a thin plate of thickness h in the z direction, which is very small compared to the size of the plate in the other two, x and y directions. This situation is relevant to graphene and various other materials that can be produced in the form of 2D, atomically thin layers. The thin plate can be analyzed as an isotropic solid in the x , y dimensions. We imagine that the plate is slightly bent, so that it deviates locally by a very small amount from being planar. Thus, the displacements u , v , w along the x , y , z axes, respectively, will be small, and speciﬁcally we will take the displacement along z to depend only on the position along the plane of the plate, w (x , y ). Referring back to the deﬁnition of the various components of the stress in Fig. 7.13 in the limit where the solid has inﬁnitesimal extent along the z axis, we realize that we must set: σxz
= σyz = σzz = 0
Then, using the stress–strain relation for an isotropic solid, Eq. (7.112), we deduce that for this situation we have: ²xz = ²yz = 0. We will next use the deﬁnition of the shear strains in
370
7
Table 7.4
B
Bulk moduli
Lattice Vibrations and Deformations
(GPa) and elastic constants,
C11 , C12 , C44
(Mbar) for representative cubic
crystals at room temperature. Sources : D. R. Lide, (Ed.), CRC Handbook of Chemistry and Physics (CRC Press, Boca Raton, FL, 19992000); S. Haussühl,
DIA
= diamond,
ZBL
= zincblende,
Z. Phys. 159, 223 (1960). The names of crystal structures are
CUB
= cubic,
FCC
BCC
= face centered cubic,
= body
centered cubic (see also Chapter 1).
B
C11
C12
C44
C (DIA) Si (DIA) Ge (DIA)
443 98.8 77.2
10.76 1.658 1.284
1.250 0.639 0.482
5.760 0.796 0.667
AlSb (ZBL) GaP (ZBL) GaAs (ZBL) GaSb (ZBL) InP (ZBL) InAs (ZBL) InSb (ZBL)
58.2 88.7 74.8 57.0 71.0 60.0 47.4
0.894 1.412 1.188 0.884 1.022 0.833 0.672
0.443 0.625 0.537 0.403 0.576 0.453 0.367
0.416 0.705 0.594 0.432 0.460 0.396 0.302
ZnS (ZBL) ZnSe (ZBL) ZnTe (ZBL)
77.1 62.4 51.0
1.046 0.807 0.713
0.653 0.488 0.408
0.461 0.441 0.312
LiCl (CUB) NaCl (CUB) KCl (CUB) RbCl (CUB) CsCl (CUB)
36.9 28.6 20.8
0.493 0.495 0.407 0.361 0.364
0.231 0.129 0.071 0.062 0.088
0.250 0.129 0.063 0.047 0.080
Crystal
B
C11
C12
C44
320 310 273 230 220 200 190 186 181 170 168 162 137 101 72.2 46.0 11.6 6.8 3.2 3.1 1.6
5.800 5.224 4.637 3.467 1.924 2.602 3.398 2.481 2.271 2.465 2.260 2.287 1.683 1.240 1.067 0.497 0.135 0.074 0.037 0.030 0.025
2.420 2.044 1.578 2.507 1.630 1.545 0.586 1.549 1.760 1.345 1.400 1.190 1.221 0.937 0.604 0.423 0.114 0.062 0.031 0.025 0.021
2.560 1.608 1.092 0.765 0.420 0.826 0.990 1.242 0.717 0.287 1.160 0.432 0.757 0.461 0.283 0.150 0.088 0.042 0.019 0.017 0.015
Crystal Ir (FCC) W (BCC) Mo (BCC) Pt (FCC) Au (FCC) Ta (BCC) Cr (BCC) Ni (FCC) Pd (FCC) Nb (BCC) Fe (BCC) V (BCC) Cu (FCC) Ag (FCC) Al (FCC) Pb (FCC) Li (BCC) Na (BCC) K (BCC) Rb (BCC) Cs (BCC)
terms of the displacements, Eq. (7.83), and integrate once to obtain:
´
² xz
= 0 ⇒ ∂∂wx = −∂∂ uz ⇒ u = − ∂∂wx
µ
z,
² yz
´
= 0 ⇒ ∂∂wy = −∂∂ vz ⇒ v = − ∂∂wy
µ z
where we have set the constants of integration to zero, to reﬂect the fact that without any deformation the strains are zero and the plate is ﬂat, lying on the x , y plane. From these results we can calculate the different components of the strain, ﬁnding: ² xx
∂u
Ç
∂2w
= ∂x = − ∂x2
È
z,
² yy
∂v
Ç
∂ 2w
= ∂ y = − ∂ y2
È
z,
² xy
=
1 2
´
∂u ∂y
∂v
²zz (1
− ν ) + ν (²xx + ²yy ) ⇒ ²zz = 1 − ν
Ç
∂ 2w ∂x2
+
Ç
∂ 2w
+ ∂x = − ∂x∂y
Similarly, the condition for σzz vanishing, from Eq. (7.83), leads to: ν
µ
∂ 2w ∂y2
È
z
È z
Having calculated all the components of the strain for this case, we can use them in the expression for the strain energy density, Eq. (7.114), which then becomes, after grouping
371
7.8
Application: Phonons of Graphene
terms:
µ plt
= 1 −μ ν
⎡Ç ∂2w z2 ⎣ ∂x2
+
∂ 2w
È2
∂y2
⎧Ç È ⎨ ∂ 2w 2
+ 2(1 − ν ) ⎩
∂x∂y
⎫⎤
⎬ ∂2w ∂2w
−
∂ x 2 ∂ y2
⎦ ⎭
(7.128)
To obtain the total free energy of the plate we must integrate this expression over the entire volume of the plate. This volume extends from z = − h/2 to z = h /2 in the z direction at each point ( x, y), and over the entire x, y plane. Thus, the free energy per unit area of the x , y plane will be given by: 3
γ
= 24(1Yh− ν 2 )
⎡Ç 2 ⎣ ∂ w ∂ x2
2
⎧Ç È ⎨ ∂2w 2
È2
+ ∂∂ yw2 + 2(1 − ν ) ⎩
∂ x∂ y
−
⎫⎤ ⎬ ∂ w∂ w ⎦ ∂ x2 ∂ y 2 ⎭ 2
2
(7.129)
where we have used the relations of Eq. (7.110) to express μ in terms of Y , ν . To derive the equation of equilibrium of the plate, we need to perform a variational calculation to ensure that the energy is at a minimum, and set the expression obtained in this way to the sum of the external forces fz , acting per unit area of the plate in the direction perpendicular to it. This is a rather elaborate calculation, performed in detail in the book by L. D. Landau and E. M. Lifshitz, Theory of Elasticity (see Further Reading). The result is: fz
Yh 3
− 12(1 − ν 2)
Ç
∂2w ∂x2
+
∂2w
È2
∂y2
=0
(7.130)
where w , f z are both functions of the inplane variables x, y.
7.8
Application: Phonons of Graphene
As a case study in applying the concepts developed above, we examine the phonon spectrum of graphene, a 2D layer of C atoms forming a honeycomb lattice. The structure is illustrated in Fig. 7.14, along with ﬁrstneighbor and secondneighbor interactions associated with the two basis atoms of the primitive unit cell, labeled A and B , in the Born forceconstant model. The lattice constants and atomic positions are deﬁned as:
a1
= 2a
·√
¸
3xˆ + y ˆ , a2 =
a
2
·√
¸
3xˆ − y ˆ , tA
= √a xˆ , 3
tB
=0
Even though all atoms lie on the x , y plane in the lowestenergy conﬁguration, we will consider their motion in all three dimensions. From the ﬁrstneighbor interactions, which couple atoms at different sites (A with B ), with bondstretching and bondbending constants denoted as κr , κ θ , the contributions to
372
7
Lattice Vibrations and Deformations
a1
B
A a2
Fig. 7.14
The Born forceconstant model for graphene. Gray circles represent the C atoms on the plane and black lines the bonds between them. The red arrows indicate the primitive lattice vectors a1 , a2 with the two basis atoms in the unit cell labeled A and B, with ﬁrstneighbor interactions indicated by blue lines. Secondneighbor interactions are also shown, by magenta lines, only for site A situated at the center of a hexagon outlined by thin dashed lines (see Problem 13).
the potential energy from all terms that involve at least one site within the primitive unit cell are:
−κ ±U AB = 2 κr
¹·
S A00 − SB01
κθ
2
θ
¸
Å ¹· º2
SA00 − S B00
· Rˆ AB + 01
¹·
¸
º2
· Rˆ AB + 00
SB00 − SA1¯ 0
¸
¹· º2
SA00 − S B10
· Rˆ BA + 1¯ 0
¹·
¸
º2
· Rˆ AB + 10
S B00 − SA01¯
¸
· Rˆ BA 01¯
º2 Æ
+
ÅÄ Ä Æ Ä Ä Ä Ä Ä Ä Ä Ä ÄS A − S B Ä2 + ÄS A − SB Ä2 + ÄSA − S B Ä2 + ÄSB − S A Ä2 + ÄS B − SA Ä2 Ä Ä Ä 00 Ä 00 Ä 00 Ä 00 Ä 00 01 Ä 10 Ä 00 Ä 01¯ 1¯ 0
where S Anm stands for the displacement of an atom at site A in the unit cell displaced relative to the origin by na1 + m a2 (and similarly for SBnm ) and the unit vectors along the bonds are given by:
ˆ AB R nm
= ttA −− ((ttB ++ nnaa1 ++ mm aa2)) A
B
1
2
with n , m = 0, ´1 and 1¯ stands for −1. Taking derivates of this expression, according to Eq. (7.18), to derive the dynamical matrix, we ﬁnd the matrix shown in Table 7.5. First, we note that the 6 × 6 dynamical matrix, coupling the motion of atoms at sites A and B in all three dimensions, splits into two smaller diagonal matrices, one being a 4 × 4 matrix that couples the x , y components of the displacements, and another being a 2 × 2 matrix that couples the z components of the displacements. This implies that within the Born forceconstant model, the motion out of the plane is completely decoupled from the inplane motion, which has important consequences, as discussed below. The various entries in this table are calculated as follows. The diagonal matrix elements for the ﬁrstneighbor interactions are: 3 D xy = (κr + κθ ) , D z = 3κ θ 2
373
7.8
Table 7.5
Application: Phonons of Graphene
Dynamical matrix for graphene in the Born
forceconstant model, including contributions from ﬁrst nearest neighbors only. The various entries are given explicitly in the text.
Ax Ay Az Bx By Bz
Ax
Ay
Az
Bx
By
Bz
Dxy 0 0 C ∗( k) E ∗ (k) 0
0 Dxy 0 E ∗ (k) F ∗ ( k) 0
0 0 Dz 0 0 G∗ (k)
C( k) E( k) 0 Dxy 0 0
E (k) F (k) 0 0 Dxy 0
0 0 G(k) 0 0 Dz
while the offdiagonal matrix elements are:
· · ¸ ¸ = −κr − κr +43κ eik·a + eik·a F (k) = −κ − 3κr 4+ κ eik· a + eik·a √ ¸ · ¸ 3 (κ r − κ ) · ik ·a e E (k) = − − ei k·a , G (k) = − κ 1 + eik· a + eik ·a 4
C (k)
θ
1
θ
2
1
θ
θ
2
θ
1
1
2
2
The results from diagonalizing the matrix to obtain the frequency eigenvalues are shown in Fig. 7.15, along highsymmetry directions of the 2D Brillouin zone. We also show in this ﬁgure results from ﬁrstprinciples calculations based on DFT for comparison. The values of the force constants κr , κ θ were chosen to reproduce approximately the value of the ﬁrstprinciples results for the highest optical frequency at ³ and the lowest acoustic frequency at M; we have also allowed the value of κθ that appears in the matrix for the z displacements to be different from the one for the x, y displacements, and adjusted it to give approximately the same value as the ﬁrstprinciples calculations for the highest mode at ³. One glaring difference, which cannot be ﬁxed for any choice of parameters in the Born forceconstant model, is the behavior of the outofplane acoustic modes. Indeed, this behavior is peculiar. All three acoustic frequencies in the forceconstant model are linear in the wavevector magnitude k for small values, as for all other examples we have discussed in this chapter. In contrast to this, the lowest acoustic frequency from the ﬁrstprinciples calculations is quadratic in the wavevector magnitude k . This unusual behavior is due to the special nature of the graphene 2D sheet. Speciﬁcally, in the real material the outofplane motion of atoms is coupled to the inplane motion; in the forceconstant model, no such coupling is allowed, as a consequence of the fact that there are no outofplane bonds. Any attempt to capture this behavior within the Born forceconstant model, for example, by including nextnearestneighbor interactions as if there were effective inplane bonds between them, is doomed to failure.9 But because there are no atoms to inhibit the displacement in the direction perpendicular to the plane, the effect of the coupling between 9 To explore this issue, the reader is guided through the steps of including secondneighbor interactions in the
forceconstant model (shown schematically in Fig. 7.14) in Problem 13
374
Fig. 7.15
7
Lattice Vibrations and Deformations
The phonon spectrum of the honeycomb lattice (graphene) in 3D space. Left: Born forceconstant model with ﬁrstneighbor interactions only. The blue bands involve motion on the plane of the lattice (x, y), the green bands involve motion perpendicular to the plane (zaxis). Right: The phonon bands of graphene (red dots) as obtained from ﬁrstprinciples calculations based on DFT (performed by D. T. Larson).
inplane and outofplane motion is second order, and therefore the dependence of the frequency on the wavevector is higher order than linear. The quadratic behavior of the lowest acoustic mode is nicely captured by the analysis of the thin plate equilibrium within elasticity theory, discussed in the previous section. From Eq. (7.130), to describe the dynamical behavior of the plate we set the external forces per unit area f z equal to zero and let the total force per unit area be equal to the mass per unit area times acceleration in the z direction: Yh 3
− 12(1 − ν 2)
Ç
∂
2
w
∂x2
+
∂
2
w
È2
2
= ρh ∂∂ tw2
∂y2
where ρ is the mass density per unit volume. We deﬁne the constant ¶
=
Ç
Yh 2
È1/ 2
12 ρ (1 − ν 2 )
and introduce wavelike harmonic behavior for the variable w in both space and time: w (x , y , t )
= w 0 ei k·r e−i
ωt
with k and r being 2D vectors with x , y components only:
r = x ˆx + y yˆ , k = k x xˆ + ky yˆ Substituting the expression for w (x , y , t ) in the equation for the dynamical response of the plate, we ﬁnd that the frequency and the wavevector must satisfy the relation ω
2
= ¶2 k4 ⇒ ω = ´¶k2
375
Problems
This result explains the quadratic behavior of the frequency related to the outofplane motion for small wavevector magnitude. This type of motion is referred to as the “ﬂexural mode” of graphene. The curvature of ω for small  k is determined by the inplane Young’s modulus Y and Poisson’s ratio ν , as well as the thickness of graphene h and its mass density ρ , all of which enter in the constant ¶.
Further Reading
1. The Mathematical Theory of Elasticity , A. E. H. Love (Cambridge University Press, Cambridge, 1927). This is a classic book on the theory of elasticity, with advanced treatments of many important topics. 2. Elasticity: Tensor, Dyadic and Engineering Approaches , P. C. Cou and N. J. Pagano (Van Nostrand, Princeton, NJ, 1967). This is an accessible and concise treatment of the theory of elasticity. 3. Theory of Elasticity , 3rd English edition, L. D. Landau and E. M. Lifshitz, translated by J. B. Sykes and W. H. Reid (Pergamon Press, New York, 1986). A classic text with indepth treatment of many advanced topics. 4. Modeling Materials: Continuum, Atomistic and Multiscale Techniques , E. B. Tadmor and R. E. Miller (Cambridge University Press, Cambridge, 2011). This is a modern treatment of many important topics in modeling materials, with a very concise account of elasticity theory. 5. Theory of Dislocations , J. P. Hirth and J. Lothe (Krieger, Malabar, 1992). This is a standard reference for the physics of dislocations, which are defects responsible for the behavior of solids in the plastic regime, that is, beyond the elastic range.
Problems
1.
Use the Born forceconstant model to calculate the phonon frequencies for silicon along the L−³ −X directions, where L = (π/a)(1, 1, 1) and X = (2π/a)(1, 0, 0). Take the ratio of the bondstretching and bondbending force constants to be κ r /κθ = 16. Fit the value of κr to reproduce the experimental value for the highest optical mode at ³ , which is 15.53 THz, and use this value to obtain the frequencies of the various modes at X; compare these to the values given in Table 7.9. Determine the atomic displacements for the normal modes at ³ , the lowest acoustic branch at X and L, and the highest optical branch at X and L.
2.
Show that the kinetic and potential energy contribution to the energy of a simple harmonic oscillator are equal. Show explicitly (that is, not by invoking the analogy to a set of independent harmonic oscillators) that the same holds for the kinetic and potential energy contributions to the energy of a collection of phonons, as given in Eq. (7.42).
376
7
Lattice Vibrations and Deformations
3.
Do phonons carry physical momentum? What is the meaning of the phonon wavevector q ? How does the phonon wavevector q enter selection rules in scattering processes, such as a photon of momentum k scattering off a crystal and emerging with momentum k ± after creating a phonon of momentum q ?
4.
Show that in the Debye model all modespeciﬁc Gr¨uneisen parameters γk(l) , deﬁned in Eq. (7.74), are equal. Using this fact, ﬁnd the behavior of the thermal expansion coefﬁcient α as a function of temperature T , in the low and hightemperature limits (T → 0 and T ¸ ´ D , respectively); assume that the bulk modulus B has a very weak temperature dependence.
5.
From the third law of thermodynamics (Appendix D), the entropy is given by: S (T , V )
=
¼ 0
T
1 τ
´
∂ E (τ , V )
µ
∂τ
dτ V
at constant volume V . From this expression, using Eq. (7.52) for the internal energy, show that the entropy of a collection of phonons can be expressed as: S (T )
= kB
± k,l
(n¯ k
(l )
+ 1) ln(n¯ (kl) + 1) − n (k¯l) ln(n¯ (kl))
with n¯ (kl) the average number of phonons in the state with frequency ωk(l ). The change of variables x = h¯ ω/kB T is useful in evaluating the integral involved in the expression for the entropy by partial integration. Having expressed both the energy and the entropy in terms of the phonon frequencies and occupation numbers, derive the expression for the thermal expansion coefﬁcient given in Eq. (7.70). 6.
Using the UBER, Eq. (7.81), prove that the energy is a quadratic function of the lattice constant a near the minimum. From this result, calculate the bulk modulus B in terms of the parameters that enter in the UBER, E coh and l.
7.
Using the deﬁnitions of the normal and shear strain, Eqs (7.82) and (7.83), show that the following relations hold: ∂ 2² xx ∂y2
2
2
+ ∂∂ x²2yy = 2 ∂∂ x²∂xyy
(7.131)
plus two more similar relations obtained by cyclical permutations of the indices. Also: ∂ 2² xx ∂ y∂ z
´
= ∂∂x − ∂∂²xyz + ∂∂²yxz + ∂∂²xyz
µ
(7.132)
plus two more similar relations obtained by cyclical permutations of the indices. These are called SaintVenant strain compatibility relations. 8.
Prove the strain rotation relations, Eq. (7.87). To this end, you need to draw a simple diagram with strains identiﬁed for a rectangular element on the xy plane, and calculate the corresponding strains in the x ± y± coordinate system, which is rotated by ´ with respect to the original coordinate system. You also need to assume that strains are small, so that secondorder terms can be neglected.
377
Problems
9.
Prove the relationship between the three elastic constants of an isotropic solid, given by Eq. (7.110). To do this, consider a 2D section of an isotropic solid on the xy plane, and assume that σxz = σyz = σzz = 0; express the strains ²xx , ²yy , ²xy in terms of the stresses for this case. Next, change coordinate system to x± y ± , which is related to the original one by a rotation through ´ around the z axis, and reexpress the new strains in terms of the new stresses in the primed coordinate system. By manipulating the resulting equations, Eq. (7.110) can easily be derived.
10.
Derive the expression for the strain energy density of an isotropic solid, Eq. (7.120), starting with the general expression Eq. (7.106) and using the relevant stress–strain relations, Eq. (7.112).
11.
Derive the equations of motion for an isotropic solid without any external forces, Eq. (7.121), starting with the general relations Eq. (7.98) and using the relevant stress– strain relations, Eq. (7.112).
12.
Show that for a solid with cubic symmetry, the bulk modulus is given in terms of the elastic constants by the relation B
= C 11 +3 2C 12
To prove this, you can start with the hydrostatic pressure condition as in the case of the isotropic solid, Eq. (7.115), and use the stress–strain relations for the solid with cubic symmetry. Check to what extent the above relation holds for the values of bulk modulus and elastic constants given in Table 7.4 for various types of solids. 13.
We revisit the phonon modes of graphene discussed in Section 7.8. (a) Using the matrix of Table 7.5, ﬁnd values for the parameters κr , κ θ to produce approximately the phonon modes shown in Fig. 7.15 along the highsymmetry directions of the hexagonal BZ. (b) For the highsymmetry points (³ , K, M) ﬁnd the atomic displacement patterns that correspond to the various phonon modes. (c) Calculate the contributions of the secondneighbor interactions to the potential energy; note that these interactions only couple atoms of the same sublattice (A to A or B to B ), as shown in Fig. 7.14. Speciﬁcally, show that, with the deﬁnition a3 ≡ a1 − a2 , the new contributions to the dynamical matrix are the diagonal elements (2) (2) = 3κr(2) + 3κ(2) − 3κr 2+ κ [cos (k · a1 ) + cos (k · a2)] − 2κ (2) cos (k · a3 ) (2) (2) κr + 3κ (2) (2) (2) D (k ) = 3κ + 3κ −
D (2) x (k )
θ
θ
θ
y
D (2) z (k )
r
θ
2 [cos (k · a1 ) + cos (k · a2)] − 2κ r(2) cos (k · a3 ) θ
= 6κ (2) − 2κ(2) [cos(k · a1) + cos(k · a2 ) + cos(k · a3)] θ
θ
378
7
Lattice Vibrations and Deformations
coupling A x to A x , A y to A y, and A z to A z , respectively (and similarly for the B sites), and the offdiagonal matrix element
√ · ¸ 3 (2) (2) H (k ) = − κr − κ [cos(k · a1 ) − cos( k · a2)] 2 θ
coupling A x to A y and B x to B y . Find values of the new parameters κr(2) , κθ(2) to obtain as close a match as possible to the DFT results shown in Fig. 7.15. Comment on which features of the phonon dispersion can be affected by the inclusion of secondneighbor couplings and which cannot.
8
Phonon Interactions
In the previous chapter we considered the quantized vibrations of ions in a crystalline solid, the phonons, as independent “particles.” We used this concept to investigate some of the properties of solids related to ionic vibrations, like the speciﬁc heat and the thermal expansion coefﬁcient. In this chapter we look at the interaction of phonons with other quasiparticles, like electrons, and other particles, like neutrons, as well as with photons, the quanta of the electromagnetic ﬁeld.
8.1
Phonon Scattering Processes
The presence of phonons in a crystal is manifest, and the phonon properties can be measured, by the scattering of particles or waves when they interact with the excitated phonons. A common method for measuring phonon frequencies is by scattering of neutrons, which are electrically neutral particles of mass comparable to that of ions. We discuss ﬁrst the example of phonon scattering by particles, and then describe in more detail the theoretical framework for calculating scattering processes and their effects. The hamiltonian for the system of ions in an inﬁnite crystal and a particle being scattered by those ions is given by: 2 2 ˆ = ± Pˆ n + V( {Rn + Sn}) + pˆ + +± v (r − (Rn + Sn )) 2M 2m
H
n
n
(8.1)
n
where Rn are the positions of ions in the ideal crystal, S n ≡ δ Rn are their displacements due to phonons, as expressed in Eq. (7.37), and Pˆ n the momentum operators for the ionic coordinates; r and pˆ are the position and momentum operator for the scattering particle, m its mass, and v (r) the potential through which it interacts with the ions of the solid. The potential energy term V ( {Rn + S n}) depends on all the ionic coordinates and represents the interactions among ions. The problem now can be posed as follows: given the initial and ﬁnal states of the scattering particles, characterized by energy E 1, E 2 and momentum p1 , p2 , and the initial state of the crystal, characterized by the set of phonon occupation (l) numbers {n k ,1}, what are the possible ﬁnal states of the crystal, which will be characterized
by the new set of phonon occupation numbers {n k,2}? Each n k,s represents the number of phonons excited in the state with wavevector k of the lth phonon band, for the state of the entire system labeled s . We deﬁne the change in occupation of each phonon state as: (l )
(l)
± nk 379
≡ n (kl,2) − n (kl,1)
(l )
(8.2)
380
8
Phonon Interactions
Conservation of energy in the system gives: E1
+
± k ,l
¯
(l ) h ωk
²
(l ) n k,1
+
1 2
³
= E2 +
± k,l
¯
(l ) h ωk
²
(l ) n k,2
+
1 2
³
and using the deﬁnition of ± n(kl) , Eq. (8.2), we express the change in energy as: E2
±
− E 1 = − h¯ ωk(l)± n(kl)
(8.3)
k ,l
It takes a slightly more elaborate treatment to establish the proper expression for the change in momentum of the particle, because we have to take into account the translational symmetries of the system that are related to momentum conservation. Speciﬁcally, by following similar steps as in the proof of Bloch’s theorem (see Chapter 2), we can establish that the hamiltonian of Eq. (8.1) commutes with the translational operator for changing the particle position by a lattice vector R, because the particle–crystal interaction is invariant under such a change. This implies that the corresponding translational operator is given by:
ˆ = e−i R·ˆp h¯ /
RR
An additional symmetry comes from permutations between ionic positions, due to the indistinguishability of these positions within the crystal. The corresponding operator is:
ˆ = e−i R·K
PR
s
where the new quantity introduced, Ks , is the wavevector for the entire crystal in the phonon state labeled s , which is determined by the phonon occupation numbers n (kl,)s and is given by:
Ks
=
± k,l
k n(kl,)s
This is in close analogy to the wavevector of individual electrons that experience the effects of lattice periodicity, as discussed in detail in Chapter 2. The total translational symmetry of the system is then described by the combined operator
ˆ ˆ = e−iR·(pˆ h¯+K ) /
RR P R
s
Thus, we can use the eigenfunctions of this operator as the basis for the eigenfunctions of the hamiltonian of the system, which ensures that the eigenvalues of this operator, p /h¯ +Ks , will be conserved. This leads to the following relation for the momentum in the system at the initial and ﬁnal states: ± ± p1 ± (l) + k n k,1 + G1 = p2 + k n (kl,2) + G2 ⇒ p1 + k n (kl,1)
¯
h
¯
h
k,l
=
p2
¯
h
¯
h
k,l
+
± k,l
k,l
k n k,2 − G (l)
where we have taken advantage of the relation exp(iR · G) = 1, which holds for any Bravais lattice vector R and any reciprocalspace lattice vector G, to introduce an arbitrary lattice
381
8.1
Phonon Scattering Processes
vector G1 , G2 to each side of the equation, but their difference is simply another reciprocalspace lattice vector: G = G1 − G2 . This result then leads to the following expression for the momentum difference between initial and ﬁnal states:
p 2 − p1
±
= − h¯ k ±n (kl) + h¯ G
(8.4)
k ,l
Example 8.1 Neutron scattering by phonons We apply the general expressions derived above to analyze what happens in neutronscattering experiments that probe the phonon properties of solids. Neutrons are typically scattered by atomic nuclei in the solid through inelastic collisions that involve changes in the energy and momentum of the neutron, which imply a change in the number of phonons that are excited in the solid; this change number of phonons is determined by Eqs (8.3) and (8.4). If we assume that experimental conditions can (l) be tuned to involve a single phonon, corresponding to ±n k = ± 1, then we will have for the energy and momentum before (E 1, p 1) and after ( E 2 , p2 ) a scattering event:
= E 1 + h¯ ωk(l ), (l ) E 2 = E 1 − h¯ ωk ,
phonon absorption : E 2 phonon emission : (l)
Using the fact that ωk±G of energy:
= p1 + h¯ (k + G) p 2 = p1 − h¯ (k + G)
p2
= ω(kl) , we obtain the following relation from conservation 2
p22 2m n
= 2pm1 ± h¯ ω((lp) −p ) h¯ (8.5) n with (+) corresponding to absorption and (−) to emission of a phonon, and m n being 2
1 /
the neutron mass. In experiment, p1 is the momentum of the incident neutron beam and p2 the momentum of the scattered beam. In the situation we are considering, Eq. (8.5) has solutions only if the second term on the righthand side corresponds to a phonon frequency at some value of k in the BZ: (l)
ω( p
2
−p 1)/h¯ = ωk
(l )
In reality it is impossible to separate the singlephonon events from those that involve many phonons. Thus, for every value of the energy and momentum of neutrons there will be a broad background, corresponding to multiphonon processes. However, the ﬂux of scattered neutrons as a function of their energy, p 22/2m n , will exhibit sharp peaks in certain directions pˆ 2 which correspond to phonon frequencies that satisfy Eq. (8.5). From these peaks, one determines the phonon spectrum by scanning the energy of the scattered neutron beam along different directions.
8.1.1
Scattering Formalism
To describe phonon interactions in a more general context, we consider the scattering of a quantummechanical particle, modeled by a planewave, from a solid in the presence of
382
8
Phonon Interactions
phonons. This particle can be an electron, a photon, or even another phonon; we explore the scattering of these three types of particles in more detail in subsequent sections. We denote the incident wavevector of the particle by k and the scattered wavevector by k ² . The matrix element Mk,k ² for the scattering process will be given by the expectation value of the scattering potential, that is, the potential of all the ions in the crystal, V˜ xtl (r), between initial and ﬁnal states: Mk ,k²
´
= NV 1
PUC
e−i k · rV˜ xtl (r)ei k·r dr , ²
˜
=
Vxtl (r)
±
V ion(r
nj
− tj − Rn )
where V˜ ion (r − tj − Rn ) is the potential of an ion situated at tj in the unit cell of the crystal at the lattice vector Rn ; N is the total number of unit cells in the crystal, each of volume V PUC . For simplicity, we will assume that the solid contains only one type of ions, so there is only one type of ionic potential V˜ ion (r). Inserting the expression for the crystal potential in the scattering matrix element, and deﬁning q = k ² − k , we obtain:
+
M k,k q
= N1
±
˜
V ion(q )
± −iq ·(t +R ) j n e ,
n
˜
Vion( q)
j
=V1
PUC
´
˜
Vion (r)e
−iq ·r dr
with V˜ ion(q ) the Fourier transform of the ionic potential V˜ ion (r). If q happens to be equal to a reciprocal lattice vector G, then the scattering matrix element takes the form
+
Mk,k G
= N1
±
˜
Vion (G)
± −iG· t j e
n
j
= V˜ ion (G)S (G)
where we identiﬁed the sum over the ions in the unit cell j as the structure factor S (G), the quantity we had deﬁned in Chapter 2, Eq. (2.106); the other sum over the crystal cells n is canceled in this case by the factor 1/ N . If q ³= G, we can generalize the deﬁnition of the structure factor as follows: 1 ± −i q·(tj +R n) e S ( q) ≡ N
nj
in which case the scattering matrix element takes the form
+
M k,k q
= V˜ ion (q)S (q)
We are now interested in determining the behavior of this matrix element when, due to thermal motion, the ions are not at their ideal crystalline positions. Obviously, only the structure factor S (q) is affected by this departure of the ions from their ideal positions, so we examine its behavior. The thermal motion leads to deviations from the ideal crystal positions, which we denote by snj . With these deviations, the structure factor takes the form S (q)
= N1
± −iq·(t + R ) −iq·S j n nj e e n,j
For simplicity, we will assume from now on that there is only one ion in each unit cell, which allows us to eliminate the summation over the index j. We can express the deviations (l) of the ions from their crystalline positions Sn in terms of the amplitudes of phonons Q q ²
383
8.1
Phonon Scattering Processes
and the corresponding eigenvectors eˆ (ql²), with l denoting the phonon branch, which gives for the structure factor:
Sn =
± l ,q²
⎤
⎡
(l ) (l) i q² · Rn Q q² eq² e
ˆ
± (l) (l ) iq ² ·R 1 ± −iq· Rn n⎦ (Q q ² eˆ q² )e (8.6) e exp ⎣−iq ·
⇒ S (q) = N
l ,q ²
n
We will take the deviations from ideal positions to be small quantities and the corresponding phonon amplitudes to be small. To simplify the calculations, we deﬁne the vectors f(ql)² n as: (l )
fnq ²
= Q (ql)² eˆ (ql²)e−iq²·R
n
(8.7)
which, by our assumption above, will have small magnitude. Using this fact, we can expand the exponential with square brackets in Eq. (8.6) as follows:
⎡
exp ⎣−iq ·
± l ,q ²
⎤
l) ⎦ f (nq ² =
µ l,q²
exp
¶
·
−i q · f(nql) ² =
µ l,q²
=
¸
1 − iq · f(nql) ² −
»
º2 1¹ l) q · f(nq ² + 2
· · ·
l) Keeping only terms up to second order in f(nq ²  in the last expression gives the following result:
⎡
⎣1 − iq ·
± l,q ²
⎤
f nq ² − (l )
º ± ¹ (l ) º ¹ (l ² ) º 1 ±¹ (l) 2 q · fnq² − q · fnq ² q · fnq ²² ⎦ 2 ² l,q lq² 0
For the antiStokes mechanism, the system must start at a state with energy higher than the lowest one, so that after excitation to a virtual state it can return to a state of lower energy than the initial one; the difference in energy between ﬁnal and initial states, in this case a negative quantity, is equal to the energy of the absorbed phonon that makes the transition between the two vibrational states possible: antiStokes :
− E i = −h¯ ωq = h¯ (ωI − ωS ) < 0
Ef
In both cases, conservation of energy gives: Ef
+ h¯ ωS = E i + h¯ ωI
(8.13)
The virtual states involved in the inelastic processes will be discussed in more detail below. The inelastic processes are referred to as “Raman scattering”; they depend on the phonon modes of the solid and reveal information about these modes. The difference in frequency between incident and scattered radiation is referred to as the “Raman shift,” and as the expressions above make clear, it is equal to the frequency of either an emitted or an absorbed phonon: ±ω
= ω I − ωS  =ωq
389
8.3
Phonon–Photon Interactions
8.3.1
Infrared Absorption
A quantitative description of IR absorption relies on the same concepts as the absorption of light by electronic excitations. The underlying physical mechanism is the coupling of the electromagnetic ﬁeld to charged particles, which in this case are the ions of the solid that are undergoing collective motion described by the phonon modes. By analogy to our derivation of electron excitations (see Chapter 6), if a phonon mode has the characteristics of a charge distribution it can couple to the electromagnetic ﬁeld the familiar interaction term in the hamiltonian, Eq. (6.2), which results in transition probabilities that involve matrix elements of the dipole operator [see Eq. (6.4)] between states of the system. In the present case, these are vibrational states of the system and the transitions between them are due to phonons. We will use the notation {Q } = Q {1, Q 2, . . ., Q 3N } to represent all the phonon modes of the crystal with N ions. Generally, we are dealing with the system in its ground electronic state, which we denote with the superscript (0); for this case, we denote (0) (0) the initial and ﬁnal vibrational states as φf ({Q }), φi ({Q }) and write the expectation value of the dipole operator between them as: [αﬁ ]κ
= φµf(0)({Q })dˆ ({Q })φi(0)({Q })¶,
κ
κ
= x, y, z
In terms of this, the IR absorption intensity will be proportional to: Iﬁ
∼
±
µφf(0)({Q })dˆ ({Q })φi(0)( {Q })¶2, κ
κ
= x , y, z
κ
We next expand the dipole moment in a Taylor expansion in terms of the variables Q s which correspond to the various phonon modes, using a single index s to denote both the wavevector k and the branch l of a phonon mode, and keeping only the lowestorder terms (up to linear in Q s ):
ˆ { } = dˆ (0) +
dκ ( Q )
±
κ
ˆ =
ˆ
dκ(s )
d (κs )Q s ,
s
Á
ˆ {Q })
∂dκ(
∂Qs
Â
{Q }=0
which leads to: (0) (0) ˆ ˆ (0) (0) µφ(0) f ({Q } )d ({ Q } )φi ({ Q })¶ =d µ φf ({Q } )φi ({ Q })¶ ± (0) + dˆ (s)µφ(0) f ({Q } )Q s φi ({ Q })¶ κ
κ
s
κ
(8.14)
This expression allows us to ﬁgure out the contributions to the IR signal. For a transition between two different states, the ﬁrst term vanishes since they must be orthogonal, µφf(0)({Q })φi(0)({Q })¶ = 0. In order to have a nonvanishing contribution, at least one of the κ = x , y , z components must have both nonvanishing dˆ κ and nonvanishing matrix element µφf(0) ({Q }) Q s φi(0) ({Q }) ¶. In particular, the ﬁrst condition tells us that the phonon mode described by Q s must be related to a change in the dipole moment , such (s) that dˆ κ ³= 0, which is the most important characteristic. If, in addition, the corresponding (0) (0) matrix element µφf ({Q })Q s φi ({Q })¶ = ³ 0, then we have identiﬁed what is referred to as an “IR active” mode; the value of the matrix element determines how strongly the IR active mode contributes to the signal. (s )
390
8
Phonon Interactions
8.3.2
Raman Scattering
Inelastic scattering of radiation by phonons was discovered experimentally by C. V. Raman in 1928. The theory of Raman scattering is based on the dispersion equation, referred to as the Kramers–Heisenberg–Dirac (KHD) theory. A ﬁrst formulation that gave insight into the selection rules that govern Raman scattering was developed by J. H. Van Vleck. 1 The modern formulation of the theory was given by A. Albrecht,2 which we follow here. From KHD theory, the scattering crosssection σﬁ between an initial and a ﬁnal state denoted by i and f , as a function of the incident radiation frequency ωI and normalized by the incident intensity, is given by: σﬁ(ωI )
= 98cπ4 (ωI ± ωq )4
± ¿Ã Ä ¿ ¿ αﬁ (ωI ) ¿2 , κλ
{κ , λ} = x ,{y , z }
κ ,λ
where ωq is the frequency of the phonon involved in the scattering and α ﬁ( ωI ) is the transition amplitude (a secondrank tensor). The two different signs of the ωq term correspond to the Stokes and antiStokes contributions, mentioned earlier. The elements of the transition amplitude are:
Ã Ä αﬁ
κλ
(ωI ) =
±± j
n
Ã
E nj
Ä Ã
Ã
Ä
Ä Ã
Ä
− E i0 − h¯ ωI + iη + E nj − E f 0 + h¯ ωI + iη
M fn,0j
κ
Mni,j 0
λ
Mfn,0 j
λ
M ni,j 0
κ
(8.15)
where the matrix elements that appear in the numerators under the double summation are:
Ã
Ä
= φµ (nj) ({Q })ψj ({Q }; {r})dˆ φi(0)( {Q })ψ0({Q }; {r})¶ (8.16) Ã Ä (0) (8.17) Mfn,0 j = φµ f ({Q })ψ0({Q }; {r})dˆ φn(j )({Q })ψj ({Q }; {r})¶ (0) (0) with the following meaning: φi ({Q }), φf ({Q }) are the initial and ﬁnal vibrational states, (j) both in the ground state of the electronic system, and φn ({Q }) is an intermediate state, Mni,j 0
λ κ
λ
κ
associated with the electronic system state j (all three are functions of the phonon degrees of freedom denoted collectively by {Q }), and ψ0 ({Q }; {r}), ψj ({Q }; {r}) are wavefunctions of the electronic system, in the ground state and the excited state j, respectively, which depend both on the phonic state, indicated by {Q }, and the electronic degrees of freedom, the latter denoted collectively by {r}. E f 0 , E nj , E i0 are the corresponding energies of the system in the particular electronic and vibrational states. These expressions help us visualize what happens “behind the scenes” when the incident radiation of frequency ωI is scattered into the radiation with frequency ωS in the presence of a phonon mode in the solid. This is shown schematically in Fig. 8.3. Speciﬁcally, the term in Eq. (8.16) describes the process of starting with the electronic system in the ground state ψ0({ Q }, {r} ) at a given vibrational state labeled i, which is then excited to an electronic state labeled ψj ({Q }; {r}) and a new vibrational state labeled n within this manifold of possible states; the term in Eq. (8.17) describes the subsequent decay back to the electronic ground state ψ0 ({Q }; {r}) and a different vibrational state labeled f . The exitation takes place by 1 J. H. Van Vleck, Proc. Nat. Acad. Sci. (US) 15, 754 (1929). 2 A. C. Albrecht, J. Chem. Phys. 34 , 1476 (1961).
391
Fig. 8.3
8.3
Phonon–Photon Interactions
Illustration of excitations involved in Raman scattering processes: the wavy colored lines represent photons (absorbed or emitted) and the zigzag lines represent phonons of wavevector q and frequency ωq . Left : Excitation of an electron–hole pair by absorption of a photon of frequency ωI , followed by emission of a phonon by the electron, which is scattered to a new state and recombines with a hole to emit a photon of frequency ωS < ωI . Right: Excitation of an electron–hole pair by absorption of a photon of frequency ωI , followed by absorption of a phonon by the electron, which is scattered to a new state and recombines with a hole to emit a photon of frequency ωS > ωI .
the creation of an electron–hole pair from the absorption of a photon of energy h¯ ωI , with the electron emitting a phonon of wavevector q and frequency ωq to end up in a different excited state, from which it decays to the ground by the emission of a photon of energy h¯ ωS. At each stage energy and momentum are conserved, but the emission of the phonon of frequency ωq is what prevents the electron from returning to its original state. The phonon emission is manifest by the change in vibrational state of the system, which changes from the one labeled i to the one labeled f . The transition amplitude involves a summation over all possible phonon modes of wavevector q and frequency ωq , collectively represented by the index n, as well as over all excited electronic states labeled j that satisfy the energy and momentum conservation rules. A similar description applies to the second term in Eq. (8.15). In this case, the excited electron absorbs a phonon of wavevector q and frequency ωq , and is scattered into a new state of higher energy, from which it can decay to the ground state by emitting a photon. The Stokes mechanism gives a stronger contribution to the signal, since it is easier for the excited electron to emit phonons and lose some of its energy, rather than to have to wait to absorb a particular phonon before it can decay to the ground state. The processes that make the most signiﬁcant contributions are those for which the denominators are very small, and the matrix elements do not vanish. Typically, the energy of the incident photon h¯ ωI is much larger than that of emitted phonons. If the photon energy is close to that required for an electronic transition between states ψ0 ({Q }; {r}) and ψj ({Q } ; {r} ), then it is likely to ﬁnd phonon modes that satisfy the energy and momentum conservation rules, which leads to resonance and a large signal in the scattering crosssection. By spanning the values of the incident radiation frequency, such phonon modes can be identiﬁed. The term iη in the denominators in Eq. (8.15) serves to describe the ﬁnite lifetime of the excited electronic state and gives a ﬁnite width to the resonance. The ﬁnal result will depend on which matrix elements, for frequencies ωI close to resonance, have nonvanishing values. These are determined by symmetry considerations, similar to what we discussed for the case of electronic excitations (see Chapter 6), only
392
8
Phonon Interactions
now we need to take into consideration both electronic excitations and matrix elements that involve vibrational states of the system. To explore this further, we deﬁne: [ dˆ 0j ({Q })]κ
≡ ψµ 0 ({Q }; {r})dˆ ψj( {Q }; {r})¶
(8.18)
κ
that is, integrate over the electronic degrees of freedom ﬁrst, which gives the following expressions for the matrix elements:
Ã
Ã
Mni,j 0 Mfn,0 j
Ä
Ä
λ κ
= φµ (nj) ({Q })[dˆ j 0({Q })] φi(0)({Q })¶ (j ) ˆ = φµ (0) f ({Q } )[d 0j ({Q } )] φn ({ Q }) ¶ λ
(8.19)
κ
Next, we expand the dipole expectation value as we did for the case of IR absorption in a Taylor series in the variables of the phonon modes Q s : [dˆ 0j ({Q })]κ
= ˆ
(0) [d 0j ]κ
+
± s
ˆ { })] Q s, ˆ { })] =
(s ) [d 0j ( Q
(s ) [ d0j ( Q
κ
κ
Á
ˆ {Q })]
∂ [d 0j (
∂ Qs
Â
κ
{Q}= 0
(8.20)
which gives, for the matrix elements to lowest order in Q s :
¶
(0)
Mni,j0
·
λ
(0) (j) = [dˆ (0) j0 ] µφn ({Q } )φi ({ Q })¶ ,
¶
λ
(0)
M fn,0j
·
κ
(0) (j) = [dˆ (0) 0j ] µ φf ({ Q } )φn ({ Q } )¶ κ
Now, in contrast to the case of IR absorption, these matrix elements do not automatically vanish, because in general we will have:
µφ(nj) ({Q })φ(0) ³ 0 i ({Q } )¶ =
and
(j) µφ(0) ³ 0 f ({Q } )φn ({Q } )¶ =
since the two vibrational states involved in each product belong to different electronic states, the ground state (labeled 0) and the excited state (labeled j). Moreover, the amplitude in Eq. (8.15) involves a summation over n , that is, all the vibrational states of the excited electronic state, which guarantees that there will be some vibrational states of the excited electronic state with large overlap with the vibrational states of the electronic ground (0) state. Consequently, the leading (lowest)order terms will be proportional to [dˆ j 0 ]λ , which implies that Raman scattering is qualitatively different from the case of IR absorption, because this term involves no change in the dipole moment. The conclusion that we draw from this analysis is that Raman active modes are essentially opposite in nature to IR active modes: a mode that is IR active involves a change in the dipole moment and is therefore not active in Raman scattering, and vice versa (see also Problem 2 for further discussion).
8.4
Phonon–Electron Interactions: Superconductivity
One of the most striking manifestations of the interaction between electrons and phonons is the phenomenon of conventional superconductivity, which was discovered in 1911 by Kamerling Onnes.3 Superconductivity is an essentially manybody phenomenon which cannot be described simply within the singleparticle picture. Because of its fascinating 3 K. Onnes, Leiden Commun.
120 (1911).
393
8.4
Phonon–Electron Interactions: Superconductivity
nature and many applications, superconductivity has been the focus of intense theoretical and experimental investigations ever since its discovery. The hallmark of superconductivity is a vanishing electrical resistance below the critical temperature T c . There is no measurable DC resistance in a superconductor below this temperature, and if a current is set up it will ﬂow without dissipation practically forever: experiments trying to detect changes in the magnetic ﬁeld associated with current in a superconductor give estimates that it is constant for 106–109 years! Thus, the superconducting state is not a state of merely very low resistance, but one with a truly zero resistance. This is different from the case of very good conductors. In fact, materials which are very good conductors in their normal state typically do not exhibit superconductivity. The reason is that in very good conductors there is little coupling between phonons and electrons, since it is scattering by phonons which gives rise to the temperaturedependent resistance in a conductor, whereas electron– phonon coupling is crucial for superconductivity. The drop in resistance from its normal value above T c to zero takes place over a range of temperatures of order 10−2–10−3 T c , that is, the transition is rather sharp. For conventional superconductors, T c is in the range of a few kelvin, which has made it difﬁcult to take advantage of this extraordinary behavior in practical applications, because cooling the specimen to within a few degrees of absolute zero is quite difﬁcult (it requires the use of liquid helium, the only nonsolid substance at such low temperatures, as the coolant, which is expensive and cumbersome). We give examples of conventional superconductors in Table 8.1. A new class of superconducting materials was discovered in 1986, with T c that can exceed 130 K and thus can be cooled to the superconducting state with nitrogen which is liquid below 77 K; we mention a few important facts about these superconductors at the end of this section. The theory of superconductivity involved a long search for a proper microscopic picture of how electrons create the very special superconducting state. In addition to the microscopic picture, there are many aspects of superconductivity that can be described
Table 8.1
Critical temperature
Tc
(K), critical ﬁeld
H0
(Oe), and Debye frequency
h¯ ωD
(meV) of
elemental conventional superconductors. Source: D. R. Lide (Ed.), CRC Handbook of Chemistry and Physics (CRC Press, Boca Raton, FL, 1999–2000).
Element Al Cd Gd Hg In Ir Mo Sn W Pb Re
Tc
H0
h¯ ωD
Element
Tc
1.175 0.517 1.083 3.949 3.408 0.113 0.915 3.722 0.015 7.196 1.697
105 28 58 339 282 16 96 305 1.2 803 200
36.2 18.0 28.0 8.0 9.4 36.6 39.6 50.0 33.0 8.3 0.4
Ru Nb Ta Tc Th Ti Tl V Os Zn Zr
0.49 9.25 4.47 7.80 1.38 0.40 2.38 5.40 0.66 0.85 0.61
H0
h¯ ωD
69 2060 829 1410 1.6 56 178 1408 70 54 47
50.0 23.8 22.2 35.4 14.2 35.8 6.8 33.0 43.1 26.7 25.0
394
8
Phonon Interactions
by phenomenological theories. A full treatment of the subject is beyond the scope of the present book (we give some suggestions for texts that cover these topics in the Further Reading). Instead, we concentrate here on the microscopic theory of superconductivity as it was developed in the seminal paper of J. Bardeen, L. N. Cooper, and J. R. Schriefer4 (BCS theory); this theory relies on treating explicitly the interaction of phonons with electrons, the theme of the present section. 8.4.1
BCS Theory of Superconductivity
There are two main ingredients in the BCS theory of superconductivity. The ﬁrst is an effective attractive interaction between two electrons that have opposite momenta (larger in magnitude than the Fermi momentum) and opposite spins, which leads to the formation of the socalled “Cooper pairs.” The second is the condensation of the Cooper pairs into a single coherent quantum state, which is called the “superconducting condensate”; this is the state responsible for all the manifestations of superconducting behavior. We discuss both ingredients in some detail. The Attractive Potential Between Electrons Due to Phonons
Our starting point is the system of electrons described by the hamiltonian
ˆ = Hˆ sp0 + Hˆ int
H
with the interaction term describing the electron–electron as well as the electron–ion interactions when ions are allowed to move. The singleparticle wavefunctions  ψk ¶ are eigenfunctions of the ﬁrst term, the kinetic energy, with eigenvalues ³k :
ˆ sp  ¶ =³kψk¶
H0 ψ k
and form a complete orthonormal set. We shall examine in more detail the nature of the interaction when ions are allowed to move: it contains a new term relative to the case of ﬁxed ions, which represents electron–electron interactions mediated by the exchange of phonons. The physical origin of this new term is shown schematically in Fig. 8.4: an electron moving through the solid attracts the positively charged ions which come closer to it as it approaches and then return slowly to their equilibrium positions once the electron has passed by. We can describe this motion in terms of phonons emitted by the traveling electron. It is natural to assume that the other electrons will be affected by this distortion of the ionic positions; since the electrons themselves are attracted to the ions, the collective motion of ions toward one electron will translate into an effective attraction of other electrons toward the ﬁrst one. Fr¨olich5 and Bardeen and Pines6 showed that the effective
4 J. Bardeen, L. N. Cooper, and J. R. Schriefer, Phys. Rev. 108, 1175 (1957). 5 H. Fr¨olich, Proc. Roy. Soc. A 215, 291 (1952). 6 J. Bardeen and D. Pines, Phys. Rev. 99 , 1140 (1955).
395
Fig. 8.4
8.4
Phonon–Electron Interactions: Superconductivity
Illustration of attractive effective interaction between two electrons mediated by phonons: on the left is the distortion that the ﬁrst electron (blue dot) induces to the lattice of ions (red spheres) as it passes through; on the right is the second electron with opposite momentum near the original position, at a later time: the lattice distortion, which decays on a time scale much longer than electronic motion, favors the presence of the second electron in that position, leading to an effective attraction.
interaction between electrons due to exchange of a phonon takes a form that explains and quantiﬁes this attraction. While the full proof of the effective interaction between electrons in the presence of phonons requires a treatment based on ﬁeld theory, which is beyond the scope of the present discussion, we provide here a heuristic argument to justify the form of this interaction. We begin by noting that when the positively charged ions move, they can produce their own plasmon modes with characteristic plasma frequency given by: ´p
=
Å
4π N ion Z 2 e2
Æ1/ 2
MV
where M is the mass of the ions, Ze their valence charge, and N ion is the total number of ions in the solid of volume V (we have assumed here for simplicity that there is only one type of ions in the solid). We saw earlier (Chapter 6) that free electrons produce a dielectric function that involves the plasma frequency of the electron gas, see Eq. (6.16). We would therefore expect similar screening to be produced by the motion of the ions treated as free charges, expressed in terms of a dielectric function with exactly the same form as that of free electrons. However, in the corresponding expression for the ions, we should include not the bare plasma frequency for the ion gas, ´p , as written above, but a screened one, due to screening of the ionic motion by the presence of electrons, which is embodied in the electronic dielectric constant ε (k). Since the restoring force of the harmonic potential between ions is proportional to the square of the frequency, and the dielectric constant screens the potential itself, we conclude that the screened plasma frequency of the ions must be given by: 2
ωk
´2
= ε(kp)
with ωk representing a phonon frequency. With this modiﬁcation, the analog of Eq. (6.16) for the dielectric constant of ions, including screening from electrons, will be: εion( ω)
=1−
2
´p /ε(k ) ω2
2
= 1 − ωωk2
The combined effect of screening on the electron–electron interaction will be given by an effective dielectric function which is the product of the electronic and ionic contributions to screening, with the two components treated as independent of each other. Consistent with the qualitative nature of the argument, we will take the electronic states to be those
396
8
Phonon Interactions
of free electrons in a Hartree–Fock picture. We recall that the bare (unscreened) Coulomb interaction in this basis is: bare
Vkk²
2
2
= ψµ k²  r −e r²  ψk¶ =V k4π−e k² 2
[see Appendix A, Eq. (A.74)], where we have specialized the interaction to two electron states with wavevectors k and k ² ; in the following we deﬁne q = k − k² . For the frequencyindependent part, we can take the electronic contribution to the dielectric function to be that of the Thomas–Fermi model, that is: ε(q )
2
= 1 + qk s2
with ks the screening inverse length [see Eq. (4.115)]. Now, using the argument outlined above, we can write the effective screened interaction between the electrons as: eff Vkk²
=
1 1 εion (ω) ε(q )
bare Vkk²
=
1 4π e 2 εion (ω) V (ks2 + q 2 )
=
4π e 2 V (k 2s + q2 )
Å
ω ω2
2
Æ
− ωq2
Finally, we associate the frequency ω with the energy difference between the electronic states, ω = (³k² − ³k ) /h¯ , which allows us to rewrite the effective interaction as: eff Vkk²
=
Á
(h¯ ωq )2 4π e 2 1 + V ( ks2 + q2) ( ³k ² − ³k )2 − (h¯ ωq )2
Â
In the above expression for the effective interaction between electrons there are two terms: the ﬁrst term (corresponding to the factor 1 in the square brackets) is the screened electron interaction in the absence of ionic motion; therefore, we can associate the second term with the contribution of the phonons: phon
V kk²
2
= V (k 24π+e q2) s
(h¯ ωq )2 (³k² − ³k )2 − (h¯ ωq )2
From the form of this term, it is evident that if the magnitude of the energy difference ³k² − ³k  is smaller than the phonon energy h¯ ωq, the phonon contribution to the interaction is attractive ; in other words, if the energies of the two electrons ³k , ³k² lie within a very narrow range, so that their difference can be made very small, then the exchange of a phonon of frequency ωq between them will lead to effective attraction. The presence of the Fermi sea is what provides the conditions for realizing this situation.
The Cooper Pair Problem
To show that an attractive interaction due to phonons can actually produce binding between electron pairs, Cooper7 investigated the energy of the Fermi sea in the normal state and compared this with a state in which two electrons are removed from the sea and allowed to interact. This led to the conclusion that for an arbitrarily weak attractive interaction 7 L. N. Cooper, Phys. Rev. 104, 1189 (1956).
397
8.4
Phonon–Electron Interactions: Superconductivity
between the two electrons, the new state has a lower energy, implying that the Fermi sea is unstable with respect to the formation of pairs if there is an attractive interaction. Note that this is not yet a theory of the superconducting state; for the full theory we must also treat the manybody aspect of the problem, that is, what happens when the electrons have formed pairs. Note also that the binding between electrons from an arbitrarily weak attraction arises from the restriction of the phase space due to the presence of the Fermi sea; normally binding in 3D solids would require a ﬁnite threshold value of the attraction. To demonstrate these notions, consider two electrons described by their positions, momenta, and spins (ri , k i , s i ), i = 1, 2 in singleparticle planewave states: ψki (r)
= √1
V
eik i ·r
Anticipating an attractive interaction, we choose the spatial state to be symmetric and thus lower in energy. This means that the twoelectron system will be in an antisymmetric totalspin state, that is, described by the following twoparticle wavefunction: µ(k1 , k2 , s 1 , s 2
¶
r1, r2 ) = √1
2V
ei(k 1·r1 +k2 ·r2) + ei(k 1·r2 +k2 ·r1)
· 1
√ (↑1 ↓2 − ↓1 ↑2 ) 2
We introduce coordinates for the centerofmass ( R, K) and relative (r, k) motion:
k1 − k 2 r1 + r2 , K = k1 + k 2, r = r1 − r2, k = 2 2 and write the spatial part of the wavefunction as: R=
µ(k , K
iK· R
r, R) = e√
2V
¶
eik ·r + e−ik ·r
·
We will concentrate on states with total momentum K = 0, since we expect the lowestenergy state to have zero total momentum. In this case the individual momenta take values k1 = k , k 2 = − k , that is, we are dealing with a pair of particles with opposite momenta. The hamiltonian for this system is:
ˆ= H
1 2m e
ˆ + ˆ + Hˆ int = 2m1
(p21
p22 )
²
e
1 2 Pˆ + 2pˆ 2 2
³
+ Hˆ int
We can ignore the totalmomentum term Pˆ , because we are only considering K = 0 states. We express the wavefunction in the relative coordinate r as: φ (r)
=
±
k² >kF
² )eik ²·r
α (k
with k F the Fermi momentum, and require it to be an eigenfunction of the hamiltonian with eigenvalue E :
ˆ
Hφ (r)
= E φ (r)
To determine the coefﬁcients α(k² ), we take matrix elements of the hamiltonian with individual factors exp(−i k · r) and use the Schr¨odinger equation for φ(r) to ﬁnd:
´
e−i k·r (Hˆ − E )
±
 k² >kF
α (k
² )eik²· r dr = 0 ⇒ (2³k − E ) α(k ) + ± α(k² )µk Hˆ int k ²¶ k ²>kF
=0
398
8
Phonon Interactions
We next rewrite the last equation in terms of the density of states g (³) and switch to the energy ³k as the variable instead of the wavevector k, to obtain: (2³k
− E )α(³k) +
´
µ  ˆ  ¶α(³k² )d³k² = 0
g (³k ² ) k Hint k²
²
³k >³F
(8.21)
where ³F is the Fermi energy. Following Cooper (see footnote 7), we consider a simple model:
µkHˆ int k²¶ = V−< 0, for = 0 otherwise
³ F < ³k , ³k ² < ³F
+ δ³
(8.22)
that is, the interaction term is taken to be a constant independent of the energy for energies ³ k² , ³ k within a narrow shell of width δ³ above the Fermi level, and 0 for other energy values. We provide a rough argument to justify this choice for the interaction term; the detailed justiﬁcation has to do with subtle issues related to the optimal choice for the superconducting ground state, which lie beyond the scope of the present treatment. As indicated in Fig. 8.4, the distortion of the lattice induced by an electron would lead to an attractive interaction with any other electron put in the same position at a later time. The delay must be restricted to times of order 1/ωD , where ωD is the Debye frequency, or the distortion will decay away. These considerations lead to the estimate of the value of ³0 , the thickness of the shell above ³F where the energies ³k lie: δ³
≈ h¯ ωD
(8.23)
There is, however, no restriction on the momentum of the second electron from these considerations. It turns out that the way to maximize the effect of the interaction is to take the electrons in pairs with opposite momenta, because this ensures that no singleparticle state is double counted or left out of the manybody ground state of the system built from the electron pairs. Substituting the choice for the interaction term, Eq. (8.22), in the last equation for the coefﬁcients α(³k ), Eq. (8.21), after deﬁning the constant C , we get: C
≡V
´
+¯hωD
³F
³F
g (³k² )α (³k ² )d³k²
⇒
α ( ³k )
= 2³ C− E
(8.24)
k
and substituting this value for α (³k ) in the deﬁnition of C , we arrive at: 1=V
´
³F
+¯hωD
³F
g(³ ² )
2³ ² − E
d³ ²
We approximate the density of states in the above expression with its value at the Fermi energy, since the range of integration is a thin shell of values near ³F : 1 g (³F )V
=
´
³F
³F
+¯hωD
1
2³ ² − E
d³ ²
= 12 ln
²
2³F + 2h¯ ωD − E 2³F − E
³
399
8.4
Phonon–Electron Interactions: Superconductivity
Next, we deﬁne the binding energy of the pair ± , the amount by which the energy is lowered upon formation of the pair relative to the energy of the two independent electrons:
= 2³F − ±
E
(8.25)
and use it in the above expression to arrive at: ±
= exp[2/V2h¯gω(³D )] − 1
(8.26)
F
If the quantity V g(³F ) is small, then to a good approximation the value of ± is given by: ±
≈ 2h¯ ωD
exp[−2/V g (³F )] = 2h¯ ωD exp[−1/V g 2 (2³F )]
(8.27)
where we deﬁned the pair density of states g 2(³ ) in terms of the regular density of states g (³) as: 1 g 2 (³) = g(³/ 2) 2 This result shows that the Fermi sea is indeed unstable, since we can lower the energy of the system by the amount ± , no matter how small the interaction V is. With the expression we obtained for the coefﬁcients α(³k ), Eq. (8.24), we can write the pair wavefunction as: φ(r)
= √C
V
±
1
k >kF 2³k − E
cos( k · r) =
√C
V
±
1
k >kF 2ξk + ±
cos(k · r)
where we have deﬁned the quantities ξk = ³k − ³F , which are positive since ³k > ³F ; we have also used the deﬁnition of the binding energy ± from Eq. (8.25), which is a positive quantity. The coefﬁcients of the cos(k · r) terms in the last expansion are always positive; they take their largest value for ξ k = 0, that is, for ³k = ³F or  k =k F . For ξ k ∼ ±, the value has already fallen from its maximum value by a factor of 1/3. These considerations show that only electrons with energy within ± of ³F contribute signiﬁcantly to the summation. Since ± ¸ h¯ ωD for weak coupling, this is a very small energy range, ˆ int k² ¶ should not matter much and the details of the behavior of the matrix element µk H in this energy range, consistent with the assumption that its value is a constant, Eq. (8.22). The energy range of interest turns out to be ∼ k B T c around ³F . Note that if the pair momentum K does not vanish as we assumed in the derivation above, but is small, then the result is a binding energy given by: ± (K)
= ± − vF h¯2K
where v F is the Fermi velocity. Cooper also showed that the radius R of the bound electron pair is: R
2 ∼ mh¯ k±F
For typical values of k F and ± , this radius is R the atomic scale.
e
∼ 104A,˚ which is a very large distance on
400
8
Phonon Interactions
The BCS Ground State
The fact that creation of a Cooper pair is energetically favorable (has positive binding energy) naturally leads to the following question: What is the preferred state of the N particle system under conditions where Cooper pairs can be formed? Essentially, how can we write a manybody wavefunction that has “pairing” somehow built in? To provide the motivation for how BCS constructed such a state, we need to consider some preliminaries. Recall from the discussion in Section 4.3 that, given a complete set of singleparticle states of a noninteracting N electron system, the most general manybody wavefunction of the interacting system can be written as a sum of all possible N × N Slater determinants representing the occupancy of N electrons in all possible different singleparticle states. We could, however, take pairing explicitly into account by restricting this occupancy so that whenever a singleparticle state ψk,↑ (r) is occupied by an electron, so is the state ψ−k,↓ (r). Similarly, when the state ψk ,↑( r) is unoccupied, so is the state ψ−k,↓ (r). For simplicity, suppose now that we have only a ﬁxed number M of singleparticle states with allowed values of k = q{1, . . ., q M}. The most general manybody wavefunction with pairing built in would be:
¿ ¿ ψkj,↑ (r1 ) ¿ ¿ ψ−k ,↓ (r1) j ¿ ¿ · ¿ ± ¿ ¶ N ({r, s } ) = A (k j , . . ., k l ) ¿ · ¿ ¿ k j ,... ,k l · ¿ ¿ ψkl,↑ (r1 ) ¿ ¿ ψ−k l,↓ (r1)
¿
· · ψ· k ,↑ (rN ) ¿¿ · · ψ·−k ,↓ (rN ) ¿¿ · · ¿¿¿ · · ¿¿ · · ¿¿ ψk ,↑ (r2) · · ψ · k ,↑ (rN ) ¿¿ ψ−k ,↓ (r2 ) · · ψ ·−k ,↓ (rN ) ¿
↑ (r2) ψ−kj ,↓ (r2 ) ψk j ,
j
j
l
l
l
l
These types of Slater determinants are very clumsy to work with. A much simpler and more compact way of writing them has been developed. Since each determinant just speciﬁes that states ψk j , . . ., ψkl are occupied while all others are empty, we can introduce an “occupation number representation”8 by starting with a vacuum state  0¶ with no electrons present in any singleparticle states and then introducing “creation operators” c + k,s such that + each creation operator ck ,s acting on the vacuum state places an electron in the state ψk,s (r). In this representation, the Slater determinant we wrote above becomes:
+ +
c k ,↑ c −k ,↓ j
j
· · c +k· ,↑ c +−k ,↓ 0¶ l
l
But even with this simpliﬁed notation, dealing with a manybody wavefunction of the form
¶N ¶ =
±
k j ,... ,kl ={ q1 ,... ,qM }
+ A (kj , . . ., k l )c + k ,↑ c −k ,↓ j
j
· · c +k· ,↑ c+−k ,↓ 0¶ l
l
(8.28)
is formidable. Indeed, it is clear that it is hopeless to try to determine all the coefﬁcients A N (k 1, . . ., k M ) in this expression, since their number is on the order of: M!
∼ 10 10 (M − N /2)! (N /2)!
20
8 This formalism is also referred to as “second quantization.” We give a more extended discussion in Appendix C,
Section C.9.
401
8.4
Phonon–Electron Interactions: Superconductivity
The BCS argument is that with so many particles, it would be reasonable to use a meanﬁeld approach in which the occupancy of each state k i depends on the average occupation of the other states. This, however, relaxes the constraint that the total number of particles N should be held ﬁxed, since the occupancies are handled statistically. But the average number of particles N would be ﬁxed. The hope then is that the standard deviation N RMS , deﬁned as: N RMS
would behave as N RMS
∼
√
Ç¼ (
=
N
−N
)2 ½
=
ÈÉ
N2
Ê
− N2
N , so that:
N RMS N
∼ √1 → 0 N
for N
→ ∞ ⇒N = N
that is, in the thermodynamic limit N is the same as N , which is ﬁxed. We next prove that this expectation is borne out in the BCS choice for the groundstate wavefunction of the system in the superconducting state. This wavefunction was chosen to be of the form
⎡
⎤
µ
¶BCS¶ =⎣
k =q1 ,... ,qM
+ ⎦ (u k + v k c + k,↑ c −k,↓ ) 0 ¶
(8.29)
where uk is the probability amplitude that the pair state k is empty and v k is the probability amplitude that the pair state k is occupied. Thus, we must have:
∗ + v kv ∗ = 1
u k uk
(8.30)
k
and the u k s and v k s need to be determined variationally by minimizing the total groundstate energy of the system. Comparing  ¶BCS ¶ and ¶N ¶ from Eq. (8.28), it is apparent that we can write:
±
¶BCS¶ =
N=0,2, ...,2M
¶N ¶
if the coefﬁcients A (k j , . . ., kl ) are now chosen to be given in terms of products of the
singlepair probability amplitudes as:
A (kj , . . ., kl )
= v k · · v k·
l
j
µ k²
uk ²
where k ² runs over the remaining (M − N / 2) unoccupied pair states. As a trivial example, if we assume M = 2, then we obtain:
¶BCS ¶ =(uq + v q c +q ,↑ c +−q ,↓ )( uq + v q c+q ,↑ c +−q ,↓ )0¶ = + + + + + + + u q u q  0¶ +u q vq c + q ,↑ c −q ,↓ 0¶ +uq v q c q ,↑c −q ,↓ 0 ¶ +v q v q c q ,↑ c −q ,↓ c q ,↑ c −q ,↓ 0 ¶ The expectation is that if N is very large then the contribution to  ¶BCS ¶ from components 1
1
2
1
2
2
2
1
1
1
2
1
1
2
1
2
2
2
1
2
1
1
2
2
containing around N particles will be much larger than any other components and thus dominate the wavefunction. To explore this, let us compute the average number of particles and the rootmeansquare (RMS) value in  ¶BCS ¶. This can easily be done in the occupation
402
8
Phonon Interactions
number representation. To this end, we ﬁrst introduce the concept of a “destruction operator,” c k,s , which empties an otherwise occupied singleparticle state ψk,s ¶. Clearly:
 ¶ =0
c k ,s 0
since there are no occupied states in the vacuum that can be emptied. We also have:
+

¶ = 0,0, . . ., ψk,s, . . ., 0¶
c k,s ck ,s 0, 0, . . ., ψk ,s , . . . , 0
that is, when the product of operators c + k,s c k ,s acts on a state of the system in which only the singleparticle state  ψk,s ¶ is occupied, the destruction operator ﬁrst empties this state and the creation operator occupies it again, resulting in the same manybody state. The same product acting on a manybody wavefunction in which the state ψk,s ¶ is not occupied would give 0, because of the previous relation. Thus, this product represents the occupation number of the state ψk ,s ¶: if the state is occupied, it gives 1; if the state is empty, it gives 0. We denote this by the expression n k,s
= c +k,sc k,s
and therefore the total number operator is given by:
ˆ≡
N
±
n k,s
k,s
=
± + ck ,s c k,s
(8.31)
k ,s
In addition, since electrons are fermions, it can be shown that the creation and destruction operators must obey anticommutation rules: ck , s c + k² ,s ²
+ c +k² ,s² c k,s = δk,k² δs,s² ,
+ c+ k,s c k ² ,s²
+ c +k²,s² c+k,s = 0,
ck ,s c k² ,s ²
+ c k²,s² c k,s = 0
(8.32)
(see Appendix C, Section C.9). Finally, we can make one more simpliﬁcation by deﬁning the “paircreation” and “pairdestruction” operators as:
+ ≡ c+ c+ , k,↑ −k,↓
bk
bk
≡ c−k,↓ ck,↑
(8.33)
and show that these pairing operators satisfy the following commutator relations:
+ − b +² b
bk b k²
k
k
= (1 − n k,↑ − n −k,↓ )δk,k² ,
b k b k²
Using the pair operators, we can then write:
Á µ
¶BCS ¶ =
(u k
k
− b k² b k = 0,
+ + − b +² b + = 0 (8.34) k k
bk b k²
Â
+ v kb+k ) 0¶
(8.35)
From their deﬁnition, the pair creation–destruction operators satisfy the relation
+
bk b k
= c +k,↑ c +−k,↓ c −k,↓ c k,↑
which, taking advantage of the anticommutation relation of the singleparticle creation– destruction operators, Eq. (8.32), and if we permute c k ,↑ to the left twice, gives:
+
bk bk
= −c +k,↑c +−k,↓c k,↑c −k,↓ = c+k,↑ ck,↑ c+−k,↓ c−k,↓ = n k,↑ n−k,↓
403
8.4
Phonon–Electron Interactions: Superconductivity
but in the  ¶BCS ¶ state we have n k,↑
= n −k,↓ , so we conclude that: + 2 bk b k = n k,↑ = n k,↑
since the last number takes the value 0 or 1. Thus, from Eq. (8.31), the total number operator can be expressed as:
ˆ = ±(n k,↑ + n −k,↓ ) = 2 ± b +k bk
N
k
k
With this expression, we are now in a position to evaluate the average number N of particles: N
= ¶µ BCSNˆ ¶BCS¶ =2 =2
⎡
± k
µ0⎣
µ
(u ∗k1
k1 ³=k
± k
⎡ µ µ0 ⎣ ( u∗k k1
⎤ ⎡ µ + v ∗k1 bk1 )⎦ b +k bk ⎣ (uk2 + v k2 b+k2 )⎦ 0¶ 1 ⎤
k2
⎤
⎡
+ v ∗k b k )⎦(u ∗k + v ∗kbk )b+k b k(u k + v kb +k )⎣ 1
1
µ
k 2 ³=k
We note that in the last expression:
⎡
0²k¶ ≡⎣
µ
⎤ ⎦ (uk 2 + v k 2 b+ k 2 ) 0 ¶
⎤ (u k2
k2 ³= k
+ v k b +k )⎦ 0¶ 2
2
is a manybody wavefunction with no pairs occupied in the state with wavevector k, and therefore, for all practical purposes, can be considered as a “vacuum” for the pair state k. That is, we have:
 ¶ =0 = 0µ²kb+k
b k 0²k
Making this substitution in the expression above for N then gives: N
±
= 2 µ0²k  k
±
Ã ∗ (u
k
Ä
+ v ∗kb k)b+k b k(u k + vkb +k ) 0²k ¶
¶
·
= 2 µ0²k  u k2 b+k b k + v∗ku kb kb +k b k + u ∗kvk b+k b kb+k + vk2b kb+k b kb +k 0²k¶ k
Now clearly the ﬁrst three terms in the above expression give zero, and we are left with: N
=2
± k
vk 2µ0²kb kb +k b kb +k 0²k¶
These types of expectation values can be evaluated easily by using a basic trick of the occupation number representation: we simply perform a systematic commutation of the operators until we end up with all the destruction operators on the right, where they will operate on the vacuum to produce zero. Using the commutation relations of the pair creation–destruction operators, this leads to:
+ ² b k b+ k b k b k 0k
 ¶ =b kb +k (b+k b k + 1 − nk,↑ − n k,↓ )0²k¶ =b kb +k 0²k¶ = 0²k¶ ± ⇒ N = 2 v k2µ0²k 0²k¶ k
404
8
Phonon Interactions
We next evaluate the term µ0²k  0²k ¶:
µ0²k0²k¶ = 0µ
µ
(u ∗k1
k1 ³=k
+ v ∗k b k ) 1
1
µ
(u k2
k 2 ³=k
+ v k b +k )0¶ 2
2
but since the sets of k1 and k 2 take the same values, all different from k, we can rearrange the products so that:
µ
µ0²k0²k¶ = 0µ = 0µ = 0µ = 0µ = 0µ
( u∗k 1 + v ∗k1 bk 1 )(uk 2 + vk 2 b+ k 2 )0 ¶
k 1 =k 2 ³=k
·
µ¶ k²
uk² 2 + v ∗k² uk² bk² + u ∗k² v k² b +k² + vk² 2 bk² b+k² 0¶
µ¶ k²
·
uk² 2 + vk² 2 bk² b+k² 0¶ ·
µ¶ k²
uk² 2 + vk² 2 (b+k² bk² + 1 − nk²,↑ − n k²,↓ ) 0¶
µ¶ k²
·
uk² 2 + vk² 2 0¶ =1
where we have again used relations between the creation–destruction operators that we encountered in previous steps. With this result, N takes the form N
=2
± k
v k2
(8.36)
2 from the expression Similarly, we evaluate N RMS 2 N RMS
≡ ¶µ BCSNˆ 2¶BCS ¶ −(N )2
and obtain: 2 N RMS
=4
± k
uk2vk 2
(8.37)
2 involve a simple sum over all k values of a regular function, Now, since both N and N RMS and
± k
V
→ (2π )3
´
dk
2 they will scale the same with the volume of the system. Thus, N RMS
N RMS N
∼ N and
∼ √1 ∼ 10−10 N
as expected. Our next task is to ﬁnd the optimal values of the coefﬁcients u k , v k from a variational argument. To this end, we wish to minimize the groundstate energy E BCS by taking matrix elements of the hamiltonian in the BCS wavefunction, subject to the constraint of a ﬁxed
405
8.4
Phonon–Electron Interactions: Superconductivity
number of particles N , as we established above. This constraint will be implemented by the use of a Lagrange multiplier μ , the chemical potential of the system: (s) (s) = δ µ¶BCS Hˆ − μNˆ ¶BCS ¶ =0
δ E BCS
subject to the constraint of Eq. (8.30). The hamiltonian that BCS chose is called the “pairing hamiltonian,” and is given by:
ˆ
HBCS
=
± k
+
³k (ck ,
± + + + Vkk² c k,↑ c −k,↓ c −k² ,↓ c k² ,↑ ↑ ck ,↑ + c −k,↓ c −k,↓ ) +
(8.38)
k ,k ²
where ³k is the energy of the singleparticle state ψk ,s and Vkk² is the effective interaction that scatters a pair state (k ² , ↑; −k² , ↓) to the pair state (k , ↑ ; −k , ↓), as shown schematically in Fig. 8.5. Using the pair creation–destruction operators deﬁned above, Hˆ BCS simpliﬁes to:
ˆ
HBCS
=2
± k
+b
³k bk
k
Thus, the quantity to be minimized is: (s ) µ¶BCS 2
± k
(³k − μ)b + k bk
±
+
+
k,k ²
±
+b
Vkk² bk
+b
Vkk² b k
k ,k²
k²

(s) k ² ¶BCS
¶
Using steps similar to the derivations above, we ﬁnd that this expression yields the following two terms: (s ) 2 µ¶BCS
µ
±
k (s ) ¶BCS

(³k − μ )b+ k b k ¶BCS ¶ (s )
± k,k ²
+ Vkk² b b

(s ) k k² ¶BCS
=2
± k
±
¶ =
k ,k ²
v k2(³k − μ) ∗ ∗
Vkk² u k v k uk ² v k²
For simplicity, if we choose phases so that uk and vk are real, the groundstate energy to be minimized becomes: E BCS
initial
=2
k’
± k
k
2
v k (³k
− μ) +
± k ,k²
final
Vkk² u k v k u k² v k²
k
Fig. 8.5
k’ initial
final
q
kF k’
(8.39)
k
k’
initial
k
final
Scattering between electrons of wavevectors ±k (initial) and ±k² (ﬁnal) through the exchange of a phonon of wavevector q: in the initial state the Cooper pair of wavevector k is occupied and that of wavevector k² is not, while in the ﬁnal state the reverse is true. The shaded region indicates the Fermi sphere of radius kF .
406
8
Phonon Interactions
subject to the conditions 2
vk
+ u2k = 1
and
(s ) ˆ (s ) µ¶BCS N ¶BCS ¶ =2
To perform this minimization, we ﬁrst deﬁne the angle uk
≡ sin θ2k ,
θk
± k
2
vk
=N
(8.40)
using
≡ cos θ2k
vk
(8.41)
from which we obtain: 2
vk
= cos2 θ2k = 12 (1 + cos θk),
= cos θ2k sin θ2k = 12 sin θk
u kv k
and with these, the expression for the groundstate energy becomes: E BCS
=
± k
(³k − μ)(1 + cos θk ) +
1± Vkk² sin θk sin θ k ² 4 ² k,k
Now the only variational parameter is θk . Differentiating with respect to this parameter and setting the derivative of E BCS to zero yields: tan θk
= 2(³ 1− μ) k
± k²
V kk²
sin θk²
(8.42)
We can rewrite this equation, with some hindsight, by deﬁning the following two quantities that will later be shown to be the energygap parameter and quasiparticle excitation energy, respectively:
±
±k
≡ −
Ek
≡
¹
k² 2
±k
Vkk² u k² v k²
= −21
+ (³k − μ)2
± k²
º1/2
Vkk²
sin θk ²
(8.43) (8.44)
Substituting ±k in Eq. (8.42) gives: tan θk
= −(³ ±−k μ) ⇒ cos θk = −(³k±− μ) sin θk k k
from which we obtain: sin2 θk
+ cos2 θk = 1 = sin2 θk
Å
1+
(³k
Æ
− μ)2 ⇒ sin θ = ±k k 2 E k
±k
Using this value in Eq. (8.42) leads to: ±k
= −21
± k,k²
Vkk²
±k²
E k²
= −12
± k ,k²
Vkk²
È
±k²
(±2k²
+ (³k2² − μ)2
(8.45)
This integral equation is known as the BCS gap equation and must be solved for ±k and μ under the second constraint of Eq. (8.40), because the ﬁrst constraint is automatically satisﬁed by our choice of u k and v k in terms of the single variable θk , Eq. (8.41). Since we are working with singleparticle states that in the normal system at T = 0 are ﬁlled up to the Fermi level, with energy ³F , the chemical potential can effectively be taken to be μ = ³F .
407
8.4
Phonon–Electron Interactions: Superconductivity
The BCS Model
To make further progress in describing the state of the system within the BCS hamiltonian, we need to ﬁnd explicit solutions to Eq. (8.45). This can easily be done in a limiting case (trivial solution), or by introducing a model that simpliﬁes the equation enough to obtain an analytic result, the BCS model. We investigate these two cases next. The trivial solution is ±k = 0, which then gives v k = 1 for ³k < ³F and v k = 0 for ³ k > ³F . This is just the normal state of the system at T = 0, described by a single Slater determinant with singleparticle states occupied up to ³k = ³F . A nontrivial solution can be obtained by approximating Vkk² to be similar to the interaction used in the Cooper pair problem; this is known as the BCS model. Speciﬁcally, we take: Vkk²
= −V , for ³F − h¯ ωD < ³k, ³k² < ³F + h¯ ωD = 0, otherwise
(8.46)
This form of Vkk² implies that: ±k
= ±, for ³F − h¯ ωD < ³k , ³k² < ³F + h¯ ωD = 0, otherwise
(8.47)
The gap equation, Eq. (8.45), then simpliﬁes to the solution of ± from 1 ± 1 V È 2 2 ±2 + (³
1=
− ³F)2 ³ ² ⇒ 1 ≈ V g(³F) sinh−1 h¯ ωD k²
k
⇒ 1 = V2
´
+¯hωD
³F
−¯hωD
Ë
³F
g (³)
±2
+ (³ − ³F)2
d³
±
where, in the last two steps, we introduced the density of states g(³ ) and assumed that h¯ ωD ¸ ³F . For weak coupling, that is, if g(³F )V < 1, the result simpliﬁes further to give: ±
≈ 2h¯ ωDe−1 g( )V /
(8.48)
³F
which is an expression similar to the binding energy of a Cooper pair, Eq. (8.27). The magnitude of ± is much smaller than h¯ ωD , which in turn is much smaller than the Fermi energy, as discussed in Chapter 7: ±
¸ h¯ ωD ¸ ³F
which shows that the superconducting gap is a minuscule fraction of the Fermi energy. As yet, however, we still have not determined what the physical meaning of ± is. This will be discussed in the next subsection. Nevertheless, given ±, we can obtain the associated optimized u k , v k from v 2k
= 21
²
1−
³k
− ³F ³ = 1 ²1 −
Ek
2
ξk
Ek
³
, u 2k
= 12
²
1+
³k
− ³F ³ = 1 ²1 +
Ek
2
ξk
Ek
³
where we have also deﬁned for convenience ξ k ≡ ³k − ³F ; uk and v k are plotted in Fig. 8.6 as functions of ξ . Note that even though these results are for T = 0, the plot
408
8
Phonon Interactions
g( ) 1
vk 2
uk 2
gF
−Δ Fig. 8.6
Δ
0
ξ
−Δ
Δ
0
Features of the BCS model. Left: Cooper pair occupation variables uk 2 and vk 2 as a function of the energy ξ = ³ − ³F . Right: Superconducting density of states g( ³ ) as a function of the energy ³ ; gF is the density of states in the normal state at the Fermi level. The ﬁlled states are shown shaded in pink.
for v2k is reminiscent of the Fermi distribution function for a normal system at a nonzero temperature of order ±. As we shall see later, the transition temperature T c from normal to superconducting behavior is also of order ± . Thus, one could argue that as the system is cooled below T c , it is the relative phases of the manybody states describing the normal system that get locked into a single quantum state, rather than changes in the occupation numbers of the singleparticle states. Using the above expressions for v k and uk , the optimized groundstate energy becomes: E BCS
=
±
²
1−
ξk
k
³
ξk
Ek
2
− ±V
Now recall that ± = 0 corresponds to the normal state at T = 0. Therefore, the difference in energy between the superconducting and normal states given by δ E = E BCS − E N is: δE
=
±
²
1−
ξk
k
ξk
³
Ek
−
2
±
V
−
±
²
ξk
k
1−
ξk
³
ξk
Since ξ k /ξ k  =1 for k  > k F and −1 for k  < k F , the summation over k in the third term of the expression above will only involve terms for k  < k F . This summation can then be included in the ﬁrst term to give: δE
=
È
±
k kF
Using E k = ±2 + ξ k2 and E k = ξk  when ξ k  zero unless ξ k  < h¯ ωD . This produces: δE
= g (³F )
´ h¯ ωD Å
−¯hωD
ξ
Å
±
−Ë
>
ξ ±2
ξk
−E
2
ξk
Æ
k
2
− ±V
¯
hωD , the summations above will give 2
+ξ2
Æ
dξ −
2
±
V
and in the limit of small g (³F )V we obtain: δE
= −21 g(³F)± 2 = −2(h¯ ωD)2g (³F)e−2 g( )V /
³F
which proves that the superconductingstate energy is lower than that of the normal state.
409
8.4
Phonon–Electron Interactions: Superconductivity
Quasiparticle Excitations in BCS Theory
We consider next what the excited states of the BCS hamiltonian might look like. The quasiparticle excitation energy is simply deﬁned to be the total excitation energy when an extra electron is added to the system. Suppose we add this extra electron in the singleparticle state ψk ,↑ , with its pair state ψ−k ,↓ empty. The only effect of this on the BCS hamiltonian is to block the pair (k , ↑; −k, ↓) from participating in the pairing. Thus, the energy of the total system will be increased by the energy of the added electron ξ k and removal of terms from the total energy, Eq. (8.39), involving k. This gives a quasiparticle QP energy E k equal to: QP
Ek
= ξk − 2v 2kξk − 2u kv k
± k²
Using our earlier deﬁnitions of u k , v k in terms of the variable ±k , E k , Eqs (8.43) and (8.44), we ﬁnd: QP Ek
= ξk −
²
1−
ξk
Ek
³
ξk
(8.49)
Vkk² uk ² v k² θk ,
2
2
k
k
and the deﬁnitions of
+ ±E k ±k = Eξk + ±E k = E k k
that is, the quasiparticle excitation energy is just E k , the quantity deﬁned in Eq. (8.44). Moreover, since the minimum energy to create one quasiparticle is E k = ±k , for ξ k = 0, this validates our earlier suggestion that ±k plays the role of the quasiparticle energy gap. Interestingly, E k is also the energy to remove a particle from the state ψ−k ,↓ in the system. Again, the only energies left are ξ k and the fact that the pair (k , ↑; −k, ↓) no longer contributes. Since the minimum energy to remove a particle from the system is ± k , and to then add the particle back into the system is also ±k , any electronic transition of the system must have a minimum energy of 2± k . This effect can be directly observed experimentally. To explain this observation, we consider contact between a superconductor and a metal. Typically, the superconducting gap is small enough to allow us to approximate the density of states in the metal as a constant over a range of energies at least equal to 2± around the Fermi level. This situation is equivalent to metal–semiconductor contact, as discussed in detail in Chapter 2. We can therefore apply the results of that discussion directly to the metalsuperconductor contact. The measured differential conductance at T = 0 will be given by Eq. (2.118):
¸
dI dV b
»
T =0
= e T 2 g(S) (³F + eV b)g (M) F
with T the tunneling matrix element and g(S)(³ ), g (M) (³) the density of states of the (M) superconductor and the metal, the latter evaluated at the Fermi level, gF = g(M)(³F ). This shows that by scanning the bias voltage V b , one samples the density of states of the superconductor. Thus, the measured differential conductance will reﬂect all the features of the superconductor density of states, including the superconducting gap. However, making measurements at T = 0 is not physically possible. At nonzero temperature T > 0 the occupation number n(M) (³ ) is not a sharp stepfunction but a smooth one whose derivative is an analytic representation of the δ function (see Appendix A). In this case, when the voltage V b is scanned, the measured differential conductance is also a smooth
410
8
Phonon Interactions
function representing a smoothed version of the superconductor density of states: the superconducting gap is still clearly evident, although not as an inﬁnitely sharp feature.
BCS Theory at Nonzero Temperature
Finally, we consider the situation at nonzero temperature T . It is straightforward to generalize the T = 0 result in the following way: instead of the BCS wavefunction at T = 0, we will have some typical excited state  ¶BCS (T )¶ which will include the presence of quasiparticle excitations that will conspire to reduce the pairing interactions and consequently the superconducting gap. If we deﬁne the probability that a quasiparticle is excited at temperature T with energy E k↑ (T ) to be fk,↑ (T ), then since the quasiparticles are to a good approximation independent fermions, we have: fk ,↑ (T )
= 1 + exp[β1 E
k,↑ (T )]
where β = 1/ kB T . Let us now consider adding a quasiparticle in the state k to the system at T > 0. This will be the same as the result in Eq. (8.49) for T = 0, except that we now need to multiply the third term in that equation by the probabilities that the quasiparticle states ψk² ,↑ and ψ−k ² ,↓ are empty at T > 0. For low T , and small values of fk ² ,↑ = f −k² ,↓ , this gives: QP
E k (T )
¹
º
= ξk 1 − 2v 2k − 2ukv k ¹
= ξk 1 −
2v 2k
º
− 2u kv k
± k²
± k²
Vkk² u k² v k²
±
≡ −
k²
Vkk² u k² v k²
² Vkk² uk ² v k²
tanh
then the gap equation takes the form ±k (T )
=
tanh
E k² (T )
E k² (T )
E k (T )
= 0, we get fk,s = 0: tanh
= ²
ξ
2 k²
³
³ (8.50)
+ ±2k² (T )
E k² (T )
2 kB T
³
2 kB T
²
È
)
2 kB T
± −21 Vkk² È ±k² (T ) tanh E2kk² (TT) 2 2 B ξ k² + ±k ² (T ) k²
with
Note that when T
1 − fk ² ,↑ − f−k² ,↓
²
If we now deﬁne a new gap ±k (T )
(
³
=1
and we recover the corresponding expression as in Eq. (8.45). The new equation for the temperaturedependent gap can be used with the BCS model to calculate the transition
411
8.4
Phonon–Electron Interactions: Superconductivity
temperature T c at which the superconductor becomes normal, that is, weak coupling limit, this becomes (see Problem 5):
= 1.14h¯ ωDe−1 g V / F
k BT c
±(T c )
= 0. In the (8.51)
0
This relation provides an explanation for the socalled “isotope effect,” that is, the dependence of T c on the mass of the ions involved in the crystal. From our discussion of phonons in Chapter 7, we can take the Debye frequency to be: ωD
∼
¹ κ º 1/ 2 M
where κ is the relevant force constant and M the mass of the ions; this leads to T c ∼ M −1/ 2, the relation that quantiﬁes the isotope effect. Moreover, combining our earlier result for ± at zero temperature, Eq. (8.48), with Eq. (8.51), we ﬁnd: 2±
= 3.52kB Tc
(8.52)
where 2± is the zerotemperature value of the superconducting gap. This relation, referred to as the “law of corresponding states,” is obeyed quite accurately by a wide range of conventional superconductors, conﬁrming the BCS theory. 8.4.2
The McMillan Formula for Tc
We close this section with a brief discussion of how the T c in conventional superconductors, arising from electron–phonon coupling as described by the BCS theory, can be calculated. McMillan9 proposed a formula to evaluate T c as: Tc
=
¸
1.04(1 + λ) exp − 1.45 λ − μ ∗ − 0.62 λμ∗ ²D
»
(8.53)
where ² D is the Debye temperature, λ is a constant describing electron–phonon coupling strength, and μ∗ is another constant describing the repulsive Coulomb interaction strength. This expression is valid for λ < 1.25. The value of μ∗ is difﬁcult to obtain from calculations, but in any case the value of this constant tends to be small. For sp metals like Pb, its value has been estimated from tunneling measurements to be μ ∗ ∼ 0.1; for other cases this value is scaled by the density of states at the Fermi level, g F , taking the value of gF for Pb as the norm. The exponential dependence of T c on the other parameter, λ, necessitates a more accurate estimate of its value. It turns out that λ can actually be obtained from electronic structure calculations. We outline the calculation of λ following the treatment of Chelikowsky and Cohen.10 λ is expressed as the average over all phonon (l) modes of the constants λk : λ
=
±´ l
(l )
λk
dk
9 W. G. McMillan, Phys. Rev. 167, 331 (1968). 10 J. R. Chelikowsky and M. L. Cohen, “Ab initio pseudopotentials and the structural properties of semicon
ductors,” in P. T. Landsberg (Ed.), Handbook on Semiconductors 1992).
, Vol. 1, p. 59 (North Holland, Amsterdam,
412
8
Phonon Interactions
which describes the coupling of an electron to a particular phonon mode identiﬁed by the index l and the wavevector k (see Chapter 7): (l)
λk
½
2g F ¼
=
¯
M (n, q, n² , q² ; l, k)2 F
(l)
h ωk
where M(n , q , n² , q² ; l, k ) is the electron–phonon matrix element and µ· · F· denotes ¶ an average over the Fermi surface. The electron–phonon matrix elements are given by:
² ² M (n, q, n , q ; l , k) =
± j
Ì
»
¸
¯ µψ (n) eˆ (l) · δV ψ (n² ² )¶δ(q − q² − k) q q kj (l) δt
h
2 M j ωk
j
(8.54)
where the summation on j is over the ions of mass M j at positions tj in the unit ²
cell, ψq(n) , ψq(n² ) are electronic wavefunctions in the ideal crystal, and eˆ (kjl) is the phonon polarization vector (more precisely, the part of the polarization vector corresponding to the position of ion j). The term δV /δtj is the change in crystal potential due to the presence of the phonon. This term can be evaluated as:
± l
eˆ kj
(l)
· δδVt =
(l)
Vk
j
− V0 (l)
uk
(8.55)
(l)
where V0 is the ideal crystal potential, Vk is the crystal potential in the presence of the (l ) phonon mode identiﬁed by l , k, and uk is the average ionic displacement corresponding to this phonon mode. The terms in Eq. (8.55) can readily be evaluated through the computational methods discussed in Chapter 6, by introducing ionic displacements u(kjl) corresponding to a phonon mode and evaluating the crystal potential difference resulting from this distortion, with: (l)
uk
=N
⎛ ⎞ 1/ 2 ± 1 ⎝ u(kjl) 2⎠ ion
j
the ionic displacement averaged over the N ion ions in the unit cell. Using this formalism, it was predicted and later veriﬁed experimentally that Si under high pressure would be a superconductor. 11 8.4.3
HighTemperature Superconductors
Finally, we discuss very brieﬂy the new class of hightemperature superconductors, discovered in 1986 by Bednorz and M¨uller, in which the T c is much higher than in conventional superconductors: in general it is in the range of ∼ 90 K, but in certain compounds it can exceed 130 K (see Table 8.2). This is well above the freezing point of N 2 (77 K), so this much more abundant and cheap substance can be used as the coolant to bring the superconducting materials below their critical point. The new superconductors have complex crystal structures characterized by Cu–O octahedra arranged in various ways, as in 11 K. J. Chang and M. L. Cohen, Phys. Rev. B 31, 7819 (1985).
413
8.4
Table 8.2
Phonon–Electron Interactions: Superconductivity
Critical temperature
Tc
(K) of representative hightemperature superconductors. In several
x X,Y
cases there is fractional occupation of the dopant atoms, denoted by equivalent structures with two diﬀerent elements, denoted by ( highest
Tc
(with
0 0.5 T, the voltages show quantized values, which become more pronounced as B increases: The Hall voltage VH exhibits plateaus for certain regions of B values, which correspond to quantized values of the resistivity ρxy given by (h/ e2) /( l + 1) with l an integer, and for the same regions the longitudinal voltage V L , and hence the diagonal conductivity ρxx , vanishes.
motion of electrons with effective mass m in the x , y plane. The presence of the magnetic ﬁeld is represented by the vector potential A(r), which we choose as:
A(r)
= −By xˆ ⇒ B = ∇r × A(r) = B zˆ
(9.3)
a choice known as the “Landau gauge.” As far as the presence of the electric ﬁeld is concerned, an estimate of the relative magnitude of the components E x and E y , for typical setups where L ² W in the geometry for the Hall measurements shown in Fig. 9.2, indicates that E y is larger than E x by at least two orders of magnitude. In other words, other than setting up the current in the x direction, the electric ﬁeld component E x can be ignored compared to the E y component. We let the value of the latter, at steady state, be equal to −E 0, so that the potential energy of electrons associated with this ﬁeld, which appears in the hamiltonian, is V (r) = eE 0 y. The full hamiltonian is then:
ˆ =
HL
¹2 1 ¸ e p + A(r) + eE 0y 2m c
=
1 2m
º¶
The solutions to this hamiltonian are of the form ¯ (x , y ) = √1 ei kx xφkx (y ), k x ψ L
px
−
eBy
·2
c
= 2πL k ,
»
+ p2y + eE 0 y
(9.4)
k : integer
where we have imposed Born–von Karman boundary conditions in the x direction through the choice of the wavevector kx , a process with which we are familiar from the discussion of Chapter 2. We next substitute this expression for the wavefunction in the Schr¨odinger equation to obtain:
¼
1 2m
º¶
¯ −
hk x
eBy c
·2
+
»
2 py
+ eE 0 y
½
φkx (y )
= ±k φk (y) x
x
423
9.1
Electrons in External Electromagnetic Fields
To solve for the eigenvalues and eigenfunctions of this equation, we add to and subtract from the hamiltonian the term m
¶
cE 0
2
·2
B
which allows us to complete the square in the y variable, and we arrive at:
º
p 2y
2m
+
1 m 2
¶
eB mc
·2 (y
− y )¯
»
2
φkx ( y)
=
º
± kx
−
mc 2
¶
2
E0
·2
B
+ eE 0y¯
» φkx (y )
(9.5)
where we have introduced the variable y¯ , deﬁned as: k xc ¯ = h¯eB + mceB E2 0 2
y
(9.6)
The equation for the eigenfunctions and eigenvalues of the y variable has now become that of the harmonic oscillator potential with the origin shifted to y¯ , and the energy levels of the harmonic oscillator are shifted by the two terms that appear in the square bracket of the righthand side. The spring constant κ for the harmonic potential and the corresponding characteristic frequency ωc are given by:
=m
κ
¶
eB
·2
mc
⇒ ωc =
¸ κ ¹ 1/ 2 m
= eB mc
(9.7)
with the latter referred to as the “cyclotron frequency”; in terms of this, the energy levels of the harmonic oscillator are given by:
¶
¯ = j+
±
(j )
·
1 h¯ ωc , j 2
= 0, 1, 2, . . .
(see Appendix C). The original eigenvalues of the energy will then be given by: (j)
±k
x
¶
·
= j + 12 h¯ ωc + mc2
2
¶
E0
·2
B
¶
·
−eE 0 y¯ = j + 12 h¯ ωc − mc2
2
¶
E0 B
·2
− h¯k x c EB0
(9.8)
These energy levels are known as “Landau levels”; the full wavefunctions ψ¯ ( x, y) consist (j) of a component φkx (y ) coming from the harmonic potential in the y variable, centered at y¯ , and a planewave component in the x variable with wavevector k x. How many electrons can each Landau level accommodate? To answer this question, we consider the different possible values of y¯, the position of the center of the harmonic oscillator wavefunction. From the deﬁnition of the value of y¯ , Eq. (9.6), we have:
¯ δkx = h¯c 2π δ k = δ y¯ = eB eB L hc
¶
hc
·
e
1 BL
(9.9)
since k is an integer (recall that h¯ = h /2π ). δ y¯ are the steps in the value of y¯ , and since the total width of the sample in the y direction is W , the number of possible positions of the center is given by: NL
= δWy¯ = hce (WL )B = hce AB
424
9
Dynamics and Topological Constraints
where we have used A = WL for the area of the sample. This is a very interesting result, because ² = AB is the total magnetic ﬂux through the sample and the quantity φ0 = (hc /e ) is the magnetic ﬂux quantum, so this result shows that the number of states accommodated by the Landau level is the total number of ﬂux quanta: φ0
= hce ⇒ N L = (hcAB/e) = φ²
9.1.3
0
(9.10)
Quantum Hall Eﬀect
The quantization of electron states in Landau levels plays a central role in the description of the quantized version of the Hall effect. The basic picture for explaining the quantum Hall effect (QHE) was constructed by R. B. Laughlin.3 An important role in the manifestation of this phenomenon is played by states at the edge of the sample, an issue that was elucidated by the elegant treatment of these states by B. I. Halperin.4 The edge states of 2D systems have become the focus of much attention recently as they underlie very interesting physics phenomena, to which we return in later sections of this chapter. We present here the main ideas of Laughlin and Halperin that led to the explanation of the QHE. We begin by considering the system in a loop, rather than a planar, ribbon geometry, which will facilitate the justiﬁcation of how various terms arise from changes in the external magnetic ﬁeld. In this geometry, the x direction becomes the tangential direction along the loop of total circumference L , the y direction is perpendicular to x and lies on the loop surface which had width W , and the z direction becomes the radial direction perpendicular to the loop surface, as illustrated in Fig. 9.4. This is consistent with our assumption of Born–von Karman periodic boundary conditions in the x direction, with the
W
I x y E0
ΔV=VH Fig. 9.4
Loop geometry for establishing the quantum Hall effect (after R. B. Laughlin, see footnote 3). 3 R. B. Laughlin, Phys. Rev. B 23, 5632 (1981). 4 B. I. Halperin, Phys. Rev. B 25, 2185 (1982).
425
9.1
Electrons in External Electromagnetic Fields
sample length L in this direction being much larger than the sample width W ; in the limit L → ∞we recover the planar ribbon geometry discussed above. We will assume that there is a magnetic ﬂux ² through the torus, and any changes in it will produce an electromotive force E according to Faraday’s law: E
= −1c dd²t
that drives a current along the x direction of the loop. A small adiabatic change in the ﬂux, δ², introduced over a small time interval δ t will produce a current I , and in order to maintain this current work δ U must be produced at the rate δU δt
δU = −E I = 1c I δ² ⇒ I =c δt δ²
Now suppose the change in ﬂux δ² is associated with changes in the magnetic ﬁeld B ∇ ×A: δ²
=δ
¶¾
·
S
∇ ×A · dS = δ
¶¿
L
A · dl
=
·
where dS is the surface element of the surface S that the ﬁeld B pierces, and d l = dx ˆx is the length element along the circumference of the loop L that encloses the surface S . If we choose the vector potential to be A = A x xˆ , consistent with the Landau gauge, Eq. (9.3), we obtain: δ²
= L δA x
since the geometry of the loop is ﬁxed. This result, together with the above expression for the current I , produces the expression I
= Lc δδAU
x
Next we calculate the change in internal energy of the system δ U when the vector potential is adiabatically changed by a small amount δ A = δ A x xˆ . This change introduces a change in the hamiltonian of Eq. (9.4):
p →p+
e c
ˆ
δA x x
Since the wavefunctions ψ¯ (x, y ) have been factorized into products of functions that depend only on the x variable, or only on the y variable, we examine how this change in the x component of the momentum operator affects the x dependent part of the wavefunction only, which is a plane wave with wavenumber kx = 2π k /L with k an integer. The change in the momentum operator produces gauge transformation of the wavefunction: p 2x
2m
f (x )
= ± f (x ) ⇒ 21m
¸
px
¹
2 + ce δA x f¯( x) = ±f¯ (x )
that is, the original solution f (x ) to the planewave equation is replaced by f¯ (x ), which is given by:
¯f (x ) = f (x ) exp{−i[(e /h¯c )δ A x ]x }
426
9
Dynamics and Topological Constraints
Generally, there are two classes of states, localized and extended. For a localized state, which obeys the Schr¨odinger equation
´
µ ¹2 1 ¸ e ˜ p + δ A x xˆ + V (x, y ) ψ˜ (x, y) 2m c
= ±ψ˜ ( x, y)
the above gauge transformation is still valid, and because the state is conﬁned to a small region of (x , y ) values, it amounts to a change in phase which does not lead to a change in the energy eigenvalue ±˜ . For an extended state, in order to have a valid gauge transformation, we must have: exp{−i[(e /h¯c )δ A x ]x }
=exp{−i[( e/h¯c )δA x ](x + L)} ⇒δ A x = hce Li ,
i : integer
but this leaves all the states unchanged due to periodic boundary conditions, and therefore their energies do not change. This suggests that any change in the total energy of the system must come from changes in the occupancy of the levels, without any change in the energy levels themselves. Connecting all this to our analysis of the Landau levels, we see that a change in the vector potential from A to A³ by δ A xxˆ implies a change
A³ = (−By + δ A x )xˆ =
−B
¶
y
δ Ax
−
·
B
ˆ = −By ³ xˆ ⇒ y³ = y − δBA x
x
in other words, the change in the vector potential is equivalent to shifting all values of the y variable, and hence the centers of the harmonic oscillator orbits, by −(δ A x /B ). Using the expression that we derived above for δ A x in the case of extended states, we ﬁnd that the shift in the position of the harmonic oscillator orbits is then given by:
¶
δA x
¯ = −B = −
δy
hc
·
e
i LB
,
i : integer
which is an integer multiple of the spacing between positions of the centers in the y coordinate, as we found earlier, Eq. (9.9). This already suggest that, since all the orbits are contained within the width W of the ribbon in the y direction, some of them must be transferred from one edge to the opposite. To simplify the discussion, let us assume that i= − 1 in the above expression, that is, the change in vector potential is: δA x
=
¶
hc
·
e
1 L
= φ0 L1
which is equivalent to changing the ﬂux by one ﬂux quantum, φ0 . We had also found earlier [see Eq. (9.9)] that the change in y¯ corresponds to a change in the k x wavevector: δk x
eB δ y¯ = = eB h¯c h¯c
¶
hc
·
e
1 BL
= 2Lπ
and
δk x
= 2Lπ δk ⇒ δ k = 1
that is, under this change in vector potential all the values of the index k are shifted by unity, which gives: (j )
±k
x
(δ A x ) = ±k³ (0), k x (j ) x
= 2πL k , k ³x = 2π ( kL+ 1) ,
k : integer
427
9.1
Electrons in External Electromagnetic Fields
With these considerations, we can now calculate the change in internal energy of the system induced by the change in ﬂux: δU
=
±² j,k
(j) ±k (δ A x ) x
−
(j ) ± k (0) x
³
⎡
=⎣
±
j,k+1
⎤
(j) ±k ⎦ x
⎡ ⎤ ± (j) ±² − ⎣ ±k ⎦ = ±k(j) j ,k
x
j
max
− ±(kj)
³
min
where kmin , kmax are the minimum and maximum values of the wavevector k x . From the expression for the Landaulevel energies, Eq. (9.8), we ﬁnd that the energy difference between the levels that correspond to these two values is given by:
− ±k(j) = −eE 0 ³y¯ = −eV H with ³y¯ the total difference in values of the variable y¯ , that is, ³y¯ = W , and the Hall voltage being given by V H = E 0 W . We can now sum over the index j = 0, 1, . . ., l with l (j)
±k
max
min
the index value of the highest occupied Landau level, to obtain:
2
δU
= −eV H (l + 1) ⇒ I = Lc δδAU = −φec ( l + 1)V H ⇒ ρxy = −VIH = ec (lφ+0 1) = (lh+/e 1) x
0
This is an important result, since it establishes that the resistivity is quantized and takes values that are integer fractions of h /e 2, the quantum of resistivity: 2
ρxy
B = nec = (lh+/e 1)
(9.11)
The entire argument presented above to establish the quantization of the Hall resistivity rests on the assumption that it is possible to change the occupancy of the Landau levels by transferring edge states from one side of the sample to the other, in the y direction. Now the states in the interior of the ribbon are separated in energy by a ﬁnite amount, h¯ ωc , and hence no change in their occupancy can be achieved by a small change in ﬂux δ². This leaves as the only option that edge states corresponding to a Landau level are degenerate with a level of different index value. This type of degeneracy was established through an elegant argument by B. I. Halperin. We shall brieﬂy present parts of this argument. For the purposes of this discussion, we focus on the harmonic oscillator equation that the y dependent part of the wavefunctions obeys, Eq. (9.5), and put aside the extra terms on the righthand side that depend on the ﬁeld E 0 (we will return to them later); accordingly, we also drop the subscript k x of the wavefunctions, which obey:
º
p2y
2m
+
1 m ω2c (y − y )¯2 2
»
¯ (j)(y ; y¯ ) = ± (¯j )(y¯ )φ¯ (j)( y; y¯ )
φ
As long as ¯y is far from the edges of the ribbon, y = ´ W /2, the solution to this equation is the usual set of eigenfunctions and eigenvalues of the harmonic oscillator potential (see Appendix C): ¶ · 1 (j) ±¯ (¯ y) = j + h¯ ωc, ¯y ±W /2 2 If ¯y approaches one of the edges, the wavefunctions must be distorted to ensure that they vanish at the edge, y = ´ W /2, while they preserve the number of nodes that the harmonic
428
9
Dynamics and Topological Constraints
oscillator solutions have. We examine what happens for y¯ = W /2 (analogous results are obtained for the other case, y¯ = − W /2). In this case, the wavefunction must obey
¯ (j) (y , W /2) → 0
for y
φ
→ −∞and y = W /2
and has j nodes, including the one at y = W /2, but this is the same as the wavefunction of the harmonic oscillator with index 2j + 1, centered at W /2. The consequence of this result is that the energy of the state with index j, when y¯ = W /2, will be equal to that of the harmonic oscillator state with index 2j + 1 far from the edge, that is:
¯ (j )(W /2) =
¶
±
(2j + 1) +
1 2
·
¯ =
¶
h ωc
2j +
·
3 h¯ ωc 2
The values of y¯ can also lie outside the interval [−W /2, W / 2], but then the energy becomes even higher, and rises eventually as m ω2c (¯y  −W /2)2 /2, for ¯y  > W /2 + r c , where r c is the characteristic length scale of the harmonic oscillator wavefunction (see Appendix C). The energy levels of the states as a function of the distance of their center ¯y from the edges of the ribbon at y = ´ W /2 are shown in Fig. 9.5. This establishes the degeneracy of edge states connected to a Landau level to states of a different index value, making the change of occupancy possible. The resulting density of states exhibits similar features with that of the system with disorder, see Fig. 9.7 later. This treatment allows us to make an analogy with the classical picture of electrons in a 2D ribbon on the x , y plane, on which a magnetic ﬁeld B = B ˆz is applied perpendicular to the ribbon plane, as illustrated in Fig. 9.6. For classical charged particles of charge e , the magnetic ﬁeld will induce circular orbits in the interior of the ribbon, of radius r c = mcv / eB (the cyclotron radius), where v is the magnitude of the original velocity of the
(y )
Fig. 9.5
5
11 2
5
9 2
4
9 2
4
7 2
3
7 2
3
5 2
2
5 2
2 1
3 2
1
3 2
1 2
j=0
h
c
1 2
j =0 W 2
11 2
0
W 2
y
g( )
Left: The energy levels ±¯ (j )( y¯ ) of states in the ribbon as a function of the position of their centers y¯ from the edges at y = ´ W / 2; the red lines correspond to the ideal harmonic oscillator levels, separated by h¯ ωc (after B. I. Halperin, see footnote 4). Right: The density of states g(± ) for the states that include edge effects (blueshaded regions) and the ideal harmonic oscillator levels, represented by sharp δfunctionlike peaks in red.
429
Fig. 9.6
9.1
Electrons in External Electromagnetic Fields
Schematic representation of classical orbits of charged particles, in the bulk (red circles) and at the edges (blue skipping orbits), of a ribbon on the x, y plane with external magnetic ﬁeld B = B ˆz perpendicular to it.
particles.5 At the edges, there is not enough space for circular orbits, so skipping edge orbits are induced. These are chiral states, that is, they travel in opposite directions at the two opposite edges of the ribbon. The bulk circular orbits do not contribute to any current along the ribbon length. The only states that can carry current along the ribbon are edge states. If the number of occupied states at the two opposite edges of the ribbon is the same, the net current is zero. Therefore, the occupancy of the states at opposite edges must be different. This is consistent with our earlier discussion, which established that the energy levels of the opposite edge states differ by −eV H , that is, their distance from the Fermi level will differ by this amount and their occupancy will indeed be different, leading to the net current I . Finally, Halperin also showed that weak disorder will not affect this picture. Since the edge states are not destroyed by disorder or by scattering from bulk states, the quantization of the Hall resistance is a robust effect, as manifest by the plateaus in the experimental measurements, see Fig. 9.3. What leads to the existence of plateaus in the value of ρxy is the fact that not all states in the system are extended Bloch states. In a real system, the Landau levels are not δ functions in energy but are broadened due to the presence of impurities, as indicated in Fig. 9.7. Only those states with energy very close to the ideal Landau levels are extended and participate in the current, while the states lying between ideal Landau levels are localized and do not participate in the current. As the magnetic ﬁeld is varied and localized states with energy away from an ideal Landau level are being ﬁlled, there can be no change in the conductivity of the system, which remains stuck to its quantized value corresponding to the ideal Landau level. This produces the plateaus in the Hall resistivity ρxy . The plateaus in Hall resistivity can be measured with unprecedented precision, reaching 1 part in 107. This has led to advances in metrology, since the ratio e 2/ h appears in several fundamental units. For example, the ﬁne structure constant is given by: α
e2
= hc = ¯
À
e2 h
Á¶
2π
·
c
and the speed of light c is known to be 1 part in 109 from independent measurements. Thus, using phenomena related to the behavior of electrons in a solid, one can determine the value of a fundamental constant that plays a central role in highenergy physics! 5 The use of the same symbol, r , for the cyclotron radius and the characteristic length of the harmonic oscillator c
is intentional, because for the physical system discussed here the two quantities are of the same order of magnitude (see footnote 4).
430
9
Dynamics and Topological Constraints
increasing B
l +3 l +1
l +2 l +1
l localized
l
l 1
extended
l 1
g( ) Fig. 9.7
F
g( )
Density of states g( ± ) and ﬁlling of Landau levels, including the effects of disorder, at different values of the magnetic ﬁeld B. When the magnetic ﬁeld takes the values B = nch /e( l + 1), with l = 0, 1, 2, . . ., exactly l + 1 Landau levels are ﬁlled and the Fermi level, denoted by a horizontal dashed line, lies between levels with index l and l + 1 in the ﬁgure on the left. In the ﬁgure on the right, corresponding to a smaller value of the magnetic ﬁeld B = nch/ e(l + 2) and l + 2 Landau levels ﬁlled, the Fermi level lies between levels with index l + 1 and l + 2. The spacing between levels is h¯ ωc = h¯ (eB /mc). The disorder broadens the sharp δfunctionlike DOS of the ideal system and creates states (blueshaded regions) between those of the ideal system.
Fascinating though the discovery of the IQHE may have seemed, an even more remarkable observation was in store: a couple of years after the experiments of von Klitzing and coworkers, experiments on samples of very high purity at high magnetic ﬁelds and low temperatures by Tsui, St¨ormer, and Gossard6 revealed that the plateaus in the Hall resistivity can also occur for values larger than (h /e 2). In particular, they occur at values 3, 3/ 2, 5, 5/2, 5 /3, . . ., in units of (h /e 2). This discovery was called the fractional quantum Hall effect (FQHE). The explanation of the FQHE involves very interesting manybody physics, which lies beyond the scope of the present treatment. Sufﬁce to say that the FQHE has generated enormous interest in the condensed matter physics community. A hierarchy of states at fractions
= 2qpp+ 1
ν
with p , q integers, that lead to plateaus in the Hall conductivity, has been predicted theoretically7 and observed experimentally; all these fractions have odd denominators. The states corresponding to the partial ﬁllings are referred to as “incompressible quantum ﬂuids.” Laughlin originally postulated a manybody wavefunction8 to describe the states with ν = 1/(2q + 1), where q is a positive integer; this wavefunction for N e electrons has the form ´q (r1, . . ., rNe )
=
Ne Â
(ζj
j b 0 = 1, l = 0 N
A
We can now calculate the magnetization M , deﬁned as: M
≡ −A1 ∂∂ UB = −NAe µB , =
Ne A
²
µB
for b > 1, l = 0
³
2(l2 + 3l + 2)b − (2l + 3) , for
A plot of the magnetization in units of n µB as a function of the variable b , which is the magnetic ﬁeld in units of nφ0 , is shown in Fig. 9.8: the magnetization shows oscillations between positive and negative values as a function of the magnetic ﬁeld! Although we showed how it arises in a 2D system, the effect is observed in 3D systems as well, in which case the discontinuities in the magnetization are rounded off. A number of other physical quantities exhibit the same type of oscillations as a function of the magnetic ﬁeld B ; examples include the conductivity (this is known as the Shubnikov–de Haas effect and is usually easier to measure than the de Haas–van Alphen effect), the sound attenuation, the magnetoresistance, and the magnetostriction (strain induced on the sample by the magnetic ﬁeld). The oscillations of the magnetization as a function of the magnetic ﬁeld can be used to map out the Fermi surface of metals, through the following argument, due to Onsager. 10 When a 3D metal is in an external magnetic ﬁeld, the plane perpendicular to the ﬁeld will intersect the Fermi surface of the metal, producing a crosssectional area that depends on the shape of the Fermi surface. Of course, there are many crosssections of a 3D Fermi 10 L. Onsager, Phil. Mag. 43, 1006 (1952).
433
9.1
Electrons in External Electromagnetic Fields
M
1
B
1
Fig. 9.8
1 1 1 5 4 3
1 2
1
Illustration of the de Haas–van Alphen effect in a 2D electron gas: the magnetization M , measured in units of ( Ne /A) µB , exhibits oscillations as a function of the magnetic ﬁeld B, measured in units of Ne φ0/ A = nφ0 .
belly neck
Fig. 9.9
The Fermi surface of Au [adapted from M. Gradhand et al., Phys. Rev. B80, 224413 (2009)]. The thin gray lines show the ﬁrst Brillouin zone of the FCC crystal. The smallest and largest crosssections in the (111) direction are indicated as “neck” (blackﬁlled circles on the hexagonal faces of the BZ) and “belly” (blue circles).
surface along a certain direction, but the relevant ones are those with the largest and smallest areas (the extremal values), as illustrated in Fig. 9.9. These crosssectional areas will play a role analogous to the area of the plane on which the electrons were conﬁned in the above example. Thus, our simple treatment of electrons conﬁned in two dimensions becomes relevant to the behavior of electrons with wavevectors lying on a certain plane that intersects the Fermi surface. Although additional complications arise from the band structure, in principle, we can use the oscillations of the magnetization to determine the extremal crosssectional areas enclosed by the Fermi surface on this plane. By changing the orientation of the metal with respect to the direction of the ﬁeld, different crosssections of the Fermi surface come into play, which makes it possible to determine the entire 3D Fermi surface by reconstructing it from its various crosssections. Usually, a bandstructure calculation of the type discussed in detail in Chapter 5 is indispensable in reconstructing the exact Fermi surface, in conjunction with magnetic measurements which give the precise values of the extremal areas on selected planes.
434
9
9.2
Dynamics and Topological Constraints
Dynamics of Crystal Electrons: SingleBand Picture
Up to this point we have treated electrons as essentially free particles, conﬁned only by an external potential that restricts their motion on the x , y plane, and examined what happens when we subject them to external electromagnetic ﬁelds; we have paid no attention to the effects of atomicscale potentials, such as that provided by the ions in a solid. To complete the picture of the dynamics of electrons in real solids, we will need to introduce again the features of the atomic structure of solids. As we have done in previous chapters, we will focus on the crystalline case, which can also form the basis for treating a wider range of systems (see the discussion in Chapter 1). We will describe the dynamics of crystal electrons in two stages: ﬁrst, in this section, we will discuss a picture that establishes a connection between the forces exerted on electrons by external electromagnetic ﬁelds and the intrinsic features of electronic motion due to the crystal potential, that is, the Bloch character of electronic states. Speciﬁcally, we will derive the intuitively pleasing results that the expectation values of the velocity and of the acceleration of crystal electrons are (n) related to derivatives of the crystal energy ±k with respect to the crystal momentum h¯ k. This picture, however, does not capture the full range of the electronic response. Then, in later sections of this chapter, we will explore more subtle effects of how crystal electrons respond to external forces; these include important changes in the phase of electronic wavefunctions (Berry’s phase) that are manifest in experimentally measurable quantities. We start by deriving expressions for the time evolution of the position and velocity of a crystal electron in the state ψk(n). To this end, we will need to allow the crystal momentum to acquire a time dependence, k = k(t ), and include its time derivatives where appropriate. Since we are dealing with a particular band, we will omit the band index n for simplicity. Considering the timedependent position of a crystal electron r(t ) as a quantummechanical operator, we have from the usual formulation in the Heisenberg picture (see Appendix C): dr(t) dt
²
³
= hi Hˆ , r ⇒ ψµ k(n)  ddr(tt ) ψk(n)¶ =hi µψk(n) [Hˆ , r]ψk(n) ¶ ¯ ¯
(9.13)
with [Hˆ , r] the commutator of the hamiltonian with the position operator. Now we can take advantage of the following identity:
∇k
¸
ˆ ei k·r e−ik ·r H
¹
= ie−ik· r [Hˆ , r]ei k·r
whose proof involves simple differentiations of the exponentials with respect to k, and we recall the relation derived in Eq. (2.24), to rewrite the righthand side of the previous equation as: i
µ h¯
 ˆ 
(n ) (n) ψk [H, r] ψk
i
¾
¶ ≡h ¯¾ 1 =h ¯¾ 1 =h ¯
(n)∗
uk
(n)∗
uk
(n)∗
uk
(r)e− ik·r [Hˆ , r]eik ·r u k (r)dr (n)
(r) (r)
²
∇k
²
¸
ˆ ei k·r e−ik ·r H
¹³
³
∇kHˆ (p + h¯ k, r)
(n)
u k (r)dr
(n )
u k (r)dr
435
9.2
Dynamics of Crystal Electrons: SingleBand Picture
By comparing the last expression to the original one, Eq. (9.13), we derive the interesting (n) result that the operator that gives the average velocity in a band, with the basis u k ¶, is: (n )
vk
²
³
= h1 ∇kHˆ (p + h¯ k, r) ⇒ vµ(kn)¶ =1h µu (kn)  ∇kHˆ (p + h¯ k, r) u (kn) ¶ ¯ ¯
(9.14)
a result that will prove useful in the following section. Next, we move the differentiation with respect to k, ∇k , outside the integral and subtract the additional terms produced by this change, which leads to:
¾
µψ (n) [Hˆ , r]ψk(n) ¶ =1h ∇k u (kn)∗ (r)Hˆ (p + h¯ k, r)u (kn) (r)dr h¯ k ¯ ´¾ ¸ ¾ ¹ ¸ ¹ µ 1 (n)∗ −h ∇ku k (r) Hˆ (p + h¯ k, r)(kn)(r)dr + u(kn)∗ (r) Hˆ ( p + h¯ k, r) ∇k u(kn)( r) dr ¯ i
(n )
We deal with the last two terms in the above expression separately. Recalling that uk (r) is an eigenfunction of the hamiltonian Hˆ (p + h¯ k , r) with eigenvalue ±k , we obtain for these two terms:
µ∇ku (k¸n)Hˆ (p + h¯ k)u (kn)¶ + u (kµn) Hˆ (¹p + h¯ k)∇ ku(kn) ¶ = (n ) (n ) (n) (n ) (n ) (n ) ± k µ∇k u k  uk ¶ + u kµ ∇k u k ¶ = ± k ∇ k µ uk  uk ¶ =0 since µuk u k ¶ =1 for properly normalized wavefunctions. This is a special case of the more general Hellmann–Feynman theorem, which we encountered in Chapter 4. This leaves the following result:
µ
(n )
(n)
(n) ψk
 drd(tt) ψk(n) ¶
1
=h ∇k ¯
¾
(n)∗
ψk
ˆ k (r)dr ⇒ vµk (r)Hψ (n )
(n )
¶ =h1 ∇k±k(n) ¯
(9.15)
where we have identiﬁed the velocity µvk ¶ of a crystal electron in state ψk with the expectation value of the time derivative of the operator r(t ) in that state. This result is equivalent to Eq. (2.50), which we derived earlier for the momentum of a crystal electron (n ) in state ψk . The results derived so far are correct when dealing with electronic states describing the ground state of the system without any external perturbations. Using these results to describe the response of the system to external ﬁelds would therefore be incomplete. Nevertheless, we will proceed here to do just this for the purpose of discussing the dynamics of electrons in external ﬁelds in a simple and intuitive, even if incomplete, picture. We will then derive a more complete description in the following section. To continue the discussion of electron dynamics in this simple picture, we take a derivative of the velocity in state ψk(n) with respect to time, and using the chain rule for differentiation with respect to k, we ﬁnd: (n )
dµvk dt
(n)
¶ = 1 ¶ dk · ∇· ∇ ± (n) k k k h¯ dt
(n)
436
9
Dynamics and Topological Constraints
which we can write in terms of cartesian components (i, j = x , y , z ) as: dµv k,i ¶ (n )
dt
=
± ¶ dk j ·
¯ dt
h
j
º
1
¯
(n)
∂ 2± k
»
h 2 ∂ kj∂ ki
=
± ¶ d kj ·
¯ dt
h
j
1 (n) m ji (k )
(9.16)
where we have identiﬁed the term in square brackets as the inverse effective mass tensor derived in Eq. (2.51). With this identiﬁcation, this last equation has the form acceleration = force ×
1 mass
as might be expected, but the mass is not a simple scalar quantity as it would be in the case of free electrons; instead, the mass is now a secondrank tensor corresponding to the behavior of crystal electrons. The form of Eq. (9.16) compels us to identify the quantities in parentheses on the righthand side as the components of the external force acting on the crystal electron: dk ¯ dt = F
h
(9.17)
We note two important points. First, the identiﬁcation of the time derivative of h¯ k with the external force is not a proper proof but only an inference from dimensional analysis; external forces could actually change the wavefunctions and the eigenvalues of the singleparticle hamiltonian, an issue to which we return below. Second, this relation is a stateindependent equation, implying that the wavevectors evolve in the same manner for all states. For instance, if crystal electrons were subject to a constant external electric ﬁeld E, they would experience a force F = − e E and according to Eq. (9.17), this would lead to: dk h¯ = −e E (9.18) dt We discuss below how this picture applies to a simple 1D example.
Example 9.1 Motion of electrons in one dimension, oneband model We consider the simplest case, a 1D crystal with a single energy band, given by: ±k
= ± + 2τ cos(ka )
with ± a reference energy and τ a negative constant; since we are dealing with a single band, we are going to dispense with the band index n, to simplify the notation. This is shown in Fig. 9.10: the lattice constant is a, so the ﬁrst BZ for this crystal extends from −π/a to π/a , and the energy ranges from a minimum of ± + 2τ (at k = 0) to a maximum of ± − 2τ (at k = ´ π/a ). The momentum for this state is given by: m e d±k 2 me τ a p (k ) = p (k )xˆ = xˆ = − sin(ka )xˆ h¯ dk h¯
437
9.2
Dynamics of Crystal Electrons: SingleBand Picture
k
k
holes F
F
electrons
π
0
a Fig. 9.10
a k
0
a
a k
Singleparticle energy eigenvalues ±k for the simple example that illustrates the motion of electrons and holes in a oneband, 1D crystal.
When the system is in an external electric ﬁeld E the time evolution of the wavevector will be: dk dt
= −E 0 xˆ with E 0 a positive constant,
= −he E ⇒ ddkt = he E 0 ¯ ¯
We will consider some limiting cases for this idealized system. (1) A single electron in this band would start at k = 0 at t = 0 (before the application of the external ﬁeld it occupies the lowestenergy state), then its k would increase at a constant rate (eE 0 /h¯ ) until the value π/a is reached, and then it would reenter the ﬁrst BZ at k = − π/a and continue this cycle. The same picture would hold for a few electrons initially occupying the bottom of the band. (2) If the band were completely full, then all the wavevectors would be changing in the same way, and all states would remain completely full. Since this creates no change in the system, we conclude that no current would ﬂow: a full band cannot contribute to current ﬂow in an ideal crystal! (3) If the band were mostly full, with only a few states empty at wavevectors near the boundaries of the ﬁrst BZ (at k = ´ π/a) where the energy is a maximum, then the total current would be:
I=
−e
± k≤kF
v(k )
= −e
± p (k ) k≤kF
me
⎡
xˆ = ⎣−e
± p(k ) k∈ BZ
me
+e
⎤ ± p (k ) ⎦
k >kF
me
xˆ = e
± p (k ) k >kF
me
xˆ
where, in the ﬁrst two sums, the summation is over k values in the ﬁrst BZ, restricted to k ≤ k F , that is, over occupied states only, whereas in the last sum it is restricted over k > k F , that is, over unoccupied states only. The last equality follows from the fact that the sum over all values of k ∈ BZ corresponds to the full band, which as explained above does not contribute to the current. Thus, in this case the system behaves like a set of positively charged particles (holes) corresponding to the unoccupied states near the top of the band. In our simple 1D example we can use the general expression for the effective mass derived in Eq. (2.51), to ﬁnd:
438
9
1 m
=
Dynamics and Topological Constraints
1 d2 ±k h¯ 2 dk 2
⎛º » 2 d ± k ⇒ m = h¯ 2 ⎝ 2 dk
⎞−1 ⎠
k =´π/a
2 = 2τh¯ a 2
(9.19)
which is a negative quantity (recall that τ < 0). Using the Taylor expansion of the cosine function near k 0 = ´ π/ a, we can write the energy near the top of the band as:
µ
´
´
+
± (π/a) k
= ± + 2τ −1 + 21 (ka )2 + · · =· (± − 2τ ) + τ a 2k 2 = (± − 2τ ) + h¯2mk
2 2
(9.20)
with the effective mass m being the negative quantity found in Eq. (9.19). From the general expression Eq. (9.19), we ﬁnd the time derivative of the current in our 1D example to be: dI dt
=e
± 1 dp(k ) k>kF
me
dt
xˆ = e
± d ¶1 d
k >kF
dt
¯
h dk
·
±k
xˆ =
e m
± dk
¯ dt xˆ
h
k>k F
where we have used Eq. (2.50) to obtain the second equality and Eq. (9.20) to obtain the third equality. Now, assuming that we are dealing with a singlehole state at the top of the band, and using the general result of Eq. (9.17), we obtain dI dt
= e mF
which is simply Newton’s equation of motion for a positively charged particle of charge +e with negative effective mass m to an external force F.
9.3
TimeReversal Invariance
So far we have treated time as a new variable, separate from the other degrees of freedom of the hamiltonian. In the most general case, the hamiltonian can also contain a time dependence, usually due to the time dependence of external ﬁelds (like the electromagnetic ﬁeld). When the hamiltonian is time independent, there is a deep and important symmetry that governs the behavior of electrons, the timereversal symmetry. We brieﬂy touched upon this in our discussion of symmetries of the band structure for crystal electrons, when the spin degree of freedom is not explicitly taken into account (see Chapter 3). Since time is a variable of central importance in dynamics, we revisit the issue of timereversal symmetry in a more careful manner. This is accomplished by working with the Dirac equation that treats the wavefunctions as spinors, that is, it includes the spin degree of freedom explicitly. We consider the state of a particle with spin s , described by its wavefunction ψs (r, t ), where s is the spin. We will specialize the discussion to particles with spin s = 1/2, since this is the case relevant to electrons. A more detailed discussion of the Dirac equation for spin1/2 particles is provided in Appendix C (see Section C.8), including the deﬁnition of Pauli matrices, Eq. (C.43), that are used in the following discussion.
439
9.3
TimeReversal Invariance
We seek to deﬁne the timereversal operator Tˆ such that when it is applied to an eigenstate ψs (r, t) of the hamiltonian Hˆ it produces a state ψ˜ (r, −t ) with the time direction inverted (t → −t) and a new spin value denoted ˜s , which is also a solution of the Dirac equation. The fact that time reversal of the state ψs (r, t) produces another solution of the Dirac equation is a consequence of the fact that the hamiltonian appearing in the Dirac equation, Eq. (C.69), has no explicit time dependence. Our strategy will be to ﬁrst work out the conditions that this operator must satisfy, then guess its form and prove that this form works. From the deﬁnition of the operator we have:
ˆ
T ψs (r, t)
= ψ˜ ˜s(r, −t)
such that ih¯
∂ ψs ∂t
ˆ s ⇒ ih¯ ∂ ψ˜ s˜ = Hˆ ψ˜ s˜ = Hψ ∂t
(9.21)
We next consider the inverse of the timereversal operator Tˆ −1 , and use it to undo the effect of time reversal, that is, to restore the direction of time:
ˆ −1ψ˜ ˜s(r, −t ) = Tˆ −1 Tˆ ψs(r, t ) = ψs(r, t )
T
and
ˆ −1 ∂ ψ˜ ˜s = −∂ Tˆ −1ψ˜ s˜ = −∂ ψs ∂t ∂t ∂t
T
We will use these relations in ﬁguring out how the inverse of the timereversal operator should affect the Dirac equation for the state ψ˜ ˜s : we apply Tˆ −1 to the equation for ψ˜ ˜s and insert the product Tˆ Tˆ −1 = 1 between the factor (ih¯ ) and the time derivative of ψ˜ ˜s on the lefthand side of the Dirac equation, and between the hamiltonian and ψ˜ on the righthand side. The result is:
ˆ −1 (ih¯ )Tˆ Tˆ −1 ∂ ψ˜ s˜ = Tˆ −1Hˆ Tˆ Tˆ −1ψ˜ ˜s ⇒ −Tˆ −1(ih¯ )Tˆ ∂ ψs = Tˆ −1Hˆ Tˆ ψs ∂t ∂t
T
(9.22)
where we have used the relations derived earlier. If Tˆ is indeed the right operator for time reversal, then Eqs (9.21) and (9.22) must be compatible, that is, we must have:
− Tˆ −1(i h¯ )Tˆ = ih¯
and
ˆ −1 Hˆ Tˆ = Hˆ
T
(9.23)
An expression that satisﬁes these conditions is given by:
ˆ = SCˆ,
T
S=i
¶
σy
0
0 σy
·
ˆ = complex
,
C
conjugation
(9.24)
where σy is one of the Pauli spin matrices [see Appendix C, Eq. (C.43)]. This expression for Tˆ and the properties of the Pauli matrices prove that the two conditions above are satisﬁed (the reader is guided through this proof by the steps of Problem 2). We emphasize that this choice is not unique, because multiplying the operator by an arbitrary phase factor exp(iθ ) gives a valid timereversal operator. For example, another convenient choice for the timereversal operator is:
ˆ = exp
T
(see Problem 3).
²
³
i SCˆ 2 π
(9.25)
440
9
Dynamics and Topological Constraints
9.3.1
Kramers Degeneracy
We will next consider the implications of time reversal for a state which is composed of a stationary and a timedependent part, with the stationary part being identiﬁed by its momentum p = h¯ k and its spin s . The proof that Tˆ is a proper timereversal operator also shows that it commutes with the hamiltonian:
ˆ −1 Hˆ Tˆ = Hˆ ⇒ Hˆ Tˆ = Tˆ Hˆ
T
which means that if the state ψk,s (r) is a stationary eigenstate of the hamiltonian with energy eigenvalue ±k,s then its timereversed partner Tˆ ψk ,s (r, t) will also be an eigenstate with the same eigenvalue:
ˆ
ˆ k,s = ±k,sTˆ ψk,s ⇒ Hˆ (Tˆ ψk,s) = ±k,s(Tˆ ψk,s) = ±k,sψk,s ⇒ Tˆ Hψ Now we denote as k˜ and s˜ the momentum and spin labels of the stationary part in the timereversed state ψ˜ ; these are quantities whose values we will need to ﬁgure out. With these Hψk,s
deﬁnitions, the above relation takes the form
ˆ ˜ ˜ ˜ = ±k,sψ˜ k˜ ,s˜ Since we know the form of the operator Tˆ , we can determine how the stationary part of the Hψk,s
state is affected by time reversal. Speciﬁcally, the timereversed state will have the opposite momentum k˜ = − k , since the momentum operator changes sign under Tˆ . Moreover, from the form of the matrix S in the expression for Tˆ , we conclude that the spin of the original state must be ﬂipped in the timereversed state (recall that our assumption at the beginning of the section was that we are dealing with spin1/2 particles). In the following we will use the notation ↑ and ↓ to denote states whose expectation value µσ z ¶ of the Pauli spin matrix σ z is either positive or negative, respectively. We emphasize that in the presence of terms in the hamiltonian that include the spin operator, like the spin–orbit coupling term, the eigenfunctions can no longer be described in terms of the up or downspin states. These considerations establish that if the original stationary state has labels k and ↑ for the momentum and the spin, the corresponding stationary part in the timereversed state will have labels −k and ↓, that is, the energies and stationary parts of the two wavefunctions will be related by:
− ↓ = ±k ,↑ ,
± k,
− ↓ (r) = i σy ψk∗,↑ (r)
ψ k,
(9.26)
These relations are known as “Kramers degeneracy” for particles with spin 1/2.
9.4
Berry’s Phase
The discussion so far is missing a key ingredient, which is the arbitrary phase ϕ that can multiply a system’s wavefunction ψ ¶, without changing the expectation value of any operator Oˆ that corresponds to a physical observable:
ψ ¶ →ψ˜ ¶ =ei ψ ¶ ⇒ ψµOˆ ψ ¶ = ψ˜ µOˆ ψ˜ ¶ ϕ
441
9.4
Berry’s Phase
This holds because the action of the operator Oˆ does not affect the phase factor eiϕ , which is just a constant complex number of magnitude 1. It turns out that there exist physical observables that cannot be described by the expectation value of any operator; the arbitrary phase can play a key role in the description of such observables. This can occur when the system has a parametric dependence in its hamiltonian. In this case, the phase is often referred to as the “geometric” phase, since it describes the dependence of the wavefunction on parameters related to geometric features of the system. We encountered one such general example in the discussion of the Born–Oppenheimer approximation in Chapter 4. We note that in a truly isolated system, where the hamiltonian is not a function of some parametric variable, Berry’s phase is not obtained. 9.4.1
General Formulation
To deﬁne Berry’s phase in a general context, let us deﬁne a generic parametric hamiltonian such that:
ˆ  ¶ =±qψq¶
H(q ) ψq
where q is some parameter. At this point we leave the nature of the parameter q intentionally undeﬁned, because as we will see later, it can be associated with different features of the system.11 When solving the Schr¨odinger equation for the wavefunction of a system, either analytically or numerically, an arbitrary phase ϕ appears in the form eiϕ ; we assume we are dealing with the system in its ground state. When ﬁnding an analytic solution, we may choose the simplest mathematical expression for the wavefunction, but this implies choosing the value of this phase to be zero; when calculating a numerical solution, the algorithm we use typically selects a random value for this phase, which is not set by the differential equation. Suppose that this phase for two different ground states of the system, identiﬁed by different values of the geometric parameter q , takes the values ϕ1 and ϕ2 for the values of the parameter q1 and q2 . Next, suppose that we wish to explicitly remove the phase ϕ for each case, so we would multiply the ﬁrst wavefunction by e−iϕ 1 and the second by e−iϕ 2 :
ψq ¶ → ψ˜ q ¶ =e−i ψq ¶, ψq ¶ →ψ˜ q ¶ =e−i ψq ¶ 1
ϕ1
1
2
2
1
ϕ2
2
a process which is called “choosing a gauge.” Then the overlap of the two phasecorrected wavefunctions would be:
µψ˜ q ψ˜ q ¶ =ei( 1
2
ϕ1
−ϕ2) µψq
 ¶
1 ψ q2
But since in this last expression we have removed all arbitrary phase dependence, the lefthand side of the equation must be the magnitude of the overlap, µψq 1 ψq2 ¶, which gives a useful way of deﬁning the relative phase ³ϕ12 = (ϕ1 − ϕ2 ) as: e−i³ϕ12
= µµψψq ψψq ¶¶ 1
2
q1
q2
(9.27)
11 The discussion in this section follows closely the treatment in the review articles by R. Resta and by D. Xiao,
M.C. Chang, and Q. Niu (see Further Reading).
442
9
Dynamics and Topological Constraints
By separating real and imaginary parts in the above deﬁnition, we can obtain an alternative way for expressing the relative phase as:
= −Im
³ϕ12
Ã (
)Ä
µψq ψq ¶
ln
1
(9.28)
2
In the limit of small difference ³ q between q 1 and q2 , which corresponds to a change ³ϕ in phase, the above expressions become: e−i³ϕ
= µµψψqψψq+ q¶¶ ⇒ −i³ϕ ≈ ψµ q ∇qψq ¶ ³· q q q+ q ³
(9.29)
³
where we have assumed that our choice of gauge ensures a differentiable phase and we have kept the leadingorder terms in the Taylor expansion of both sides. For inﬁnitesimal changes dq , the inﬁnitesimal change in the phase becomes: dϕ = iµψq ∇q ψq ¶ d· q
(9.30)
With this last expression, we can now calculate the total change in phase, that is, Berry’s phase γ , along a closed path C in the space of the parameter q : γ
¿
=
C
dϕ = i
¿
C
µψq∇q ψq ¶ d· q
(9.31)
The interesting property of γ is that it is gauge invariant . To show this explicitly, we consider a new wavefunction  ψ˜ q ¶ that involves a gauge transformation by a phase ϕ(q ) which is a continuous differentiable function of the variable q :
ψ˜ q ¶ =e−i (q) ψq¶
(9.32)
ϕ
Differentiating with q we obtain
Ã
Ä
∇q ψ˜ q¶ = −i∇qϕ(q) ψ˜ q ¶ +e−i
ϕ (q)
Ã
∇qψq¶
Ä
and using this result to calculate the Berry phase for the new wavefunction we ﬁnd:
¿
¿
¿
˜ = i µψ˜ q∇qψ˜ q¶ d· q = i µψ˜ qe−i (q)∇qψq¶ d· q + ∇qϕ(q) · dq = γ
γ
ϕ
C
C
C
since from the deﬁnition of  ψ˜ q ¶ we have:
µψ˜ q = ψµqei (q) ⇒ ψµ˜ qe−i (q) ∇q ψq¶ = ψµq∇q ψq¶ and the integral of ∇q ϕ(q) over a closed loop vanishes identically. ϕ
ϕ
A different way of establishing gauge invariance is by using the expression of Eq. (9.28), and splitting the closed path into N inﬁnitesimal intervals of size dq starting at q 0 and ending at qN+1 = q 0, with q i+1 = q i + dq (we are assuming the limit N → ∞is properly deﬁned). The result becomes: ³ϕ
= −Im
º
» )
N ± ( i=0
ln
µψq ψq + ¶ = −Im i
i 1
º À ln
N Â i= 0
µψq ψq + ¶ i
Á»
i 1
In the last expression, if we were to introduce a gauge transformation of the type given in Eq. (9.32), the phases cancel between successive steps because they arise from bras
443
9.4
Berry’s Phase
and kets with the same index, and the phases at the initial and ﬁnal points of the path are the same so they also cancel; thus, the whole expression is gauge invariant. This is in contrast to the value of the integrand in Eq. (9.31), which is gauge dependent. The fact that γ is gauge invariant is crucial; otherwise, there would be no hope of relating it to a physical observable. The value of γ actually depends on the path we choose for the contour integration, as is evident from the discussion of the Aharonov–Bohm effect presented in Section 9.5. In the following, we shall encounter several cases where the parameter q is a real (as opposed to complex) 3D vector, as this is the most usual situation for application of these concepts. In this case, the expressions above naturally lead to two new quantities. The ﬁrst is the integrand of Eq. (9.31) itself, called “Berry connection”: A(q)
= iµψq∇ qψq ¶
(9.33)
which is a threecomponent vector. The second is an antisymmetric secondrank tensor, called “Berry curvature”: µαβ (q)
∂ Aβ (q)
=
∂qα
− ∂ A∂ q (q) α
(9.34)
β
´
µ
= i µ ∂∂ψq q  ∂∂ψq q ¶ − ∂∂ψµq q  ∂∂ψq q ¶ = −2 Im µ ∂∂ψq q  ∂∂ψq q ¶ α
β
β
α
α
β
Since we are working with threecomponent vectors, we can associate the elements of the secondrank tensor µαβ with the components of a vector ± by the cyclic permutations of the indices, for instance, in cartesian coordinates µxy would be the ˆz component of ±, and so on (this is formally known as “using the Levi–Civita antisymmetric tensor ±αβ γ ” in the relation µαβ = ±αβ γ µγ ). This allows us to write the vector ± as the curl of the vector A, leading to the expression ±(q)
= ∇q × A(q)
(9.35)
These deﬁnitions simplify the expression for Berry’s phase, which becomes: γ
=
¿ C
A(q )
· dq =
¾
S
∇q × A(q) · dS =
¾
S
±(q)
· dS
(9.36)
where S is the surface enclosed by the curve C and dS is the inﬁnitesimal element on it with the surface unit vector pointing in the direction determined by the righthand rule, given the direction in which C is traversed. The second expression for γ in Eq. (9.36) is obtained from the ﬁrst using Stokes’ theorem [see Appendix A, Eq. (A.23)] and justiﬁes the name “Berry curvature” for µ. These expressions are interesting not only for their formal simplicity and elegance, but also because they are related to familiar physical quantities and have an important manifestation, as we describe next. An alternate way for calculating Berry’s phase, expressed as a surface integral of the Berry curvature, Eq. (9.36), is the following. From perturbation theory, and introducing superscripts to identify the ground state. ψq(0) , ±q(0) and excited states ψq(n) , ±q(n) of the
444
9
Dynamics and Topological Constraints
system, we have: (0) (n ) (0) ± ˆ  ∂∂ψqq ¶ = ψ (n) ¶ µψq ∂(0)Hq/∂ q(n)ψq ¶ ± q − ±q n¸=0 α
α
and from this, the Berry curvature takes the form µαβ (q)
⎡ ⎤ (0) ( n ) ( n ) (0) ± ˆ ˆ −2 Im ⎢⎣ µψq ∂ Hq/∂ qα¸ψq ¶µψq ¹2∂ Hq/∂ q β ψq ¶ ⎥⎦
=
(0) ±q
n¸=0
−
(n ) ±q
(9.37)
This expression has the advantage that we do not need to calculate derivatives of the (n ) wavefunctions ψq with respect to components of q; the derivatives apply only to the hamiltonian Hˆ q . Its disadvantage is that it involves a sum over all excited states.
Example 9.2 Berry’s phase for spin in a magnetic monopole ﬁeld A useful model for illustrating the notions of Berry curvature and Berry’s phase consists of a spin interacting with a magnetic monopole (referred to as the “Dirac monopole”) ﬁeld. We consider a spin S = S σ situated at r, where σ is the usual vector with components the Pauli matrices, σ = σx ˆx + σy yˆ + σz zˆ. The Dirac monopole of magnitude M situated at the origin produces a magnetic ﬁeld at the position r given by: B=
M r3
r=
M r2
ˆr
with rˆ the unit vector in the radial direction and r =r the distance from the origin which we will take to be ﬁxed. The interaction hamiltonian is:
ˆ = B · S = M3 r · (S σ ) = h · σ ,
H
r
h = ±0 rˆ,
±0
= MS r2
(9.38)
with ±0 a constant expressed in terms of the parameters M , S, and r of the model. Although this system is hypothetical, it serves as a simple prototypical model because the hamiltonians of other physically motivated models are equivalent to it. The components of r in terms of the polar and azimuthal angles θ , φ are given by: x
= r sin(θ ) cos(φ), y = r sin(θ ) sin(φ), z = r cos(θ )
as illustrated in Fig. 9.11. This leads to the hamiltonian
ˆ = h · σ = ±0 Ãσx sin(θ ) cos(φ ) + σy sin(θ ) sin(φ) + σz cos(θ )Ä
Hω
which depends on two variables, θ and φ, collectively denoted as the twocomponent vector ω = (θ , φ). The two eigenvalues of this hamiltonian are: (1)
±ω
= −±0,
(2)
±ω
= ±0
(9.39)
445
9.4
Berry’s Phase
z
S r
C
r M
y
x
Fig. 9.11
The position vector r (red arrow) appearing in the ﬁeld of the Dirac monopole M situated at the origin, to illustrate the calculation of Berry’s phase in a system with two independent variables, the polar angle θ and the azimuthal angle φ . The horizontal circle (constant latitude, θ ) C , shown in blue, is the closed path around which the spin S (green arrow) is moved.
and the corresponding eigenfunctions are:
¶
−i φ ·
θ /2)e ψ (1)¶ = sin( − cos(θ /2) ω
¶
,
ψ (2)¶ = ω
cos(θ /2) sin(θ /2)ei φ
· (9.40)
as can easily be checked. The two wavefunctions are orthogonal:
¶
− iφ ·† ¶ cos(θ /2) ·
θ /2)e µψ (1)ψ (2)¶ = sin( − cos(θ /2) ω
·
ω
sin(θ /2)ei φ
=0
where (·)† stands for the hermitian conjugate, that is, the conjugate transpose of (·). They are also properly normalized:
µψ (1) ψ (1)¶ = ψµ(2)ψ (2)¶ =1 We note that when the spin is at the North pole, θ = 0, the two wavefunctions become: ω
ω
ω
¶
ψ0(1)¶ = −01
¶ ·
·
,
ψ0(2)¶ =
conversely, when the spin is at the South pole, θ
¶ −iφ · e
ψ ¶ = (1)
π
0
ω
,
1 0
= π , the two wavefunctions become: ¶
ψ ¶ = (2)
π
0 eiφ
·
but these are not well deﬁned because φ can have any value in the interval [0, 2π ), for the same position of the spin , which means the wavefunctions are multiply valued; we conclude that the South pole is a singular point. We can now imagine that the spin is moved around a horizontal (constantlatitude) circle, which means θ is ﬁxed and φ ∈ [0, 2 π ), and ask what is Berry’s phase for this change in position. We will discuss only the ground state ψω(1) ¶. We calculate ﬁrst the Berry connection components:
446
9
(1)
Aθ
(1)
Aφ
Dynamics and Topological Constraints
¶
(θ , φ ) = iµψω
 ∂ θ ψ ¶ =i
(θ , φ ) = iµψω
 ∂ φ ψ ¶ =i
(1) ∂
(1)
ω
(1) ∂
(1)
¶
sin(θ /2)e−iφ − cos(θ /2)
sin(θ / 2)e−iφ − cos(θ / 2)
ω
θ) = 1 − cos( 2
·† ¶ 1
·
·† ¶
2
cos( θ /2)e−iφ 1 2 sin(θ /2)
−i · −i sin(θ0/2)e
·
φ
=0
·
From these we can also calculate the Berry curvature: (1)
µθ φ (θ , φ)
=
(1)
∂ Aφ
(1)
− ∂ A∂ φ = 12 sin(θ )
(9.41)
θ
∂θ
We can calculate Berry’s phase in two ways. First, we use the Berry connection integrated over the closed path around the horizontal circle C (see Fig. 9.11), with the variable of integration denoted by ω³ = (θ , φ ³ ), so that the path C is described by dω ³ = φˆ dφ ³, with φ³ ∈ [0, 2π ): γ
(1)
(θ ) =
¿
C
A
(1)
(ω³ ) · dω ³
=
¾
0
2π
(1)
Aφ
(θ , φ ³ )dφ ³
= π (1 − cos(θ ))
Second, we the Berry curvature, integrated over the surface enclosed by the circle C , that is, the part of the sphere north of the horizontal circle in which the wavefunction is well deﬁned. This gives: γ
(1)
(θ )
=
¾
2π
dφ ³
0
¾
θ
0
(1)
µθ φ (θ
³ , φ³ )dθ ³ = 2π
¾ 0
θ
1 sin(θ ³ )dθ ³ 2
= π (1 − cos(θ ))
If we let θ → π (without actually acquiring this value because the wavefunction there is not properly deﬁned), we ﬁnd that the integral of the Berry curvature over the entire sphere becomes:
¾ 0
2π
d φ³
¾ 0
π
(1)
µθ φ (θ
³, φ³ )dθ ³ = lim [π (1 − cos( θ ))] = 2π θ →π
that is, it becomes an integral multiple of 2π . This is related to the ﬁrst Chern number for this state, a topic we discuss in more detail below (see also Problem 4).
9.4.2
Berry’s Phase for Electrons in Crystals
We turn next to electrons in a crystal and the manifestations of Berry’s phase in this physical system. We have seen in Section 9.2 that it is convenient to deal with the system (n) in terms of the wavefunctions u k ¶ which have full translational periodicity, rather than (n) (n ) the true Bloch states  ψk ¶. The hamiltonian that applies to the states  uk ¶ is:
ˆ
Hk (p,
r)
= 2m1 [−i h¯ ∇r + h¯ k]2 + V(r) e
447
9.4
Berry’s Phase
to which we will later add the electric ﬁeld as an external perturbation. We calculate ﬁrst the Berry curvature for this system. The parameter that characterizes the hamiltonian and the states is evidently k , the wavevector. With the deﬁnitions introduced above, the Berry connection and Berry curvature for the n th band are given by: A
±
(n) (n)
(k) (k)
= iµ ∇ (n ) uk
(n ) ku k
¶ ⇒µ
(n ) αβ
(k ) = i
º
(n)
(n)
∂uk
∂uk
α
β
(n )
∂ uk
(n )
∂ uk
µ ∂ k  ∂ k ¶ − ∂µk  ∂ k ¶ β
= iµ∇ku (kn)  × k∇u (kn)¶
»
(9.42)
α
(9.43)
and the expression for Berry’s phase takes the form γ
(n )
=
¿
C
iµu(kn)∇k u(kn) ¶ d· k
(9.44)
where the closed path C is in the space of wavevectors k, that is, the BZ of the crystal. A closed path can also be realized by moving from one point in k space to the point k + G, where G is a reciprocal lattice vector, since the two points are then equivalent, as we have seen earlier (see the discussion in Chapter 2). In this case, γ is known as “Zak’s phase.” 12 All the quantities deﬁned so far are intrinsic properties of the band structure as they depend exclusively on the band wavefunctions. A closed path C is required to obtain Berry’s phase (n ) γ (n), but is not necessary in the deﬁnition of the Berry curvature ± (k ), which is a gaugeinvariant quantity. We will see some manifestations of this in the following. A related important issue is what happens when the hamiltonian acquires a time dependence due to a term that does not destroy the translational periodicity of the crystal. We seek a general result that will not depend on the nature of the perturbation, so it can be applied in any situation. For a sufﬁciently weak perturbation, we can still use the original wavefunctions as the basis to express the new states that are perturbed by a small amount. We use a Taylor expansion for the perturbed states:
˜ ¶ =  ¶ +  ¶ =  ¶ +δt (n ) uk
(n ) uk
(n ) δ uk
(n ) uk
(n )
∂ uk ∂t
¶
and then develop a way to express them in terms of the unperturbed ones. One perspective is to use perturbation theory (see Appendix C) and consider the time derivative of the hamiltonian as the perturbation itself. Another perspective is to start with the timedependent Schr¨odinger equation (see Appendix C) and take the time derivative to be the ratio of the small differences δψ = ψ (t) − ψ (t0 ) and δ t = t − t0 , which leads to the identiﬁcation of the small time interval δ t with the inverse of the hamiltonian operator, shifted by the energy of the unperturbed state, and multiplied by ih¯ . From either approach we arrive at the general expression for the perturbation of the wavefunction that involves an expansion over the unperturbed states: δ
±  u(km )¶µu (km)  ∂ u (kn)
u(kn) ¶ = i−h¯
12 J. Zak, Phys. Rev. Lett. 62 , 2747 (1989).
(n ) m¸=n ± k
− ±k(m)

∂t
¶
448
9
Dynamics and Topological Constraints
With this, we calculate the expectation of the velocity operator, Eq. (9.14), in the perturbed states to obtain, for the velocity:
±
µv(kn)¶ =h µu (kn) ∇kHˆ ku (kn)¶ −i ¯ m ¸=n 1
º
µu(kn) ∇kHˆ ku (km) ¶µu k(m)∂ u(kn) /∂ t ¶ − c.c. (n ) (m) ±k − ±k
»
(9.45)
with c.c. standing for the complex conjugate. The ﬁrst term in this expression was worked out in the previous section, where we found that it is equal to the result of Eq. (9.15). For the second term, we follow the same steps of the derivation that led to Eq. (9.15) together with the orthogonality of the wavefunctions u (kn) ¶ and the completeness of this basis (see Problem 5), and we write the derivative with respect to k in the equivalent notation ∇k = ∂/∂ k to arrive at the following expression for the velocity: 1
µ ¶ =h ∇ ¯ v(kn)
º
(n ) k ±k
−i µ
(n)
∂uk
∂k

(n)
∂uk ∂t
(n )
∂ uk
¶ − ∂µ t 
(n )
∂ uk
∂k
¶
»
(9.46)
In the second term of this expression we recognize a quantity that has the same structure as the Berry curvature of the band, but is now expressed with respect to the two independent parameters k and t. This is an important result with several consequences that we explore further in the next section.
Example 9.3 Berry’s phase for the 2D honeycomb lattice We revisit the 2D honeycomb lattice, discussed in Chapter 2, to apply the concepts developed so far; recall that this example is actually relevant to a real physical system, graphene (that is, a single plane of threefold sp 2bonded C atoms). In the 2D honeycomb lattice, there are two sites per unit cell, labeled A and B , each forming a 2D hexagonal sublattice, with realspace lattice vectors a1 , a2: a1
= (a /2)
¸√
¹
3xˆ + y ˆ , a2
= (a /2)
¸√
¹
3xˆ − y ˆ
(9.47)
The two sites can be equivalent as in graphene, corresponding to two identical C atoms, or inequivalent as in hBN, corresponding to the B and N atoms. We already investigated the model for equivalent A and B sites, at the level of the tightbinding hamiltonian with nearestneighbor hopping matrix elements in Chapter 2. To include inequivalent sites in the model, at the same level of tightbinding treatment, we need to make the onsite energies different, say ±A ¸= ±B . We can then deﬁne:
¯ = ±A +2 ±B , V0 = ±A −2 ±B ⇒ ±A = ± ¯+ V0, ±B = ± ¯− V0 and set ±¯ = 0, since this is the same as a constant shift of all the energy values which ±
does not affect the physics. This leaves a hamiltonian with diagonal matrix elements V0 and −V0, a variation of the graphene model (this model was introduced by M. J. Rice and E. J. Melea). This model amounts to breaking the inversion symmetry,
449
9.4
Berry’s Phase
3 2
A
) t( ygrenE
a1 B
a2
1 0
1 2 3 0
Fig. 9.12
0.5
1
1.5
2
k
2.5
3
Left: The honeycomb lattice with the primitive lattice vectors a1 , a2 (red arrows) and the primitive unit cell highlighted in blue; the sites A and B can be inequivalent, when the onsite energies ±A ¸= ±B . The black lines indicate the nearestneighbor hopping matrix elements of strength tπ . Right: The corresponding band structure, in solid lines, along the highsymmetry directions of the BZ; the model parameters are V0 = 0.5tπ , leading to ±gap ( K ) = 2V 0 = tπ . The band structure of the lattice with inversion symmetry is shown in dashed lines for comparison.
also referred to as P symmetry, of the honeycomb lattice for V0 ¸= 0, as illustrated in Fig. 9.12. For this case, we have chosen the unit cell to be a rhombus, and the origin of the coordinate system to be at the midpoint of the nearestneighbor distance between sites A and B . This choice of origin demonstrates the inversion symmetry of the lattice if the two sites are equivalent, which is broken for the case of inequivalent sites. (a different choice of origin that demonstrates the inversion symmetry is the center of the hexagon formed by the atoms, that is, a corner of the blueshaded rhombus in Fig. 9.12). We had found that the tightbinding hamiltonian for graphene is given by [see Eq. (2.86)]:
ˆk = H
¶
±p
tπ fk
tπ fk∗ ±p
·
, fk
²
= 1 + eik· a + eik· a 1
2
³
With the addition of the symmetrybreaking diagonal terms, after setting hamiltonian can be written in the more compact form
ˆk = H
¶
t π f k∗
±p
= 0, the
·
(9.48) −V0 = h( k) · σ = h x (k)σx + h y (k)σ y + h z(k) σz where σ = σx xˆ +σ yyˆ + σz ˆz with σx , σy , σz the Pauli spin matrices, and we have deﬁned V0
tπ fk
the vector operator h(k) with components
≡t h y (k) ≡ t
h x (k)
π π
[1 + cos(k · a1 ) + cos(k · a2 )],
[sin(k · a1) + sin(k · a2)], h z (k ) ≡ V0
The band structures for both the case with inversion symmetry (V0 broken inversion symmetry (V0 ¸= 0) are shown in Fig. 9.12.
= 0) and with
450
9
Dynamics and Topological Constraints
We investigate ﬁrst the solution of this hamiltonian for V0 eigenvalues and corresponding eigenfunctions are given by:
¶ ∗ · fk / fk 
1 = −t f k, u (1) k ¶ =√
(1)
±k
π
(2)
±k
1 = t f k, u (2) k ¶ =√ π
= 0. For this case, the
−1
2¶
1
·
 
fk / fk
2
Using these, we can calculate the Berry curvature for this model. The components of the Berry connection for the ﬁrst state are given by: (1)
Aj
(k ) = iµuk
(1)
¸
1  ∂∂k u (1) k ¶ = − 2 2f k  j
with the deﬁnitions A k ,j
≡
¸
a 1,j eik ·a1
A k,j fk∗
+ a2,j eik·a
2
¹
+ A ∗k,jf k , j
¹
, j = x, y
(9.49)
= x, y
From these, we ﬁnd that the Berry curvature (1)
µk k ( k) x y
(1)
(1)
x
y
= ∂ A∂yk (k) − ∂ A∂xk (k)
vanishes identically as long as the expressions for the Berry connection are analytic. These expressions are analytic everywhere except when fk = 0, which happens at the six corners of the BZ, labeled K, K³ , see Fig. 9.13. When these points are excluded from a closed path of integration around the BZ boundary, the contribution of remaining straight lines along the boundary is zero, because the portions on opposite sides of the hexagon are traversed in opposite directions and are equivalent by symmetry (they are related by reciprocalspace vectors). Thus, we only need to calculate the contribution of these points. We deﬁne the coordinates of the representative points K and K³ as:
K=
2π a
¶
1
√ xˆ + 3
·
1 yˆ , K³ 3
= −K
with each one having two other equivalent points by symmetry (related by reciprocalspace vectors), as shown in Fig. 9.13. Next, we expand in Taylor series around these points, k = K + q or k ³ = K³ − q = − (K + q) = − k with q →0, identiﬁed by the blue arrows in Fig. 9.13. We treat the case of k near K ﬁrst, which leads to the hamiltonian √ ˆHK+q = h(q) · σ , h(q) = ei φ˜ 3at π (h¯ q) 2h¯ where we have explicitly included the hopping matrix element t π and factors of h¯ , to make the connection to the Dirac equation. We have also included a phase factor, exp[iφ˜ ], where φ˜ depends on the arbitrary choice of cartesian coordinate axes, used to express the lattice vectors. However, this phase does not affect the physics: it does not enter into the expression for the energy eigenvalues and only introduces
451
Fig. 9.13
9.4
Berry’s Phase
Brillouin zone of the 2D honeycomb lattice, with the highsymmetry points ¶ , K, K³ , M identiﬁed. The thick black lines and small circular arcs subtending an angle of 2π/3 each indicate the integration path around the BZ boundary that avoids the singularities at the corners. The green arrows indicate reciprocal lattice vectors ´b1 and ´(b1 + b2 ) (horizontal arrows) for displacement of the circular arcs to complete a circle around a single K or K³ point. The arbitrary point in the neighborhood of K or K³ is denoted by the vectors k, k³ .
a constant phase in the wavefunctions, so we can safely ignore it in the rest of the discussion; this is simply equivalent to rotating the cartesian axes by an angle that sets φ˜ = 0, which leaves all dot products invariant. Since h¯ q has the dimensions of momentum, the above hamiltonian is exactly equivalent to the Dirac hamiltonian for massless particles (see Appendix C, section C.8), the only difference being that here the equivalent of the “speed of light” is the expression vF
=
√
3at π 2h¯
that is, the Fermi velocity of the particles at these points in the BZ. Near the point K, the quantities that appear in the wavefunctions u (ki )¶, i = 1, 2, take the form fK+q
=
√
3a (qx 2
+ iq y ),
√ fK+q = 23a q
We switch to spherical coordinates for the vector q:
Ã
q = q  sin(θ ) cos(φ )xˆ + sin(θ ) sin( φ)yˆ
Ä
+ cos(θ )zˆ
in which we must set θ = π/2, since q is a vector on the ( qx , q y ) plane. This leads to the following expressions for the eigenvalues and eigenfunctions near the corners of the BZ:
452
9
Dynamics and Topological Constraints
= −h¯v Fq, 
(1) ± K+q
(1) u K+q
(2)
+
±K q
¶ −iφ · e
1
¶ =√
2
1 = h¯v F q, u (2) K+ q ¶ =√
2
¶
−1
1 ei φ
·
Both eigenvalues are linear in the magnitude of q , that is, they correspond to the Dirac cones at the corners of the BZ, as discussed in Chapter 2. As far as the eigenfunctions are concerned, these are exactly the solutions for the spin in the monopole ﬁeld that we found in the previous example, when we set in those expressions θ
= π2 ⇒ sin (θ /2) = cos (θ /2) = √1
2
due to the 2D nature of the vector q. Thus, for the case of V0 = 0, the energy– momentum dispersion relation of the two solutions is linear in q  and the eigenfunctions correspond to the solutions of the spin in a monopole ﬁeld constrained to the equator of the sphere. With this approach we have solved the problem of analyticity of the wavefunctions near the points K and K³ . We can now perform the integration around the whole path shown in Fig. 9.13, including the six circular arcs that avoid the corners of the BZ and take the limit q  →0. By translational periodicity in reciprocal space, the six circular arcs combine to make a full circle around one of the three equivalent K points and another full circle around one of the three equivalent K³ points, since each arc subtends an angle of 2π/3 (see Fig. 9.13). We can also directly borrow the results we derived for the Berry connection of a spin in a monopole ﬁeld: 1 2 where we have used θ = π/2, and then integrate over a full circle of radius q  in reciprocal space around the point K, denoted as C (K), to obtain: (1)
Aθ
(π/ 2, φ ) = 0,
¿
C(K)
A
(1)
(1)
Aφ
(ω ) · dω
=
(π/2, φ ) = sin2 (π/4) =
¾
2π
(1)
Aφ
0
(π/2, φ )dφ =
π
The result for the integration around a full circle centered at K³ , denoted as C (K³ ), gives the opposite result:
¿
C(K³ )
A
(1)
(ω) · dω =
¾
−
0
2π
(1)
Aφ
(π/2, φ )dφ =
−π
so adding these two contributions we get as ﬁnal answer a zero value for Berry’s phase. We next solve the model in which V0 is not zero, starting again with the hamiltonian of Eq. (9.48); we will take V0 > 0 for the moment, and mention the case V0 < 0 at the end of the discussion. The two eigenvalues of the hamiltonian are: (1)
±k
Å
= − t2 fk 2 + V02, π
(2)
±k
=
Å
  + V02
tπ2 f k 2
453
9.4
Berry’s Phase
and the new band structure is shown in Fig. 9.13, for the choice V 0 = 0.5t π  . In the neighborhood of the six corners of the BZ, with q  →0, we deﬁne the new variable κz = V0 /h ¯v F , so that the hamiltonian becomes:
ˆ
+
HK q
= h(q) · σ ,
Ã
h(q ) ≡ h¯v F q x xˆ + q y yˆ + κ z ˆz
Ä
For a ﬁxed value of q , we recognize that this hamiltonian is equivalent to the model of a spin interacting with the ﬁeld of a monopole, discussed in the previous example; here, the relevant vector which determines the position of the spin has components (q x, qy , κz ). Solving for the eigenvalues of this hamiltonian in the limit κ z ² q →0, we obtain: Å q2 (1) V0 − h ± K+q = − h¯v F q 2 + κz2 ≈ − ¯v F 2κz (2)
+
±K q
Å 2 = h¯v F q2 + κz2 ≈ V0 + h¯v F 2qκ z
This is a spectrum of energy values qualitatively different from the case because there is a gap between the two eigenvalues for q  =0, given by: ±gap (K)
= qlim →0
²
(2)
+
±K q
V0
=
0
³
− ±K(1)+q = 2V0
For both eigenvalues, the dependence of the energy on q  is quadratic, with an effective mass m given by: 2 2 2 ´h¯v F 2qκ = h¯ 2mq ⇒ m = ´h¯vκz = ´V20
z
vF
F
(2)
(1)
with the positive value corresponding to ±K+q (electrons) and the negative to ±K+q (holes). Because the effective mass m is proportional to the symmetrybreaking term V0 , the latter is usually referred to as simply the “mass” in the literature, as it leads to massive quasiparticles at the valence and conduction band edges. These features are clearly seen in the band structure of the model in Fig. 9.13. (1) In order to obtain the two eigenfunctions corresponding to the eigenvalues ±K+q , (2)
±K q ,
+ we deﬁne an angle θ which is determined by the values of its cosine and sine: cos (θ /2) ≡ Æ
2κz
q2 + (2κz )2
q q2 + (2κz)2
, sin (θ /2) ≡ Æ
(9.50)
With the use of these quantities, we ﬁnd that the eigenfunctions corresponding to the (1) (2) eigenvalues ±K+q , ±K+q turn out to be exactly the same as the eigenfunctions of the spin in a monopole ﬁeld discussed in the previous example! In the limit q  →0 we have θ = 0, that is, the solutions correspond to the spin being at the North pole. For small but ﬁnite values of q, the spin is at some point in the northern hemisphere; the latitude is determined by the relative values of κz = V0 /h¯v F and q . If V0 < 0 the
454
9
Dynamics and Topological Constraints
role of the states labeled (1) and (2) is interchanged, and the spin is in the southern hemisphere. Having made these connections to the model of a spin interacting with the monopole ﬁeld, we can then import all the results obtained for that model, for the Berry curvature and Berry’s phase of the present model; we leave this as an exercise for the reader (see Problem 9). a M. J. Rice and E. J. Mele, Phys. Rev. Lett. 49, 1455 (1982).
9.5
Applications of Berry’s Phase
We consider next some important manifestations of Berry’s phase, which include the Aharonov–Bohm effect, the proper deﬁnition of the polarization in crystals, and the motion of electrons in crystals under the inﬂuence of a uniform external electric ﬁeld; this last case will complete the picture that we presented in Section 9.2. 9.5.1
Aharonov–Bohm Eﬀect
An interesting application of the concepts introduced so far is the Aharonov–Bohm effect. Our quantummechanical system consists of an electron state ψ (r) localized in space by a conﬁning potential V (r), which obeys the Schr¨odinger equation
º
»
ˆ (r) = − ¯ ∇ + V (r) Hψ 2m h2 r2
ψ (r)
e
= ±ψ (r)
in free space. Now we imagine that the origin of the conﬁning potential is shifted by R, so that the hamiltonian acquires a parametric dependence on R:
»
º
2 2 ˆ RψR(r) = − h¯ ∇r + V (r − R) H 2m
e
ψR (r)
= ±RψR(r)
but due to the translational invariance of the system, the wavefunction is simply shifted by R and the energy of this state remains the same: ψR (r)
= ψ (r − R),
±R
=±
We can allow the parameter R to span a closed path C along which the above relations will hold. Next we consider that there is a constant magnetic ﬁeld B generated by a long solenoid within a small region of the area enclosed by the path C , and this region is very far from the path, as shown in Fig. 9.14. The new hamiltonian for the system is (see Appendix C):
²
³
ˆ = 1 −ih¯ ∇r + e A(r) 2 + V (r − R) 2m c
HR
e
455
9.5
Applications of Berry’s Phase
B R
S
R
C z x Fig. 9.14
y
Illustration of Aharonov–Bohm effect description in terms of Berry’s phase: the localized wavefunction ψR is transported around a closed path C which is far from the region where a uniform magnetic ﬁeld exists; the wavefunction acquires a Berry’s phase γ during this process.
where A(r) is the vector potential of the magnetic ﬁeld, B wavefunction for this hamiltonian is given by:
¶
ψR (r)
ie
= exp − hc ¯
¾
r
R
A(r³ ) · dr³
·
ψ (r
= ∇r × A( r). The new − R)
that is, the wavefunction has acquired a phase ϕR : ϕ R (r)
= −hec ¯
¾
r
R
A(r³ ) · dr³
which evidently depends on the path which makes the wavefunction illdeﬁned (it is not singlevalued). For the situation illustrated in Fig. 9.14, we can restore singlevaluedness by carefully choosing the path of integration: the vector potential is zero for values of the integration variable r³ away from the region where the magnetic ﬁeld exists, so as long as the wavefunction is localized and the magnetic ﬁeld is far from the path of R, the wavefunction can be chosen to be wellbehaved (singlevalued). This does not mean that the wavefunction does not change when it is displaced around the closed path: it acquires a Berry’s phase which can be calculated from the theory outlined above. The Berry connection for this example is:
¾ − e A(R) = iµ ψR ∇R ψR ¶ = A(R) + i h¯c
ψ
∗( r − R)∇R ψ (r − R) · dr
We can show that the last term is identically zero by the following argument. We deﬁne r³ = r − R and use the chain rule to switch the variable of differentiation to r³ :
¾
³ ³ ∗ ³ ψ (r )∇r ³ ψ (r ) · d r
¶
∂r
³·
∂R
¾
= −
ψ
∗ (r³ )∇r³ ψ (r³ ) · dr³
but this last expression is proportional to the expectation value of momentum in the state ψ ¶, which for a bound state is zero. Berry’s phase is then given by: γ
= −hce ¯
¿
C
A(R) · dR =
−e ¾ (∇ × A(r)) · dS = −e ¾ B · dS = −2π ² r φ0 h¯c S h¯ c S
456
9
Dynamics and Topological Constraints
with S the surface enclosed by the path C and the ﬁrst equality being the result of Stokes’ theorem; φ0 = (hc /e ) is the ﬂux quantum. We conclude that the value of γ is simply proportional to the total ﬂux ² of the B ﬁeld through the surface enclosed by the path C . Note that this ﬂux is entirely due to the small region in which B exists, and this region is not sampled directly by the localized wavefunction ψR ( r) as it is transported around the closed path. This surprising result, predicted by Aharonov and Bohm,16 is counterintuitive in terms of classical physics because the path of the particle’s displacement is far from the region where the magnetic ﬁeld exists, so it is a manifestation of the quantum nature of the system. The fact that this phase has been measured in interference experiments17 is a remarkable validation of quantum theory. 9.5.2
Polarization of Crystals
An important application of the results we have derived above is the ability to calculate the polarization of crystals. As we have seen, there are positive and negative charges in crystals and their distribution in space can give rise to a net dipole moment per unit volume, which we call the polarization P and deﬁne as:
P=
1
¾
V PUC
VPUC
rρ (r)dr
(9.51)
where ρ (r) is the total charge density within the primitive unit cell and V PUC is its volume; the polarization is proportional to the net electric dipole moment of the system (see also Appendix B); equivalently, we can integrate over the volume of the entire crystal and divide by it. The calculation of P was a vexing problem, because the expression in Eq. (9.51) depends on the choice of the origin of the unit cell, a problem inherent to the periodic crystal, as illustrated in Fig. 9.15, but absent in a ﬁnite system (see Problem 6). In several seminal papers that established the modern theory of polarization, R. Resta18 and independently D. Vanderbilt and coworkers 19 took a different approach which solved the problem of properly calculating the polarization of crystals and established the connection to the Berry curvature. The key insight was to use the current j(r, t ) rather than the charge density ρ (r, t), because the current is periodic in the crystal, while rρ (r, t) is not. To establish the connection between polarization and current, we consider what happens when small changes are introduced in the charge distribution of a crystal by adiabatically turning on an external ﬁeld. The change in the α component of the polarization, ³P α, the only experimentally measurable quantity, can be expressed as: ³P α
16 17 18 19
=
¾
λ2
λ1
∂P α ∂λ
dλ
(9.52)
Y. Aharonov and D. Bohm, Phys. Rev. 115, 485 (1959). See M. Peshkin and A. Tonomura, The Aharonov–Bohm Effect (Springer, Berlin, 1989). R. Resta, Ferroelectrics , 136, 51 (1992). R. D. KingSmith and D. Vanderbilt, Phys. Rev. B 47, 1651 (1993); D. Vanderbilt and R. D. KingSmith, Phys. Rev. B 48, 4442 (1993).
457
9.5
Applications of Berry’s Phase
a p = +qa
p=0
(a)
p +qa
(b)
(c)
0
p=0
(a)
a
(a)
qa
p = qa
a x0
2
(d)
(d)
(c) Fig. 9.15
(b)
Illustration of the ambiguity in determining the dipole moment p in the unit cell of a 1D crystal with period a, which contains localized positive (red curves) and negative (blue curves) charges in each unit cell; the diagram on the right gives the value of p as a function of the position of the unit cell origin x0 (denoted by a black circle).
where λ is a parameter used to express the adiabatic change in the hamiltonian that produces the polarization. We can actually relate λ to the time t by considering a timedependent hamiltonian whose change over a period from t = 0 to t = T produces the polarization. This can be established from the relation between the dipole moment (or, equivalently, the polarization) per unit volume P, the charge density ρ ( r), derived from Eq. (9.51), and the continuity equation (see Appendix B for details), which together give:
∇r · P(r) = −ρ( r),
∂ρ ∂t
+ ∇r · j = 0 ⇒ ∇r ·
¶
∂P ∂t
·
−j = 0
Up to a divergencefree component of the current, which is usually related to the magnetization current that vanishes in the bulk solid (for more details, see the review article by Xiao et al. in Further Reading), we can integrate this last expression over time to get: ³P α
=
¾
T ∂P α ∂t
0
dt =
¾
T 0
jα d t
We can now employ Eq. (9.46) for the velocity, multiplied by the charge by the volume V , to get the current per unit volume: (n )
jα (k , t )
e
= −hV ¯
(n )
∂ ±k
∂kα
e
º
(n )
∂ uk
+ i V µ ∂k  α
(n)
∂uk ∂t
(n )
(n )
∂uk
∂uk
−e and divided
¶ − ∂µ t  ∂ k ¶
»
α
for the contribution of band n at k . For the total current, we need to integrate over the entire BZ and sum over the ﬁlled bands, which produces the total change in polarization. Upon integration over k, the ﬁrst term of the current vanishes because of the symmetry of the bands, Eq. (2.41), while in the second term we recognize the Berry curvature of each band:
º
(n ) µk t (k, t) α
(n )
∂uk
= i µ ∂k  α
(n )
∂uk ∂t
(n)
∂uk
(n)
∂uk
»
¶ − ∂µ t  ∂ k ¶ α
458
9
Dynamics and Topological Constraints
in the parameters k α and t . Putting these results together produces the following expression for the change in polarization: ³P α
± ¾
=e
¾
T
n:ﬁlled BZ 0
dk (2π )3
(n)
µk t (k , t )dt α
In the same manner that we have assumed the polarization to be induced by an adiabatic change in a timedependent hamiltonian, we could also allow the changes to be induced by variation of another physical parameter λ ; this could for instance, be, a smooth, adiabatic deformation of the crystal lattice, which we will take to vary between 0 and 1, leading to the more general expression ³Pα
± ¾
=e
n:ﬁlled
¾
1
BZ 0
(n)
µk
αλ
(k , λ)dλ
dk (2π )3
In this case, we can take advantage of the relation between the Berry curvature and Berry connection: (k, λ) = λ
(n )
µk
α
(n )
∂ Aλ
∂kα
−
(n )
∂ Ak
α
∂λ
to perform the integrals. For the term ∂ A(λn) /∂ k α , we perform ﬁrst the integral over the BZ, (n) which vanishes as long as we choose the parameter λ to make sure that Aλ is periodic (n) in reciprocal space, in the same sense that the wavefunctions u k (r) are periodic, see Eq. (n) (2.42). For the term ∂ Ak /∂ λ, we perform ﬁrst the integral over λ, which gives simply the integrand evaluated at the end points, leading to: α
³P α
= −e
± ¾ n:ﬁlled
²
BZ
(n ) Ak α
³λ=1 dk
=0 (2π )3
λ
= (2−πie)3
± ¾ n:ﬁlled
BZ
´
µ  ∂k  (n ) u k,λ
∂
α
(n ) u k ,λ
µλ =1
¶
λ
=0
dk
where in the last expression we have written explicitly the Berry connection in terms of the wavefunctions which contain the λ dependence from the hamiltonian; this is the expression derived by KingSmith and Vanderbilt for the polarization of crystals that has made possible unambiguous calculations of this important property. Note that by integrating over λ we lose any information about the actual path in λspace. Therefore, the value of the polarization is given up to a multiple of the quantum of polarization (e R/V PUC ), with R being one of the Bravais lattice vectors with smallest magnitude. This means that the path of integration may have passed several times from one end of the PUC to its opposite end, separated by R, a fact lost when only the end points of the path are considered. 9.5.3
Crystal Electrons in Uniform Electric Field
We next consider the effects of an external electric ﬁeld. If we were to express the electric ﬁeld in terms of the electrostatic potential E(r) = −∇ r ²(r), a constant (smooth over large distances in the crystal) ﬁeld would require a linearly increasing potential ²( r) which would destroy the crystal periodicity. Instead, we can use a timedependent vector potential A(r, t ) to express the electric ﬁeld as E(r) = (−1/c )∂ A(r, t)/∂ t (see Appendix B). This
459
9.6
Chern Numbers
choice, at the cost of introducing the independent variable t , allows us to maintain the Bloch states as the basis for describing the physics. We also know that the introduction of such a term changes the hamiltonian to (see Appendix C):
ˆ
Hk (p , r, t )
= 2m1
²
e
e
³2
p + h¯ k + A(r, t ) c
+ V (r)
We can now use the result of Eq. (9.46) in this situation where the origin of the adiabatic change of the wavefunctions with time is the presence of the external electric ﬁeld. First, we deﬁne a new variable q: e ¯ = h¯ k + c A(r, t)
hq
(9.53)
which contains both the k dependence and the t dependence of the hamiltonian. Since we assumed that A(r, t) preserves the translational symmetry of the hamiltonian, k is still a good quantum number, and is therefore a constant of motion, which implies: ∂k ∂t
= 0 ⇒ h¯ ∂∂qt = ec ∂∂At = −eE
In Eqs (9.17) and (9.18) we assumed that a similar expression held for the wavevector k. Here we have proved that it holds instead for the variable q . We can then use these expressions in Eq. (9.46) for the velocity (see Problem 7), which becomes:
µv(kn) ¶ =h1 ∇k ±k(n) + eh E × ±(n)(k) ¯ ¯
(9.54)
with ±(n) (k) the Berry curvature of the band, Eq. (9.43). The ﬁrst term in the above expression is the contribution from band dispersion, the result we had derived from the treatment of the pure crystal that led to Eq. (9.15). The second term is an additional contribution to the velocity, which was referred to as “anomalous velocity” before its relation to the Berry curvature was recognized (for original references, see the review article by Xiao et al. in Further Reading). This term is transverse to the electric ﬁeld and will therefore give rise to a Hall current. This observation makes evident that the Berry curvature and Berry’s phase have an important relation to Hall physics. As a case in (n ) point, we show in Fig. 9.16 the calculated Berry curvature µxy (k) for the highest occupied (valence) band of an interesting 2D solid, MoS2 (see also the discussion in Chapter 5). The Berry curvature takes opposite values in different regions of the BZ, indicating that electrons of different wavevectors will experience opposite forces, leading to interesting behavior. It is evident from this plot that the strongest contribution will be at the corners of the hexagonal BZ, referred to as K and K³ valleys. Manipulating these effects for applications in electronic devices has been termed “valleytronics.”
9.6
Chern Numbers
We will next address some interesting implications of the Berry curvature and Berry connection. We will motivate these implications through a physical argument on a simple
460
Fig. 9.16
9
Dynamics and Topological Constraints
Left: The band structure of a single layer of MoS2 . The highest valence band is shown enclosed in a red rectangle near the Fermi level (zero value on the energy axis). Right: The calculated Berry ˚ −2 ) for the highest valence band; the white hexagon shows the ﬁrst Brillouin zone curvature (A [from S. Fang and E. Kaxiras, Phys. Rev. B 93, 235153 (2016)].
example, and then present a more general argument. Along the way, we will introduce the notion of the Chern number, an important quantity that characterizes the features of the Berry curvature and is intimately related to Berry’s phase. Building on the last result we derived for electrons in a uniform electric ﬁeld, we assume that the carriers are conﬁned in a 2D sheet (the x , y plane) and that the electric ﬁeld is in the xˆ direction, E = E x xˆ , as illustrated in Fig. 9.2. Consistent with these assumptions and the geometry shown in Fig. 9.2, the electron wavefunctions have no dependence on the k z component of the wavevector, and the velocity of electrons from Eq. (9.54) will be given by: µv(kn) ¶ =1 ∇k±(kn) − e E x µ(xyn) (k) ˆy
¯
¯
h
h
This is the contribution from band n at the k value of the wavevector. To get the total current per unit volume, we need to multiply by the charge −e and integrate over the whole BZ. As we have argued in the previous section, integration over the entire BZ of the ﬁrst term gives a zero contribution due to the symmetry of the bands, Eq. (2.41), while the second term gives: 2
jy
±
2
jy e (n ) = eh E x V1 = µxy (k) ⇒ Ex h¯ ¯ k∈BZ
¾
(n )
BZ
µxy
(k)
d kx d k y (2π )2
since we are dealing with a purely 2D situation. The last expression, identiﬁed as the Hall conductivity σxy = jy /E x , can also be written as: 2
σxy
= eh C (1n) ,
(n )
C1
(n )
≡ 21π
¾
BZ
(n )
µxy
(k )dk x dky
(9.55)
where we have deﬁned the quantity C 1 , called the “ﬁrst Chern number” of the band, and expressed the conductivity in units of the quantum of conductance, e 2/h . For this simple example, the Hall conductivity must be equal to an integer number of quanta of
461
9.6
Chern Numbers
conductance, because its value is determined by the number of electrons transferred from one side of the sample to the opposite side in the xˆ direction. In other words, at least for the simple case considered here, we have shown that the ﬁrst Chern number of the band must be an integer. We note that, due to the 2D nature of the system, the Berry curvature takes the form
º
±
(n)
(k)
(n )
(n )
(n)
»
(n)
∂ uk
∂ uk
∂uk
∂uk
x
y
y
x
= i µ ∂ k  ∂ k ¶ − ∂µk  ∂ k ¶ zˆ = µ(xyn) (k)zˆ
and dkx dk y is the surface element dS k = dk x dk y ˆz in reciprocal space for a surface contained within the boundary of the BZ. These considerations compel us to write the ﬁrst Chern number as: ¾ 2π C (1n) ≡
(n )
±
BZ
(k) · dS k
(9.56)
and in this expression we recognize Berry’s phase on the righthand side. The conclusion is that, if the ﬁrst Chern number is an integer, then Berry’s phase for a path that goes around the BZ is an integer multiple of 2π , which produces an invariant of the wavefunction. The reason for introducing the notion of the Chern number is that it constitutes a mathematically precise way of classifying the properties of the surface described by the Berry curvature. Higher Chern numbers can also be deﬁned by proper generalization of the surface curvature.20 What is relevant for the purposes of our discussion is that the integer value of the ﬁrst Chern number describes the torus in 2D space that the symmetric nature of the BZ forms: recall that the functions u(kn) (r) are periodic in k , with the BZ being the unit cell of this periodic pattern, see Eq. (2.42). We next give another argument, beyond the simple motivational example discussed so far, why the ﬁrst Chern number is an integer. We consider a 2D case again, and assume a square lattice which implies that the ﬁrst BZ is given by the region shown in Fig. 9.17. We perform the integral that deﬁnes the ﬁrst Chern number for this case, Eq. (9.56). Instead of actually doing the surface integral, we use Stokes’ theorem to turn it into a line integral of the Berry connection along the boundary of the BZ, the four segments AB–BC–CD–DA (to simplify the notation we use the symbols 1 for the values kx = π/a and k y = π/a and 1¯ for k x = − π/a and k y = − π/a ): 2π C 1(n)
= = =
¿
A
¾
(n)
ABCD
(k x , k y ) · dk
¯
(n ) Ax (kx , 1)d k x
AB ¾ 1 Ã 1¯
A x (kx ,
+
¾
BC
(n) Ay (1, k y )dk y
Ä
1¯ ) − Ax (k x , 1) dk x +
¾
1Ã
1¯
+
¾ CD
(n) A x (k x , 1)dk x
A y(1, k y )
+ Ä
− Ay (1¯ , k y )
(n )
(k x , k y ) = i µu k
(n)
DA
d ky
Now we recall that Aj
¾
 ∂∂k u (kn)¶, j = x , y j
20 S. S.